Survey

* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

Survey

Document related concepts

no text concepts found

Transcript

Springer Series in solid-state sciences Springer Series in solid-state sciences Series Editors: M. Cardona P. Fulde K. von Klitzing R. Merlin H.-J. Queisser H. Störmer The Springer Series in Solid-State Sciences consists of fundamental scientiﬁc books prepared by leading researchers in the ﬁeld. They strive to communicate, in a systematic and comprehensive way, the basic principles as well as new developments in theoretical and experimental solid-state physics. Phase Separation in Soft Matter Physics Micellar Solutions, Microemulsions, Critical Phenomena By P.K. Khabibullaev and A.A. Saidov Optical Response of Nanostructures Microscopic Nonlocal Theory By K. Cho Fractal Concepts in Condensed Matter Physics By T. Nakayama and K. Yakubo Excitons in Low-Dimensional Semiconductors Theory, Numerical Methods, Applications By S. Glutsch Two-Dimensional Coulomb Liquids and Solids By Y. Monarkha and K. Kono X-Ray Multiple-Wave Diﬀraction Theory and Application By S.-L. Chang Physics of Transition Metal Oxides By S. Maekawa, T. Tohyama, S.E. Barnes, S. Ishihara, W. Koshibae, and G. Khaliullin Point-Contact Spectroscopy By Y.G. Naidyuk and I.K. Yanson Optics of Semiconductors and Their Nanostructures Editors: H. Kalt and M. Hetterich Electron Scattering in Solid Matter A Theoretical and Computational Treatise By J. Zabloudil, R. Hammerling, L. Szunyogh, and P. Weinberger Physical Acoustics in the Solid State By B. Lthi Solitary Waves in Complex Dispersive Media Theory · Simulation · Applications By V.Yu. Belashov and S.V. Vladimirov Topology in Condensed Matter Editor: M.I. Monastyrsky Particle Penetration and Radiation Eﬀects By P. Sigmund Magnetism From Fundamentals to Nanoscale Dynamics By H.C. Siegmann and J. Sthr Quantum Chemistry of Solids The LCAO First Principles Treatment of Crystals By R.A. Evarestov Low-Dimensional Molecular Metals By N. Toyota, M. Lang and J. Mller Diﬀusion in Solids Fundamentals, Methods, Materials, Diﬀusion-Controlled Processes By H. Mehrer Volumes – are listed at the end of the book. Helmut Mehrer Diffusion in Solids Fundamentals, Methods, Materials, Diﬀusion-Controlled Processes With Figures and Tables 123 Professor Dr. Helmut Mehrer Universität Münster Institut für Materialphysik Wilhelm-Klemm-Str. Münster Germany Series Editors: Professor Dr., Dres. h. c. Manuel Cardona Professor Dr., Dres. h. c. Peter Fulde∗ Professor Dr., Dres. h. c. Klaus von Klitzing Professor Dr., Dres. h. c. Hans-Joachim Queisser Max-Planck-Institut für Festkörperforschung, Heisenbergstrasse , Stuttgart, Germany ∗ Max-Planck-Institut für Physik komplexer Systeme, Nöthnitzer Strasse Dresden, Germany Professor Dr. Roberto Merlin Department of Physics, East University, University of Michigan Ann Arbor, MI -, USA Professor Dr. Horst Störmer Dept. Phys. and Dept. Appl. Physics, Columbia University, New York, NY and Bell Labs., Lucent Technologies, Murray Hill, NJ , USA Library of Congress Control Number: ISSN - ISBN ---- Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September , , in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com © Springer-Verlag Berlin Heidelberg The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting and production: LE-TEX Jelonek, Schmidt & Vöckler GbR, Leipzig Cover design: eStudioCalamar S.L., F. Steinen-Broo, Girona, Spain SPIN //YL – Printed on acid-free paper For Karin and my family, who wonder what I did all the time. In particular I express my enduring thanks to my wife Karin. Without her patience, understanding, and love I could not have completed this book. Preface Diﬀusion is the transport of matter from one point to another by thermal motion of atoms or molecules. It is relatively fast in gases, slow in liquids, and very slow in solids. Diﬀusion plays a key rôle in many processes as diverse as intermixing of gases and liquids, permeation of atoms or molecules through membranes, evaporation of liquids, drying of timber, doping silicon wafers to make semiconductor devices, and transport of thermal neutrons in nuclear power reactors. Rates of important chemical reactions are limited by how fast diﬀusion can bring reactants together or deliver them to reaction sites on enzymes or other catalysts. Diﬀusion in solid materials is the subject of this book. Already in ancient times reactions in the solid state such as surface hardening of steels were in use, which according to our present knowledge involves the diﬀusion of carbon atoms in the crystal lattice of iron. Nevertheless, until the end of the nineteenth century the paradigm ‘Corpora non agunt nisi ﬂuida’ was widely accepted by the scientiﬁc community. It was mainly due to the pioneering work of William Roberts-Austen and Georg von Hevesy that this paradigm had to be abandoned. Diﬀusion in solids is fundamental in the art and science of materials and thus an important topic of solid-state physics, physical chemistry, physical metallurgy, and materials science. Diﬀusion processes are relevant for the kinetics of many microstructural changes that occur during preparation, processing, and heat treatment of materials. Typical examples are nucleation of new phases, diﬀusive phase transformations, precipitation and dissolution of a second phase, homogenisation of alloys, recrystallisation, high-temperature creep, and thermal oxidation. Diﬀusion and electrical conduction in ionic conductors are closely related phenomena. Direct technological applications of diﬀusion concern, e.g., doping during fabrication of microelectronic devices, solid electrolytes for batteries and fuel cells, surface hardening of steel through carburisation or nitridation, diﬀusion bonding, and sintering. Appreciable diﬀusion in solids mostly takes place at temperatures well above room temperature. Knowledge of diﬀusion is therefore particularly important for scientists who design materials for elevated temperatures and for engineers who build equipment for operation at such temperatures. However, processes connected with diﬀusion at room temperature pose problems, too. VIII Creep, atmospheric corrosion, and embrittlement of solders are among the more prominent of those. With the downscaling of microelectronic circuits to nanometer dimensions, diﬀusion and electromigration in these circuits must be taken into account. A deeper knowledge about diﬀusion requires information on the position of atoms and how they move in solids. The atomic mechanisms of diﬀusion in crystalline solids are closely connected with defects. Point defects such as vacancies or interstitials are the simplest defects and often mediate diﬀusion in crystals. Dislocations, grain-boundaries, phase boundaries, and free surfaces are other types of defects. They can act as high-diﬀusivity paths (diﬀusion short circuits), because the mobility of atoms along such defects is usually much higher than in the lattice. In solids with structural disorder such as glasses or crystals with highly disordered sublattices the concept of defects is no longer useful. Nevertheless, diﬀusion is fundamental for transport of matter and for ionic conduction in disordered materials. The content of this book is divided into seven parts. After a historical introduction and a diﬀusion bibliography, Part I introduces basic concepts of diﬀusion in solid matter such as continuum description, random walk theory, point defects, atomic mechanisms, correlation eﬀects, dependence of diﬀusion on temperature, pressure and isotope mass, diﬀusion with driving forces , and some remarks about the relation between diﬀusion and thermodynamics of irreversible processes. The necessary background is a course in solid-state physics. In Part II we describe experimental methods for the determination of diﬀusion coeﬃcients in solid matter. Direct methods based on Fick’s laws and indirect methods such as anelastic relaxation, internal friction, nuclear magnetic relaxation, Mössbauer spectroscopy, quasielastic neutron scattering, impedance spectroscopy, and spreading resistance measurements are treated. In further parts we provide access to information on diﬀusion in various types of materials such as metals, intermetallics and quasicrystalline alloys (Part III ), semiconductors (Part IV ), ionic materials including fast ion conductors (Part V ), metallic and oxide glasses (Part VI ). Finally, rapid diffusion paths such as grain-boundary diﬀusion and diﬀusion in nanomaterials are considered (Part VII ). Although these parts cannot replace a comprehensive data collection, typical up-to-date resources available on diﬀusion for various types of materials are noted. A thorough understanding of diﬀusion in materials is crucial for materials development and engineering. Graduate students in solid state physics, physical metallurgy, physical and inorganic chemistry, and geophysical materials will beneﬁt from this book as will physicists, chemists and metallurgists, working in academia and industry. Münster, May 2007 Helmut Mehrer Acknowledgements Like any author of a scientiﬁc book, I am indebted to previous writers on diffusion and allied subjects. In particular I acknowledge the encouragement of colleagues and friends who provided invaluable assistance during the preparation of the book. Prof. Hartmut Bracht, Prof. Klaus Funke, and Dr. Nikolaas Stolwijk, all from the University of Münster, have read many chapters as they unfolded. Prof. Gabor Erdelyi, Debrecen, Hungary, Prof. Andry Gusak, Cherkassy, Ukraine, Dr. J.N. Mundy, USA, and Prof. Malcom Ingram, University of Aberdeen, Great Britain, stayed in my University as guest scientist for some time and have also reviewed several chapters of the book. Dr. M. Hirscher, Max-Planck-Institut für Metallforschung, Stuttgart, provided comments for the chapter on hydrogen diﬀusion. Prof. Gerhard Wilde from the University of Münster made useful suggestions for the chapter on nanomaterials. Prof. Graeme Murch, Newcastle, Australia, did a great job in reading the whole book, polishing my English, and providing many helpful suggestions. To my collaborators Dr. Serguei Divinski, Dr. Arpad Imre, Dr. Halgard Staesche and my PhD students and postdocs Dr. Robert Galler, Dr. Marcel Salamon, Dr. Serguei Peteline, Dr. Eugene Tanguep Nijokep, Dr. Stephan Voss, and to my secretary Sylvia Gurnik I owe many thanks for critically reading parts of the book. Dr. Arpad Imre was a great help in preparing most ﬁgures. The contributions and constructive criticisms of all these persons were most helpful. Contents 1 History and Bibliography of Diﬀusion . . . . . . . . . . . . . . . . . . . . 1 1.1 Pioneers and Landmarks of Diﬀusion . . . . . . . . . . . . . . . . . . . . . . 2 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16 1.2 Bibliography of Solid-State Diﬀusion . . . . . . . . . . . . . . . . . . . . . . 18 Part I Fundamentals of Diﬀusion 2 Continuum Theory of Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Fick’s Laws in Isotropic Media . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Fick’s First Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.2 Equation of Continuity . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.3 Fick’s Second Law – the ‘Diﬀusion Equation’ . . . . . . . . 2.2 Diﬀusion Equation in Various Coordinates . . . . . . . . . . . . . . . . . 2.3 Fick’s Laws in Anisotropic Media . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27 27 28 29 30 31 33 35 3 Solutions of the Diﬀusion Equation . . . . . . . . . . . . . . . . . . . . . . . 3.1 Steady-State Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Non-Steady-State Diﬀusion in one Dimension . . . . . . . . . . . . . . 3.2.1 Thin-Film Solution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 Extended Initial Distribution and Constant Surface Concentration . . . . . . . . . . . . . . . . 3.2.3 Method of Laplace Transformation . . . . . . . . . . . . . . . . . 3.2.4 Diﬀusion in a Plane Sheet – Separation of Variables . . 3.2.5 Radial Diﬀusion in a Cylinder . . . . . . . . . . . . . . . . . . . . . . 3.2.6 Radial Diﬀusion in a Sphere . . . . . . . . . . . . . . . . . . . . . . . 3.3 Point Source in one, two, and three Dimensions . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37 37 39 39 Random Walk Theory and Atomic Jump Process . . . . . . . . . 4.1 Random Walk and Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.1 A Simpliﬁed Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.2 Einstein-Smoluchowski Relation . . . . . . . . . . . . . . . . . . . . 4.1.3 Random Walk on a Lattice . . . . . . . . . . . . . . . . . . . . . . . . 55 56 56 58 60 4 41 45 47 50 51 52 53 XII Contents 4.1.4 Correlation Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62 4.2 Atomic Jump Process . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 66 5 Point Defects in Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Pure Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.1 Vacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.2 Divacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.3 Determination of Vacancy Properties . . . . . . . . . . . . . . . 5.1.4 Self-Interstitials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Substitutional Binary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Vacancies in Dilute Alloys . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.2 Vacancies in Concentrated Alloys . . . . . . . . . . . . . . . . . . . 5.3 Ionic Compounds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Frenkel Disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.2 Schottky Disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 69 70 70 72 74 79 80 81 82 83 84 85 86 88 91 6 Diﬀusion Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Interstitial Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Collective Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 Vacancy Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Divacancy Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Interstitialcy Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Interstitial-substitutional Exchange Mechanisms . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 95 95 97 98 100 100 102 103 7 Correlation in Solid-State Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 7.1 Interstitial Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Interstitialcy Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3 Vacancy Mechanism of Self-diﬀusion . . . . . . . . . . . . . . . . . . . . . . 7.3.1 A ‘Rule of Thumb’ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.2 Vacancy-tracer Encounters . . . . . . . . . . . . . . . . . . . . . . . . 7.3.3 Spatial and Temporal Correlation . . . . . . . . . . . . . . . . . . 7.3.4 Calculation of Correlation Factors . . . . . . . . . . . . . . . . . . 7.4 Correlation Factors of Self-diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 7.5 Vacancy-mediated Solute Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 7.5.1 Face-Centered Cubic Solvents . . . . . . . . . . . . . . . . . . . . . . 7.5.2 Body-Centered Cubic Solvents . . . . . . . . . . . . . . . . . . . . . 7.5.3 Diamond Structure Solvents . . . . . . . . . . . . . . . . . . . . . . . 7.6 Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105 107 107 108 108 109 112 112 115 116 117 120 121 122 124 Contents XIII 8 Dependence of Diﬀusion on Temperature and Pressure . . . 8.1 Temperature Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.1 The Arrhenius Relation . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.2 Activation Parameters – Examples . . . . . . . . . . . . . . . . . 8.2 Pressure Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.1 Activation Volumes of Self-diﬀusion . . . . . . . . . . . . . . . . . 8.2.2 Activation Volumes of Solute Diﬀusion . . . . . . . . . . . . . . 8.2.3 Activation Volumes of Ionic Crystals . . . . . . . . . . . . . . . . 8.3 Correlations between Diﬀusion and Bulk Properties . . . . . . . . . 8.3.1 Melting Properties and Diﬀusion . . . . . . . . . . . . . . . . . . . 8.3.2 Activation Parameters and Elastic Constants . . . . . . . . 8.3.3 Use of Correlations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 127 127 127 130 132 135 139 140 141 141 146 147 147 9 Isotope Eﬀect of Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 Single-jump Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Collective Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Isotope Eﬀect Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 151 151 155 155 159 10 Interdiﬀusion and Kirkendall Eﬀect . . . . . . . . . . . . . . . . . . . . . . . 10.1 Interdiﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.1.1 Boltzmann Transformation . . . . . . . . . . . . . . . . . . . . . . . . 10.1.2 Boltzmann-Matano Method . . . . . . . . . . . . . . . . . . . . . . . . 10.1.3 Sauer-Freise Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Intrinsic Diﬀusion and Kirkendall Eﬀect . . . . . . . . . . . . . . . . . . . 10.3 Darken Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4 Darken-Manning Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 Microstructural Stability of the Kirkendall Plane . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 161 161 162 163 166 168 170 172 173 176 11 Diﬀusion and External Driving Forces . . . . . . . . . . . . . . . . . . . . 11.1 Overview . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 Fick’s Equations with Drift . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3 Nernst-Einstein Relation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.4 Nernst-Einstein Relation for Ionic Conductors and Haven Ratio . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5 Nernst-Planck Equation – Interdiﬀusion in Ionic Crystals . . . . 11.6 Nernst-Planck Equation versus Darken Equation . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 179 179 181 182 12 Irreversible Thermodynamics and Diﬀusion . . . . . . . . . . . . . . . 12.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2 Phenomenological Equations of Isothermal Diﬀusion . . . . . . . . 12.2.1 Tracer Self-Diﬀusion in Element Crystals . . . . . . . . . . . . 191 191 193 193 184 186 188 189 XIV Contents 12.2.2 Diﬀusion in Binary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . 12.3 The Phenomenological Coeﬃcients . . . . . . . . . . . . . . . . . . . . . . . . 12.3.1 Phenomenological Coeﬃcients, Tracer Diﬀusivities, and Jump Models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.2 Sum Rules – Relations between Phenomenological Coeﬃcients . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 195 199 202 204 205 Part II Experimental Methods 13 Direct Diﬀusion Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.1 Direct versus Indirect Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2 The Various Diﬀusion Coeﬃcients . . . . . . . . . . . . . . . . . . . . . . . . 13.2.1 Tracer Diﬀusion Coeﬃcients . . . . . . . . . . . . . . . . . . . . . . . 13.2.2 Interdiﬀusion and Intrinsic Diﬀusion Coeﬃcients . . . . . 13.3 Tracer Diﬀusion Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.3.1 Proﬁle Analysis by Serial Sectioning . . . . . . . . . . . . . . . . 13.3.2 Residual Activity Method . . . . . . . . . . . . . . . . . . . . . . . . . 13.4 Isotopically Controlled Heterostructures . . . . . . . . . . . . . . . . . . . 13.5 Secondary Ion Mass Spectrometry (SIMS) . . . . . . . . . . . . . . . . . 13.6 Electron Microprobe Analysis (EMPA) . . . . . . . . . . . . . . . . . . . . 13.7 Auger-Electron Spectroscopy (AES) . . . . . . . . . . . . . . . . . . . . . . 13.8 Ion-beam Analysis: RBS and NRA . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 209 209 212 212 214 215 217 222 223 224 227 230 231 234 14 Mechanical Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2 Anelasticity and Internal Friction . . . . . . . . . . . . . . . . . . . . . . . . . 14.3 Techniques of Mechanical Spectroscopy . . . . . . . . . . . . . . . . . . . . 14.4 Examples of Diﬀusion-related Anelasticty . . . . . . . . . . . . . . . . . . 14.4.1 Snoek Eﬀect (Snoek Relaxation) . . . . . . . . . . . . . . . . . . . 14.4.2 Zener Eﬀect (Zener Relaxation) . . . . . . . . . . . . . . . . . . . . 14.4.3 Gorski Eﬀect (Gorski Relaxation) . . . . . . . . . . . . . . . . . . 14.4.4 Mechanical Loss in Ion-conducting Glasses . . . . . . . . . . . 14.5 Magnetic Relaxation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 237 237 239 242 244 244 247 248 249 250 251 15 Nuclear Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2 Nuclear Magnetic Relaxation (NMR) . . . . . . . . . . . . . . . . . . . . . 15.2.1 Fundamentals of NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2.2 Direct Diﬀusion Measurement by Field-Gradient NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2.3 NMR Relaxation Methods . . . . . . . . . . . . . . . . . . . . . . . . . 253 253 253 254 256 258 Contents XV 15.3 Mössbauer Spectroscopy (MBS) . . . . . . . . . . . . . . . . . . . . . . . . . . 15.4 Quasielastic Neutron Scattering (QENS) . . . . . . . . . . . . . . . . . . 15.4.1 Examples of QENS studies . . . . . . . . . . . . . . . . . . . . . . . . 15.4.2 Advantages and Limitations of MBS and QENS . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 264 269 278 279 281 16 Electrical Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.1 Impedance Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Spreading Resistance Proﬁling . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 285 285 290 293 Part III Diﬀusion in Metallic Materials 17 Self-diﬀusion in Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2 Cubic Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.1 FCC Metals – Empirical Facts . . . . . . . . . . . . . . . . . . . . . 17.2.2 BCC Metals – Empirical Facts . . . . . . . . . . . . . . . . . . . . . 17.2.3 Monovacancy Interpretation . . . . . . . . . . . . . . . . . . . . . . . 17.2.4 Mono- and Divacancy Interpretation . . . . . . . . . . . . . . . . 17.3 Hexagonal Close-Packed and Tetragonal Metals . . . . . . . . . . . . 17.4 Metals with Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 297 297 299 299 301 302 303 306 308 311 18 Diﬀusion of Interstitial Solutes in Metals . . . . . . . . . . . . . . . . . 18.1 ‘Heavy’ Interstitial Solutes C, N, and O . . . . . . . . . . . . . . . . . . . 18.1.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.1.2 Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.1.3 Interstitial Diﬀusion in Dilute Interstial Alloys . . . . . . . 18.2 Hydrogen Diﬀusion in Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.2 Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.3 Examples of Hydrogen Diﬀusion . . . . . . . . . . . . . . . . . . . . 18.2.4 Non-Classical Isotope Eﬀects . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313 313 313 314 316 317 317 318 320 323 324 19 Diﬀusion in Dilute Substitutional Alloys . . . . . . . . . . . . . . . . . . 19.1 Diﬀusion of Impurities . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.1.1 ‘Normal’ Impurity Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 19.1.2 Impurity Diﬀusion in Al . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2 Impurity Diﬀusion in ‘Open’ Metals – Dissociative Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3 Solute Diﬀusion and Solvent Diﬀusion in Alloys . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 327 327 327 332 333 336 338 XVI Contents 20 Diﬀusion in Binary Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . 20.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.2 Inﬂuence of Order-Disorder Transitions . . . . . . . . . . . . . . . . . . . . 20.3 B2 Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.1 Diﬀusion Mechanisms in B2 Phases . . . . . . . . . . . . . . . . . 20.3.2 Example B2 NiAl . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.3 Example B2 Fe-Al . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4 L12 Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.5 D03 Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.6 Uniaxial Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.6.1 L10 Intermetallics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.6.2 Molybdenum Disilicide (C11b structure) . . . . . . . . . . . . . 20.7 Laves Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.8 The Cu3 Au Rule . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 341 341 344 346 347 351 353 355 357 360 360 362 364 366 367 21 Diﬀusion in Quasicrystalline Alloys . . . . . . . . . . . . . . . . . . . . . . . 21.1 General Remarks on Quasicrystals . . . . . . . . . . . . . . . . . . . . . . . . 21.2 Diﬀusion Properties of Quasicrystals . . . . . . . . . . . . . . . . . . . . . . 21.2.1 Icosahedral Quasicrystals . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.2 Decagonal Quasicrystals . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 371 371 373 374 379 381 Part IV Diﬀusion in Semiconductors 22 General Remarks on Semiconductors . . . . . . . . . . . . . . . . . . . . . 22.1 ‘Semiconductor Age’ and Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . 22.2 Speciﬁc Features of Semiconductor Diﬀusion . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 385 386 389 392 23 Self-diﬀusion in Elemental Semiconductors . . . . . . . . . . . . . . . 23.1 Intrinsic Point Defects and Diﬀusion . . . . . . . . . . . . . . . . . . . . . . 23.2 Germanium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23.3 Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 395 396 398 402 406 24 Foreign-Atom Diﬀusion in Silicon and Germanium . . . . . . . . 24.1 Solubility and Site Occupancy . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.2 Diﬀusivities and Diﬀusion Modes . . . . . . . . . . . . . . . . . . . . . . . . . 24.2.1 Interstitial Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.2.2 Dopant Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.2.3 Diﬀusion of Hybrid Foreign Elements . . . . . . . . . . . . . . . 24.3 Self- and Foreign Atom Diﬀusion – a Summary . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 409 409 412 414 416 420 421 422 Contents XVII 25 Interstitial-Substitutional Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 25.1 Combined Dissociative and Kick-out Diﬀusion . . . . . . . . . . . . . . 25.1.1 Diﬀusion Limited by the Flow of Intrinsic Defects . . . . 25.1.2 Diﬀusion Limited by the Flow of Interstitial Solutes . . 25.1.3 Numerical Analysis of an Intermediate Case . . . . . . . . . 25.2 Kick-out Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25.2.1 Basic Equations and two Solutions . . . . . . . . . . . . . . . . . 25.2.2 Examples of Kick-Out Diﬀusion . . . . . . . . . . . . . . . . . . . . 25.3 Dissociative Mechanism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25.3.1 Basic Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25.3.2 Examples of Dissociative Diﬀusion . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 425 425 427 429 430 431 431 434 439 439 440 445 Part V Diﬀusion and Conduction in Ionic Materials 26 Ionic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.2 Point Defects in Ionic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.2.1 Intrinsic Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.2.2 Extrinsic Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.3 Methods for the Study of Defect and Transport Properties . . . 26.4 Alkali Halides . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.4.1 Defect Motion, Tracer Self-diﬀusion, and Ionic Conduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.4.2 Example NaCl . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.4.3 Common Features of Alkali Halides . . . . . . . . . . . . . . . . . 26.5 Silver Halides AgCl and AgBr . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.5.1 Self-diﬀusion and Ionic Conduction . . . . . . . . . . . . . . . . . 26.5.2 Doping Eﬀects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 449 449 451 452 454 456 458 27 Fast Ion Conductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27.1 Fast Silver-Ion Conductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27.1.1 AgI and related Simple Anion Structures . . . . . . . . . . . . 27.1.2 RbAg4 I5 and related Compounds . . . . . . . . . . . . . . . . . . . 27.2 PbF2 and other Halide Ion Conductors . . . . . . . . . . . . . . . . . . . . 27.3 Stabilised Zirconia and related Oxide Ion Conductors . . . . . . . 27.4 Perovskite Oxide Ion Conductors . . . . . . . . . . . . . . . . . . . . . . . . . 27.5 Sodium β-Alumina and related Materials . . . . . . . . . . . . . . . . . . 27.6 Lithium Ion Conductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27.7 Polymer Electrolytes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 475 477 477 479 480 481 482 482 484 485 488 458 462 467 468 469 471 473 XVIII Contents Part VI Diﬀusion in Glasses 28 The Glassy State . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.1 What is a Glass? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.2 Volume-Temperature Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.3 Temperature-Time-Transformation Diagram . . . . . . . . . . . . . . . 28.4 Glass Families . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 493 493 494 496 498 501 29 Diﬀusion in Metallic Glasses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29.2 Structural Relaxation and Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . 29.3 Diﬀusion Properties of Metallic Glasses . . . . . . . . . . . . . . . . . . . 29.4 Diﬀusion and Viscosity in Glass-forming Alloys . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 503 503 506 509 517 518 30 Diﬀusion and Ionic Conduction in Oxide Glasses . . . . . . . . . 30.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.2 Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.3 Gas Permeation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.4 Examples of Diﬀusion and Ionic Conduction . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 521 521 526 529 530 542 Part VII Diﬀusion along High-Diﬀusivity Paths and in Nanomaterials 31 High-diﬀusivity Paths in Metals . . . . . . . . . . . . . . . . . . . . . . . . . . 31.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 31.2 Diﬀusion Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 31.3 Empirical Rules for Grain-Boundary Diﬀusion . . . . . . . . . . . . . . 31.4 Lattice Diﬀusion and Microstructural Defects . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 547 547 548 549 551 552 32 Grain-Boundary Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32.2 Grain Boundaries . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32.2.1 Low- and High-Angle Grain Boundaries . . . . . . . . . . . . . 32.2.2 Special High-Angle Boundaries . . . . . . . . . . . . . . . . . . . . . 32.3 Diﬀusion along an Isolated Boundary (Fisher Model) . . . . . . . . 32.4 Diﬀusion Kinetics in Polycrystals . . . . . . . . . . . . . . . . . . . . . . . . . 32.4.1 Type A Kinetics Regime . . . . . . . . . . . . . . . . . . . . . . . . . . 32.4.2 Type B Kinetics Regime . . . . . . . . . . . . . . . . . . . . . . . . . . 32.4.3 Type C Kinetics Regime . . . . . . . . . . . . . . . . . . . . . . . . . . 553 553 554 555 557 559 568 568 570 574 Contents XIX 32.5 Grain-Boundary Diﬀusion and Segregation . . . . . . . . . . . . . . . . . 576 32.6 Atomic Mechanisms of Grain-Boundary Diﬀusion . . . . . . . . . . . 579 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 580 33 Dislocation Pipe Diﬀusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33.1 Dislocation Pipe Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33.2 Solutions for Mean Thin Layer Concentrations . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 583 584 586 591 34 Diﬀusion in Nanocrystalline Materials . . . . . . . . . . . . . . . . . . . . 34.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.2 Synthesis of Nanocrystalline Materials . . . . . . . . . . . . . . . . . . . . 34.2.1 Powder Processing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.2.2 Heavy Plastic Deformation . . . . . . . . . . . . . . . . . . . . . . . . 34.2.3 Chemical and Related Synthesis Methods . . . . . . . . . . . . 34.2.4 Devitriﬁcation of Amorphous Precursors . . . . . . . . . . . . 34.3 Diﬀusion in Poly- and Nanocrystals . . . . . . . . . . . . . . . . . . . . . . . 34.3.1 Grain Size and Diﬀusion Regimes . . . . . . . . . . . . . . . . . . 34.3.2 Eﬀective Diﬀusivities in Poly- and Nanocrystals . . . . . . 34.4 Diﬀusion in Nanocrystalline Metals . . . . . . . . . . . . . . . . . . . . . . . 34.4.1 General Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.4.2 Structural Relaxation and Grain Growth . . . . . . . . . . . . 34.4.3 Nanomaterials with Bimodal Grain Structure . . . . . . . . 34.4.4 Grain Boundary Triple Junctions . . . . . . . . . . . . . . . . . . . 34.5 Diﬀusion and Ionic Conduction in Nanocrystalline Ceramics . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 593 593 594 594 596 598 598 599 599 604 606 606 607 608 612 612 618 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 639 Part I Fundamentals of Diﬀusion 1 History and Bibliography of Diﬀusion If a droplet of ink is placed without stirring at the bottom of a bottle ﬁlled with water, the colour will slowly spread through the bottle. At ﬁrst, it will be concentrated near the bottom. After a few days, it will penetrate upwards a few centimeters. After several days, the solution will be coloured homogeneously. The process responsible for the movement of the coloured material is diﬀusion. Diﬀusion is caused by the Brownian motion of atoms or molecules that leads to complete mixing. In gases, diﬀusion progresses at a rate of centimeters per second; in liquids, its rate is typically fractions of millimeters per second; in solids, diﬀusion is a fairly slow process and the rate of diﬀusion decreases strongly with decreasing temperature: near the melting temperature of a metal a typical rate is about one micrometer per second; near half of the melting temperature it is only of the order of nanometers per second. The science of diﬀusion in solids had its beginnings in the 19th century, although the blacksmiths and metal artisans of antiquity already used the phenomenon to make such objects as swords of steel, gilded copper or bronce wares. Diﬀusion science is based on several corner stones. The most important ones are: (i) The continuum theory of diﬀusion originated from work of the German scientist Adolf Fick, who was inspired by elegant experiments on diﬀusion in gases and of salt in water performed by Thomas Graham in Scotland. (ii) The Brownian motion was detected by the Scotish botanist Robert Brown. He observed small particles suspended in water migrating in an erratic fashion. This phenomenon was interpreted many decades later by Albert Einstein. He realised that the ‘dance’ described by Brown was a random walk driven by the collisions between particles and the water molecules. His theory provided the statistical cornerstone of diﬀusion and bridged the gap between mechanics and thermodynamics. It was veriﬁed in beautiful experiments by the French Nobel laureate Jean Baptiste Perrin. (iii) The atomistics of solidstate diﬀusion had to wait for the birth date of solid-state physics heralded by the experiments of Max von Laue. Equally important was the perception of the Russian and German scientists Jakov Frenkel and Walter Schottky that point defects play an important rôle for properties of crystalline substances, most notably for those controlling diﬀusion and the many properties that stem from it. This chapter is not meant to be a systematic history of diﬀusion science. It is devoted in its ﬁrst section to some major landmarks and eminent people 2 1 History and Bibliography of Diﬀusion in the ﬁeld. The second section contains information about bibliography of diﬀusion in textbooks, monographs, conference proceedings, and data collections. 1.1 Pioneers and Landmarks of Diﬀusion Establishment of the diﬀusion law: Experimental studies of diﬀusion were probably performed for the ﬁrst time by Thomas Graham (1805–1869). Graham was born in Glasgow. His father was a successful textile manufacturer. He wished his son to enter the Church of Scotland. Defying his father’s wishes he studied natural sciences, developed a strong interest in chemistry and became professor of chemistry in 1830 at the Andersonian Institute (now Strathclyde University) in Glasgow. Later he became professor of chemistry at several colleges including the Royal College of Science and Technology and the University of London in 1837. Graham helped to found the Chemical Society of London and became its ﬁrst president. In 1854 Graham succeeded Sir John Herschel as Master of the Mint in London following the tradition – established by Sir Isaac Newton – of distinguished scientists occupying the post. Graham is one of the founders of physical chemistry and he discovered the medical method of ‘dialysis’. He initiated the quantitative study of diﬀusion in gases, largely conducted in the years of 1828 to 1833 [1, 2]. In one of his articles he explicitly stated what we now call Graham’s law: ‘The diﬀusion or spontaneous intermixture of two gases is eﬀected by an interchange in position of indeﬁnitely minute volumes of the gases, which volumes are not of equal magnitude, being, in the case of each gas, inversely proportional to the square root of the density of that gas.’ The crucial point about Graham’s work on diﬀusion in gases was that it could be understood by the kinetic theory of gases developed by Maxwell and Clausius shortly after the middle of the 19th century. Graham’s law can be attributed to the equipartition of kinetic energies between molecules with diﬀerent molecular masses. In this way diﬀusion was connected with the thermal motion of atoms or molecules, and the idea of the mean free path entered science. Graham also extended his studies to diﬀusion of salts in liquids [3] and to the uptake of hydrogen in metals. He showed that diﬀusion in liquids was at least several thousand times slower than in gases. The next major advance in the ﬁeld of diﬀusion came from the work done by Adolf Eugen Fick (1829–1901). He was born in Kassel, Germany, as the youngest of ﬁve siblings. His father, a civil engineer, was a superintendent of buildings. During his secondary schooling, Adolf Fick was delighted by mathematics, especially by the work of Fourier and Poisson. He entered the University of Marburg with the intention to specialise in mathematics, but switched to medicine on the advice of an elder brother, a professor of anatomy. He got his doctorate with a thesis on ‘Visual Errors due to Astigmatism’. He 1.1 Pioneers and Landmarks of Diﬀusion 3 spent the years from 1852 to 1668 at the University of Zürich, Switzerland, in various positions. After sixteen years in Zürich he accepted a chair in physiology in Würzburg, Germany. Graham’s work on diﬀusion of salts in water stimulated Fick to develop a mathematical framework to describe the phenomena of diﬀusion using the analogy between Fourier’s law of thermal conduction and diﬀusion [4, 5]. Fick signed his papers on diﬀusion as ‘Demonstrator of Anatomy, Zürich’. They were published in high-ranking journals. His approach was a phenomenological one and uses a continuum description. Nowadays, we would call his theory a ‘linear response’ approach. Fick is even better known in medicine. He published a well-rounded monography on ‘Medical Physics’ [6] and a textbook on ‘The Anatomy of Sense Organs’. He became an outstanding person in the small group of nineteenth century physiologists who applied concepts and methods of physics to the study of living organisms, and thereby laid the foundations of modern physiology. Fick’s vital contribution to the ﬁeld of diﬀusion was to deﬁne the diﬀusion coeﬃcient and to measure it for diﬀusion of salt in water. Mathematical solutions of Fick’s equations began with the nineteenth century luminaries Jozef Stephan [7] and Franz Neumann, who were among the ﬁrst to recognise the signiﬁcance of boundary conditions for solutions of the diﬀusion equation. Roberts-Austen – discovery of solid-state diﬀusion: William Chandler Roberts-Austen (1843–1902) graduated from the Royal School of Mines, London, in 1865 and became personal assistant to Graham at the Mint. After Graham’s death in 1869 Roberts-Austen became ‘Chemist and Assayer of the Mint’, a position he occupied until his death. He was appointed professor of metallurgy at the Royal School of Mines in 1880 and was knighted in 1899 by Queen Victoria. He was a man of wide interests, with charm, and an understanding of people, which made him very popular. He conducted studies on the eﬀects of impurities on the physical properties of pure metals and alloys and became a world authority on the technical aspects of minting coins. His work had many practical and industrial applications. Austenite – a nonmagnetic solution of carbon in iron – is named after Sir Roberts-Austen. He records his devotion to diﬀusion research as follows [8]: ‘. . . My long connection with Graham’s researches made it almost a duty to attempt to extend his work on liquid diﬀusion to metals.’ Roberts-Austen perfected the technique for measuring high temperatures adopting Le Chatelier’s platinumbased thermocouples and studied the diﬀusion of gold, platinum, and rhodium in liquid lead; of gold, silver, and lead in liquid tin; and of gold in bismuth. These solvents were selected because of their relatively low melting temperatures. The solidiﬁed samples were sectioned and the diﬀused species determined in each section using the high precision assaying techniques developed for use in the Mint. Typically six or seven sections were taken and diﬀusion coeﬃcients determined. Even more importantly, Roberts-Austen applied these techniques to the study of gold diﬀusion in solid lead as well. It is interesting 4 1 History and Bibliography of Diﬀusion to observe that the values of the diﬀusion coeﬃcient of gold in lead reported by him are very close to those determined by modern techniques using radioactive isotopes. The choice of the system gold in lead was really fortunate. Nowadays, we know that the diﬀusion of noble metals in lead is exceptionally fast in comparison to most other diﬀusion processes in solids. Arrhenius law of solid-state diﬀusion: The most surprising omission in Roberts-Austen’s work is any discussion of the temperature dependence of the diﬀusion coeﬃcient. Historically, the temperature dependence of reaction rates, diﬀusivities etc., now generally referred to as ‘Arrhenius law’, is named after the Swedish scientist Svante August Arrhenius (1859–1927). Arrhenius got a doctorship in chemistry in Uppsala, Sweden, in 1884 with a thesis about electrolytic dissociation. He was awarded a travel fellowship which enabled him to work with Ostwald in Riga, now Latvia, and with Kohlrausch in Würzburg, Germany. He also cooperated with Boltzmann in Graz, Austria, in 1887 and with Van’t Hoﬀ in Amsterdam, The Netherlands, in 1888. He was appointed for a chair in chemistry at the University of Stockholm in 1891. He abandoned this position in 1905 to become director of the Nobel Institute of Physical Chemistry. Arrhenius was awarded the 1903 Nobel prize in chemistry for his theory of electrolytic dissociation. It appears that the Arrhenius law for chemical reactions was proposed by the Dutch scientist Jacobus Hendrik van’t Hoﬀ (1852–1921), the ﬁrst Nobel laureate in chemistry (1901). The suggestion that the diﬀusivity in solids should obey that law was apparently made by Dushman and Langmuir in 1922 [9]. Von Hevesy – the ﬁrst measurements of self-diﬀusion: The idea of self-diﬀusion was already introduced by Maxwell, when treating the rate of diﬀusion of gases. The ﬁrst attempts to measure self-diﬀusion in condensed matter were those of Georg Karl von Hevesy (1885–1966), who studied selfdiﬀusion in liquid [10] and in solid lead [11] by using a natural radioactive isotope of lead. Von Hevesy had a fascinating scientiﬁc career. He was born in Budapest, Austria-Hungary, and studied at the Universities of Budapest, Berlin and Freiburg. He did research work in physical chemistry at the ETH in Zürich, with Fritz Haber in Karlsruhe, with Ernest Rutherford in Manchester, and with Fritz Paneth in Vienna. After World War I he teached for six months at the University of Budapest, and from 1920 to 1926 he worked with Niels Bohr at the University of Copenhagen. Together with the Dutch physicist Dirk Coster he discovered the new element ‘hafnium’ among the oreg of zirconium. He was professor at the University of Freiburg, Germany, from 1926 to 1934. During his eight years in Freiburg he initiated work with radiotracers in solids and in animal tissues. Fleeing from the Nazis in Germany, he moved to the Niels Bohr Institute in Copenhagen in 1934 and from there to Stockholm. In 1944 the Swedish Royal Academy of Sciences awarded him the Nobel prize in Chemistry of the year 1943 for ‘. . . his work on the use of isotopes as tracers in the study of chemical processes.’ He became 1.1 Pioneers and Landmarks of Diﬀusion 5 a Swedish citizen and was appointed professor of organic chemistry at the University of Stockholm in 1959. Von Hevesy, who married Pia Riis, daughter of a Danish ship owner, had four children, died in Freiburg, Germany. Von Hevesy is also the founder of radioistope applications in nuclear medicine. For example, the hospital of the author’s University has a station called ‘von Hevesy station’. Wolfgang Seith, who collaborated with von Hevesy in Freiburg, was appointed as the ﬁrst professor in physical chemistry at the author’s University in Münster, Germany. Brownian motion: The phenomenon of irregular motion of small particles suspended in a liquid had been known for a long time. It had been discovered by the Scottish scientist Robert Brown (1773–1858). Brown was the son of an episcopalian priest. He studied medicine at Edinburgh University, but did not obtain his degree. At the age of twenty-one he enlisted in a newly raised Scottish regiment. At that time he already knew that his true interests lay not in medicine but in botany, and he already had acquired some reputation as a botanist. On a visit to London in 1798 to recruit for his regiment, he met the botanist Sir Joseph Banks, president of the Royal Society, who recommended Brown to the Admiralty for the post of a naturalist aboard a ship. The ship was to embark on a surveying voyage at the coasts of Australia. Brown made extensive plant collections in Australia and it took him about 5 years to classify approximately 3900 species he had gathered, almost all of which were new to science. By that time, Robert Brown was already a renowned botanist. Much later Charles Darwin referred to him as ‘. . . princeps botanicorum’. In addition to collecting and classifying, Brown made several important discoveries. Perhaps the most celebrated one by biologists is his discovery that plant cells have a nucleus. Robert Brown is best known in science for his description of the random movement of small particles in liquid suspension, ﬁrst described in a pamphlet entitled ‘A brief account of microscopical observations in the months June, July and August 1827 on the particles contained in pollen . . . ’, which was originally intended for private circulation, but was reprinted in the archival literature shortly after its appearance [12]. Brown investigated the way in which pollen acted during impregnation. A plant he studied under the microscope was Clarkia pulchella, a wildﬂower found in the Paciﬁc Northwest of the United States. The pollen of this plant contains granules varying from about ﬁve to six micrometers in linear dimension. It is these granules, not the whole pollen grains, upon which Brown made his observation. He wrote ‘. . . While examining the form of these particles immersed in water, I observed many of them very evidently in motion . . . These motions were such as to satisfy me, after frequently repeated observation, that they arose neither from currents in the ﬂuid, nor from its gradual evaporation, but belonged to the particle itself ’. The inherent, incessant motion of small particles is nowadays called Brownian motion in honour of Robert Brown. 6 1 History and Bibliography of Diﬀusion Einstein’s and Smoluchowski’s theory of Brownian motion: In the period between 1829 and about 1900 not much progress was made in the understanding of Brownian motion, although developments in the theory of heat and kinetic theory stimulated new experiments and conjectures. It is striking that the founders and developers of kinetic theory, Maxwell, Boltzmann, and Clausius, never published anything on Brownian motion. The reason for the lack in progress was that the major studies of that period focused on the particle velocities. Measurements of the particle velocities gave puzzling results. The path of a small particle, on the length scales available from observations in a microscope, is an extremely erratic curve. In modern language we would say that it is a fractal. Such curves are diﬀerentiable almost nowhere. Consequently, the particles whose trajectories they represent have no velocity, as usually deﬁned. It was not until the work of Einstein and Smoluchowski that it was understood that the velocity is not a useful thing to measure in this context. Albert Einstein (1879–1955), born in Ulm, Germany, is certainly the best known physicist of the twentieth century, perhaps even of all time. In the year of 1905, he published four papers that at once raised him to the rank of a physicist of the highest caliber: the photon hypothesis to explain the photo eﬀect, for which he received the Nobel prize in physics in 1922 for the year 1921, his ﬁrst paper on Brownian motion, and his two ﬁrst papers on relativity theory. At that time Einstein was employed at the ‘The Eidgenössische Amt für Geistiges Eigentum’ in Bern, Switzerland. He did not receive the doctoral degree until the following year, 1906. Interestingly, his thesis was on none of the above problems, but rather concerned with the determination of the dimensions of molecules. His ﬁrst paper on Brownian motion was entitled ‘Die von der molekularkinetischen Theorie der Wärme geforderte Bewegung von in ruhenden Flüssigkeiten suspendierten Teilchen’ [13]. A second paper was entitled ‘Zur Theorie der Brownschen Bewegung’ [14]. Einstein published two additional short papers on this topic [15, 16], but these were of relatively minor interest. Einstein was the ﬁrst to understand, contrary to many scientists of his time, that the basic quantity is not the velocity but the mean-square displacement of particles. He related the mean-square displacement to the diﬀusion coeﬃcient. The Polish physicist and mountaineer Marian Smoluchowski (1872–1917) was born in Vienna, Austria. During his lifetime, Poland was not an independent country; it was partitioned between Russia, Prussia, and Austria. Marian Smoluchowski entered the University of Vienna and studied physics under Joseph Stephan and Franz Exner. He was impressed by the work of Ludwig Boltzmann. In his later life he was called ‘der geistige Nachfolger Boltzmanns’ (the intellectual successor of Boltzmann). He got his PhD and his ‘venia legendi’ from the University of Vienna and was appointed full professor at Lvov University (now Ukraine) in 1903. He accepted a chair in physics at the Jagellonian University at Cracow in 1913, when he was a wellknown physicist of 1.1 Pioneers and Landmarks of Diﬀusion 7 worldwide recognition. Smoluchowski also served as president of the Polish Tatra Society and received the ‘Silberne Edelweiss’ from the German and Austrian Alpine Society, an award given to distinguished alpinists. Smoluchowski’s interest for molecular statistics led him already around 1900 to consider Brownian motion. He did publish his results not before 1906 [17, 18], under the impetus of Einstein’s ﬁrst paper. Smoluchowski later studied Brownian motion for particles under the inﬂuence of an external force [19, 20]. Einstein’s and Smoluchowski’s scientiﬁc paths crossed again, when both considered the theory of the scattering of light near the critical state of a ﬂuid, the critical opalescence. Smoluchowski died as a result of a dysentery epidemic, aggravated by wartime conditions in 1917. Einstein wrote a sympathetic obituary for him with special reference to Smoluchowski’s interest in ﬂuctuations [21]. Atomic reality – Perrin’s experiments: The idea that matter was made up of atoms was already postulated by Demokrit of Abdeira, an ancient Greek philosopher, who lived about four hundred years before Christ. However, an experimental proof had to wait for more than two millennia. The concept of atoms and molecules took strong hold of the scientiﬁc community since the time of English scientist John Dalton (1766–1844). It was also shown that the ideas of the Italian scientist Amadeo Avogadro (1776–1856) could be used to construct a table of atomic weights, a central idea of chemistry and physics. Most scientists were willing to accept atoms as real, since the facts of chemistry and the kinetic theory of gases provided strong indirect evidence. Yet there were famous sceptics. Perhaps the most prominent ones were the German physical chemist and Nobel laureate Wilhelm Ostwald (1853–1932) and the Austrian physicist Ernst Mach (1938–1916). They agreed that atomic theory was a useful way of summarising experience. However, the lack of direct experimental veriﬁcation led them to maintain their scepticism against atomic theory with great vigour. The Einstein-Smoluchowski theory of Brownian motion provided ammunition for the atomists. This theory explains the incessant motion of small particles by ﬂuctuations, which seems to violate the second law of thermodynamics. The question remained, what ﬂuctuates? Clearly, ﬂuctuations can be explained on the basis of atoms and/or molecules that collide with a Brownian particle and push it around. The key question was then, what is the experimental evidence that the Einstein-Smoluchowski theory is quantitatively correct? The answer had to wait for experiments of the French scientist Jean Baptiste Perrin (1870–1942), a convinced atomist. The experiments were difﬁcult. In order to study the dependence of the mean-square displacement on the particle radius, it was necessary to prepare monodisperse suspensions. The experiments of Perrin were successful and showed agreement with the Einstein-Smoluchowski theory [22, 23]. He and his students continued reﬁning the work and in 1909 Perrin published a long paper on his own and his students’ research [24]. He became an energetic advocate for the reality of 8 1 History and Bibliography of Diﬀusion atoms and received the 1926 Nobel prize in physics ‘. . . for his work on the discontinuous structure of matter . . . ’. Crystalline solids and atomic defects: Solid-state physics was born when Max von Laue (1879–1960) detected diﬀraction of X-rays on crystals. His experiments demonstrated that solid matter usually occurs in three-dimensional periodic arrangements of atoms. His discovery, published in 1912 together with Friedrich and Knipping, was awarded with the 1914 Nobel prize in physics. However, the ideal crystal of Max von Laue is a ‘dead’ crystal. Solid-state diﬀusion and many other properties require deviations from ideality. The Russian physicist Jakov Il’ich Frenkel (1894–1952) was the ﬁrst to introduce the concept of disorder in the ﬁeld of solid-state physics. He suggested that thermal agitation causes transitions of atoms from their regular lattice sites into interstitial positions leaving behind lattice vacancies [25]. This kind of disorder is now called Frenkel disorder and consists of pairs of vacant lattice sites (vacancies) and lattice atoms on interstitial sites of the host crystal (self-interstitials). Only a few years later, Wagner and Schottky [26] generalised the concept of disorder and treated disorder in binary compounds considering the occurrence of vacancies, self-interstititals and antisite defects on both sublattices. Nowadays, it is common wisdom that atomic defects are necessary to mediate diﬀusion in crystals. The German physicist Walter Schottky (1886–1976) taught at the universities of Rostock and Würzburg, Germany, and worked in the research laboratories of Siemens. He had a strong inﬂuence on the development of telecommunication. Among Schottky’s many achievements a major one was the development of a theory for the rectifying behaviour of metal-semiconductor contact, which revolutionised semiconductor technology. Since 1973 the German Physical Society decorates outstanding achievements of young German scientists in solid-state physics with the ‘Walter-Schottky award’. Kirkendall eﬀect: A further cornerstone of solid-state diﬀusion comes from the work of Ernest Kirkendall (1914–2005). In the 1940s, it was still a widespread belief that atomic diﬀusion in metals takes place via direct exchange or ring mechanisms. This would suggest that in binary alloys the two components should have the same coeﬃcient of self-diﬀusion. Kirkendall and coworkers observed the inequality of copper and zinc diﬀusion during interdiﬀusion between brass and copper, since the interface between the two diﬀerent phases moves [27–29]. The direction of the mass ﬂow was such as might be expected if zinc diﬀuses out of the brass more rapidly than copper diﬀuses in. Such phenomena have been observed in the meantime in many other binary alloys. The movement of inert markers placed at the initial interface of a diﬀusion couple is now called the Kirkendall eﬀect. Kirkendall’s discovery, which took the scientiﬁc world about ten years to be appreciated, is nowadays taken as evidence for a vacancy mechanism of diﬀusion in metals 1.1 Pioneers and Landmarks of Diﬀusion 9 and alloys. Kirkendall left research in 1947 and served as secretary of the American Institute of Mining, Metallurgical and Petroleum Engineers. He then became a manager at the United Engineering Trustees and concluded his career as a vice president of the American Iron and Steel Institute. Thermodynamics of irreversible processes: The Norwegian Nobel laureate in chemistry of 1968 Lars Onsager (1903–1976) had widespread interests, which include colloids, dielectrics, order-disorder transitions, hydrodynamics, thermodynamics, and statistical mechanics. His work had a great impact on the ‘Thermodynamics of Irreversible Processes’. He received the Nobel prize for the reciprocity theorem, which is named after him. This theorem states that the matrix of phenomenological coeﬃcients, which relate ﬂuxes and generalised forces of transport theory, is symmetric. The nondiagonal terms of the Onsager matrix also include cross-phenomena, such as the inﬂuence of a gradient in concentration of one species upon the ﬂow of another one or the eﬀect of a temperature gradient upon the ﬂow of various atomic species, both of which can be signiﬁcant for diﬀusion processes. Solid-state diﬀusion after World War II: The ﬁrst period of solid-state diﬀusion under the guidance of Roberts-Austen, von Hevesy, Frenkel, and Schottky was followed by a period which started in the mid 1930s, when ‘artiﬁcial’ radioactive isotopes, produced in accelerators, became available. Soon after World War II nuclear reactors became additional sources of radioisotopes. This period saw ﬁrst measurements of self-diﬀusion on elements other than lead. Examples are self-diﬀusion of gold [30, 31], copper [32], silver [33], zinc [34], and α-iron [35]. In all these experiments the temperature dependence of diﬀusion was adequately described by the Arrhenius law, which by about 1950 had become an accepted ‘law of nature’. It is hardly possible to review the following decades, since the ﬁeld has grown explosively. This period is characterised by the extensive use of radioactive isotopes produced in nuclear reactors and accelerators, the study of the dependence of diﬀusion on the tracer mass (isotope eﬀect), and of diﬀusion under hydrostatic pressure. Great improvements in the precision of diﬀusion measurements and in the accessible temperature ranges were achieved by using reﬁned proﬁling techniques such as electron microprobe analysis, sputter sectioning, secondary ion mass spectroscopy, Rutherford back-scattering, and nuclear reaction analysis. Methods not directly based on Fick’s law to study atomic motion such as the anelastic or magnetic after-eﬀect, internal friction, and impedance spectroscopy for ion-conducting materials were developed and widely applied. Completely new approaches making use of nuclear methods such as nuclear magnetic relaxation (NMR) [36], Mössbauer spectroscopy (MBS), and quasielastic neutron scattering (QENS) have been successfully applied to diﬀusion problems. Whereas diﬀusion on solid surfaces nowadays can be recorded by means of scanning tunnelling microscopy, the motion of atoms inside a solid is still 10 1 History and Bibliography of Diﬀusion diﬃcult to observe in a direct manner. Nevertheless, diﬀusion occurs and it is the consequence of a large number of atomic or molecular jumps. The mathematics of the random-walk problem allows one to go back and forth between the diﬀusion coeﬃcient and the jump distances and jump rates of the diﬀusing atoms. Once the diﬀusion coeﬃcient was interpreted in this way, it was only a question of time before attempts were made to understand the measured values in terms of atomistic diﬀusion mechanisms. The past decades have seen a tremendous increase in the application of computer modeling and simulation methods to diﬀusion processes in materials. Along with continuum modeling aimed at describing complex diﬀusion problems by diﬀerential equations, atomic-level modeling such as ab-initio calculations, molecular dynamics studies, and Monte Carlo simulations, play an increasingly important rôle as means of gaining fundamental insights into diﬀusion processes. Grain-boundary diﬀusion: By 1950, the fact that grain-boundary diﬀusion exists had been well documented by autoradiographic images [37], from which the ratio of grain-boundary to lattice-diﬀusion coeﬃcients in metals was estimated to be a few orders of magnitude [38]. Fisher published his now classical paper presenting the ﬁrst theoretical model of grain-boundary diﬀusion in 1951 [39]. That pioneering paper, together with concurrent experimental work by Hoﬀman and Turnbull (1915–2007) [40], initiated the whole area of quantitative studies of grain-boundary diﬀusion in solids. Nowadays, grain-boundary diﬀusion is well recognised to be a transport phenomenon of great fundamental interest and of technical importance in normal polycrystals and in particular in nanomaterials. Distinguished scientists of solid-state diﬀusion: In what follows some people are mentioned, who have made or still make signiﬁcant contributions to the ﬁeld of solid-state diﬀusion. The author is well aware that such an attempt is necessarily incomplete and perhaps biased by personal ﬂavour. Wilhelm Jost (1903–1988) was a professor of physical chemistry at the University of Göttingen, Germany. He had a very profound knowledge of diﬀusion not only for solids but also for liquids and gases. His textbook ‘Diffusion in Solids, Liquids and Gases’, which appeared for the ﬁrst time in 1952 [41], is still today a useful source of information. Although the author of the present book never had the chance to meet Wilhelm Jost, it is obvious that Jost was one of the few people who overlooked the whole ﬁeld of diﬀusion, irrespective whether diﬀusion in condensed matter or in gases is concerned. John Bardeen (1908–1991) and C. Herring, both from the Bell Telephone Laboratories, Murray Hill, New Jersey, USA, recognised in 1951 that diﬀusion of atoms in a crystal by a vacancy mechanism is correlated [42]. After this pioneering work it was soon appreciated that correlation eﬀects play an important rôle for any solid-state diﬀusion process, when point defects act as 1.1 Pioneers and Landmarks of Diﬀusion 11 diﬀusion vehicles. Nowadays, a number of methods are available for the calculation of correlation factors. Correlation factors of self-diﬀusion in elements with cubic lattices are usually numbers characteristic for a given diﬀusion mechanism. Correlation factors of foreign atom diﬀusion are temperature dependent and thus contribute to the activation enthalpy of foreign atom diﬀusion. It may be interesting to mention that John Bardeen is one of the very few scientists, who received the Nobel prize twice. Schockley, Bardeen, and Brattain were awarded for their studies of semiconducors and for the development of the transition in 1956. Bardeen, Cooper, and Schriefer received the 1972 Nobel price for the so-called BCS theory of superconductivity. Yakov E. Geguzin (1918–1987) was born in the town of Donetsk, now Ukraine. He graduated from Gor’kii State University at Kharkov, Ukraine. After years of industrial and scientiﬁc work in solid-state physics he became professor at the Kharkov University. He founded the Department of Crystal Physics, which he headed till his death. The main scientiﬁc areas of Geguzin were diﬀusion and mass transfer in crystals. He carried our pioneering studies of surface diﬀusion, diﬀusion and mass transfer in the bulk and on the surface of metals and ionic crystals, interdiﬀusion and accompanying eﬀects in binary metal and ionic systems. He was a bright person, a master not only to realise experiments but also to tell of them. His enthusiasm combined with his talent for physics attracted many students. His passion is reﬂected in numerous scientiﬁc and popular books, which include topics such as defects in metals, physics of sintering, diﬀusion processes on crystal surfaces, and an essay on diﬀusion in crystals [43]. Norman Peterson (1934–1985) was an experimentalist of the highest calibre and a very active and lively person. His radiotracer diﬀusion studies performed together with Steven Rothman, John Mundy, Himanshu Jain and other members of the materials science group of the Argonne National Laboratory, Illinois, USA, set new standards for high precision measurements of tracer diﬀusivities in solids. Gaussian penetration proﬁles of lattice diﬀusion over more than three orders of magnitude in tracer concentration were often reported. This high precision allowed the detection of small deviations from Arrhenius behaviour of self-diﬀusion, e.g., in fcc metals, which could be attributed to the simultaneous action of monovacancy and divacancy mechanisms. The high precision was also a prerequisite for successful isotope eﬀect experiments of tracer diﬀusion, which contributed a lot to the interpretation of diﬀusion mechanisms. Furthermore, the high precision permitted reliable studies of grain-boundary diﬀusion in poly- and bi-crystals with tracer techniques. The author of this book collaborated with Norman Peterson, when Peterson spent a sabbatical in Stuttgart, Germany, as a Humboldt fellow. The author and his groups either at the University of Stuttgart, Germany, until 1984 or from then at the University of Münster, Germany, struggled hard to fulﬁll ‘Peterson standards’ in own tracer diﬀusion experiments. 12 1 History and Bibliography of Diﬀusion John Manning (1933–2005) had strong interests in the ‘Diﬀusion Kinetics of Atoms in Crystals’, as evidenced by the title of his book [44]. He received his PhD from the University of Illinois, Urbana, USA. Then, he joined the metals physics group at the National Bureau of Standards (NBS/NIST) in Washington. Later, he was the chief of the group until his retirement. He also led the Diﬀusion in Metals Data Center together with Dan Butrymowics and Michael Read. The obituary published by NIST has the following very rightful statement: ‘His papers have explained the signiﬁcance of the correlation factor and brought about an appreciation of its importance in a variety of diﬀusion phenomena’. The author of this book met John Manning on several conferences, Manning was a great listener and a strong advocate, fair, honest, friendly, courteous, kind and above all a gentleman. Paul Shewmon is professor emeritus in the Department of Materials Science and Engineering at the Ohio State Univeristy, USA. He studied at the University of Illinois and at the Carnegie Mellon University, where he received his PhD. Prior to becoming a professor at the Ohio State University he served among other positions as director of the Materials Science Division of the Argonne National Laboratory, Illinois, and as director of the Division of Materials Research for the National Science Foundation of the United States. Shewmon is an outstanding materials scientists of the United States. He has also written a beautiful textbook on ‘Diﬀusion in Solids’, which is still today usefull to introduce students into the ﬁeld. It appeared ﬁrst in 1963 and in slightly revised form in 1989 [45]. The diﬀusion community owes many enlightening contributions to the British theoretician Alan B. Lidiard from AEA Technology Harwell and the Department of Theoretical Chemistry, University of Oxford, GB. He co-authored the textbook ‘Atomic Transport in Solids’ together with A.R. Allnatt from the Department of Chemistry, University of Western Ontario, Canada [46]. Their book provides the fundamental statistical theory of atomic transport in crystals, that is the means by which processes occurring at the atomic level are related to macroscopic transport coeﬃcients and other observable quantities. Alan Lidiard is also the father of the so-called ‘ﬁvefrequency model’ [47]. This model provides a theoretical framework for solute and solvent diﬀusion in dilute alloys and permits to calculate correlation factors for solute and solvent diﬀusion. It has been also successfully applied to foreign atom diﬀusion in ionic crystals. Jean Philibert, a retired professor of the University Paris-sud, France, is an active member and highly respected senior scientist of the international diﬀusion community. Graduate students in solid-state physics, physical metallurgy, physical and inorganic chemistry, and geophysical materials as well as physicists, metallurgists in science and industrial laboratories beneﬁt from his comprehensive textbook ‘Atom Movements – Diﬀusion and Mass Transport in Solids’, which was translated from the French-language book of 1985 by Steven J. Rothman, then senior scientist at the Argonne National Labora- 1.1 Pioneers and Landmarks of Diﬀusion 13 tory, Illinois, USA [48]. David Lazarus, then a professor at the University of Illinois, Urbana, USA, wrote in the preface to Philiberts book: ‘This is a work of love by a scientist who understands the ﬁeld thoroughly and deeply, from its fundamental atomistic aspects to the most practical of its ‘real-world’ applications.’ The author of the present book often consulted Philibert’s book and enjoyed Jean Philibert’s well-rounded contributions to scientiﬁc discussions during conferences. Graeme Murch, head of the theoretical diﬀusion group at the University of Newcastle, Australia, serves the international diﬀusion community in many respects. He is an expert in computer modeling of diﬀusion processes and has a deep knowledge of irreversible thermodynamics and diﬀusion. He authored and co-authored chapters in several specialised books on diﬀusion, standalone chapters on diﬀusion in solids, and a chapter about interdiﬀusion in a data collection [69]. He also edited books on certain aspects of diﬀusion. Graeme Murch is since many years the editor-in-chief of the international journal ‘Defect and Diﬀusion Forum’. This journal is an important platform of the solid-state diﬀusion community. The proceedings of many international diﬀusion conferences have been published in this journal. Other people, who serve or served the diﬀusion community with great success, can be mentioned only shortly. Many of them were also involved in the laborious and time-consuming organisation of international conferences in the ﬁeld of diﬀusion: The Russian scientists Semjon Klotsman, the retired chief of the diﬀusion group in Jekaterinburg, Russia, and Boris Bokstein, head of the thermodynamics and physical chemistry group at the Moscow Institute of Steels and Alloys, Moscow, Russia, organised stimulating international conferences on special topics of solid-state diﬀusion. Deszö Beke, head of the solid-state physics department at the University of Debrecen, Hungary, and his group contribute signiﬁcantly to the ﬁeld and organised several conferences. The author of this book has a very good remembrance to DIMETA-82 [49], which took place at lake Balaton, Hungary, in 1982. This conference was one of the very ﬁrst occasions where diﬀusion experts from western and eastern countries could participate and exchange experience in a fruitful manner, although the ‘iron curtain’ still did exist. DIMETA-82 was the starting ignition for a series of international conferences on diﬀusion in materials. These were: DIMETA-88 once more organised by Beke and his group at lake Balaton, Hungary [50]; DIMAT-92 organised by Masahiro Koiwa and Hideo Nakajima in Kyoto, Japan [51]; DIMAT-96 organised by the author of this book and his group in Nordkirchen near Münster, Germany [52]; DIMAT-2000 organised by Yves Limoge and J.L. Bocquet in Paris, France [53]; DIMAT-2004 organised by Marek Danielewski and colleagues in Cracow, the old capital of Poland [54]. Devendra Gupta, retired senior scientist from the IBM research laboratories in Yorktown Heights, New York, USA, was one of the pioneers of 14 1 History and Bibliography of Diﬀusion grain-boundary and dislocation diﬀusion studies in thin ﬁlms. He organised symposia on ‘Diﬀusion in Ordered Alloys’ and on ‘Diﬀusion in Amorphous Materials’ and co-edited the proceedings [55, 56]. Gupta also edited a very useful book on ‘Diﬀusion Processes in Advanced Technological Materials’, which appeared in 2005 [57]. Yuri Mishin, professor at the Computational Materials Science group of Georg Mason University, Fairfax, Virginia, USA, is an expert in grainboundary diﬀusion and in computer modeling of diﬀusion processes. He coauthored a book on ‘Fundamentals of Grain and Interphase Boundary Diﬀusion’ [58] and organised various symposia, e.g., one on ‘Diﬀusion Mechanisms in Crystalline Materials’ [59]. Frans van Loo, retired professor of physical chemistry at the Technical University of Eindhoven, The Netherlands, is one of the few experts in multiphase diﬀusion and of diﬀusion in ternary systems. He is also a distinguished expert in Kirkendall eﬀect studies. Van Loo and his group have made significant contributions to the question of microstructural stability of the Kirkendall plane. It was demonstrated experimentally that binary systems with stable, unstable, and even with several Kirkendall planes exist. Mysore Dayananda is professor of the School of Engineering of Purdue University, West Lafayette, Indiana, USA. His research interests mainly concern interdiﬀusion, multiphase diﬀusion and diﬀusion in ternary alloys. Dayananda has also organised several specialised diﬀusion symposia and coedited the proceedings [60, 61]. The 150th anniversary of the laws of Fick and the 100th anniversary of Einstein’s theory of Brownian motion was celebrated on two conferences. One conference was organised by Jörg Kärger, University of Leipzig, Germany, and Paul Heitjans, University of Hannover, Germany, at Leipzig in 2005. It was was devoted to the ‘Fundamentals of Diﬀusion’ [62]. Heitjans and Kärger also edited a superb text on diﬀusion, in which experts cover various topics concerning methods, materials and models [63]. The anniversaries were also celebrated during a conference in Moscow, Russia, organised by Boris Bokstein and Boris Straumal with the topics ‘Diﬀusion in Solids – Past, Present and Future’ [64]. Andreas Öchsner, professor at the University of Aveiro, Portugal, organised a ﬁrst international conference on ‘Diﬀusion in Solids and Liquids (DSL2005)’ in 2005 [65]. The interesting idea of this conference was, to bring diﬀusion experts from solid-state and liquid-state diﬀusion together again. Obviously, this idea was successful since many participants also attended DSL2006 only one year later [66]. Diﬀusion research at the University of Münster, Germany: Finally, one might mention, that the ﬁeld of solid-state diﬀusion has a long tradition at the University of Münster, Germany – the author’s university. Wolfgang Seith (1900–1955), who had been a coworker of Georg von Hevesy at the University of Freiburg, Germany, was full professor of physical chemistry at the 1.1 Pioneers and Landmarks of Diﬀusion 15 University of Münster from 1937 until his early death in 1955. He established diﬀusion research in Münster under aggravated war-time and post-war conditions. He also authored an early textbook on ‘Diﬀusion in Metallen’, which appeared in 1939 [66]. A revised edition of this book was published in 1955 and co-authored by Seith’s associate Heumann [67]. Theodor Heumann (1914– 2002) was full professor and director of the ‘Institut für Metallforschung’ at the University of Münster from 1958 until his retirement in 1982. Among other topics, he continued research in diﬀusion, introduced radiotracer techniques and electron microprobe analysis together with his associate Christian Herzig. As professor emeritus Heumann wrote a new book on ‘Diﬀusion in Metallen’, which appeared in 1992 [68]. Its German edition was translated to Japanese language by S.-I. Fujikawa. The Japanese edition appeared in 2006. The author of the present book, Helmut Mehrer, was the head of a diﬀusion group at the University of Stuttgart, Germany, since 1974. He was then appointed full professor and successor on Heumann’s chair at the University of Münster in 1984 and retired in 2005. Diﬀusion was reinforced as one of the major research topics of the institute. In addition to metals, further classes of materials have been investigated and additional techniques applied. These topics have been pursued by the author and his colleagues Christian Herzig, Nicolaas Stolwijk, Hartmut Bracht, and Serguei Divinski. The name of the institute was changed into ‘Institut für Materialphysik’ in accordance with the wider spectrum of materials in focus. Metals, intermetallic compounds, metallic glasses, quasicrystals, elemental and compound semiconductors, and ion-conducting glasses and polymers have been investigated. Lattice diﬀusion has been mainly studied by tracer techniques using mechanical and/or sputter-sectioning techniques and in cooperation with other groups by SIMS proﬁling. Interdiﬀusion and multi-phase diﬀusion was studied by electron microprobe analysis. The pressure and mass dependence of diﬀusion has been investigated with radiotracer techniques on metals, metallic and oxide glasses. Grain-boundary diﬀusion and segregation into grain boundaries has been picked up as a further topic. Ionic conduction studied by impedance spectroscopy combined with element-speciﬁc tracer measurements, provided additional insight into mass and charge transport in ion-conducting oxide glasses and polymer electrolytes. Numerical modeling of diﬀusion processes has been applied to obtain a better understanding of experimental data. A data collection on diﬀusion in metals and alloys was edited in 1990 [69], DIMAT-96 was organised in 1996 and the conference proceedings were edited [52]. Further reading on history of diﬀusion: An essay on the early history of solid-state diﬀusion has been given by L. W. Barr in a paper on ‘The origin of quantitative diﬀusion measurements in solids. A centenary view’ [71]. Jean Philibert has written a paper on ‘One and a Half Century of Diﬀusion: Fick, Einstein, before and beyond’ [72]. Remarks about the more recent history can be found in an article of Steven Rothman [70], Masahiro Koiwa [73], and 16 1 History and Bibliography of Diﬀusion Alfred Seeger [74]. Readers interested in the history of diﬀusion mechanisms of solid-state diﬀusion may beneﬁt from C. Tuijn’s article on ‘History of models for solid-state diﬀusion’ [75]. Steven Rothman ends his personal view of diﬀusion research with the conclusion that ‘. . . Diﬀusion is alive and well’. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. T. Graham, Quaterly Journal of Science, Literature and Art 27, 74 (1829) T. Graham, Philos. Mag. 2, 175, 222, 351 (1833) T. Graham, Philos. Trans. of the Roy. Soc. of London 140, 1 (1950) A.E. Fick, Annalen der Physik und Chemie 94, 59 (1855) A.E. Fick, Philos. Mag. 10, 30 (1855) A.E. Fick, Gesammelte Abhandlungen, Würzburg (1903) J. Stephan, Sitzungsberichte d. Kaiserl. Akad. d. Wissenschaften II 79, 161 (1879) W.C. Roberts-Austen, Phil. Trans. Roy. Soc. A 187 , 383 (1896) S. Dushman and I. Langmuir, Phys. Rev. 20, 113 (1922) J. Groh, G. von Hevesy, Ann. Physik 63, 85 (1920) J. Groh, G. von Hevesy, Ann. Physik 65, 216 (1921) R. Brown, Edin. New. Phil. J 5, 358–371 (1828); Edin. J. Sci. 1, 314 (1829) A. Einstein, Annalen der Physik 17, 549 (1905) A. Einstein, Annalen der Physik 19, 371 (1906) A. Einstein, Z. für Elektrochemie 13, 98 (1907) A. Einstein, Z. für Elektrochemie 14, 235 (1908) M. van Smoluchowski, Annalen der Physik 21, 756 (1906) M. van Smoluchowski, Physikalische Zeitschrift 17, 557 (1916) M. van Smoluchowski, Bull. Int. de l’Acad. de Cracovie, Classe de Sci. math.nat. A, 418 (1913) M. van Smoluchowski, Annalen der Physik 48, 1103 (1915) A. Einstein, Naturwissenschaften 50, 107 (1917) J. Perrin, C.R. Acad. Sci. Paris 147, 475 (1908) J. Perrin, C.R. Acad. Sci. Paris 147, 530 (1908) J. Perrin, Ann. de Chim. et de Phys. 18, 1 (1909) J.I. Frenkel, Z. Physik 35, 652 (1926) C. Wagner, W. Schottky, Z. Phys. Chem. B 11, 163 (1930) E.O. Kirkendall, L. Thomassen, C. Upthegrove, Trans. AIME 133, 186 (1939) E.O. Kirkendall, Trans. AIME 147, 104 (1942) A.D. Smigelskas, E.O. Kirkendall, Trans. AIME 171, 130 (1947) A.M. Sagrubskij, Phys. Z. Sowjetunion 12, 118 (1937) H.A.C. McKay, Trans. Faraday Soc. 34, 845 (1938) B.V. Rollin, Phys. Rev. 55, 231 (1939) W.A. Johnson, Trans. Americ. Inst. Min. Met. Engrs. 143, 107 (1941) P.H. Miller, R.R. Banks, Phys. Rev. 61, 648 (1942) C.E. Birchenall, R.F. Mehl, J. Appl. Phys. 19, 217 (1948) N. Bloembergen, E.H. Purcell, and R.V. Pound, Phys. Rev. 73, 674 (1948) R.S. Barnes, Nature 166 , 1032 (1950) A.D. Le Claire, Philos. Mag. 42, 468 (1951) References 17 39. J.C. Fisher, J. Appl. Phys. 22, 74 (1951) 40. R.E. Hoﬀman, D. Turnbull, J. Appl. Phys. 22, 634 (1951) 41. W. Jost, Diﬀusion in Solids, Liquids, and Gases, Academic Press, New York, 1952 42. J. Bardeen, C. Herring, in: Atom Movements, ASM Cleveland, p. 87, 1951 43. Y.E. Geguzin, German edition: Grundzüge der Diﬀusion in Kristallen, VEB Verlag für Grundstoﬃndustrie, Leipzig, 1977 44. J.R. Manning, Diﬀusion Kinetics of Atoms in Crystals, van Norstrand Comp., 1968 45. P.G. Shewmon, Diﬀusion in Solids, 1st edition, MacGraw Hill Book Company, 1963; 2nd edition, The Minerals, Metals & Materials Society, Warrendale, USA, 1989 46. A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1991 47. A.B. Lidiard, Philos. Mag. 40, 1218 (1955) 48. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, Cedex A, France, 1991 49. DIMETA-82, Diﬀusion in Metals and Alloys, F.J. Kedves, D.L. Beke (Eds.), Defect and Diﬀusion Monograph Series No. 7, Trans Tech Publications, Switzerland, 1983 50. DIMETA-88, Diﬀusion in Metals and Alloys, F.J. Kedves, D.L. Beke (Eds.), Defect and Diﬀusion Forum 66–69, 1989 51. DIMAT-92, Diﬀusion in Materials, M. Koiwa, K. Hirano, H. Nakajima, T. Okada (Eds.), Trans Tech Publications, Zürich, Switzerland, 1993; also Defect and Diﬀusion Forum 95–98, 1993 52. DIMAT-96, Diﬀusion in Materials, H. Mehrer, Chr. Herzig, N.A. Stolwijk, H. Bracht (Eds.), Scitec Publications, Zürich-Uetikon, Switzerland, 1997; also Defect and Diﬀusion Forum 143–147, 1997 53. DIMAT-2000, Diﬀusion in Materials, Y. Limoge, J.L.Bocquet (Eds.), Scitec Publications, Zürich-Uetikon, Switzerland, 2001; also Defect and Diﬀusion Forum 194–199, 2001 54. DIMAT-2004, Diﬀusion in Materials, M. Danielewski, R. Filipek, R. Kozubski, W. Kucza, P. Zieba (Eds.), Trans Tech Publications, Zürich-Uetikon, Switzerland, 2005; also Defect and Diﬀusion Forum 237–240, 2005 55. B. Fultz, R.W. Cahn, D. Gupta (Eds.), Diﬀusion in Ordered Alloys, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, USA, 1993 56. H. Jain, D. Gupta (Eds.), Diﬀusion in Amorphous Materials, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, 1993 57. D. Gupta (Ed.), Diﬀusion Processes in Advanced Technological Materials, William Andrew, Inc., 2005 58. I. Kaur, Y. Mishin, W. Gust, Fundamentals of Grain and Interphase Boundary Diﬀusion, John Wiley & Sons, Ltd., 1995 59. Y. Mishin, G. Vogl, N. Cowern, R. Catlow, R. Farkas (Eds.), Diﬀusion Mechanism in Crystalline Materials, Mat. Res. Soc. Symp. Proc. Vol. 527, Materials Research Society, Warrendale, Pennsylvania, USA, 1997 60. D. Gupta, A.D. Romig, M.A. Dayananda (Eds.), Diﬀusion in High Technological Materials, Trans Tech Publications, Aedermannsdorf, Switzerland, 1988 61. A.D. Romig, M.A. Dayanada (Eds.), Diﬀusion Analysis and Applications, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, 1989 18 1 History and Bibliography of Diﬀusion 62. J. Kärger, F. Grindberg, P. Heitjans (Eds.), Diﬀusion Fundamentals – Leipzig 2005, Leipziger Universitätsverlag GmbH, 2005 63. P. Heitjans, J. Kärger (Eds.), Diﬀusion in Condensed Matter – Methods, Materials, Models, Springer-Verlag, 2005 64. B.S. Bokstein, B.B. Straumal (Eds.), Diﬀusion in Solids – Past, Present, and Future, Trans Tech Publications, Ltd., Switzerland, 2006; also Defect and Diffusion Forum 249, 2006 65. A. Öchsner, J. Gracio, F. Barlat (Eds.), First International Conference on Diffusion in Solids and Liquids – DSL 2005, Centre for Mechanical Technology and Automation and Department of Mechanical Engineering, University of Aveiro, Portugal, Editura MEDIAMIRA, Cluj-Napoca, 2006 66. W. Seith, Diﬀusion in Metallen, Verlag Julius Spriger, 1939 67. W. Seith, Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, 1955 68. Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, 1992; Japanese language edition 2006 translated by S.-I. Fujikawa 69. H. Mehrer (Vol. Ed.), Diﬀusion in Solid Metals and Alloys, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 70. S.J. Rothman, Defect and Diﬀusion Forum 99–100, 1 (1993) 71. L.W. Barr, Defect and Diﬀusion Forum 143–147, 3 (1997); see also [52] 72. J. Philibert, in: Diﬀusion Fundamentals – Leipzig 2005, Universitätsverlag Leipzig 2005, p.8; see also [62] 73. M. Koiwa, in: Proc. of PRIMCN -3, Honolulu, Hawai, July 1998 74. A. Seeger, Defect and Diﬀusion Forum 143–147, 21 (1997); see also [52] 75. C. Tuijn, Defect and Diﬀusion Forum 143–147, 11 (1997); see also [52] 1.2 Bibliography of Solid-State Diﬀusion In this section, we list diﬀusion-related bibliography from the past four or ﬁve decades. Textbooks on diﬀusion in solids and some books that are devoted to the mathematics of diﬀusion are supplemented by monographs and/or books on speciﬁc topics or materials, and by stand-alone chapters on diﬀusion. Conference proceedings of international conferences on diﬀusion in solids and comprehensive collections of diﬀusion data complete the bibliography. The literature is ordered in each section according to the year of publication. General Textbooks R.M. Barrer, Diﬀusion in and through Solids, Cambridge, The Syndics of the Cambridge University Press, ﬁrst printed 1941, reprinted with corrections 1951 L.A. Girifalco, Atomic Migration in Crystals, Blaisdell Publ. Comp., New York, 1964 W. Jost, Diﬀusion in Solids, Liquids, Gases, Academic Press, Inc., New York, 1952, 4th printing with addendum, 1965 Y. Adda and J. Philibert La Diﬀusion dans les Solides, 2 volumes, Presses Universitaires de France, 1966 1.2 Bibliography of Solid-State Diﬀusion 19 J.R. Manning, Diﬀusion Kinetics of Atoms in Crystals, D. van Norstrand Company, Inc., Princeton, 1968 C.P. Flynn, Point Defects and Diﬀusion, Clarendon Press, Oxford, 1972 J.P. Stark, Solid-State Diﬀusion, John Wiley & Sons, New York, 1976 S. Mrowec, Defects and Diﬀusion – an Introduction, Materials Science Monographs, Vol. 5, Elsevier, Amsterdam, 1980 R.J. Borg and G.J. Dienes, An Introduction to Solid-State Diﬀusion, Academic Press, Inc., 1988 P.G. Shewmon, Diﬀusion in Solids, 1st edition, MacGraw-Hill Book Company, Inc., 1963; 2nd edition, The Minerals, Metals & Materials Society, Warrendale, USA, 1989 J.S. Kirkaldy and D.J. Young, Diﬀusion in the Condensed State, The Institute of Metals, London, 1987 J. Philibert, Atom Movement – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, Cedex A, France, 1991 A.R. Allnatt and A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 D.S. Wilkinson, Mass Transport in Solids and Liquids, Cambridge University Press, 2000 M.E. Glicksman, Diﬀusion in Solids – Field Theory, Solid-State Principles and Applications, John Wiley & Sons, Inc., 2000 Mathematics of Diﬀusion H.S. Carslaw and J.C. Jaeger, Conduction of Heat in Solids, Clarendon Press, Oxford, 1959 J. Crank, The Mathematics of Diﬀusion, 2nd edition, Oxford University Press, 1975 R. Ghez, A Primer of Diﬀusion Problems, John Wiley & Sons, Inc., 1988 J. Crank, Free and Moving Boundary Problems, Oxford University Press, Oxford, 1984; reprinted in 1988, 1996 R.M. Mazo, Brownian Motion – Fluctuations, Dynamics, and Applications, Clarendon Press, Oxford, 2002 Specialised Books and Monographs on Solid-State Diﬀusion W. Seith and Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, Berlin, 1955 B.I. Boltaks, Diﬀusion in Semiconductors, translated from Russian by J.I. Carasso, Infosearch Ltd., London, 1963 G.R. Schulze, Diﬀusion in metallsichen Werkstoﬀfen, VEB Verlag für Grundstoﬃndustrie, Leipzig, 1970 G. Neumann and G.M. Neumann, Surface Self-diﬀusion of Metals, Diﬀusion and Defect Monograph Series No. 1, edited by Y. Adda, A.D. Le Claire, L.M. Slifkin, F.H. Wöhlbier, Trans Tech SA, Switzerland, 1972 D. Shaw (Ed.), Atomic Diﬀusion in Semiconductors, Plenum Press, New York, 1973 J.N. Pratt and P.G.R. Sellors, Electrotransport in Metals and Alloys, Trans Tech Publications, Zürich, 1973 20 1 History and Bibliography of Diﬀusion G. Frischat, Ionic Diﬀusion in Oxide Glasses, Diﬀusion and Defect Monograph Series No. 3/4, edited by Y. Adda, A.D. Le Claire, L.M. Slifkin, F.H. Wöhlbier, Trans Tech SA, Switzerland, 1973 B. Tuck, Introduction to Diﬀusion in Semiconductors, IEE Monograph Series 16, Inst. Electr. Eng., 1974 A.S. Nowick, J.J. Burton (Eds.), Diﬀusion in Solids – Recent Developments, Academic Press, Inc. 1975 H. Wever, Elektro- und Thermotransport in Metallen, Johann Ambrosius Barth, Leipzig, 1975 G.E. Murch, Atomic Diﬀusion Theory in Highly Defective Solids, Diﬀusion and Defect Monograph Series No. 6, edited by Y. Adda, A.D. Le Claire, L.M. Slifkin, F.H. Wöhlbier, Trans Tech SA, Switzerland, 1980 L.N. Larikov, V.V. Geichenko, and V.M. Fal’chenko, Diﬀusion Processes in Ordered Alloys, Kiev 1975, English translation published by Oxonian Press, New Dehli, 1981 G.E. Murch and A.S. Nowick (Eds.), Diﬀusion in Crystalline Solids, Academic Press, Inc., 1984 G.B. Fedorov and E.A. Smirnov, Diﬀusion in Reactor Materials, Trans Tech Publications, Zürich, Switzerland, 1984 B. Tuck, Diﬀusion in III-V Semiconductors, A. Hilger, London, 1988 W.R. Vieth, Diﬀusion in and through Polymers – Principles and Application, Carl Hanser Verlag, Munich, 1991 G.E. Murch (Ed.), Diﬀusion in Solids – Unsolved Problems, Trans Tech Publications, Ltd., Zürich, Switzerland, 1992 Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, 1992 I. Kaur, Y. Mishin, and W. Gust, Fundamentals of Grain and Interphase Boundary Diﬀusion, John Wiley & Sons, Ltd., 1995 H. Schmalzried, Chemical Kinetics of Solids, VCH Verlagsgesellschaft mbH, Weinheim, Germany, 1995 E.L. Cussler, Diﬀusion – Mass Transfer in Fluid Systems, Cambridge University Press, 1997 J. Kärger, P. Heitjans, and R. Haberlandt (Eds.), Diﬀusion in Condensed Matter, Friedr. Vieweg & Sohn Verlagsgesellschaft mbH, Braunschweig/Wiesbaden, Germany, 1998 D.S. Wilkinson, Mass Transport in Solids and Liquids, Cambridge University Press, 2000 V.I. Dybkov, Reaction Diﬀusion and Solid State Chemical Kinetics, The IPMS Publications, Kyiv, Ukraine, 2002 G. Neumann and C. Tuijn, Impurity Diﬀusion in Metals, Scitec Publications Ltd, Zürich-Uetikon, Switzerland, 2002 R.H. Doremus, Diﬀusion of Reactive Molecules in Solids and Melts, John Wiley and Sons, Inc., 2002 D.L. Beke (Ed.) Nanodiﬀusion, Special Issue of J. of Metastable and Nanocrystalline Materials 19, 2004 A. Gusak, Diﬀusion, Reactions, Coarsening – Some New Ideas, Cherkassy National University, 2004 J. Maier, Physical Chemistry of Ionic Materials – Ions and Electrons, J. Wiley & Sons, Ltd., 2004 D. Gupta (Ed.), Diﬀusion Processes in Advanced Technological Materials, William Andrew, Inc., 2005 1.2 Bibliography of Solid-State Diﬀusion 21 P. Heitjans, J. Kärger (Eds.), Diﬀusion in Condensed Matter – Methods, Materials, Models, Springer-Verlag, 2005 Y. Iijima (Ed.), Diﬀusion Study in Japan 2006, Research Signpost, Kerala, India, 2006 Stand-alone Chapters on Diﬀusion in Solids R.E. Howard and A.B. Lidiard, Matter Transport in Solids, Reports on Progress in Physics 27, 161 (1964) A.D. Le Claire, Diﬀusion, in: Treatise in Solid State Chemistry, Vol. 4, Reactivity of Solids, edited by N.B. Hannay, Plenum Press, 1975 S.J. Rothman, The Measurement of Tracer Diﬀusion Coeﬃcients in Solids, in: Diffusion in Crystalline Solids, edited by G.E. Murch and A.S. Nowick, Academic Press, Orlando, Fl, 1984 G.E. Murch, Diﬀusion Kinetics in Solids, Ch. 3 in Phase Transformations in Materials, G. Kostorz (Ed.), Wiley-VCh Verlag GmbH, Weinheim, Germany, 2001 J. L Bocquet, G. Brebec, and Y. Limoge, Diﬀusion in Metals and Alloys, Ch. 7 in Physical Metallurgy, 4th edition, R.W. Cahn and P. Haasen (Eds.), Elsevier Science BV, 1996 H. Mehrer, Diﬀusion in Metals, in: Diﬀusion in Condensed Matter, edited by J. Kärger, P. Heitjans, and R. Haberlandt, Friedr. Vieweg & Sohn Verlagsgesellschaft mbH, Braunschweig/Wiesbaden, Germany, 1998 H. Mehrer, Diﬀusion: Introduction and Case Studies in Metals and Binary Alloys, Ch. 1 in: Diﬀusion in Condensed Matter – Methods, Materials, Models, Springer-Verlag, 2005. Braunschweig/Wiesbaden, Germany, 1998 Conference Proceedings J.A. Wheeler, Jr. and F.R. Winslow (Eds.), Diﬀusion in Body-Centered Cubic Metals, American Society for Metals, Metals Park, Ohio, 1965 J.N. Sherwood, A.V. Chadwick, W.M. Muir, and F.L. Swinton (Eds.), Diﬀusion Processes, 2 volumes, Gordon and Breach Science Publishers, London, 1971 H.I. Aaronson (seminar coordinator), Diﬀusion, American Society for Metals, Metals Park, Ohio, 1973 P. Vashista, J.N. Mundy, and G.K. Shenoy (Eds.), Fast Ion Transport in Solids – Electrodes and Electrolytes, Elsevier North-Holland, Inc., 1979 F.J. Kedves and D.L. Beke (Eds.), DIMETA-82 – Diﬀusion in Metals and Alloys, Defect and Diﬀusion Monograph Series No. 7, Trans Tech Publications, Switzerland, 1983 G.E. Murch, H.K. Birnbaum, and J.R. Cost (Eds.), Nontraditional Methods in Diffusion, The Metallurgical Society of AIME, Warrendale, Pennsylvania, USA, 1984 D. Gupta, A.D. Romig, and M.A. Dayananda (Eds.), Diﬀusion in High Technology Materials, Trans Tech Publications, Aedermannsdorf, Switzerland, 1988 F.J. Kedves and D.L. Beke (Eds.), DIMETA-88 – Diﬀusion in Metals and Alloys, Defect and Diﬀusion Forum 66–69, 1989 A.L. Laskar, J.L. Bocquet, G. Brebec, and C. Monty (Eds.), Diﬀusion in Materials, NATO ASI Series, Kluwer Academic Publishers, The Netherlands, 1989 22 1 History and Bibliography of Diﬀusion A.D. Romig, Jr. and M.A. Dayananda (Eds.), Diﬀusion Analysis and Applications, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, 1989 J. Nowotny (Ed.), Diﬀusion in Solids and High Temperature Oxidation of Metals, Trans Tech Publications, 1992 B. Fultz, R.W. Cahn, and D. Gupta (Eds.), Diﬀusion in Ordered Alloys, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, USA, 1993 M. Koiwa, K. Hirano, H. Nakajima, and T. Okada (Eds.), Diﬀusion in Materials – DIMAT-92, 2 volumes, Trans Tech Publications, Zürich, Switzerland, 1993; and Defect and Diﬀusion Forum 95–98, 1993 H. Jain and D. Gupta (Eds.), Diﬀusion in Amorphous Materials, The Minerals, Metals & Materials Society, Warrendale, Pennsylvania, USA, 1993 J. Jedlinki (Ed.), Diﬀusion and Reactions – from Basics to Applications, Scitec Publications, Ltd., Switzerland, 1995; also Solid State Phenomena 41, 1995 D.L. Beke, I.A. Szab (Eds.), Diﬀusion and Stresses, Scitec Publications Ltd., Zürich-Uetikon, Switzerland; also: Defect and Diﬀusion Forum 129–130, 1996 H. Mehrer, Chr. Herzig, N.A. Stolwijk, and H. Bracht (Eds.), Diﬀusion in Materials – DIMAT-96, 2 volumes, Scitec Publications, Ltd., Zürich-Uetikon, Switzerland, 1997; also Defect and Diﬀusion Forum 143–147, 1997 Y. Mishin, G. Vogl, N. Cowern, R. Catlow, and D. Farkas (Eds.), Diﬀusion Mechanisms in Crystalline Materials, Mat. Res. Soc. Symp. Proc. Vol. 527, Materials Research Society, Warrendale, Pennsylvania, USA, 1997 M. Danielewski (Ed.), Diﬀusion and Reactions, Scitec Publications, Ltd., ZürichUetikon, Switzerland, 2000 Y. Limoge and J.L. Bocquet (Eds.), Diﬀusion in Materials – DIMAT-2000, 2 volumes, Scitec Publications, Ltd., Zürich-Uetikon, Switzerland, 2001; also: Defect and Diﬀusion Forum 194–199, 2001 B.S. Bokstein and B.B. Straumal (Eds.), Diﬀusion, Segregation and Stresses in Materials, Scitec Publications, Ltd., Zürich-Uetikon, Switzerland, 2003; also: Defect and Diﬀusion Forum 216–217, 2003 M. Danielewski, R. Filipek, R. Kozubski, W. Kucza, P. Zieba, Z. Zurec (Eds.), Diﬀusion in Materials – DIMAT-2004, 2 volumes, Tans Tech Publications, Ltd., Zürich-Uetikon, Switzerland, 2005; also: Defect and Diﬀusion Forum 237– 240, 2005 A. Öchsner, J. Grácio, F. Barlat (Eds.), First International Conference on Diﬀusion in Solids and Liquids – DSL 2005, Centre for Mechanical Technology and Automation and Department of Mechanical Engineering, University of Aveiro, Editura MEDIAMIRA, Cluj-Napoca, 2005 J. Kärger, F. Grindberg, P. Heitjans (Eds.), Diﬀusion Fundamentals – Leipzig 2005, Leipziger Universitätsverlag GmbH 2005 B.S. Bokstein, B.B. Straumal (Eds.), Diﬀusion in Solids – Past, Present and Future, Trans Tech Publications, Ltd., Switzerland, 2006; also: Defect and Diﬀusion Forum 249, 2006 A. Öchsner, J. Grácio (Eds.), Diﬀusion in Solids and Liquids – DSL 2006, Proc. of 2nd Int. Conf. on Diﬀusion in Solids and Liquids, Mass Transfer-Heat TransferMicrostructure and Properties, Areiro, Portugal, 2006; also: Defect and Diﬀusion Forum 258–260, 2006 J. Čermak, I. Stloukal (Eds.), Diﬀusion and Thermodynamics of Materials – DT 2006, Proc. of 9th Seminar on Diﬀusion and Thermodynamics of Materials, Brno, Czech Republik, 2006; also: Defect and Diﬀusion Forum 263, 2007 1.2 Bibliography of Solid-State Diﬀusion 23 Compilations of Diﬀusion Data I. Kaur, W. Gust, L. Kozma, Handbook of Grain and Interphase Boundary Diﬀusion Data, 2 volumes, Ziegler Press, Stuttgart, 1989 H. Mehrer (Vol. Ed.), Diﬀusion in Solid Metals and Alloys, Landolt-Börnstein, New Series, Group III, Vol. 26, Springer-Verlag, 1990 D.L. Beke (Vol. Ed.), Diﬀusion in Semiconductors and Non-Metallic Solids, Subvolume A, Diﬀusion in Semiconductors, Landolt-Börnstein, New Series, Group III, Vol. 33, Springer-Verlag, 1998 D.L. Beke (Vol. Ed.), Diﬀusion in Semiconductors and Non-Metallic Solids, Subvolume B1, Diﬀusion in Non-Metallic Solids (Part 1), Landolt-Börnstein, New Series, Group III, Vol. 33, Springer-Verlag, 1999 Diﬀusion and Defect Data, Journal of Abstracts, published by Trans Tech Publications, Aedermannsdorf, Switzerland, 1974–2003 2 Continuum Theory of Diﬀusion The equations governing diﬀusion processes are Fick’s laws. These laws represent a continuum description and are purely phenomenological. The original work of Adolf Fick appeared in 1855 [1] and described a salt-water system undergoing diﬀusion. Fick introduced the concept of the diﬀusion coeﬃcient and suggested a linear response between the concentration gradient and the mixing of salt and water. Already in 1807 Josef Fourier had developed an analogous relation between the ﬂow of heat and the temperature gradient [2]. Fick’s laws describe the diﬀusive transport of matter as an empirical fact without claiming that it derives from basic concepts. It is, however, indicative of the power of Fick’s continuum description that all subsequent developments have in no way aﬀected the validity of his approach. A deeper physical understanding of diﬀusion in solids is based on random walk theory and on the atomic mechanisms of diﬀusion, which are treated later in this book. 2.1 Fick’s Laws in Isotropic Media In an isotropic medium, physical and chemical properties are independent of direction, whereas in anisotropic media properties depend on the direction considered. Diﬀusion is isotropic in gases, most liquids, in glassy solids, in polycrystalline materials without texture, in cubic crystals and in icosahedral quasicrystals. In isotropic materials the diﬀusivity (introduced below) is a scalar quantity. Numerous engineering materials have cubic structures. Examples are face-centered cubic metals (Cu, Ag, Au, Al, Pb, Ni, . . . ), bodycentered cubic metals (V, Nb, Ta, Cr, Mo, W, β-Ti, β-Zr, . . . ), α-Fe and ferritic steels, which are body-centered cubic, and austenitic steels which are face-centered cubic. All of these important materials, and vastly more of their alloys, share cubic symmetry and exhibit scalar diﬀusivities. The elemental semiconductors Si and Ge crystallise in the diamond structure which is cubic. Many compound semiconductors occur in the cubic zinc blende structure. Many ionic crystals such as alkali halides and many oxides are cubic or have cubic modiﬁcations. Diﬀusion is anisotropic in non-cubic crystals and in some quasicrystals. Anisotropic diﬀusion is discussed in Sect. 2.3. 28 2 Continuum Theory of Diﬀusion 2.1.1 Fick’s First Law Let us ﬁrst consider the ﬂux of diﬀusing particles in one dimension (xdirection) illustrated in Fig. 2.1. The particles can be atoms, molecules, or ions. Fick’s ﬁrst law for an isotropic medium can be written as Jx = −D ∂C . ∂x (2.1) Here Jx is the ﬂux of particles (diﬀusion ﬂux) and C their number density (concentration). The negative sign in Eq. (2.1) indicates opposite directions of diﬀusion ﬂux and concentration gradient. Diﬀusion is a process which leads to an equalisation of concentration. The factor of proportionality, D, is denoted as the diﬀusion coeﬃcient or as the diﬀusivity of the species considered. Units: The diﬀusion ﬂux is expressed in number of particles (or moles) traversing a unit area per unit time and the concentration in number of particles per unit volume. Thus the diﬀusivity D has the dimension of length2 per time and bears the units [cm2 s−1 ] or [m2 s−1 ]. Fick’s ﬁrst law in three dimensions: Fick’s ﬁrst law is easily generalised to three dimensions using a vector notation: J = −D∇C . (2.2) The vector of the diﬀusion ﬂux J is directed opposite in direction to the concentration gradient vector ∇C. The nabla symbol, ∇, is used to express the vector operation on the right-hand side of Eq. (2.2). The nabla operator acts on the scalar concentration ﬁeld C(x, y, z, t) and produces the concentrationgradient ﬁeld ∇C. The concentration-gradient vector always points in that direction for which the concentration ﬁeld undergoes the most rapid increase, Fig. 2.1. Illustration of Fick’s ﬁrst law 2.1 Fick’s Laws in Isotropic Media 29 and its magnitude equals the maximum rate of increase of concentration at the point. For an isotropic medium the diﬀusion ﬂux is antiparallel to the concentration gradient. Equations (2.1) and (2.2) represent the simplest form of Fick’s ﬁrst law. Complications leading to modiﬁcations of Eq. (2.2) may arise from anisotropy, concentration dependence of D, chemical reactions of the diﬀusing particles, external ﬁelds, and high-diﬀuasivity paths. Anisotropy is considered in Sect. 2.3. Further complications are treated in later chapters of this book. Analogous equations: As already mentioned Fick’s ﬁrst law is formally equivalent to Fourier’s law of heat ﬂow J q = −κ∇T , where J q is the ﬂux of heat, T the temperature ﬁeld, and κ the thermal conductivity. It is also analogous to Ohm’s law J e = −σ∇V , where J e is the electric current density, V the electrostatic potential, and σ the electrical conductivity. Fick’s law describes the transport of particles, Fourier’s law the transport of heat, and Ohm’s law the transport of electric charge. 2.1.2 Equation of Continuity Usually, in diﬀusion processes the number of diﬀusing particles is conserved1 . For a diﬀusing species which obeys a conservation law an equation of continuity can be formulated. To this end, let us choose an aribitrary point P located at (x, y, z) and a test volume of size ∆x, ∆y, and ∆z (Fig. 2.2). The diﬀusion ﬂux J and its components Jx , Jy , Jz vary across the test volume. If the sum of the ﬂuxes leaving and entering the test volume do not balance, a net accumulation (or loss) must occur. This material balance can be expressed as inﬂow - outﬂow = accumulation (or loss) rate. The ﬂux components can be substituted into this equation to yield [Jx (P ) − Jx (P + ∆x)] ∆y∆z+ [Jy (P ) − Jy (P + ∆y)] ∆x∆z+ [Jz (P ) − Jz (P + ∆z)] ∆x∆y = accumulation (or loss) rate . 1 This implies that the diﬀusing species neither undergoes reactions nor exchanges with internal sources or sinks. Sources and sinks are important for intrinsic point defects. Reactions of the diﬀusing species with intrinsic point defects can be important as well. Such complications are treated later in the relevant chapters. 30 2 Continuum Theory of Diﬀusion Fig. 2.2. Inﬁnitesimal test volume. The in- and outgoing y-components of the diﬀusion ﬂux are indicated by arrows. The other components (not shown) are analogous Using Taylor expansions of the ﬂux components up to their linear terms, the expressions in square brackets can be replaced by ∆x∂Jx /∂x, ∆y∂Jy /∂y, and ∆z∂Jz /∂z, respectively. This yields ∂Jx ∂Jy ∂Jz ∂C + + ∆x∆y∆z , (2.3) − ∆x∆y∆z = ∂x ∂y ∂z ∂t where the accumulation (or loss) rate in the test volume is expressed in terms of the partial time derivative of the concentration. For inﬁnitesimal size of the test volume Eq. (2.3) can be written in compact form by introducing the vector operation divergence ∇·, which acts on the vector of the diﬀusion ﬂux: −∇ · J = ∂C . ∂t (2.4) Equation (2.4) is denoted as the continuity equation. 2.1.3 Fick’s Second Law – the ‘Diﬀusion Equation’ Fick’s ﬁrst law Eq. (2.2) and the equation of continuity (2.4) can be combined to give an equation which is called Fick’s second law or sometimes also the diﬀusion equation: ∂C = ∇ · (D∇C) . (2.5) ∂t From a mathematical viewpoint Fick’s second law is a second-order partial diﬀerential equation. It is non-linear if D depends on concentration, which 2.2 Diﬀusion Equation in Various Coordinates 31 is, for example, the case when diﬀusion occurs in a chemical composition gradient. The composition-dependent diﬀusivity is usually denoted as the interdiﬀusion coeﬃcient. For arbitrary composition dependence D(C), Eq. (2.5) usually cannot be solved analytically. The strategy to deal with interdiﬀusion is described in Chap. 10. If the diﬀusivity is independent of concentration, which is the case for tracer diﬀusion in chemically homogenous systems or for diﬀusion in ideal solid solutions, Eq. (2.5) simpliﬁes to ∂C = D∆C , ∂t (2.6) where ∆ denotes the Laplace operator. This form of Fick’s second law is sometimes also called the linear diﬀusion equation. It is a linear second-order partial diﬀerential equation for the concentration ﬁeld C(x, y, z, t). One can strive for solutions of this equation, if boundary and initial conditions are formulated. Some solutions are considered in Chap. 3. Analogous equations: If one combines Fourier’s law for the conduction of heat with an equation for the conservation of heat energy, assuming a constant thermal conductivity κ, one arrives at ∂T κ = ∆T , ∂t ρCV where T (x, y, z, t) is the temperature ﬁeld, ρ the mass density, and CV the speciﬁc heat for constant volume. This equation for time-dependent heat conduction is mathematically identical with the linear diﬀusion equation. The time-dependent Schrödinger equation for free particles can be written in a similar way: ∂Ψ i 2 = − ∆Ψ . ∂t 2m Here Ψ (x, y, z, t) denotes the wave function, the Planck constant divided by 2π, and i the imaginary unit. Similar mathematical concepts such as the method of separation of variables can be used to solve diﬀusion and Schrödinger equations. We note, however, that C is a function with real values, whereas the wave function Ψ is a function with a real and an imaginary part. 2.2 Diﬀusion Equation in Various Coordinates As already mentioned, Fick’s second law for constant diﬀusivity is a linear second-order partial diﬀerential equation. The Laplacian operator on the right-hand side of Eq. (2.6) has diﬀerent representations in diﬀerent coordinate systems (Fig. 2.3). Using these representations we get for isotropic diﬀusion the following forms of the linear diﬀusion equation [3, 4]. 32 2 Continuum Theory of Diﬀusion Fig. 2.3. Cartesian (left), cylindrical (middle), and spherical (right) coordinates Cartesian coordinates x, y, z: ∂C =D ∂t ∂2C ∂2C ∂2C + + 2 2 ∂x ∂y ∂z 2 ; (2.7) Cylindrical coordinates r, Θ, z: D ∂ 1 ∂C ∂C ∂C ∂ ∂ ∂C = r + + r ; ∂t r ∂r ∂r ∂Θ r ∂Θ ∂z ∂z (2.8) Spherical coordinates r, Θ, ϕ: D ∂ ∂C 1 ∂ ∂C 1 ∂2C 2 ∂C = 2 r + sin Θ + ∂t r ∂r ∂r sin Θ ∂Θ ∂Θ sin2 Θ ∂ 2 ϕ =D ∂2C 1 ∂2C 2 ∂C 1 ∂2C 1 ∂C + 2 2 + + 2 + 2 cot Θ 2 2 ∂r r ∂r r ∂Θ2 r ∂Θ r sin Θ ∂ϕ . (2.9) Experimental diﬀusion studies often use simple geometric settings, which impose special symmetries on the diﬀusion ﬁeld. In the following we mention some special symmetries: Linear ﬂow in x-direction is a special case of Eq. (2.7), if ∂/∂y = ∂/∂z = 0: ∂2C ∂C =D 2 . ∂t ∂x (2.10) Axial ﬂow in r-direction is a special case of Eq. (2.8), if ∂/∂z = ∂/∂Θ = 0: 2 ∂ C ∂C 1 ∂C =D + . (2.11) ∂t ∂r2 r ∂r 2.3 Fick’s Laws in Anisotropic Media 33 Spherical ﬂow in r-direction is a special case of Eq. (2.9), if ∂/∂φ = ∂/∂Θ = 0: 2 ∂ C ∂C 2 ∂C =D + . (2.12) ∂t ∂r2 r ∂r Such symmetries are conducive to analytical solutions, of which some are discussed in Chap. 3. 2.3 Fick’s Laws in Anisotropic Media Aniosotropic media have diﬀerent diﬀusion properties in diﬀerent directions. Anisotropy is encountered, for example, in non-cubic single crystals, composite materials, textured polycrystals, and decagonal quasicrystals. Anisotropy aﬀects the directional relationship between the vectors of the diﬀusion ﬂux and of the concentration gradient. For such media, for arbitrary directions the direction of the diﬀusion ﬂux at an arbitrary is not normal to the surface of constant concentration. The generalisation of Fick’s ﬁrst law for anisotropic media is J = −D∇C . (2.13) Application of Neumann’s principle [5] shows that the diﬀusivity is a secondrank tensor D. Furthermore, as a consequence of Onsager’s reciprocity relations from the thermodynamics of irreversible processes (see, e.g., [3, 6–8] and Chap. 12) the diﬀusivity tensor is symmetric. Any symmetric secondrank tensor can be transformed to its three orthogonal principal axes. The diﬀusivity tensor then takes the form ⎞ ⎛ D1 0 0 D = ⎝ 0 D2 0 ⎠ , 0 0 D3 where D1 , D2 , and D3 are called the principal diﬀusion coeﬃcients or the principal diﬀusivities (self-diﬀusivities, solute diﬀusivities, . . . ). There are thus not more than three coeﬃcients of diﬀusion. There are, however, always p ≤ 6 independent parameters; the p − 3 others deﬁne the orientations of the principal axes. The number p varies according to the symmetry of the crystal system as indicated in Table 2.1. If x1 , x2 , x3 denote the principal diﬀusion axes and J1 , J2 , J3 the pertinent components of the diﬀusion ﬂux, Eq. (2.13) can be written as ∂C , ∂x1 ∂C , J2 = −D2 ∂x2 ∂C J3 = −D3 . ∂x3 J1 = −D1 (2.14) 34 2 Continuum Theory of Diﬀusion Table 2.1. Number of parameters, p, decribing the principal diﬀusivities plus the orientations of principal axes System triclinic monoclinic orthorhombic p 6 4 hexagonal tetragonal rhombohedral (or trigonal) cubic 3 2 1 principal axes and one principal axis isotropic crystal axes coincide parallel crystal axis These equations imply that the diﬀusion ﬂux J and the concentration gradient ∇C usually point in diﬀerent directions. Let us describe a selected diﬀusion direction by its angles Θ1 , Θ2 , Θ3 with respect to the principal diﬀusion axes (Fig. 2.4) and introduce the direction cosines of the diﬀusion direction by α1 ≡ cos Θ1 , α2 ≡ cos Θ2 , α3 ≡ cos Θ3 . (2.15) Then the diﬀusion coeﬃcient for that direction, D(α1 , α2 , α3 ), can be written as (2.16) D(α1 , α2 , α3 ) = α21 D1 + α22 D2 + α23 D3 . Equation (2.16) shows that for given principal axes, anisotropic diﬀusion can be completely described by the principal diﬀusion coeﬃcients. Fig. 2.4. Diﬀusion direction in a single-crystal with principal diﬀusion axes x1 , x2 , x3 References 35 For crystals with triclinic, monoclinic, and orthorhombic symmetry all three principal diﬀusivities are diﬀerent: D1 = D2 = D3 . (2.17) Among these crystal systems only for crystals with orthorhombic symmetry the principal axes of diﬀusion do coincide with the axes of crystallographic symmetry. For uniaxial materials, such as trigonal, tetragonal, and hexagonal crystals and decagonal or octagonal quasicrystals, with their unique axis parallel to the x3 -axis we have D1 = D2 = D3 . (2.18) For uniaxial materials Eq. (2.16) reduces to D(Θ) = D1 sin2 Θ + D3 cos2 Θ , (2.19) where Θ denotes the angle between diﬀusion direction and the crystal axis. For cubic crystals and icosahedral quasicrystals D1 = D2 = D3 ≡ D and the diﬀusivity tensor reduces to a scalar quantity (see above). The majority of experiments for the measurement of diﬀusion coeﬃcients in single crystals are designed in such a way that the ﬂow is one-dimensional. Diﬀusion is one-dimensional if a concentration gradient exists only in the x-direction and both, C and ∂C/∂x, are everywhere independent of y and z. Then the diﬀusivity depends on the crystallographic direction of the ﬂow. If the direction of diﬀusion is chosen parallel to one of the principal axis (x1 , or x2 , or x3 ) the diﬀusivity coincides with one of the principal diﬀusivities D1 , or D2 , or D3 . For an arbitrary direction, the measured D is given by Eq. (2.16). For uniaxial materials the diﬀusivity D(Θ) is measured when the crystal or quasicrystal is cut in such a way that an angle Θ occurs between the normal of the front face and the crystal axis. For a full characterisation of the diﬀusivity tensor in crystals with orthorhombic or lower symmetry measurements in three independent directions are necessary. For uniaxial crystals two measurements in independent directions suﬃce. For cubic crystals one measurement in an arbitrary direction is suﬃcient. References 1. A. Fick, Annalen der Phyik und Chemie 94, 59 (1855); Philos. Mag. 10, 30 (1855) 36 2 Continuum Theory of Diﬀusion 2. J.B.J. Fourier, The Analytical Theory of Heat, translated by A. Freeman, University Press, Cambridge, 1978 3. J. Crank, The Mathematics of Diﬀusion, 2nd edition, Oxford University Press, 1975 4. I.N. Bronstein, K.A. Semendjajew, Taschenbuch der Mathematik, 9. Auﬂage, Verlag Harri Deutsch, Zürich & Frankfurt, 1969 5. J.F. Nye, Physical Properties of Crystals: their Representation by Tensors and Matrices, Clarendon Press, Oxford, 1957 6. S.R. de Groot, P. Mazur, Thermodynamics of Irreversible Processes, NorthHolland Publ. Comp., 1952 7. J. Philibert, Atom Movement – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, Cedex A, France, 1991 8. M.E. Glicksman, Diﬀusion in Solids – Field Theory, Solid-State Principles and Applications, John Wiley & Sons, Inc., 2000 3 Solutions of the Diﬀusion Equation The aim of this chapter is to give the reader a feeling for properties of the diﬀusion equation and to acquaint her/him with frequently encountered solutions. No attempt is made to achieve completeness or full rigour. Solutions of Eq. (2.6), giving the concentration as a function of time and position, can be obtained by various means once the boundary and initial conditions have been speciﬁed. In certain cases, the conditions are geometrically highly symmetric. Then it is possible to obtain explicit analytic solutions. Such solutions comprise either Gaussians, error functions and related integrals, or they are given in the form of Fourier series. Experiments are often designed to satisfy simple initial and boundary conditions (see Chap. 13). In what follows, we limit ourselves to a few simple cases. First, we consider solutions of steady-state diﬀusion for linear, axial, and spherical ﬂow. Then, we describe examples of non-steady state diﬀusion in one dimension. A powerful method of solution, which is mentioned brieﬂy, employs the Laplace transform. We end this chapter with a few remarks about instantaneous point sources in one, two, and three dimensions. For more comprehensive treatments of the mathematics of diﬀusion we refer to the textbooks of Crank [1], Jost [2], Ghez [3] and Glicksman [4]. As mentioned already, the conduction of heat can be described by an analogous equation. Solutions of this equation have been developed for many practical cases of heat ﬂow and are collected in the book of Carslaw and Jaeger [5]. By replacing T with C and D with the corresponding thermal property these solution can be used for diﬀusion problems as well. In many other cases, numerical methods must be used to solve diﬀusion problems. Describing numerical procedures is beyond the scope of this book. Useful hints can be found in the literature, e.g., in [1, 3, 4, 6, 7]. 3.1 Steady-State Diﬀusion At steady state, there is no change of concentration with time. Steady-state diﬀusion is characterised by the condition ∂C = 0. ∂t (3.1) 38 3 Solutions of the Diﬀusion Equation For the special geometrical settings mentioned in Sect. 2.2, this leads to diﬀerent stationary concentration distributions: For linear ﬂow we get from Eqs. (2.10) and (3.1) D ∂2C =0 ∂x2 and C(x) = a + Ax , (3.2) where a and A in Eq. (3.2) denote constants. A constant concentration gradient and a linear distribution of concentration is established under linear ﬂow steady-state conditions, if the diﬀusion coeﬃcient is a constant. For axial ﬂow substitution of Eq. (3.1) into Eq. (2.8) gives ∂ ∂C r = 0 and C(r) = B ln r + b , (3.3) ∂r ∂r where B and b denote constants. For spherical ﬂow substitution of Eq. (3.1) into Eq. (2.9) gives ∂ Ca 2 ∂C + Cb . r = 0 and C(r) = ∂r ∂r r (3.4) Ca and Cb in Eq. (3.4) denote constants. Permeation through membranes: The passage of gases or vapours through membranes is called permeation. A well-known example is diﬀusion of hydrogen through palladium membranes. A steady state can be established in permeation experiments after a certain transient time (see Sect. 3.2.4). Based on Eqs. (3.2), (3.3), and (3.4) a number of examples are easy to formulate and are useful in permeation studies of diﬀusion: Planar Membrane: If δ is the thickness, q the cross section of a planar membrane, and C1 and C2 the concentrations at x = 0 and x = δ, we get from Eq. (3.2) C1 − C2 C2 − C1 x; J = qD . (3.5) C(x) = C1 + δ δ If J, C1 , and C2 are measured in an experiment, the diﬀusion coeﬃcient can be determined from Eq. (3.5). Hollow cylinder: Consider a hollow cylinder, which extends from an inner radius r1 to an outer radius r2 . If at r1 and r2 the stationary concentrations C1 and C2 are maintained, we get from Eq. (3.3) C(r) = C1 + r C1 − C2 ln . ln(r1 /r2 ) r1 (3.6) Spherical shell: If the shell extends from an inner radius r1 to an outer radius r2 , and if at r1 and r2 the stationary concentrations C1 and C2 are maintained, we get from Eq. (3.4) C(r) = C1 r1 − C2 r2 (C1 − C2 ) 1 . + 1 r1 − r2 ( r1 − r12 ) r (3.7) 3.2 Non-Steady-State Diﬀusion in one Dimension 39 For the geometrical conditions treated above, it is also possible to solve the steady-state equations, if the diﬀusion coeﬃcient is not a constant [8]. Solutions for concentration-dependent and position-dependent diﬀusivities can be found, e.g., in the textbook of Jost [2]. 3.2 Non-Steady-State Diﬀusion in one Dimension 3.2.1 Thin-Film Solution An initial condition at t = 0, which is encountered in many one-dimensional diﬀusion problems, is the following: C(x, 0) = M δ(x) . (3.8) The diﬀusing species (diﬀusant) is deposited at the plane x = 0 and allowed to spread for t > 0. M denotes the number of diﬀusing particles per unit area and δ(x) the Dirac delta function. This initial condition is also called instantaneous planar source. Sandwich geometry: If the diﬀusant (or diﬀuser) is allowed to spread into two material bodies occupying the half-spaces 0 < x < ∞ and −∞ < x < 0, which have equal and constant diﬀusivity, the solution of Eq. (2.10) is x2 M exp − C(x, t) = √ . (3.9) 4Dt 2 πDt Thin-ﬁlm geometry: If the diﬀuser is deposited initially onto the surface of a sample and spreads into one half-space, the solution is x2 M exp − C(x, t) = √ . (3.10) 4Dt πDt These solutions are also denoted as Gaussian solutions. Note that Eqs. (3.9) and (3.10) diﬀer by a factor of 2. Equation (3.10) is illustrated in Fig. 3.1 and some of its further √ properties in Fig. 3.2. The quantity 2 Dt is a characteristic diﬀusion length, which occurs frequently in diﬀusion problems. Salient properties of Eq. (3.9) are the following: 1. The diﬀusion process is subject to the conservation of the integral number of diﬀusing particles, which for Eq. (3.9) reads +∞ −∞ x2 M √ exp − dx = 4Dt 2 πDt +∞ M δ(x)dx = M . (3.11) −∞ 2. C(x, t) and ∂ 2 C/∂x2 are even functions of x. ∂C/∂x is an odd function of x. 40 3 Solutions of the Diﬀusion Equation Fig. 3.1. Gaussian √ solution of the diﬀusion equation for various values of the diﬀusion length 2 Dt Fig. 3.2. Gaussian solution of the diﬀusion equation and its derivatives 3. The diﬀusion ﬂux, J = −D∂C/∂x, is an odd function of x. It is zero at the plane x = 0. 4. According to the diﬀusion equation the rate of accumulation of the diffusing species ∂C/∂t is an even function of x. It is negative for small |x| und positive for large |x|. 3.2 Non-Steady-State Diﬀusion in one Dimension 41 The tracer method for the experimental determination of diﬀusivities exploits these properties (see Chap. 13). The Gaussian solutions are also applicable if the thickness of the deposited layer is very small with respect to the diﬀusion length. 3.2.2 Extended Initial Distribution and Constant Surface Concentration So far, we have considered solutions of the diﬀusion equation when the diﬀusant is initially concentrated in a very thin layer. Experiments are also often designed in such a way that the diﬀusant is distributed over a ﬁnite region. In practice, the diﬀusant concentration is often kept constant at the surface of the sample. This is, for example, the case during carburisation or nitridation experiments of metals. The linearity of the diﬀusion equation permits the use of the ‘principle of superposition’ to produce new solutions for diﬀerent geometric arrangements of the sources. In the following, we consider examples which exploit this possibility. Diﬀusion Couple: Let us suppose that the diﬀusant has an initial distribution at t = 0 which is given by: C = C0 for x < 0 and C = 0 for x > 0 . (3.12) This situation holds, for example, when two semi-inﬁnite bars diﬀering in composition (e.g., a dilute alloy and the pure solvent material) are joined end to end at the plane x = 0 to form a diﬀusion couple. The initial distribution can be interpreted as a continuous distribution of instantaneous, planar sources of inﬁnitesimal strength dM = C0 dξ at position ξ spread uniformly along the left-hand bar, i.e. for x < 0. A unit length of the left-hand bar initially contains M = C0 · 1 diﬀusing particles per unit area. Initially, the right-hand bar contains no diﬀusant, so one can ignore contributions from source points ξ > 0. The solution of this diﬀusion problem, C(x, t), may be thought as the sum, or integral, of all the inﬁnitesimal responses resulting from the continuous spatial distribution of instantaneous source releases from positions ξ < 0. The total response occurring at any plane x at some later time t is given by the superposition 0 C(x, t) = C0 −∞ exp −(x − ξ)2 /4Dt C0 √ dξ = √ π 2 πDt ∞ exp(−η 2 )dη . (3.13) √ x/2 Dt √ Here we used the variable substitution η ≡ (x − ξ)/2 Dt. The right-hand side of Eq. (3.13) may be split and rearranged as ⎡ ⎤ √ C0 ⎢ 2 C(x, t) = ⎣√ 2 π ∞ x/2 Dt ⎥ exp (−η 2 )dη ⎦ . 2 exp (−η )dη − √ π 2 0 0 (3.14) 42 3 Solutions of the Diﬀusion Equation It is convenient to introduce the error function 1 z 2 erf (z) ≡ √ π exp (−η 2 )dη , (3.15) 0 which is a standard mathematical function. Some properties of erf (z) and useful approximations are discussed below. Introducing the error function we get x C0 x C0 √ √ C(x, t) = erfc ≡ , (3.16) erf (∞) − erf 2 2 2 Dt 2 Dt where the abbreviation erfc(z) ≡ 1 − erf(z) (3.17) is denoted as the complementary error function. Like the thin-ﬁlm solution, Eq. (3.16) is applicable when the diﬀusivity is constant. Equation (3.16) is sometimes called the Grube-Jedele solution. Diﬀusion with Constant Surface Concentration: Let us suppose that the concentration at x = 0 is maintained at concentration Cs = C0 /2. The Grube-Jedele solution Eq. (3.16) maintains the concentration in the midplane of the diﬀusion couple. This property can be exploited to construct the diﬀusion solution for a semi-inﬁnite medium, the free end of which is continuously exposed to a ﬁxed concentration Cs : x √ C = Cs erfc . (3.18) 2 Dt The quantity of material which diﬀuses into the solid per unit area is: M (t) = 2Cs Dt/π . (3.19) Equation (3.18) is illustrated in Fig. 3.3. The behaviour of this solution reveals several general features of diﬀusion problems in inﬁnite or semi-inﬁnite media, where the initial concentration at the boundary equals some constant for all time: The concentration ﬁeld C(x, t) in these cases may be expressed with 1 The probability integral introduced by Gauss is deﬁned as 2 Φ(a) ≡ √ 2π Za exp (−η 2 /2)dη . 0 The error function and the probability integral are related via √ erf(z) = Φ( 2z) . 3.2 Non-Steady-State Diﬀusion in one Dimension 43 Fig. 3.3. Solution of the diﬀusion equation for√constant surface concentration Cs and for various values of the diﬀusion length 2 Dt √ a single variable z = x/2 Dt, which is a special combination of space-time ﬁeld variables. The quantity z is sometimes called a similarity variable which captures both, the spatial and temporal features of the concentration ﬁeld. Similarity scaling is extremely useful in applying the diﬀusion solution to diverse situations. For example, if the average diﬀusion length is increased by a factor of ten, the product of the diﬀusivity times the diﬀusion time would have to increase by a factor of 100 to return to the same value of z. Applications of Eq. (3.18) concern, e.g., carburisation or nitridation of metals, where in-diﬀusion of C or N into a metal occurs from an atmosphere, which maintains a constant surface concentration. Other examples concern in-diﬀusion of foreign atoms, which have a limited solubility, Cs , in a matrix. Diﬀusion from a Slab Source: In this arrangement a slab of width 2h having a uniform initial concentration C0 of the diﬀusant is joined to two half-spaces which, in an experiment may be realised as two bars of the pure material. If the slab and the two bars have the same diﬀusivity, the diﬀusion ﬁeld can be expressed by an integral of the source distribution −h (x − ξ)2 exp − dξ . 4Dt +h C0 C(x, t) = √ 2 πDt (3.20) This expression can be manipulated into standard form and written as x−h x+h C0 √ √ C(x, t) = + erf . (3.21) erf 2 2 Dt 2 Dt 44 3 Solutions of the Diﬀusion Equation Fig. 3.4. Diﬀusion from a slab of width 2h for various values of √ Dt/h The normalised concentration ﬁeld, C(x/h, √ t)/C0 , resulting from Eq. (3.21) is shown in Fig. 3.4 for various values of Dt/h. Error Function and Approximations: The error function deﬁned in Eq. (3.15) is an odd function and for large arguments |z| approaches asymptotically ±1: erf (−z) = erf (z), erf (±∞) = ±1, erf (0) = 0 . (3.22) The complementary error function deﬁned in Eq. (3.17) has the following asymtotic properties: erfc(−∞) = 2, erfc(+∞) = 0, erfc(0) = 1 . (3.23) Tables of the error function are available in the literature, e.g., in [4, 9–11]. Detailed calculations cannot be performed just relying on tabular data. For advanced computations and for graphing one needs, instead, numerical estimates for the error function. Approximations are available in commercial mathematics software. In the following, we mention several useful expressions: 1. For small arguments, |z| < 1, the error function is obtained to arbitrary accuracy from its Taylor expansion [10] as 2 z5 z7 z3 erf (z) = √ z − + − + ... . (3.24) π (3 × 1)! (5 × 2)! (7 × 3)! 3.2 Non-Steady-State Diﬀusion in one Dimension 45 2. For large arguments, z 1, it is approximated by its asymptotic form exp(−z 2 ) 1 √ erf(z) = 1 − (3.25) 1− 2 + ... . 2 π 2z 3. A convenient rational expression reported in [11] is the following: 1 (1 + 0.278393z + 0.230389z 2 + 0.000972z 3 + 0.078108z 4)4 + (z) . (3.26) erf (z) = 1 − This expression works for z > 0 with an associated error (z) less than 5 × 10−4 . 3.2.3 Method of Laplace Transformation The Laplace transformation is a mathematical procedure, which is useful for various problems in mathematical physics. Application of the Laplace transformation to the diﬀusion equation removes the time variable, leaving an ordinary diﬀerential equation, the solution of which yields the transform of the concentration ﬁeld. This is then interpreted to give an expression for the concentration in terms of space variables and time, satisfying the initial and boundary conditions. Here we deal only with an application to the one-dimensional diﬀusion equation, the aim being to describe rather than to justify the procedure. The solution of many problems in diﬀusion by this method calls for no knowledge beyond ordinary calculus. For more diﬃcult problems the theory of functions of a complex variable must be used. No attempt is made here to explain problems of this kind, although solutions obtained in this way are quoted, e.g., in the chapter on grain-boundary diﬀusion. Fuller accounts of the method and applications can be found in the textbooks of Crank [1], Carslaw and Jaeger [5], Churchill [12] and others. Deﬁnition of the Laplace Transform: The Laplace transform f¯(p) of a known function f (t) for positive values of t is deﬁned as ∞ f¯(p) = exp(−pt)f (t)dt . (3.27) 0 p is a number suﬃciently large to make the integral Eq. (3.27) converge. It may be a complex number whose real part is suﬃciently large, but in the following discussion it suﬃces to think of it in terms of a real positive number. Laplace transforms are common functions and readily constructed by carrying out the integration in Eq. (3.27) as in the following examples: 46 3 Solutions of the Diﬀusion Equation ∞ f¯(p) = f (t) = 1, exp(−pt)dt = 1 , p (3.28) 0 ∞ f¯(p) = f (t) = exp(αt), 1 , p−α exp(−pt) exp(αt)dt = 0 ∞ f¯(p) = f (t) = sin(ωt), exp(−pt) sin(ωt)dt = p2 ω . + ω2 (3.29) (3.30) 0 Semi-inﬁnite Medium: As an application of the Laplace transform, we consider diﬀusion in a semi-inﬁnite medium, x > 0, when the surface is kept at a constant concentration Cs . We need a solution of Fick’s equation satisfying this boundary condition and the initial condition C = 0 at t = 0 for x > 0. On multiplying both sides of Fick’s second law Eq. (2.6) by exp(−pt) and integrating, we obtain ∞ D ∂2C exp(−pt) 2 dt = ∂x 0 ∞ exp(−pt) ∂C dt . ∂t (3.31) 0 By interchanging the orders of diﬀerentiation and integration, the left-hand term is then ∞ D ∂2C ∂2 exp(−pt) 2 dt = D 2 ∂x ∂x 0 ∞ C exp(−pt)dt = D ∂ 2 C̄ . ∂x2 (3.32) 0 Integrating the right-hand term of Eq. (3.31) by parts, we have ∞ exp(−pt) ∂C ∞ dt = [C exp(−pt)]0 + p ∂t 0 ∞ C exp(−pt)dt = pC̄ , (3.33) 0 since the term in brackets vanishes by virtue of the initial condition and through the exponential factor. Thus Fick’s second equation transforms to D ∂ 2 C̄ = pC̄ . ∂x2 (3.34) The Laplace transformation reduces Fick’s second law from a partial diﬀerential equation to the ordinary diﬀerential equation Eq. (3.34). By treating the boundary condition at x = 0 in the same way, we obtain ∞ C̄ = Cs exp(−pt)dt = 0 Cs . p (3.35) 3.2 Non-Steady-State Diﬀusion in one Dimension 47 The solution of Eq. (3.34), which satisﬁes the boundary condition and for which C̄ remains ﬁnite for large x is p Cs exp C̄ = x. (3.36) p D Reference to a table of Laplace transforms [1] shows that the function whose transform is given by Eq. (3.36) is the complementary error function x √ . (3.37) C = Cs erfc 2 Dt We recognise that this is the solution given already in Eq. (3.16). 3.2.4 Diﬀusion in a Plane Sheet – Separation of Variables Separation of variables is a mathematical method, which is useful for the solution of partial diﬀerential equations and can also be applied to diﬀusion problems. It is particularly suitable for solutions of Fick’s law for ﬁnite systems by assuming that the concentration ﬁeld can be expressed in terms of a periodic function in space and a time-dependent function. We illustrate this method below for the problem of diﬀusion in a plane sheet. The starting point is to strive for solutions of Eq. (2.10) trying the ‘Ansatz’ C(x, t) = X(x)T (t) , (3.38) where X(x) and T (t) separately express spatial and temporal functions of x and t, respectively. In the case of linear ﬂow, Fick’s second law Eq. (2.10) yields 1 d2 X 1 dT = . (3.39) DT dt X dx2 In this equation the variables are separated. On the left-hand side we have an expression depending on time only, while the right-hand side depends on the distance variable only. Then, both sides must equal the same constant, which for the sake of the subsequent algebra is chosen as −λ2 : 1 ∂T 1 ∂2X = ≡ −λ2 . DT ∂t X ∂2x (3.40) We then arrive at two ordinary linear diﬀerential equations: one is a ﬁrst-order equation for T (t), the other is a second-order equation for X(x). Solutions to each of these equations are well known: T (t) = T0 exp (−λ2 Dt) (3.41) X(x) = a sin (λx) + b cos (λx) , (3.42) and 48 3 Solutions of the Diﬀusion Equation where T0 , a, and b are constants. Inserting Eqs. (3.41) and (3.42) in (3.38) yields a particular solution of the form C(x, t) = [A sin (λx) + B cos (λx)] exp (−λ2 Dt) , (3.43) where A = aT0 and B = bT0 are again constants of integration. Since Eq. (2.10) is a linear equation its general solution is obtained by summing solutions of the type of Eq. (3.43). We get C(x, t) = ∞ [An sin (λn x) + Bn cos (λn x)] exp (−λ2n Dt) , (3.44) n=1 where An , Bn and λn are determined by the initial and boundary conditions for the particular problem. The separation constant −λ2 cannot be arbitrary, but must take discrete values. These eigenvalues uniquely deﬁne the eigenfunctions of which the concentration ﬁeld C(x, t) is composed. Out-diﬀusion from a plane sheet: Let us consider out-diﬀusion from a plane sheet of thickness L. An example provides out-diﬀusion of hydrogen from a metal sheet during degassing in vacuum. The diﬀusing species is initially distributed with constant concentration C0 and both surfaces of the sheet are kept at zero concentration for times t > 0: at t = 0 Initial condition C = C0 , for 0 < x < L Boundary condition C = 0, for x = 0 and x = L at t > 0. The boundary conditions demand that Bn = 0 and λn = nπ , L where n = 1, 2, 3, . . . (3.45) The numbers λn are the eigenvalues of the plane-sheet problem. Inserting these eigenvalues, Eq. (3.44) reads nπ n2 π 2 D x exp − C(x, t) = An sin t . L L2 n=1 ∞ (3.46) The initial conditions require that C0 = ∞ n=1 An sin nπ x . L (3.47) By multiplying both sides of Eq. (3.47) by sin(pπx/L) and integrating from 0 to L we get L nπx pπx sin dx = 0 (3.48) sin L L 0 3.2 Non-Steady-State Diﬀusion in one Dimension 49 for n = p and L/2 for n = p. Using these orthogonality relations all terms vanish for which n is even. Thus An = 4C0 ; n = 1, 3, 5, . . . nπ (3.49) The ﬁnal solution of the problem of out-diﬀusion from a plane sheet is ∞ 4C0 1 (2j + 1)2 π 2 D (2j + 1)π C(x, t) = sin x exp − t , (3.50) π j=0 2j + 1 L L2 where for convenience 2j + 1 was substituted for n so that j takes values 0, 1, 2, . . . . Each term in Eq. (3.50) corresponds to a term in the Fourier series (here a trigonometrical series) by which for t = 0 the initial distribution Eq. (3.47) can be represented. Each term is also characterised by a relaxation time L2 , j = 0, 1, 2, . . . (3.51) τj = (2j + 1)2 π 2 D The relaxation times decrease rapidly with increasing j, which implies that the series Eq. (3.50) converges satisfactorily for moderate and large times. Desorption and Absorption: It is sometimes of interest to consider the average concentration in the sheet, C̄, deﬁned as C̄(t) = 1 L L C(x, t)dx . (3.52) 0 Inserting Eq. (3.50) into Eq. (3.52) yields ∞ C̄(t) 1 8 t = 2 exp − . C0 π j=0 (2j + 1)2 τj (3.53) We recognise that for t τ1 the average concentration decays exponentially with the relaxation time L2 (3.54) τ0 = 2 . π D Direct applications of the solution developed above concern degassing of a hydrogen-charged metal sheet in vacuum or decarburisation of a sheet of steel. If we consider the case t τ1 , we get πx t 4C0 sin exp − C(x, t) ≈ . (3.55) π L τ0 The diﬀusion ﬂux from both surfaces is then given by 8DC0 t ∂C . = exp − |J| = 2D ∂x x=0 L τ0 (3.56) 50 3 Solutions of the Diﬀusion Equation Fig. 3.5. Absorption/desorption of a diﬀusing species of/from a thin sheet for various values of Dt/l2 An experimental determination of |J| and/or of the relaxation time τ0 can be used to measure D. The solution for a plane sheet with constant surface concentration maintained at Cs and uniform initial concentration C0 inside the sheet (region −l < x < +l) is a straightforward generalisation of Eq. (3.50). We get ∞ (2j + 1)π C − C0 (2j + 1)2 π 2 D 4 (−1)j cos x exp − = 1− t . Cs − C0 π j=0 2j + 1 2l 4l2 (3.57) For Cs < C0 this solution describes desorption and for Cs > C0 absorption. It is illustrated for various normalised times Dt/l2 in Fig. 3.5. 3.2.5 Radial Diﬀusion in a Cylinder We consider a long circular cylinder, in which the diﬀusion ﬂux is radial everywhere. Then the concentration is a function of radius r and time t, and the diﬀusion equation becomes 1 ∂ ∂C ∂C = rD . (3.58) ∂t r ∂r ∂r Following the method of separation of the variables, we see that for constant D (3.59) C(r, t) = u(r) exp(−Dα2 t) 3.2 Non-Steady-State Diﬀusion in one Dimension 51 is a solution of Eq. (3.58), provided that u satisﬁes ∂ 2 u 1 ∂u + α2 u = 0 , + ∂r2 r ∂r (3.60) which is the Bessel equation of order zero. Solutions may be obtained in terms of Bessel functions, suitably chosen so that the initial and boundary conditions are satisﬁed. Let us suppose that the surface concentration is constant and that the initial distribution of the diﬀusant is f (r). For a cylinder of radius R, the conditions are: C = C0 , r = R, t ≥ 0; C = f (r), 0 < r < R, t = 0. The solution to this problem is [1] ∞ 2 1 J0 (rαn ) C(r, t) = C0 1 − exp(−Dα2n t) R n=1 αn J1 (Rαn ) + ∞ J0 (rαn ) 2 exp(−Dα2n t) 2 2 R n=1 J1 (Rαn ) rf (r)J0 (rαn )dr . (3.61) In Eq. (3.61) J0 is the Bessel function of the ﬁrst kind and order zero and J1 the Bessel function of ﬁrst order. The αn are the positive roots of J0 (Rαn ) = 0. If the concentration is initially uniform throughout the cylinder, we have f (r) = C1 and Eq. (3.61) reduces to ∞ C − C1 2 exp(−Dα2n t)J0 (αn r) . =1− C0 − C1 R n=1 αn J1 (αn R) (3.62) If M (t) denotes the quantity of diﬀusant which has entered or left the cylinder in time t and M (∞) the corresponding quantity at inﬁnite time, we have ∞ 4 M (t) =1− exp(−Dα2n t) . 2 R2 M (∞) α n=1 n (3.63) . 3.2.6 Radial Diﬀusion in a Sphere The diﬀusion equation for a constant diﬀusivity and radial ﬂux takes the form 2 ∂ C ∂C 2 ∂C =D + . (3.64) ∂t ∂r2 r ∂r 52 3 Solutions of the Diﬀusion Equation By substituting u(r, t) = C(r, t)r , (3.65) Eq. (3.64) becomes ∂2u ∂u (3.66) =D 2 . ∂t ∂r This equation is analogous to linear ﬂow in one dimension. Therefore, solutions of many problems of radial ﬂow in a sphere can be deduced from those of the corresponding linear ﬂow problems. If we suppose that the sphere is initially at a uniform concentration C1 and the surface concentration is maintained constant at C0 , the solution is [1] ∞ nπr C − C1 2R (−1)n sin exp(−Dn2 π 2 t/R2 ) . =1+ C0 − C1 π n=1 n R (3.67) The concentration at the centre is given by the limit r → 0, that is by ∞ C − C1 =1+2 (−1)n exp(−Dn2 π 2 t/R2 ) . C0 − C1 n=1 (3.68) If M (t) denotes the quantity of diﬀusant which has entered or left the sphere in time t and M (∞) the corresponding quantity at inﬁnite time, we have ∞ 6 1 M (t) =1− 2 exp(−Dn2 π 2 t/R2 ) . M (∞) π n=1 n2 The corresponding solutions for small times are ∞ C − C1 (2n + 1) + r R (2n + 1) − r √ √ − erfc = erfc C0 − C1 r n=0 2 Dt 2 Dt and M (t) =6 M (∞) ∞ Dt Dt 1 nR √ +2 −3 2 , ierfc √ 2 R π R Dt n=1 (3.69) (3.70) (3.71) where ierfc denotes the inverse of the complementary error function. 3.3 Point Source in one, two, and three Dimensions In the previous section, we have dealt with one-dimensional solutions of the linear diﬀusion equation. As examples for diﬀusion in higher dimensions, we consider now diﬀusion from instantaneous sources in two- and threedimensional media. The diﬀusion response for a point source in three dimensions and for a line source in two dimensions diﬀers from that of the thin-ﬁlm source in one dimension given by Eq. (3.9). Now we ask for particular solutions of References 53 Fick’ second law under spherical or axial symmetry conditions described by Eqs. (2.12) and (2.11). Let us suppose that in the case of spherical ﬂow a point source located at |r 3 | = 0 releases at time t = 0 a ﬁxed number N3 of diﬀusing particles into an inﬁnite and isotropic medium. Let us also suppose that in the case of axial ﬂow a line source located at |r 2 | = 0 releases N2 diﬀusing particles into an inﬁnite and isotropic medium. The diﬀusion ﬂow will be either spherical or axisymmetric, respectively. The concentration ﬁelds that develop around instantaneous plane-, line-, and point-sources in one, two, three dimensions, can all be expressed in homologous form by Nd |rd |2 exp − C(r d , t) = (d = 1, 2, 3). (3.72) 4Dt (4πDt)d/2 In Eq. (3.72) r d denotes the d-component vector extending from the source located at rd = 0 to the ﬁeld point, r d , of the concentration ﬁeld. If the source strength Nd denotes the number of particles in all three dimensions, the diﬀusion ﬁelds predicted by Eq. (3.72) must be expressed in dimensionalitycompatible concentration units. These are [number per length] for d = 1, [number per length2 ] for d = 2, and [number per length3 ] for d = 3. We note that the source solutions are all linear, in the sense that the concentration response is proportional to the initial source strength. References 1. J. Crank, The Mathematics of Diﬀusion, 2nd edition, Oxford University Press, Oxford, 1975 2. W. Jost, Diﬀusion in Solids, Liquids, Gases, Academic Press, Inc., New York, 1952, 4th printing with addendum 1965 3. R. Ghez, A Primer of Diﬀusion Problems, Wiley and Sons, 1988 4. M.E. Glicksman, Diﬀusion in Solids, John Wiley and Sons, Inc. 2000 5. H.S. Carslaw, J.C. Jaeger, Conduction of Heat in Solids, Clarendon Press, Oxford, 1959 6. L. Fox, Moving Boundary Problems in Heat Flow and Diﬀusion, Clarendon Press, Oxford, 1974 7. J. Crank, Free and Moving Boundary Problems, Oxford University Press, Oxford, 1984; reprinted in 1988, 1996 8. R.M. Barrer, Proc. Phys. Soc. (London) 58, 321 (1946) 9. Y. Adda, J. Philibert, La Diﬀusion dans les Solides, 2 volumes, Presses Universitaires de France, 1966 10. I.S. Gradstein, L.M. Ryshik, Tables of Series, Products, and Integrals, Verlag MIR, Moscow, 1981 11. A. Milton, I.A. Stegun (Eds.), Handbook of Mathematical Functions, Applied Mathematical Series 55, National Bureau of Standards, U.S. Government Printing Oﬃce, Washington, DC, 1964 12. R.V. Churchill, Modern Operational Mathematics in Engineering, McGraw Hill, new York , 1944 4 Random Walk Theory and Atomic Jump Process From a microscopic viewpoint, diﬀusion occurs by the Brownian motion of atoms or molecules. As mentioned already in Chap. 1, Albert Einstein in 1905 [1] published a theory for the chaotic motion of small particles suspended in a liquid. This phenomenon had been observed by the Scotish botanist Robert Brown more than three quarters of a century earlier in 1827, when he studied the motion of granules from pollen in water. Einstein argued that the motion of mesoscopic particles is due to the presence of molecules in the ﬂuid. He further reasoned that molecules due to their Boltzmann distribution of energy are always subject to thermal movements of a statistical nature. These statistical ﬂuctuations are the source of stochastic motions occurring in matter all the way down to the atomic scale. Einstein related the mean square displacement of particles to the diﬀusion coeﬃcient. This relation was, almost at the same time, developed by the Polish scientist Smoluchowski [2, 3]. It is nowadays called the Einstein relation or the Einstein-Smoluchowski relation. In gases, diﬀusion occurs by free ﬂights of atoms or molecules between their collisions. The individual path lengths of these ﬂights are distributed around some well-deﬁned mean free path. Diﬀusion in liquids exhibits more subtle atomic motion than gases. Atomic motion in liquids can be described as randomly directed shuﬄes, each much smaller than the average spacing of atoms in a liquid. Most solids are crystalline and diﬀusion occurs by atomic hops in a lattice. The most important point is that a separation of time scales exists between the elementary jump process of particles between neighbouring lattice sites and the succession of steps that lead to macroscopic diﬀusion. The elementary diﬀusion jump of an atom on a lattice, for instance, the exchange of a tracer atom with a neighbouring vacancy or the jump of an interstitial atom, has a duration which corresponds to about the reciprocal of the Debye frequency (≈ 10−13 s). This process is usually very rapid as compared to the mean residence time of an atom on a lattice site. Hence the problem of diﬀusion in lattices can be separated into two diﬀerent tasks: 1. The more or less random walk of particles on a lattice is the ﬁrst topic of the present chapter. Diﬀusion in solids results from many individual displacements (jumps) of the diﬀusing particles. Diﬀusive jumps are usually 56 4 Random Walk Theory and Atomic Jump Process single-atom jumps of ﬁxed length(s), the size of which is of the order of the lattice parameter. In addition, atomic jumps in crystals are frequently mediated by lattice defects such as vacancies and/or self-interstitials. Thus, the diﬀusivity can be expressed in terms of physical quantities that describe these elementary jump processes. Such quantities are the jump rates, the jump distances of atoms, and the correlation factor (see below). 2. The second topic of this chapter concerns the rate of individual jumps. Jump processes are promoted by thermal activation. Usually an Arrhenius law holds for the jump rate Γ : ∆G 0 . (4.1) Γ = ν exp − kB T The prefactor ν 0 denotes an attempt frequency of the order of the Debye frequency of the lattice. ∆G is the Gibbs free energy of activation, kB the Boltzmann constant, and T the absolute temperature. A detailed treatment can be found in the textbook of Flynn [4] and in a more recent review of activated processes by Hänggi et al. [5]. We consider the jump rate in the second part of this section. 4.1 Random Walk and Diﬀusion The mathematics of the random-walk problem allows us to go back and forth between the diﬀusion coeﬃcient deﬁned in Fick’s laws and the underlying physical quantities of diﬀusing atoms. This viewpoint is most exciting since it transforms the study of diﬀusion from the question how a system will homogenise into a tool for studying the atomic processes involved in a variety of reactions in solids and for studying defects in solids. 4.1.1 A Simpliﬁed Model Before going through a more rigorous treatment of random walks, it may be helpful to study a simple situation: unidirectional diﬀusion of interstitials in a simple cubic crystal. Let us assume that the diﬀusing atoms are dissolved in low concentrations and that they move by jumping from an interstitial site to a neighbouring one with a jump length λ (Fig. 4.1). We suppose a concentration gradient along the x-direction and introduce the following deﬁnitions: Γ : jump rate (number of jumps per unit time) from one plane to the neigbouring one, n1 : number of interstitials per unit area in plane 1, n2 : number of interstitials per unit area in plane 2. 4.1 Random Walk and Diﬀusion 57 Without a driving force, forward and backward hops occur with the same jump rate and the net ﬂux J from plane 1 to 2 is J = Γ n1 − Γ n2 . (4.2) The quantities n1 and n2 are related to the volume concentrations (number densities) of diﬀusing atoms via C1 = n1 , λ C2 = n2 . λ (4.3) Usually in diﬀusion studies the concentration ﬁeld, C(x, t), changes slowly as a function of the distance variable x in terms of interatomic distances. From a Taylor expansion of the concentration-distance function, keeping only the ﬁrst term (Fig. 4.1), we get C1 − C2 = −λ ∂C . ∂x (4.4) Inserting Eqs. (4.3) and (4.4) into Eq. (4.2) we arrive at J = −λ2 Γ ∂C . ∂x (4.5) By comparison with Fick’s ﬁrst law we obtain for the diﬀusion coeﬃcient D = Γ λ2 . (4.6) Fig. 4.1. Schematic representation of unidirectional diﬀusion of atoms in a lattice 58 4 Random Walk Theory and Atomic Jump Process Taking into account that in a simple cubic lattice the jump rate of an atom to one of its six nearest-neighbour interstices is related to its total jump rate via Γtot = 6Γ , we obtain 1 D = Γtot λ2 . (4.7) 6 This equation shows that the diﬀusion coeﬃcient is essentially determined by the product of the jump rate and the jump distance squared. We will show later that this expression is true for any cubic Bravais lattice as long as only nearest-neighbour jumps are considered. 4.1.2 Einstein-Smoluchowski Relation Let us now consider the random walk of diﬀusing particles in a more rigorous way. The total displacement R of a particle is composed of many individual displacements r i . Imagine a cloud of diﬀusing particles starting at time t0 from the origin and making many individual displacements during the time t − t0 . We then ask the question, what is the magnitude characteristic of a random walk after some time t − t0 = τ ? We shall see below that the mean square displacement plays a prominent rôle. The total displacement of a particle after many individual displacements R = (X, Y, Z) (4.8) is composed of its components X, Y, Z along the x, y, z-axes of the coordinate system and we have (4.9) R2 = X 2 + Y 2 + Z 2 . To keep the derivation general, the medium is taken not necessarily as isotropic. We concentrate on the X-component of the total displacement and introduce a distribution function W (X, τ ). The quantity W denotes the probability that after time τ the particle will have travelled a path with an x-projection X. We assume that W is independent of the choice of the origin and depends only on τ = t − t0 . These assumptions entail that diﬀusivity and mobility are independent of position and time. Y - and Z-component of the displacement can be treated in analogous way. Fortunately, the precise analytical form of W need not to be known in the following. Consider now the balance for the number of the diﬀusing particles (concentration C) located in the plane x at time t+τ . These particles were located in the planes x − X at time t. We thus have C(x − X, t)W (X, τ ) , (4.10) C(x, t + τ ) = X where the summation must be carried over all values of X. The rate at which the concentration is changing can be found by expanding C(x, t + τ ) and C(x − X, t) around X = 0, τ = 0. We get 4.1 Random Walk and Diﬀusion C(x, t) + τ ∂C + ··· = ∂t 59 C(x, t) − X X X 2 ∂2C ∂C + + . . . W (X, τ ) . ∂x 2 ∂x2 (4.11) The derivatives of C are to be taken at plane x for the time t. It is convenient to deﬁne the nth -moments of X in the usual way: W (X, τ ) = 1 X X n W (X, τ ) = X n . (4.12) X The ﬁrst expression in Eq. (4.12) states that W (X, τ ) is normalised. The second expression deﬁnes the so-called n-th moment X n of X. The average values of X n must be taken over a large number of diﬀusing particles. In particular, we are be interested in the ﬁrst and second moment. The second moment X 2 is also denoted as the mean square displacement. The derivatives ∂C/∂t, ∂C/∂x, ∂ 2C/∂x2 . . . have ﬁxed values for time t and position x. For small values of τ , the higher order terms on the left-hand side of Eq. (4.11) are negligible. In addition, because of the nature of diﬀusion processes, W (X, τ ) becomes more and more localised around X = 0 when τ is small. Therefore, for suﬃciently small τ terms higher than second order on the right-hand side of Eq. (4.11) can be omitted as well. The terms C(x, t) cancel and we get 2 X ∂C X ∂ 2C ∂C . (4.13) =− + ∂t τ ∂x 2τ ∂x2 We recognise that the ﬁrst term on the right-hand side corresponds to a drift term and the second one to the diﬀusion term. In the absence of a driving force, we have X = 0 and Eq. (4.13) reduces to Fick’s second law with the diﬀusion coeﬃcient 2 X . (4.14) Dx = 2τ This expression relates the mean square displacement in the x-direction with the pertinent component Dx of the diﬀusion coeﬃcient. Analogous equations hold between the diﬀusivities Dy , Dz and the mean square displacements in the y- and z-directions: 2 2 Y Z ; Dz = . (4.15) Dy = 2τ 2τ In an isotropic medium, in cubic crystals, and in icosahedral quasicrystals the displacements in x-, y-, and z-directions are the same. Hence X2 = Y 2 = Z2 = 1 2 R 3 (4.16) 60 4 Random Walk Theory and Atomic Jump Process and R2 . (4.17) 6τ Equations (4.14) or (4.17) are the relations already mentioned at the entrance of this chapter. They are denoted as the Einstein relation or as the EinsteinSmoluchowski relation. D= 4.1.3 Random Walk on a Lattice In a crystal, the total displacement of an atom is composed of many individual jumps of discrete jump length. For example, in a coordination lattice (coordination number Z) each jump direction will occur with the probability 1/Z and the jump length will usually be the nearest-neighbour distance. According to Fig. 4.2 the individual path of a particle in a sequence of n jumps is the sum n n R= ri or X = xi , (4.18) i=1 i=1 where r i denotes jump vectors with x-projections xi . The squared magnitude of the net displacement is R2 = n ri2 + 2 i=1 X2 = n i=1 n−1 n ri r j , i=1 j=i+1 x2i + 2 n−1 n xi xj . i=1 j=i+1 If we perform an average over an ensemble of particles, we get Fig. 4.2. Example for a jump sequence of a particle on a lattice (4.19) 4.1 Random Walk and Diﬀusion 61 n n−1 n 2 2 R = ri + 2 rirj , 2 X = i=1 i=1 j=i+1 n n−1 2 xi + 2 i=1 n xi xj . (4.20) i=1 j=i+1 The ﬁrst term contains squares of the individual jump lengths only. The double sum contains averages between jump i and all subsequent jumps j. Uncorrelated random walk: Let us consider for the moment a random walker that executes a sequence of jumps in which each individual jump is independent of all prior jumps. Thereby, we deny the ‘walker’ any memory. Such a jump sequence is sometimes denoted as a Markov sequence (memory free walk) or as an uncorrelated random walk. The double sum in Eq. (4.20) contains n(n − 1)/2 average values of the products xi xj or r i rj . These terms contain memory eﬀects also denoted as correlation eﬀects. For a Markov sequence these average values are zero, as for every pair xi xj one can ﬁnd for another particle of the ensemble a pair xi xj equal and opposite in sign. Thus, we get from Eq. (4.20) for a random walk without correlation R2random = n r i2 , i=1 2 Xrandom = n x2i . (4.21) i=1 The index ‘random’ is used to indicate that a true random walk is considered with no correlation between jumps. In a crystal lattice the jump vectors can only take a few deﬁnite values. For example, in a coordination lattice (coordination number Z), in which nearestneighbour jumps occur (jump length d with x-projection dx ), Eq. (4.21) reduces to 2 Rrandom = n d2 , 2 Xrandom = n d2x . (4.22) Here n denotes the average number of jumps of a particle. It is useful to introduce the jump rate Γ of an atom into one of its Z neighbouring sites via n . Zt (4.23) 1 2 d2 d ZΓ = . 6 6τ̄ (4.24) Γ ≡ We then get D= 62 4 Random Walk Theory and Atomic Jump Process Table 4.1. Geometrical properties of cubic Bravais lattices with lattice parameter a Lattice Coordination number Z Jump length d Primitive cubic Body-centered cubic (bcc) Face-centered cubic (fcc) 6 8 12 a√ a√3/2 a 2/2 This equation describes diﬀusion of interstitial atoms in a dilute interstitial solid solution1 . The quantity 1 τ̄ = (4.25) ZΓ is the mean residence time of an atom on a certain site. For cubic Bravais lattices, the jump length d and the lattice parameter a are related to each other as indicated in Table 4.1. Using these parameters we get from Eq. (4.24) D = a2 Γ . (4.26) 4.1.4 Correlation Factor Random walk theory, to this point, involved a series of independent jumps, each occurring without any memory of the previous jumps. However, several atomic mechanisms of diﬀusion in crystals entail diﬀusive motions of atoms which are not free of memory eﬀects. Let us for example consider the vacancy mechanism (see also Chap. 6). If vacancies exchange sites with atoms a memory eﬀect is necessarily involved. Upon exchange, vacancy and ‘tagged’ atom (tracer) move in opposite directions. Immediately after the exchange the vacancy is for a while available next to the tracer atom, thus increasing the probability for a reverse jump of the tracer. Consequently, the tracer atom does not diﬀuse as far as expected for a completely random series of jumps. This reduces the eﬃciency of a tracer walk in the presence of positional memory eﬀects with respect to an uncorrelated random walk. Bardeen and Herring in 1951 [7, 8] recognised that this can be accounted for by introducing the correlation factor n−1 f = lim n→∞ 1 R 2 R2random = 1+ n rirj i=1 j=i+1 2 lim n n→∞ r i2 i=1 , In a non-dilute interstitial solution correlation eﬀects can occur, because some of the neighbouring sites are not available for a jump. 4.1 Random Walk and Diﬀusion n−1 fx = lim n→∞ X 2 2 Xrandom = 1+ n 63 xi xj i=1 j=i+1 2 lim n n→∞ x2i i=1 . (4.27) The correlation factor in Eq. (4.27) equals the sum of two terms: (i) the leading term +1, associated with uncorrelated (Markovian) jump sequences and (ii) the double summation contains the correlation between jumps. It has been argued above that for an uncorrelated walk the double summation is zero. Diﬀusion in solids is often defect-mediated. Then, successive jumps occur with higher probability in the reverse direction and the contribution of the double sum is negative. Equation (4.27) also shows that one may deﬁne the correlation factor as the ratio of the diﬀusivity of tagged atoms, D∗ , and a hypothetical diﬀusivity arising from uncorrelated jump sequencies, Drandom , via D∗ . (4.28) f ≡ Drandom Correlation eﬀects are important in solid-state diﬀusion of crystalline materials, whenever diﬀusion is mediated by a diﬀusion vehicle (see Table 4.2). Examples for diﬀusion vehicles are vacancies, vacancy pairs, self-interstitials, etc. An equivalent statement is to say, there must be at least three identiﬁable ‘species’ involved in the diﬀusion process. For example, during tracer diﬀusion via vacancies in pure crystals, the three participating ‘species’ are vacancies, host atoms, and tracer atoms. Interstitial diﬀusion in a dilute interstitial solution is uncorrelated, because no diﬀusion vehicle is involved. Let us consider once more diﬀusion in a cubic Bravais lattice. When correlation occurs, Eq. (4.24) must be replaced by D∗ = 1 2 f d ZΓ = f a2 Γ. 6 (4.29) We will return to the correlation factor in Chap. 7, after having introduced point defects in Chap. 5 and the major mechanisms of diﬀusion in crystals in Chap. 6. Table 4.2. Correlation eﬀects of diﬀusion for crystalline materials f =1 f <1 Markovian jump sequence No diﬀusion vehicle involved: direct interstitial diﬀusion Non-Markovian jump sequence Diﬀusion vehicle involved: vacancy, divacancy, self-interstitial, . . . mechanisms 64 4 Random Walk Theory and Atomic Jump Process 4.2 Atomic Jump Process In preceding sections, we have considered many atomic jumps on a lattice. Equally important are the rates at which jumps occur. Let us take a closer look to the atomic jump process illustrated in Fig. 4.3. An atom moves into a neighbouring site, which could be either a neighbouring vacancy or an interstitial site. Clearly, the jumping atom has to squeeze between intervening lattice atoms – a process which requires energy. The energy necessary to promote the jump is usually large with respect to the thermal energy kB T . At ﬁnite temperatures, atoms in a crystal oscillate around their equilibrium positions. Usually, these oscillations are not violent enough to overcome the barrier and the atom will turn back to its initial position. Occasionally, large displacements result in a successful jump of the diﬀusing atom. These activation events are infrequent relative to the frequencies of the lattice vibrations, which are characterised by the Debye frequency. Typical values of the Debye frequency lie between 1012 and 1013 s−1 . Once an atom has moved as the result of an activation event, the energy ﬂows away from this atom relatively quickly. The atom becomes deactivated and waits on the average for many lattice vibrations before it jumps again. Thermally activated motion of atoms in a crystal occurs in a series of discrete jumps from one lattice site (or interstitial site) to the next. The theory of the rate at which atoms move from one site to a neighbouring one was proposed by Wert [9] and has been reﬁned by Vineyard [10]. Vineyard’s approach is based upon the canonical ensemble of statistical mechanics for the distribution of atomic positions and velocities. The jump process can be viewed as occurring in an energy landscape characterised by Fig. 4.3. Atomic jump process in a crystalline solid: the black atom moves from an initial conﬁguration (left) to a ﬁnal conﬁguration (right) pushing through a saddlepoint conﬁguration (middle) 4.2 Atomic Jump Process 65 the diﬀerence in Gibbs free energy GM between the saddle-point barrier and the equilibrium position (Fig. 4.3). GM is denoted as the Gibbs free energy of migration (superscript M ) of the atom. It can be separated according to GM = H M − T S M , (4.30) where H M denotes the enthalpy of migration and S M the entropy of migration. Using statistical thermodynamics, Vineyard [10] has shown that the jump rate ω (number of jumps per unit time to a particular neighbouring site) can be written as M S GM HM ω = ν 0 exp − exp − = ν 0 exp , (4.31) kB T kB kB T where ν 0 is called the attempt frequency. It is of the order of the Debye frequency. Its rigorous meaning is as follows: ν 0 is the vibration frequency around the equilibrium site but in the direction of the reaction path. The entropy of migration corresponds to the change in lattice vibrations associated with the displacement of the jumping atom from its equilibrium to the saddle point conﬁguration. Vineyard’s treatment also provides an expression for the migration entropy: ⎡ ⎤ 3N −1 3N −1 hνj hνj ⎦. (4.32) ln − ln S M = kB ⎣ kB T A kB T SP j=0 j=0 The νj are the 3N − 1 normal mode frequencies for vibrations around the equilibrium site A while νj are the frequencies of the system when it is constrained to move within the hyperface which passes through the saddle point (SP) perpendicular to the jump direction. The theory of the rates at which atoms move from one lattice site to another covers one of the fundamental aspects of diﬀusion. For most practical purposes, a few general conclusions are important: 1. Atomic migration in a solid is the result of a sequence of localised jumps from one site to another. 2. Atomic jumps in crystals usually occur from one site to a nearestneighbour site. Molecular dynamic simulations mostly conﬁrm this view. Multiple hops are rare, although their occurrence is indicated in some model substances. Jumps with magnitudes larger than the nearestneighbour distance are more common on surfaces or in grain boundaries (see Chap. 32). 3. The jump rate ω has an Arrhenius-type dependence on temperature as indicated in Eq. (4.31). 4. The concept of an atomic jump developed above applies to all the diﬀusion mechanisms discussed in Chap. 6. Of course, the values of GM , H M , 66 4 Random Walk Theory and Atomic Jump Process and S M depend on the diﬀusion mechanism and on the material under consideration: For interstitial diﬀusion, the quantities GM , H M , and S M pertain to the saddle point separating two interstitial positions. For a dilute interstitial solution, virtually every interstitial solute is surrounded by empty interstitial sites. Thus, for an atom executing a jump the probability to ﬁnd an empty site next to its starting position is practically unity. For vacancy-mediated diﬀusion, GM , H M , and S M pertain to the saddlepoint separating the vacant lattice site and the jumping atom on its equilibrium site. 5. There are cases – mostly motion of hydrogen in solids at low temperatures – where a classical treatment is not adequate [16]. However, the end result of diﬀerent theories including quantum eﬀects is still a movement in a series of distinct jumps from one site to another [17]. For atoms heavier than hydrogen and its isotopes, quantum eﬀects can usually be disregarded. For more detailed discussions of the problem of thermally activated jumps the reader may consult the textbook of Flynn [3] and the reviews by Franklin [11], Bennett [12], Jacucci [13], Hänngi et al. [15] Pontikis [14] and Flynn and Stoneham [17]. Molecular dynamic calculations become increasingly important and are used to check and to supplement analytical theories. Atomistic computer simulations of diﬀusion processes have been reviewed, e.g., by Mishin [18]. Nowadays, simulation methods present a powerful approach to gain fundamental insight into atomic jump processes in materials. The capabilities of simulations have drastically improved due to the development of new simulation methods reinforced by increased computer power. Reliable potentials of atomic interaction have been developed, which allow a quantitative description of point defect properties. Simulation of atomic jump processes have been applied to ordered intermetallic compounds, surface diﬀusion, grainboundary diﬀusion, and other systems. The challenge is to understand, describe, and calculate diﬀusion coeﬃcients in a particular metal, alloy, or compound. In some – but not all – of the rare cases, when this has been done, the agreement with experiments is encouraging. References 1. A. Einstein, Annalen der Physik 17, 549 (1905) 2. M. van Smoluchowski, Annalen der Physik 21, 756 (1906) 3. M. van Smoluchowski, Z. Phys. 13, 1069 (1912); and Physikalische Zeitschrift 17, 557 (1916) 4. C.P. Flynn, Point Defects and Diﬀusion, Clarendon Press, Oxford, 1972 5. P. Hänggi, P. Talkner, M. Borkovec: Rev. Mod. Phys. 62, 251 (1990) References 67 6. J.R. Manning, Diﬀusion Kinetics for Atoms in Crystals, D. van Norstrand Comp., Inc., 1968 7. J. Bardeen, C. Herring, in: Atom Movements, A.S.M. Cleveland, 1951, p. 87 8. J. Bardeen, C. Herring, in: Imperfections in Nearly Perfect Solids, W. Shockley (Ed.), Wiley, New York, 1952, p. 262 9. C. Wert, Phys. Rev. 79, 601 (1950) 10. G. Vineyard, J. Phys. Chem. Sol. 3, 121 (1957) 11. W.M. Franklin, in: Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.), Academic Press, Inc., 1975, p.1 12. C.H. Bennett, in: Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.), Academic Press, Inc., 1975, p.74 13. G. Jacucci, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, Inc., 1984, p.431 14. V. Pontikis, Thermally Activated Processes, in: Diﬀusion in Materials, A.L. Laskar, J.L. Bocqut, G. Brebec, C. Monty (Eds.), Kluwer Academic Publishers, Dordrecht, The Netherlands, 1990, p.37 15. P. Hänngi, P. Talkner, M. Borkovec, Rev. Mod. Phys. 62, 251 (1990) 16. J. Völkl, G. Alefeld, in: Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.), Academic Press, Inc., 1975 17. C.P. Flynn, A.M. Stoneham, Phys. Rev. B1, 3966 (1970) 18. Y. Mishin, Atomistic Computer Simulation of Diﬀusion, in: Diﬀusion Processes in Advanced Technological Materials, D. Gupta (Ed.), William Andrews, Inc., 2005 5 Point Defects in Crystals The Russian scientist Frenkel in 1926 [1] was the ﬁrst author to introduce the concept of point defects (see Chap. 1). He suggested that thermal agitation causes transitions of atoms from their normal lattice sites into interstitial positions leaving behind lattice vacancies. This type of disorder is nowadays denoted as Frenkel disorder and contained already the concepts of vacancies and self-interstitials. Already in the early 1930s Wagner and Schottky [2] treated a fairly general case of disorder in binary AB compounds considering the occurrence of vacancies, self-interstitials, and of antisite defects on both sublattices. Point defects are important for diﬀusion processes in crystalline solids. This statement mainly derives from two features: one is the ability of point defects to move through the crystal and to act as ‘vehicles for diﬀusion’ of atoms; another is their presence at thermal equilibrium. Of particular interest in this chapter are diﬀusion-relevant point defects, i.e. defects which are present in appreciable thermal concentrations. In a defect-free crystal, mass and charge density have the periodicity of the lattice. The creation of a point defect disturbs this periodicity. In metals, the conduction electrons lead to an eﬃcient electronic screening of defects. As a consequence, point defects in metals appear uncharged. In ionic crystals, the formation of a point defect, e.g., a vacancy in one sublattice disturbs the charge neutrality. Charge-preserving defect populations in ionic crystals include Frenkel disorder and Schottky disorder, both of which guarantee global charge neutrality. Frenkel disorder implies the formation of equal numbers of vacancies and self-interstitials in one sublattice. Schottky disorder consists of corresponding numbers of vacancies in the sublattices of cations and anions. For example, in AB compounds like NaCl composed of cations and anions with equal charges opposite in sign the number of vacancies in both sublattices must be equal to preserve charge neutrality. Point defects in semiconductors introduce electronic energy levels within the band gap and thus can occur in neutral or ionised states, depending on the position of the Fermi level. In what follows, we consider at ﬁrst point defects in metals and then proceed to ionic crystals and semiconductors. Nowadays, there is an enormous body of knowledge about point defects from both theoretical and experimental investigations. In this chapter, we 70 5 Point Defects in Crystals provide a brief survey of some features relevant for diﬀusion. For more comprehensive accounts of the ﬁeld of point defects in crystals, we refer to the textbooks of Flynn [3], Stoneham [4], Agullo-Lopez, Catlow and Townsend [5], to a review on defect in metals by Wollenberger [6], and to several conference proceedings [9–12]. For a compilation of data on point defects properties in metals, we refer to a volume edited by Ullmeier [13]. For semiconductors, data have been assembled by Schulz [14], Stolwijk [15], Stolwijk and Bracht [16], and Bracht and Stolwijk [17]. Properties of point defects in ionic crystals can be found in reviews by Barr and Lidiard [7] and Fuller [8] and in the chapters of Benière [18] and Erdely [19] of a data collection edited by Beke. 5.1 Pure Metals 5.1.1 Vacancies Statistical thermodynamics is a convenient tool to deduce the concentration of lattice vacancies at thermal equilibrium. Let us consider an elemental crystal, which consists of N atoms (Fig. 5.1). We restrict the discussion to metallic elements or to noble gas solids in which the vacancies are in a single electronic state and we suppose (in this subsection) that the concentration is so low that interactions among them can be neglected. At a ﬁnite temperature, n1V vacant lattice sites (monovacancies, index 1V ) are formed. The total number of lattice sites then is N = N + n1V . (5.1) The thermodynamic reason for the occurrence of vacancies is that the Gibbs free energy of the crystal is lowered. The Gibbs free energy G(p, T ) of the Fig. 5.1. Vacancies in an elemental crystal 5.1 Pure Metals 71 crystal at temperature T and pressure p is composed of the Gibbs function of the perfect crystal, G0 (p, T ), plus the change in the Gibbs function on forming the actual crystal, ∆G: G(p, T ) = G0 (p, T ) + ∆G , (5.2) ∆G = n1V GF 1V − T Sconf . (5.3) where GF 1V In Eq. (5.3) the quantity represents the Gibbs free energy of formation of an isolated vacancy. It corresponds to the work required to create a vacancy by removing an atom from a particular, but arbitrary, lattice site and incorporating it at a surface site (‘Halbkristalllage’). Not only surfaces also grain boundaries and dislocations can act as sources or sinks for vacancies. If a vacancy is created, the crystal lattice relaxes around the vacant site and the vibrations of the crystal are also altered. The Gibbs free energy can be decomposed according to F F GF 1V = H1V − T S1V (5.4) F F into the formation enthalpy H1V and the formation entropy S1V . The last term on the right-hand side of Eq. (5.3) contains the conﬁgurational entropy Sconf , which is the thermodynamic reason for the presence of vacancies. In the absence of interactions, all distinct conﬁgurations of n1V vacancies on N lattice sites have the same energy. The conﬁgurational entropy can be expressed through the equation of Boltzmann Sconf = kB ln W1V , (5.5) where W1V is the number of distinguishable ways of distributing n1V monovacancies among the N lattice sites. Combinatoric rules tell us that W1V = N ! . n1V !N ! (5.6) The numbers appearing in Eq. (5.6) are very large. Then, the formula of Stirling, ln x! ≈ x ln x, approximates the factorial terms and we get ln W1V ≈ (N + n1V ) ln(N + n1V ) − n1V ln n1V − N ln N . (5.7) Thermodynamic equilibrium is imposed on a system at given temperature and pressure by minimising its Gibbs free energy. In the present case, this means ∆G ⇒ Min . (5.8) The equilibrium number of monovacancies, neq 1V , is obtained, when the Gibbs free energy in Eq. (5.3) is minimised with respect to n1V , subject to the constraint that the number of atoms, N , is ﬁxed. Inserting Eqs. (5.5) and (5.7) 72 5 Point Defects in Crystals into Eq. (5.3), we get from the necessary condition for thermal equilibrium, ∂∆G/∂n1V = 0: F F − T S1V + kB T ln H1V neq 1V =0 N + neq 1V (5.9) By deﬁnition we introduce the site fraction of monovacancies 1 via: C1V ≡ n1V . N + n1V (5.10) This quantity also represents the probability to ﬁnd a vacancy on an arbitrary, eq ≡ neq but particular lattice site. In thermal equilibrium we have C1V 1V /(N + eq n1V ). Solving Eq. (5.9) for the equilibrium site fraction yields F S1V GF HF eq C1V = exp − 1V = exp exp − 1V . (5.11) kB T kB kB T This equation shows that the concentration of thermal vacancies increases via a Boltzmann factor with increasing temperature. The temperature depeneq is primarily due to the formation enthalpy term in Eq. (5.11). dence of C1V We note that the vacancy formation enthalpy is also given by F H1V = −kB eq ∂ ln C1V . ∂(1/T ) (5.12) This quantity is often determined in experiments which measure relative concentrations. Such measurements are less tedious than measurements of absolute concentrations (see below). In the analysis of experiments, it is frequently assumed that formation enthalpy and entropy are independent of temperature; this is often, though not always, justiﬁed. 5.1.2 Divacancies Divacancies (2V) are point defects that form in a crystal as the simplest complex of monovacanies (1V). This is a consequence of the mass-action equilibrium for the reaction 1V + 1V 2V . (5.13) The probability that a given lattice site in a monoatomic crystal is vacant equals the site fraction of monovacancies. Let us suppose that a divacancy consists of two monovacancies on nearest-neighbour lattice sites. For noninteracting monovacancies, the probability of forming a divacancy is proportional to (C1V )2 . For a coordination lattice (coordination number Z) the 1 Concentrations as number densities are given by C1V N , when N is taken as the number density of atoms. 5.1 Pure Metals 73 eq equilibrium fraction of divacancies C2V that form simply for statistical reaeq 2 Z sons is given by 2 (C1V ) . However, there is also a gain in enthalpy (and entropy) when two vacancies are located on adjacent lattice sites. Fewer bonds to neighbouring atoms must be broken, when a second vacancy is formed next to an already existing one. Interactions between two vacancies are accounted for by a Gibbs free energy of binding GB 2V , which according to B B GB 2V = H2V − T S2V (5.14) B B and an entropy S2V of interaction. can be decomposed into an enthalpy H2V B For G2V > 0 the interaction is attractive and binding occurs, whereas for GB 2V < 0 it is repulsive. Combining Eq. (5.14) with the mass-action law for Eq. (5.13) yields B G2V Z eq eq 2 ) . (5.15) C2V = exp (C1V 2 kB T Equation (5.15) shows that at thermal equilibrium the divacancy concentration rises faster with increasing temperature than the monovacancy concentration (see Fig. 5.2). With increasing GB 2V the equilibrium concentration of divacancies increases as well. The total equilibrium concentration of vacant lattice sites, CVeq , in the presence of mono- and divacancies (neglecting higher agglomerates) is then eq eq + 2C2V . CVeq = C1V (5.16) For a typical monovacancy site fraction in metals of 10−4 near the melting temperature (see below), the fraction of non-interacting divacancies would be Fig. 5.2. Arrhenius diagram of equilibrium concentrations of mono- and divacancies in metals (schematic) 74 5 Point Defects in Crystals × 10−8 . Typical interaction energies of a few 0.1 eV increase the divacancy concentration by factors of 10 to 100. Therefore, the divacancy concentration at thermal equilibrium is less or much less than that of monovacancies. Nevertheless, divacancies in close-packed metals can contribute to some extent to the diﬀusive transport (see Chaps. 6 and 17). The major reason is that divacancies are more eﬀective diﬀusion vehicles than monovacancies, since their mobility can be considerably higher than that of monovacancies [20]. The contribution of higher agglomerates than divacancies is usually negligible. Z 2 5.1.3 Determination of Vacancy Properties The classical method for an absolute measurement of the total vacancy concentration, Eq. (5.16), is diﬀerential dilatometry (DD). The idea is to compare macroscopic and microscopic volume changes as functions of temperature. To understand this method, we consider a monoatomic crystal with N atoms. We denote its macroscopic volume in the defect-free state as V0 and the volume per lattice site as Ω0 . A defect-free state can usually be realised by cooling slowly to low enough temperatures. As long as the thermal concentration of vacant lattice sites is negligible, we have V0 = N Ω0 . With increasing temperature the volume increases due to thermal expansion and due the formation of new lattice sites. Then, the macroscopic volume and the volume per lattice site take the values V (T ) and Ω(T ), respectively. The change in the macroscopic volume is given by ∆V ≡ V (T ) − V0 = (N + n)Ω(T ) − N Ω0 = N ∆Ω + nΩ(T ) , (5.17) where ∆Ω ≡ Ω(T ) − Ω0 . n is the number of new lattice sites. Equation (5.17) can be rearranged to give ∆V ∆Ω n Ω(T ) = + . V0 Ω0 N Ω0 (5.18) This equation reﬂects the two major physical reasons of the macroscopic volume change: ∆Ω/Ω0 is the thermal expansion of the unit cell and the second term on the right-hand side stands for the additional lattice sites. If nV vacant sites and nI self-interstitials are created, we have n = nV −nI new lattice sites. The diﬀerence between the total self-interstitial fraction, CIeq , and the total site fraction of vacant lattice sites, CVeq , is given by CVeq − CIeq = ∆V ∆Ω − . V0 Ω0 (5.19) In Eq. (5.19) the eﬀect of thermal expansion in the ratio Ω(T )/Ω0 and higher order terms in n/N have been omitted. 5.1 Pure Metals 75 In metals, self-interstitials need not to be considered as equilibrium defects (see below). We then have CVeq = ∆V ∆Ω − . V0 Ω0 For cubic crystals Eq. (5.20) can be rewritten as ∆l ∆a eq − CV = 3 , l0 a0 (5.20) (5.21) where ∆l/l0 is the relative length change of the sample and ∆a/a0 the lattice parameter change. In deriving Eq. (5.21) from Eq. (5.20) quadratic and cubic terms in ∆l/l0 and ∆a/a0 have been neglected, because already the linear terms are of the order of a few percent or less. Equation (5.21) shows what needs to be done in DD-experiments. The macroscopic length change and the expansion of the unit cell must be measured simultaneously2 . The expansion of the unit cell can be measured in very precise X-ray or neutron diﬀraction studies. As already mentioned, near the melting temperature of metallic elements CVeq does not exceed 10−3 to 10−4 (see Table 5.1) and is much smaller at lower temperatures. Thus, precise measurements of CVeq are very ambitious. Both length and lattice parameter changes must be recorded with the extremely high accuracy of about 10−6 . Diﬀerential dilatometry experiments were introduced by Feder and Nowick [21] and Simmons and Balluffi [22, 23] around 1960 and later Fig. 5.3. Length and lattice parameter change versus temperature for Au according to Simmons and Balluffi [23] 2 For uniaxial crystals measurements in two independent directions are necessary. 76 5 Point Defects in Crystals used by several authors. As an example, Fig. 5.3 shows measured length and lattice parameter expansion versus temperature for gold in the interval 900 to 1060 ◦ C according to [23]. ∆l/l is larger than ∆a/a at high temperatures due to the presence of lattice vacancies. This technique demonstrated that the dominant, thermally created defects in metals are vacancies and the exponential dependence of the vacancy concentration on temperature was also conﬁrmed. The great advantage of DD experiments is that the total vacancy content as a function of temperature can be obtained. If monovacancies are the dominant species, both the formation enthalpy and the formation entropy can be deduced. When the divacancy contribution is not negligible, additional divacancy properties can be obtained [20]. The basic weakness of DD experiments is the unsuﬃcient accuracy in the range below about CVeq ≈ 10−5 , where the divacancy contribution would be low enough to permit a direct measurement of the formation properties of monovacancies. This is illustrated for aluminium in Fig. 5.4 according to Seeger [24]. The thermal expansion measurements of various groups [25–27] cover, with a reasonable accuracy only the concentration range between 10−3 to 10−5 . Fortunately, there are additional techniques such as positron annihilation spectroscopy (see below) that supplement DD measurements very well. An analysis of DD measurements together with these additional data yields the line in Fig. 5.4, which corresponds to a monovacancy contribution with F F =0.66 eV and S1V = 0.8kB . Near the melting temperature the fraction H1V of vacant sites associated as divacancies is about 50%. Fig. 5.4. Equilibrium concentration of vacant lattice sites in Al determined by DD measurements according to [24]. DD data: + [25], • [27], × [26]. The concentration range covered by positron lifetime measurements is also indicated 5.1 Pure Metals 77 Despite the elegance of DD experiments, much information on defect properties is obtained from other ingenious experiments, which are less direct, some of which are mentioned in what follows: Formation enthalpies can be deduced from experiments which do not involve a determination of the absolute vacancy concentration. A frequently used method is rapid quenching (RQ) from high temperatures, TQ . The quenched-in vacancy population can be studied in measurements of the residual resistivity. For example, thin metal wires or foils can be rapidly quenched. Their residual resistivities before and after quenching, ρ0 and ρQ , can be measured accurately at liquid He temperature. The residual resistivity after quenching increases due to the additional scattering processes of conduction electrons at ‘frozen in’ vacancies. The increase of the residual resistivity, ∆ρ, is proportional to the frozen-in vacancy concentration CVeq (TQ ): ∆ρ ≡ ρQ − ρ0 = ρV CVeq (TQ ) . (5.22) ρV is a defect-related quantity, which accounts for the resistivity increase per vacant site. In a successful quenching experiment, the equilibrium vacancy population is completely ‘frozen in’. Vacancy losses to sinks such as dislocations, grain-boundaries, or surfaces can cause problems in quenching experiments. Since the residual resistivity increase per vacant site is usually unknown, only formation enthalpies can be determined from RQ experiments when ∆ρ is measured for various quenching temperatures. Formation entropies S F are not accessible from such experiments. Only the product ρV exp(S F /kB ) can be deduced. Transmission electron microscopy (TEM) of quenched-in vacancy agglomerates is a further possibility to determine vacancy concentrations. Upon annealing vacancies become mobile and can form agglomerates. If the agglomerates are large enough they can be studied by TEM. In addition to vacancy losses during the quenching process, the invisibility of very small agglomerates can cause problems. A very valuable tool for the determination of vacancy formation enthalpies is positron annihilation spectroscopy (PAS). The positron is the antiparticle of the electron. It is, for example, formed during the β + decay of radioisotopes. High-energy positrons injected in metals are thermalised within picoseconds. A thermalised positron diﬀuses through the lattice and ends its life by annihilation with an electron. Usually, two γ-quanta are emitted according to e+ + e → 2γ . The energy of each γ-quantum is about 511 keV. The positron lifetime depends on the total electron density. Vacancies can trap positrons. Because of the missing core electrons at the vacant lattice site, the local electron density is signiﬁcantly reduced. Therefore, the lifetime of trapped positrons is enhanced as compared to that of positrons annihilating in the perfect lattice. 78 5 Point Defects in Crystals Positrons in a vacancy-containing crystal end their life either by annihilation as free positrons or as trapped positrons. The lifetimes of both fates are diﬀerent and the trapping probability increases with the vacancy concentration. Lifetime measurements are possible using, e.g., 22 Na as a positron source. This nuclide emits γ-quanta simultaneously at the ‘birth’ of the positron. The positrons ‘death’ is accompanied by the emission of two 511 keV annihilation quanta. The interpretation of positron lifetime measurements is provided by a trapping model: a thermalised positron diﬀusing through a metal is trapped by a vacancy with the trapping rate σ. The positron lifetime in the trapped state, τt , exceeds that in the free state, τf , when the positron is located in an interstitial position of the perfect crystal. If untrapping is disregarded two distinct lifetimes of the positron are predicted by this model: (i) The trapped positron is annihilated with a lifetime τt . (ii) A positron diﬀusing through the crystal may end its existence as a ‘free’ particle either by the annihilation rate 1/τf or by being trapped by a vacancy with the trapping rate σC1V , where σ is the trapping cross section. This results in a lifetime given by τf /(1 + τf σC1V ). If one assumes that initially all positrons are free, one gets for their mean lifetime: τ̄ = τf 1 + τt σC1V . 1 + τf σC1V (5.23) Figure 5.5 shows as an example measurements of the mean lifetime of positrons in aluminium as a function of temperature [28]. The mean lifetime increases from about 160 ps near room temperature and reaches a high Fig. 5.5. Mean lifetime of positrons in Al according to Schaefer et al. [28] 5.1 Pure Metals 79 eq is given in site fractions Table 5.1. Monovacancy properties of some metals. C1V Metal F H1V /eV F S1V /kB eq C1V at Tm Method(s) Al Cu Au Ag Pb Pt Ni Mo W 0.66 1.17 0.94 1.09 0.49 1.49 1.7 3.0 4.0 0.6 1.5 1.1 – 0.7 1.3 – – 2.3 9.4 × 10−4 2 × 10−4 7.2 × 10−4 1.7 × 10−4 1.7 × 10−4 – – – 1 × 10−4 DD + PAS DD + PAS DD DD DD RQ PAS PAS RQ + TEM temperature value of about 250 ps. From a ﬁt of Eq. (5.23) to the data the product σC1V can be deduced. If the trapping cross section is known the vacancy concentration is accessible. If σ is constant, the vacancy formation enthalpy can be deduced from the temperature variation of σC1V . At high temperature, i.e. for high vacancy concentrations, all positrons are annihilated from the trapped state. Under such conditions the method is no longer sensitive to a further increase of the vacancy concentration and the curve τ̄ versus T saturates. The maximum sensitivity of positron annihilation measurements occurs for vacant site fractions between about 10−4 and 10−6 (see Fig. 5.4). A unique feature of PAS is that it is sensitive to vacancy-type defects, but insensitive to interstitials. Measurements of the mean positron lifetime is one technique of PAS. Other techniques, not described here, are measurements of the line-shape of the annihilation line and lifetime spectroscopy. Review articles on PAS applications for studies of vacancy properties in metals are provided by Seeger [24], Doyama and Hasiguti [29], Hautojärvi [30], and Schaefer et al. [31]. Vacancy properties of metals are listed in Table 5.1 according to [6]. 5.1.4 Self-Interstitials Using statistical thermodynamics and a reasoning analogous to that for vacancies, the equilibrium fraction of self-interstitials in pure metals can be written as F SI GF HIF eq I exp − = gI exp . (5.24) CI = gI exp − kB T kB kB T F F GF I denotes the Gibbs free energy of formation, SI and HI the corresponding formation entropy and enthalpy, and gI a geometric factor. For example, in fcc metals gI = 3 accounts for the fact that self-interstitials occur in the 80 5 Point Defects in Crystals Fig. 5.6. Dumbbell conﬁguration of a self-interstitial in an fcc lattice so-called dumbbell conﬁguration illustrated in Fig. 5.6, which implies three possible 100 orientations for a self-interstitial with its midpoint at the same lattice site. In close-packed metals the formation enthalpy of a self-interstitial is considerably higher than that of a vacancy (see, e.g., Table 6 in the review of Wollenberger [6] and the data compilation of Ullmaier [13]): F . HIF ≈ (2 to 3) × H1V (5.25) Therefore, at thermal equilibrium CVeq >>> CIeq , (5.26) i.e. the overwhelming thermal defect population is of the vacancy type. Self-interstitials are produced athermally (together with an equal number of vacancies), when a metal is subject to irradiation with energetic particles. Thus, self-interstitials play a signiﬁcant rôle in the radiation damage and in radiation-enhanced diﬀusion [9, 11]. In some ionic crystals, Frenkel disorder is established at thermal equilibrium (see Sect. 5.3 and Chap. 26). For example, in silver halides Frenkel pairs are formed, which consist of self-interstitials and vacancies in the cation sublattice of the crystal. Semiconductors are less densely packed than metals and oﬀer more space in their interstitial sites. Therefore, the formation enthalpies of selfinterstitials and vacancies are not much diﬀerent. Depending on the semiconductor, both types of defects can play a rôle under thermal equilibrium conditions. This is the case for example for Si, whereas in Ge vacancies dominate self-diﬀusion (see Sect. 5.5 and Chap. 23). 5.2 Substitutional Binary Alloys A knowledge of the vacancy population in substitutional alloys is of considerable interest as well. Let us consider ﬁrst dilute substituional alloys and then make a few remarks about the more complex case of concentrated alloys. 5.2 Substitutional Binary Alloys 81 5.2.1 Vacancies in Dilute Alloys A binary alloy of atoms B and A is denoted as dilute if the number of B atoms is not more than a few percent of the number of A atoms. Then, B is called the solute and A the solvent (or matrix ). Depending on the solute/solvent combination interstitial and substitutional alloys are to be distinguished. Small solutes such as H, C, and N usually form interstitial alloys whereas solute atoms, which are similar in size to the solvent atoms form substitutional alloys. In a substitutional alloy, A and B atoms and vacancies occupy sites of the same lattice. However, we have to distinguish whether a vacancy is formed on a site, where it is surrounded by A atoms only, or whether the vacancy is formed on a neighbouring site of a solute atom. In the latter case, we talk about a solute-vacancy pair (see Fig. 5.7). For simplicity let us suppose that the solute-vacancy interaction is restricted to nearest-neighbour sites, which is often reasonable for metals. The Gibbs free energy of vacancy formation in the undisturbed solvent, GF 1V (A), is diﬀerent from the Gibbs free energy of vacancy formation next to a B atom, GF 1V (B): F GF 1V (A) = G1V (B) . (5.27) F For GF 1V (A) > G1V (B) the vacancy-solute interaction is attractive, whereas F for G1V (A) < GF 1V (B) it is repulsive. According to Lomer [32] the total vacancy fraction in a dilute alloy, CVeq (CB ), is given by GF GF eq 1V (A) 1V (B) CV (CB ) = (1 − ZCB ) exp − + ZCB exp − , (5.28) kB T kB T Fig. 5.7. Vacancies in a dilute substitutional alloy 82 5 Point Defects in Crystals where Z denotes the coordination number and CB the solute fraction. Equation (5.28) is a good approximation for CB < 0.01. We recognise that the ﬁrst term corresponds to the concentration of unpaired vacancies. It is reduced by a factor (1 − ZCB ) relative to that of the pure solvent. The second term is the fraction of solute-vacancy pairs. If we introduce the Gibbs free energy of interaction between solute and vacancy F GB ≡ GF 1V (A) − G1V (B) , Eq. (5.28) can be written as B G GF (A) CVeq = exp − 1V 1 − ZCB + ZCB exp kB T kB T (5.29) (5.30) and is sometimes called the Lomer equation. The ﬁrst factor in Eq. (5.30) is the equilibrium vacancy fraction in the pure solvent. The factor in square brackets is larger/smaller than unity if GB is positive/negative. For binding/repulsion between solute and vacancy the total vacancy content in the alloy is higher/lower than in the pure solvent. In dilute alloys of the noble metals with solute elements lying to their right in the periodic table, GB is typically about 0.2 eV [13]. We note that the quantity B G eq p = C1V exp (5.31) kB T denotes the probability that a vacancy occupies a nearest-neighbour site of eq a solute, when C1V is measured in site fractions. The expressions (5.30) and (5.31) are of interest for diﬀusion in dilute alloys, which will be considered in Chap. 19. 5.2.2 Vacancies in Concentrated Alloys The Lomer equation is valid for very dilute alloys (CB ≤ 0.01). In its derivation only associates between one solute atom and vacancy are considered. In concentrated alloys, associates between several solute atoms and vacancy and interactions between atoms of an associate become also important. To the author’s knowledge robust theoretical models for the vacancy population in concentrated substitutional alloys are not available. An approximation was treated by Dorn and Mitchell [33]. These authors attribute to each associate consisting of i solute atoms and one vacancy the (same) Gibbs free energy Gi . By standard thermodynamic reasoning, they derive the following expression for the total vacancy concentration in a concentrated alloy CVeq (CB ) = Z Z Gi Z−i i CB exp − CA , i kB T i=0 (5.32) 5.3 Ionic Compounds 83 where Z denotes the coordination number. The term for i = 0 represents the vacancy content of free vacancies in the solvent. A limitation to the terms for i = 0 and i = 1 reproduces Lomer’s equation using G0 ≡ GF 1V (A) (B). In the derivation of Eq. (5.32) a random distribution of and Gi = GF 1V atoms has been assumed. For a generalisation of Eq. (5.32) by including an interaction between atoms we refer to [34]. 5.3 Ionic Compounds Let us consider thermal defects in ionic crystals such as the alkali halides, silver chloride and bromide. These materials crystallise in sodium chloride and cesium chloride structures. They are strongly stoichiometric and have wide band gaps so that thermally produced electrons or holes can be ignored. These materials are the classical ion conductors, whose conductivity arises from the presence and mobility of vacancies and/or self-interstitials. The classical ionic conductors are to be distinguished from the fast ion conductors. As a general rule, fast ion conductors are materials with an open structure, which allows for the rapid motion of relatively small ions. A famous example is silver iodide, for which fast ionic conduction was reported as early as 1914 [35]. It displays a ﬁrst order phase transition between a fast ionconducting phase (α-AgI) above 147 ◦ C and a normal conducting phase at lower temperatures. α-AgI has a body-centered cubic sublattice of practically immobile I− ions. Each unit cell displays 42 interstitial sites (6 octahedral, 12 tetrahedral, 24 trigonal) over which the two Ag+ ions per unit cell are distributed (see Fig. 27.2). Since there are many more sites than Ag+ ions, the latter can migrate easily. Other examples are β-alumina, some compounds with ﬂuorite structure such as some halides such as CaF2 and PbF2 and oxides like doped ZrO2 , which are ﬂuorine or oxygen ion conductors at elevated temperatures. These materials require a diﬀerent approach, because in the sublattice of one ionic species the fraction of vacant sites is high (see Chap. 27). To be speciﬁc, we consider here classical ionic crystals with CA stoichiometry (C=cation, A=anion). They are composed of anions and cations which carry equal charges opposite in sign. Let us further assume that all cation sites are equivalent and all anion sites likewise; in other words, there are two ﬁlled sublattices. The defect population that can develop in such a crystal has the structural constraint that the number of C atoms and of A atoms must be equal. This can also be viewed as a condition of electroneutrality by assigning ionic charges to the atoms C and A.3 Then, only charge-preserving 3 Electroneutrality must be fulﬁlled in the volume of ionic crystal. In the vicinity of charged dislocations, grain boundaries or surfaces, unbalanced point defect populations can develop. In compounds with additional electronic defects the requirements of structure and of electroneutrality are diﬀerent (see, e.g., the textbook of Maier [36]). 84 5 Point Defects in Crystals defect populations can develop. In addition, the formation of antisite defects need not to be considered due to the high Coulomb energy of an ion placed in the ‘wrong’ sublattice. In what follows, we consider two important cases of disorder in CA ionic crystals. For a more general treatment the reader is referred, e.g., to the textbook of Allnatt and Lidiard [37]. 5.3.1 Frenkel Disorder Let us suppose that vacancies (VC ) and self-interstitials (IC ) in the C sublattice are formed from cations on cation sites (CC ) according to the quasichemical reaction (5.33) CC VC + IC . This type of disorder is called Frenkel disorder (Fig. 5.8), as it was ﬁrst suggested by the Russian scientist Frenkel [1]. Pairs of vacancies and selfinterstitials are denoted as Frenkel pairs. According to the law of mass action we may write SFP HFP eq eq CVC CIC = exp (5.34) exp − ≡ KFP . kB kB T Here CVeqC and CIeqC denote equilibrium site fractions of vacancies and selfinterstitials in the C sublattice. KFP is called the Frenkel product. The formation enthalpy HFP and entropy SFP for (non-interacting) Frenkel pairs can be split according to HFP = HVFC + HIFC and SFP = SVFC + SIFC (5.35) into sums of formation enthalpies, HVFC + HIFC , and formation entropies, SVFC + SIFC , of vacancies and self-interstitials. Charge neutrality of undoped Fig. 5.8. Frenkel disorder in the cation sublattice of a CA ionic crystal 5.3 Ionic Compounds 85 crystals requires that the numbers of vacancies and self-interstitials are equal, i.e. CVeqC = CIeqC . Then we get CVeqC = CIeqC = exp SFP 2kB HFP exp − . 2kB T (5.36) Frenkel disorder occurs in the silver sublattices of silver chloride and bromide [38, 39]. Frenkel-pair formation properties of these silver halides are listed in Table 5.2. 5.3.2 Schottky Disorder Let us consider once more a binary ionic CA compound composed of cations on the C sublattice, CC , and anions on the A sublattice, AA . The constraint of electroneutrality is fulﬁlled, when vacancies in both sublattices, VC and VA , are formed according to the reaction CC + AA + 2 new lattice sites VC + VA . (5.37) in equal numbers (Fig. 5.9). Applying the law of mass-action to this reaction, we get for thermal equilibrium SSP HSP eq eq (5.38) CVC CVA = exp exp − ≡ KSP , kB kB T where CVC and CVA denote site fractions of cation and anion vacancies, respectively. HSP and SSP denote enthalpy and entropy for the formation of a Schottky pair (cation vacancy plus anion vacancy). Fig. 5.9. Schottky disorder in an CA ionic crystal 86 5 Point Defects in Crystals Table 5.2. Formation enthalpies of Schottky- and Frenkel pairs of ionic crystals Ionic compound (HSP or HFP )/eV (SSP or SFP )/kB Type of disorder NaCl KCl NaI KBr LiF LiCl LiBr LiI 2.44 2.54 2.00 2.53 2.68 2.12 1.80 1.34 9.8 7.6 7.6 10.3 Schottky Schottky Schottky Schottky Schottky Schottky Schottky Schottky AgCl AgBr 1.45–1.55 1.13–1.28 5.4–12.2 6.6–12.2 Frenkel Frenkel This type of disorder is called Schottky disorder and KSP is denoted as the Schottky product. Charge neutrality in an undoped crystal requires equal concentrations of cation and anion vacancies: SSP HSP CVeqC = CVeqA = exp exp − . (5.39) 2kB 2kB T For non-interacting Schottky pairs, the enthalpy and entropy of pair formation according to HSP = HVFC + HVFA and SSP = SVFC + SVFA (5.40) can be expressed in terms of the formation enthalpies, HVFC and HVFA , and entropies, SVFC and SVFA , of cation and anion vacancies. Experience shows that Schottky disorder dominates the defect population in most alkali halides and in many oxides. Schottky-pair formation properties are listed in Table 5.2. Crystals doped with aliovalent ions are considered in detail in Chap. 26. In doped crystals, the Schottky product is still valid. 5.4 Intermetallics Intermetallics are a fascinating group of materials, which attract attention from the viewpoints of fundamentals as well as applications [40, 41]. Binary intermetallics are composed of two metals or of a metal and a semimetal. Their crystal structures are diﬀerent from those of the elements. This definition includes both intermetallic phases and ordered alloys. Intermetallics form a numerous and manifold group of materials and comprise a greater variety of crystal structures than metallic elements [48]. They crystallise in structures with ordered atomic distributions in which atoms are preferentially surrounded by unlike atoms. Some frequent structures are illustrated 5.4 Intermetallics 87 in Chap. 20. Some intermetallics are ordered up to their melting temperature, others undergo order-disorder transitions in which an almost random arrangement of atoms is favoured at high temperatures. Such transitions occur, for example, between the β and β phases of the Cu–Zn system or in Fe–Co. There are intermetallic phases with wide phase ﬁelds and others which exist as stoichiometric compounds. Examples for both types can even be found in the same binary alloy system. For example, the Laves phase in the Co-Nb system (approximate composition Co2 Nb) exists over a composition range of about 5 at. %, whereas the phase Co7 Nb2 is a line compound. Some intermetallics occur for certain stoichiometric compositions only. Others are observed for oﬀ-stoichiometric compositions. Some phases compensate oﬀ-stoichiometry by vacancies, others by antisite atoms. Thermal defect populations in intermetallics can be rather complex and we shall conﬁne ourselves to a few remarks. Intermetallic compounds are physically very diﬀerent from the ionic compounds considered in the previous section. Combination of various types of disorder are conceivable: vacancies and/or antisite defects on both sublattices can form in some intermetallics. As self-interstitials play no rôle in thermal equilibrium for pure metals, it is reasonable to assume that this holds true also for intermetallics. To be speciﬁc, let us suppose a formula Ax By for the stoichiometric compound and that there is a single A sublattice and a single B sublattice. This is, for example, the case in intermetallics with the B2 and L12 structure (see Fig. 20.1). The basic structural elements of disorder are listed in Table 5.3. A ﬁrst theoretical model for thermal disorder in a binary AB intermetallic with two sublattices was treated in the pioneering work of Wagner and Schottky [2]. Some of the more recent work on defect properties of intermetallic compounds has been reviewed by Chang and Neumann [42] and Bakker [43]. In some binary AB intermetallics so-called triple defect disorder occurs. These intermetallics form VA defects on the A sublattice on the B rich side and AB antisites on the B sublattice on the A rich side of the stoichiometric composition. This is, for example, the case for some intermetallics with B2 structure where A = Ni, Co, Pd . . . and B = Al, In, . . . Some other intermetallics also with B2 structure such as CuZn, AgCd, . . . can maintain high concentrations of vacancies on both sublattices. Table 5.3. Elements of disorder in intermetallic compounds AA BB VA VB BA AB = = = = = = A atom on A sublattice B atom on B sublattice vacancy on A sublattice vacancy on B sublattice B antisite on A sublattice A antisite on B sublattice 88 5 Point Defects in Crystals Triple defects (2VA + AB ), bound triple defects (VA AB VA ) and vacancy pairs (VA VB ) have been suggested by Stolwijk et al. [46]. They can form according to the reactions VA + VB 2VA + AB triple defect VA AB VA bound triple defect and VA + VB VA VB . vacancy pair (5.41) Very likely bound agglomerates are important in intermetallics for thermal disorder and diﬀusion in addition to single vacancies. In this context it is interesting to note that neither triple defects nor vacancy pairs disturb the stoichiometry of the compound. The physical understanding of the defect structure of intermetallics is still less complete compared with metallic elements. However, considerable progress has been achieved. Diﬀerential dilatometry (DD) and positron annihilation studies (PAS) performed on intermetallics of the Fe-Al, Ni-Al and Fe-Si systems have demonstrated that the total content of vacancy-type defects can be one to two orders of magnitude higher than in pure metals [44, 45]. The defect content depends strongly on composition and its temperature dependence can show deviations from simple Arrhenius behaviour. According to Schaefer et al. [44] and Hehenkamp [45] typical defect concentrations in these compounds near the solidus temperature can be as high as several percent. 5.5 Semiconductors Covalent crystals such as diamond, Si, and Ge are more diﬀerent from the defect point of view as one might expect from their chemical classiﬁcation as group IV elements. Diamond is an electrical insulator, whose vacancies are mobile at high temperatures only. Si is a semiconductor which supports vacancies and self-interstitials as intrinsic defects. By contrast, Ge is a semiconductor in which vacancies as intrinsic defects predominate like in the metallic group IV elements Sn and Pb. Because Si and Ge crystallise in the diamond structure with coordination number 4, the packing density is considerably lower than in metals. This holds true also for compound semiconductors. Most compound semiconductors formed by group III and group V elements like GaAs crystallise in the zinc blende structure, which is closely related to the diamond structure. Semiconductor crystals oﬀer more space for self-interstitials than close-packed metal structures. Formation enthalpies of vacancies and self-interstitials in semiconductors are comparable. In Si, both self-interstitials and vacancies are present in thermal equilibrium and are important for self- and solute diffusion. In Ge, vacancies dominate in thermal equilibrium and appear to be the only diﬀusion-relevant defects (see Chap. 23 and [47, 50]). 5.5 Semiconductors 89 Semiconductors have in common that the thermal defect concentrations are orders of magnitude lower than in metals or ionic crystals. This is a consequence of the covalent bonding of semiconductors. Defect formation energies in semiconductors are higher than in metals with comparable melting temperatures. Neither thermal expansion measurements nor positron annihilation studies have suﬃcient accuracy to detect the very low thermal defect concentrations. Point defects in semiconductors can be neutral and can occur in various electronic states. This is because point defects introduce energy levels into the band gap of a semiconductor. Whether a defect is neutral or ionised depends on the position of the Fermi level as illustrated schematically in Fig. 5.10. A wealth of detailed information about the electronic states of point defects in these materials has been obtained by a variety of spectroscopic means and has been compiled, e.g., by Schulz [14]. Let us consider vacancies and self-interstitials X ∈ (V, I) and suppose that both occur in various ionised states, which we denote by j ∈ (0, 1±, 2±, . . . ). The total concentration of the defect X at thermal equilibrium can be written as eq eq eq eq eq eq = CX (5.42) CX 0 + CX 1+ + CX 1− + CX 2+ + CX 2− + . . . . Whereas the equilibrium concentration of uncharged defects depends only on temperature (and pressure), the concentration of charged defects is additionally inﬂuenced by the position of the Fermi energy and hence by the doping level. If the Fermi level changes due to, e.g., background doping the concentration of charged defects will change as well. The densities of electrons, n, and of holes, p, are tied to the intrinsic carrier density, ni , via the law of mass action relation np = n2i . (5.43) Fig. 5.10. Electronic structure of semiconductors, with a defect with double acceptor character (left) and donor character (right) 90 5 Point Defects in Crystals Then, Eq. (5.42) can be rewritten as n 2 ni n i eq eq eq eq eq + CX CX = CX + CX 0 + CX 1+ (ni ) 1− (ni ) 2+ (ni ) n ni n 2 n eq + CX (n ) + ... , 2− i ni (5.44) eq where CX j± (ni ) denotes the equilibrium concentration under intrinsic conditions for defect X with charge state j±. From Eq. (5.44) it is obvious that n-doping will enhance (decrease) the equilibrium concentration of negatively (positively) charged defects. Correspondingly, p-doping will enhance (decrease) the equilibrium concentration positively (negatively) charged defects. Furthermore, the ratio n/ni varies with temperature because the intrinsic carrier density according to Eg c v ni = Neﬀ Neﬀ exp − (5.45) 2kB T c v and Neﬀ denote the eﬀective denincreases with increasing temperature. Neﬀ sities of states in the conduction and valence band, respectively. The values of ni at diﬀerent temperatures are determined mainly by the band gap energy Eg of the semiconductor. For a given background doping concentration the ratio n/ni will be large at low temperatures and approaches unity at high temperatures. Then, the semiconductor reaches intrinsic conditions. The band gap energy is characteristic for a given semiconductor. It increases in the sequence Ge (0.67 eV), Si (1.14 eV), GaAs (1.43 eV). The intrinsic carrier density at a ﬁxed temperature is highest for Ge and lowest for GaAs. Thus, doping eﬀects on the concentration of charged defects are most prominent for GaAs and less pronounced for the elemental semiconductors. Let us consider as an example a defect X which introduces a single X 1− and a double X 2− acceptor state with energy levels EX 1− and EX 2− above the valence band edge. Then, the ratios between charged and uncharged defect populations in thermal equilibrium are given by eq CX Ef − EX 1− 1 1− = exp , eq CX gX 1− kB T 0 eq CX 2Ef − EX 2− − EX 1− 1 2− = exp , (5.46) eq CX gX 2− kB T 0 where Ef denotes the position of the Fermi level. The degeneracy factors gX 1− and gX 2− take into account the spin degeneracy of the defect and the degeneracy of the valence band. The total concentration of point defects in thermal equilibrium for the present example is given by eq eq CX CX 1− 2− eq eq = CX + 1 + . (5.47) CX eq eq 0 CX C X0 0 References 91 Diﬀusion in semiconductors is aﬀected by doping since defects in various charge states can act as diﬀusion-vehicles. Diﬀusion experiments are usually carried out at temperatures between the melting temperature Tm and about 0.6 Tm . As the intrinsic carrier density increases with increasing temperature, doping eﬀects in diﬀusion are more pronounced at the low temperature end of this interval. One can distinguish two types of doping eﬀects: – – Background doping is due to a homogeneous distribution of donor or acceptor atoms, that are introduced during the process of crystal growing. Background doping is relevant for diﬀusion experiments, when at the diffusion temperature the carrier density exceeds the intrinsic density. Self-doping is relevant for diﬀusion experiments of donor or acceptor elements. If the in-diﬀused dopant concentration exceeds either the intrinsic carrier density or the available background doping, complex diﬀusion proﬁles can arise. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. J.I. Frenkel, Z. Physik 35, 652 (1926) C. Wagner, W. Schottky, Z. Physik. Chem. B 11, 163 (1931) C.P. Flynn, Point Defects and Diﬀusion, Clarendon Press, Oxford, 1972 A.M. Stoneham, Theory of Defects in Solids, Clarendon Press, Oxford, 1975 F. Agullo-Lopez, C.R.A. Catlow, P. Townsend, Point Defects in Materials, Academic Press, London, 1988 H.J. Wollenberger, Point Defects, in: Physical Metallurgy, R.W. Cahn, P. Haasen (Eds.), North-Holland Publishing Company, 1983, p. 1139 L.W. Barr, A.B. Lidiard, Defects in Ionic Crystals, in: Physical Chemistry – An Advanced Treatise, Academic Press, New York, Vol. X, 1970 R.G. Fuller, Ionic Conductivity including Self-diﬀusion, in: Point Defects in Solids, J. M. Crawford Jr., L.M. Slifkin (Eds.), Plenum Press, 1972, p. 103 A. Seeger, D. Schumacher, W. Schilling, J. Diehl (Eds.), Vacancies and Interstitials in Metals, North-Holland Publishing Company, Amsterdam, 1970 N.L. Peterson, R.W. Siegel (Eds.), Properties of Atomic Defects in Metals, North-Holland Publishing Company, Amsterdam, 1978 C. Abromeit, H. Wollenberger (Eds.), Vacancies and Interstitials in Metals and Alloys; also: Materials Science Forum 15–18, 1987 O. Kanert, J.-M. Spaeth (Eds.), Defects in Insulating Materials, World Scientiﬁc Publ. Comp., Ltd., Singapore, 1993 H. Ullmaier (Vol. Ed.), Atomic Defects in Metals, Landolt-Börnstein, New Series, Group III: Crystal and Solid State Physics, Vol. 25, Springer-Verlag, Berlin and Heidelberg, 1991 M. Schulz, Landolt-Börnstein, New Series, Group III: Crystal and Solid State Physics, Vol. 22: Semiconductors, Subvolume B: Impurities and Defects in Group IV Elements and III-V Compounds, M. Schulz (Ed.), Springer-Verlag, 1989 92 5 Point Defects in Crystals 15. N.A. Stolwijk, Landolt-Börnstein, New Series, Group III: Crystal and Solid State Physics, Vol. 22: Semiconductors, Subvolume B: Impurities and Defects in Group IV Elements and III-V Compounds, M. Schulz (Ed.), Springer-Verlag, 1989, p. 439 16. N.A. Stolwijk, H. Bracht, Landolt-Börnstein, New Series, Group III: Condensed Matter, Vol. 41: Semiconductors, Subvolume A2: Impurities and Defects in Group IV Elements, IV-IV and III-V Compounds, M. Schulz (Ed.), SpringerVerlag, 2002, p. 382 17. H. Bracht, N.A. Stolwijk, Landolt-Börnstein, New Series, Group III: Condensed Matter, Vol. 41: Semiconductors, Subvolume A2: Impurities and Defects in Group IV Elements, IV-IV and III-V Compounds, M. Schulz (Ed.), SpringerVerlag, 2002, p. 77 18. F. Benière, Diﬀusion in Alkali and Alkaline Earth Halides, in: Diﬀusion in Semiconductors and Non-metallic Solids, Landolt-Börnstein, New Series, Group III: Condensed Matter, Vol. 33, Subvolume B1, D.L. Beke (Vol.Ed.). Springer-Verlag, 1999 19. G. Erdelyi, Diﬀusion in Miscelaneous Ionic Materials, in: Diﬀusion in Semiconductors and Non-metallic Solids, Landolt-Börnstein, New Series, Group III: Condensed Matter, Vol. 33, Subvolume B1, D.L. Beke (Vol.Ed.). SpringerVerlag, 1999 20. A. Seeger, H. Mehrer, Analysis of Self-diﬀusion and Equilibrium Measurements, in: Vacancies and Interstitials in Metals, A. Seeger, D. Schumacher, J. Diehl and W. Schilling (Eds.), North-Holland Publishing Company, Amsterdam, 1970, p. 1 21. R. Feder, A.S. Nowick, Phys. Rev. 109, 1959 (1958) 22. R.O. Simmons, R.W. Balluﬃ, Phys. Rev. 117, 52 (1960); Phys. Rev. 119, 600 (1960); Phys. Rev. 129, 1533 (1963); Phys. Rev. 125, 862 (1962) 23. R.O. Simmons, R.W. Balluﬃ, Phys. Rev. 125, 862 (1962) 24. A. Seeger, J. Phys. F. Metal Phys. 3, 248 1973) 25. R.O. Simmons, R.W. Balluﬃ, Phys. Rev. 117, 52 (1960) 26. G. Bianchi, D. Mallejac, Ch. Janot, G. Champier, Compt. Rend. Acad. Science, Paris 263 1404 (1966) 27. B. von Guerard, H. Peisl, R. Sizmann, Appl. Phys. 3, 37 (1973) 28. H.-E. Schaefer, R. Gugelmeier, M. Schmolz, A. Seeger, J. Materials Science Forum 15–18, 111 (1987) 29. M. Doyama, R.R. Hasiguti, Cryst. Lattice Defects 4, 139 (1973) 30. P. Hautojärvi, Materials Science Forum 15–18, 81 (1987) 31. H.-E. Schaefer, W. Stuck, F. Banhart, W. Bauer, Materials Science Forum 15–18, 117 (1987) 32. W.M. Lomer, Vacancies and other Point Defects in Metals and Alloys, Institute of Metals, 1958 33. J. E. Dorn, J.B. Mitchell, Acta Metall. 14, 71 (1966) 34. G. Berces, I. Kovacs, Philos. Mag. 15, 883 (1983) 35. C. Tubandt, E. Lorenz, Z. Phys. Chem. 87, 513, 543 (1914) 36. J. Maier, Physical Chemistry of Ionic Solids – Ions and Electrons in Solids, John Wiley & Sons, Ltd, 2004 37. A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 38. R. Friauf, Phys. Rev. 105, 843 (1957) References 93 39. R. Friauf, J. Appl. Phys. Supp. 33, 494 (1962) 40. J.H. Westbrook, Structural Intermetallics, R. Dariola, J.J. Lewendowski, C.T. Liu, P.L. Martin, D.B. Miracle, M.V. Nathal (Eds.), Warrendale, PA, TMS, 1993 41. G. Sauthoﬀ, Intermetallics, VCH Verlagsgesellschaft, Weinheim, 1995 42. Y.A. Chang, J.P. Neumann, Progr. Solid State Chem. 14, 221 (1982) 43. H. Bakker, Tracer Diﬀusion in Concentrated Alloys, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, Inc., 1984, p. 189 44. H.-E. Schaefer, K. Badura-Gergen, Defect and Diﬀusion Forum 143–147, 193 (1997) 45. Th. Hehenkamp, J. Phys. Chem. Solids 55, 907 (1994) 46. N.A. Stolwijk, M. van Gend, H. Bakker, Philos. Mag. A 42, 783 (1980) 47. W. Frank, U. Gösele, H. Mehrer, A. Seeger, Diﬀusion in Silicon and Germanium, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, Inc., 1984, p. 64 48. K. Girgis, Structure of Intermetallic Compounds, in: Physical Metallurgy, R.W. Cahn, P. Haasen (Eds.), North-Holland Physics Publishing, 1983, p. 219 49. M. Schulz (Vol.-Ed.), Impurities and Defects in Group IV Elements, IV-IV and III-V Compounds, Landolt-Börnstein, Group III, Vol. 41, Subvolume A2, Springer-Verlag, 2002 50. T.Y. Tan, U. Gösele, Diﬀusion in Semiconductors, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 6 Diﬀusion Mechanisms Any theory of atom diﬀusion in solids should start with a discussion of diffusion mechanisms. We must answer the question: ‘How does this particular atom move from here to there?’ In crystalline solids, it is possible to describe diﬀusion mechanisms in simple terms. The crystal lattice restricts the positions and the migration paths of atoms and allows a simple description of each speciﬁc atom displacements. This contrasts with a gas, where random distribution and displacements of atoms are assumed, and with liquids and amorphous solids, which are neither really random nor really ordered. In this chapter, we catalogue some basic atomic mechanisms which give rise to diﬀusion in solids. As discussed in Chap. 4, the hopping motion of atoms is an universal feature of diﬀusion processes in solids. Furthermore, we have seen that the diﬀusivity is determined by jump rates and jump distances. The detailed features of the atomic jump process depend on various factors such as crystal structure, size and chemical nature of the diﬀusing atom, and whether diﬀusion is mediated by defects or not. In some cases atomic jump processes are completely random, in others correlation between subsequent jumps is involved. Correlation eﬀects are important whenever the atomic jump probabilities depend on the direction of the previous atom jump. If jumps are mediated by atomic defects, correlation eﬀects always arise. The present chapter thus provides also the basis for a discussion of correlation eﬀects in solid-state diﬀusion in Chap. 7. 6.1 Interstitial Mechanism Solute atoms which are considerably smaller than the solvent atoms are incorporated on interstitial sites of the host lattice thus forming an interstitial solid solution. Interstitial sites are deﬁned by the geometry of the host lattice. In fcc and bcc lattices, for example, interstitial solutes occupy octahedral and/or tetrahedral interstitial sites (Fig. 6.1). An interstitial solute can diﬀuse by jumping from one interstitial site to one of its neighbouring sites as shown in Fig. 6.2. Then the solute is said to diﬀuse by an interstitial mechanism. To look at this process more closely, we consider the atomic movements during a jump. The interstitial starts from an equilibrium position, reaches the saddle-point conﬁguration where maximum lattice straining occurs, and 96 6 Diﬀusion Mechanisms Fig. 6.1. Octahedral and tetrahedral interstitial sites in the bcc (left) and fcc (right) lattice Fig. 6.2. Direct interstitial mechanism of diﬀusion settles again on an adjacent interstitial site. In the saddle-point conﬁguration neighbouring matrix atoms must move aside to let the solute atom through. When the jump is completed, no permanent displacment of the matrix atoms remains. Conceptually, this is the simplest diﬀusion mechanism. It is also denoted as the direct interstitial mechanism. It has to be distinguished from the interstitialcy mechanism discussed below, which is also denoted as the indirect interstitial mechanism. We note that no defect is necessary to mediate direct interstitial jumps, no defect concentration term enters the diﬀusivity and no defect formation energy contributes to the activation energy of diﬀusion. Since the interstitial atom does not need to ‘wait’ for a defect to perform a jump, diﬀusion coeﬃcients for atoms migrating by the direct interstitial mechanism tend to be fairly high. This mechanism is relevant for diﬀusion of small foreign atoms such as H, C, N, and O in metals and other materials. Small atoms ﬁt in interstitial sites and in jumping do not greatly displace the solvent atoms from their normal lattice sites. 6.2 Collective Mechanisms 97 Fig. 6.3. Direct exchange and ring diﬀusion mechanism 6.2 Collective Mechanisms Solute atoms similar in size to the host atoms usually form substitutional solid solutions. The diﬀusion of substitutional solutes and of solvent atoms themselves requires a mechanism diﬀerent from interstitial diﬀusion. In the 1930s it was suggested that self- and substitutional solute diﬀusion in metals occurs by a direct exchange of neighbouring atoms (Fig. 6.3), in which two atoms move simultaneously. In a close-packed lattice this mechanism requires large distortions to squeeze the atoms through. This entails a high activation barrier and makes this process energetically unfavourable. Theoretical calculations of the activation enthalpy for self-diﬀusion of Cu performed by Huntington et al. in the 1940s [1, 2], which were conﬁrmed later by more sophisticated theoretical approaches, led to the conclusion that direct exchange at least in close-packed structures was not a likely mechanism. The so-called ring mechanism of diﬀusion was proposed for crystalline solids by the American metallurgist Jeffries [3] already in the 1920s and advocated by Zener in the 1950s [4]. The ring mechanism corresponds to a rotation of 3 (or more) atoms as a group by one atom distance. The required lattice distortions are not as great as in a direct exchange. Ring versions of atomic exchanges have lower activation energies but increase the amount of collective atomic motion, which makes this more complex mechanism unlikely for most crystalline substances. Direct exchange and ring mechanisms have in common that lattice defects are not involved. The observation of the so-called Kirkendall eﬀect in alloys by Kirkendall and coworkers [5, 6] during the 1940s had an important impact on the ﬁeld (see also Chaps. 1 and 10). The Kirkendall eﬀect showed that the self-diﬀusivities of atoms in a substitutional binary alloy diffuse at diﬀerent rates. Neither the direct exchange nor the ring mechanism can explain this observation. As a consequence, the ideas of direct or ring exchanges were abandoned in the diﬀusion literature. It became evident that 98 6 Diﬀusion Mechanisms Fig. 6.4. Atom chain motion in an amorphous Ni-Zr alloy according to molecular dynamics simulations of Teichler [13] vacancies are responsible for self-diﬀusion and diﬀusion of substitutional solutes in metals in practically all cases. Further historical details can be found in [7]. There is, however, some renewed interest in non-defect mechanisms of diﬀusion in connection with the enhanced diﬀusivity near phase transitions [8, 9]. For substitutionally dissolved boron in Cu there appears to be evidence from β-NMR experiments for a non-defect mechanism of diﬀusion [10]. Collective mechanisms, which involve the simultaneous motion of several atoms appear to be quite common in amorphous systems. Molecular dynamic simulations by Teichler [13] as well as diﬀusion and isotope experiments on amorphous metallic alloys reviewed by Faupel et al. [11, 12] suggest that collective mechanism operate in undercooled metallic melts and in metallic glasses. Such collective mechanisms involve the simultaneous motion of several atoms in a chain-like or caterpillar-like fashion. An example observed in molecular dynamic simulations of an amorphous Ni-Zr alloy is illustrated in Fig. 6.4. It appears that collective jump processes play also a rôle for the motion of alkali ions in ion-conducting oxide glasses [14]. Finally, we note that interstitialcy mechanisms involving self-interstitials are collective in the sense that more than one atom is displaced permanently during a jump event (see Sect. 6.5). 6.3 Vacancy Mechanism As knowledge about solids expanded, vacancies have been accepted as the most important form of thermally induced atomic defects in metals and ionic crystals (see Chaps. 5, 17, 26). It has also been recognised that the dominant 6.3 Vacancy Mechanism 99 Fig. 6.5. Monovacancy mechanism of diﬀusion mechanism for the diﬀusion of matrix atoms and of substitutional solutes in metals is the vacancy mechanism. An atom is said to diﬀuse by this mechanism, when it jumps into a neighbouring vacancy (Fig. 6.5). The constriction, which inhibits motion of an adjacent atom into a vacancy in a close-packed lattice is small, as compared to the constriction against the direct or ring exchange. Each atom moves through the crystal by making a series of exchanges with vacancies, which from time to time are in its vicinity. In thermal equilibrium, the site fraction of vacancies in a monoatomic eq , is given by Eq. (5.11), which we repeat for convenience: crystal, C1V F S1V GF HF eq C1V = exp − 1V = exp exp − 1V . (6.1) kB T kB kB T F F GF 1V is the Gibbs free energy of vacancy formation. S1V and H1V denote the formation entropy and the formation enthalpy of a monovacancy, respectively. Typical values for the site fraction of vacancies near the melting temperature of metallic elements lie between 10−4 and 10−3 . From Eqs. (4.31) and (6.1) we get for the exchange jump rate Γ of a vacancy-mediated jump of a matrix atom to a particular neighbouring site F M F M S1V + S1V + H1V H1V eq 0 Γ = ω1V C1V = ν exp exp − . (6.2) kB kB T ω1V denotes the exchange rate between an atom and a vacancy and ν 0 the M M pertinent attempt frequency. H1V and S1V denote the migration enthalpy and eutropy of vacancy migration, respectively. The total jump rate of a matrix atom in a coordination lattice with Z neighbours is given by Γtot = ZΓ . The vacancy mechanism is the dominating mechanism of self-diﬀusion in metals and substitutional alloys. It is also relevant for diﬀusion in a number of ionic crystals, ceramic materials, and in germanium (see Parts III, IV and V of this book). In substitutional alloys, attractive or repulsive interactions between solute atoms and vacancies play an important rôle. These interactions modify the 100 6 Diﬀusion Mechanisms probability, p, to ﬁnd a vacancy on a nearest-neighbour site of a solute atom. For a dilute alloy this probability is given by the Lomer equation (see Chap. 5) B G eq p = C1V exp , (6.3) kB T where GB denotes the Gibbs free energy of binding of a solute-vacancy pair. B The quantity GF 1V − G is the Gibbs free energy for the formation of a vacancy on a nearest-neighbour site of the solute. For an attractive interaction (GB > 0) p is enhanced and for a repulsive interaction (GB < 0) p is reduced compared to the vacancy concentration in the pure solvent. For the total jump rate of a solute atom in a coordination lattice we get B G eq exp Γ2 = Zω2 p = Zω2 C1V , (6.4) kB T where ω2 is the rate of solute-vacancy exchange and Z the coordination number. 6.4 Divacancy Mechanism When a binding energy exists, which tends to create agglomerates of vacancies (divacancies, trivacancies, . . . ), diﬀusion can also occur via aggregates of vacancies. This is illustrated for divacancies in Fig. 6.6. At thermal equilibrium divacancies are formed from monovacancies and their concentration is given by Eq. (5.15). The concentrations of mono- and divacancies at equilibrium increase with temperature. However, the concentration of divacancies rises more rapidly and may become signiﬁcant at high temperatures (see Fig. 5.2). Furthermore, divacancies in fcc metals are more mobile than monovacancies. Thus, self-diﬀusion of fcc metals usually has some divacancy contribution in addition to the monovacancy mechanism. The latter is the dominating mechanism at temperatures below 2/3 of the melting temperature [15, 16]. Because of divacancay binding and the lower defect symmetry, diﬀusion via divacancies obeys slightly modiﬁed equations as compared to monovacancies (see Chap. 17). Otherwise, the two mechanisms are very similar. Diﬀusion by bound trivacancies is usually negligible. 6.5 Interstitialcy Mechanism When an interstitial atom is nearly equal in size to the lattice atoms (or the lattice atoms on a given sublattice in a compound), diﬀusion may occur by the interstitialcy mechanism also called the indirect interstitial mechanism. Let us illustrate this for self-diﬀusion. Self-interstitials – extra atoms located 6.5 Interstitialcy Mechanism 101 Fig. 6.6. Divacancy mechanism of diﬀusion in a close-packed structure Fig. 6.7. Interstitialcy mechanism of diﬀusion (colinear jumps) between lattice sites – act as diﬀusion vehicles. Figure 6.7 illustrates a colinear interstitialcy mechanism. Both atoms move in unison – a self-interstitial replaces an atom on a substitutional site, which then itself replaces a neighbouring lattice atom. Non-colinear versions of the interstitialcy mechanism, whereby the atoms move at an angle to one another also can occur (see Fig. 26.8). As already mentioned, interstitialcy mechanisms are collective mechanisms because at least two atoms move simultaneously. The equilibrium conﬁguration of a self-interstitial in metals is that of a ‘dumbbell’ (see Chap. 5). The dumbbell axis is 100 for fcc metals and 110 for bcc metals. In a dumbbell conﬁguration two atoms occupy a lattice site symmetrically, and each atom is displaced by an equal amount from the regular lattice position. The motion of a dumbbell interstitial is a fairly collective process, because the simultaneous displacements of three atoms is necessary to move the center of the dumbbell from one lattice site to the next one. In metals the interstitialcy mechanism is negligible for thermal diﬀusion. This is because self-interstitials have fairly high formation enthalpies compared to vacancies (see Chap. 5). The interstitialcy mechanism is, however, important for radiation-induced diﬀusion. When a crystal is irradiated with energetic particles (protons, neutrons, electrons, . . . ), lattice atoms are knocked out from their lattice positions. The knocked-out atom leaves behind 102 6 Diﬀusion Mechanisms a vacancy. The atom itself is deposited in the lattice as a self-interstitial. In this way, pairs of vacancies and self-interstitials (Frenkel pairs) are formed athermally. When these defects become mobile, they both mediate diﬀusion and give rise to radiation-induced diﬀusion, which is a topic of radiation damage in crystals. Self-interstitials are responsible for thermal diﬀusion in the silver sublattice of some silver halides (see Chap. 26). In silicon, the base material of microelectronic devices, both the interstitialcy and the vacancy mechanism contribute to self-diﬀusion. Self-interstitials also play a prominent rôle in the diﬀusion of some solute atoms including important doping elements in silicon (see Chap. 23). This is not surprising, since the diamond lattice of silicon is a relatively open structure with suﬃcient space for interstitial species. 6.6 Interstitial-substitutional Exchange Mechanisms Some solute atoms (B) may be dissolved on both interstitial (Bi ) and substitutional sites (Bs ) of a solvent crystal (A). Then, they can diﬀuse via one of the interstitial-substitutional exchange mechanisms ilustrated in Fig. 6.8. Such foreign atoms are denoted as ‘hybrid solutes’. The diﬀusivity of hybrid solutes in the interstitial conﬁguration, Di , is usually much higher than their diﬀusivity in the substitutional conﬁguration, Ds . In contrast, the solubility in the interstitial state, Cieq , is often less or much less than the solubility in the substitutional state, Cseq : Di Ds but Cseq > Cieq . (6.5) Under such conditions the incorporation of B atoms can occur by fast diffusion of Bi and subsequent change-over to Bs . Two types of interstitialsubstitutional exchange mechanisms can be distinguished (see also Chap. 25): When the change-over involves vacancies (V ) according to Bi + V Bs , (6.6) the mechanism is denoted as the dissociative mechanism. This mechanism was proposed by Frank and Turnbull [17] for the rapid diﬀusion of copper in germanium. Later on, diﬀusion of some foreign metallic elements in polyvalent metals such as lead, titanium, and zirconium was also attributed to this mechanism. When the change-over involves self-interstitials (Ai ) according to Bi Bs + Ai , (6.7) the mechanism is denoted as the kick-out mechanism. This mechanism was proposed by Gösele et al. [18, 19] for the fast diﬀusion of Au in silicon. Nowadays, the diﬀusion of several hybrid foreign elements, e.g., Au, Pt, Zn in silicon and Zn in gallium arsenide is also attributed to this mechanism. References 103 Fig. 6.8. Interstitial-substitutional exchange mechanisms of foreign atom diﬀusion. Top: dissociative mechanism. Bottom: kick-out mechanism For a description of diﬀusion processes which involve interstitial-substitutional exchange reactions, Fick’s equations must be supplemented by reaction terms which account for either Eq. (6.6) and/or Eq. (6.7). Because several species (interstitial solute, substitutional solute, defects) are involved, sets of coupled (non-linear) diﬀusion-reaction equations are necessary to describe the diﬀusion process. Solutions of these equations – apart from a few (but interesting) special cases – can only be obtained by numerical methods [20, 21]. These solutions also explain unusual (non-Fickian) shapes of concentrationdistance proﬁles observed for hybrid diﬀusers. Details are discussed in Part IV of this book. References 1. 2. 3. 4. 5. 6. 7. H.B. Huntington, F. Seitz, Phys. Rev. 61, 315 (1942) H.B. Huntington, Phys. Rev. 61, 325 (1942) Z. Jeﬀries, Trans. AIME 70, 303 (1924) C. Zener, Acta. Cryst. 3, 346 (1950) E.O. Kirkendall, Trans. AIME 147, 104 (1942) A.D. Smigelskas, E.O. Kirkendall, Trans. AIME 171, 130 (1947) C. Tuijn, Defect and Diﬀusion Forum 143–147, 11 (1997) 104 6 Diﬀusion Mechanisms 8. A. Seeger, in: Ultra-High-Purity Metals, K. Abiko, K. Hirokawa, S. Takaki (Eds.), The Japan Institute of Metals, Sendai, 1995, p. 27 9. A. Seeger, Defect and Diﬀusion Forum 143–147, 21 (1997) 10. B. Ittermann, H. Ackermann, H.-J. Stöckmann, K.-H. Ergezinger, M. Heemeier, F. Kroll, F. Mai, K. Marbach, D. Peters, G. Sulzer, Phys. Rev. Letters 77, 4784 (1996) 11. F. Faupel, W. Frank, H.-P. Macht, H. Mehrer, V. Naundorf, K. Rätzke, H. Schober, S. Sharma, H. Teichler, Diﬀusion in Metallic Glasses and Supercooled Melts, Rev. of Mod. Phys. 75, 237 (2003) 12. F. Faupel, K. Rätzke, Diﬀusion in Metallic Glasses and Supercooled Melts, Ch. 6 in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds:), Springer-Verlag, 2005 13. H. Teichler, J. Non-cryst. Solids 293, 339 (2001) 14. S. Voss, S. Divinski, A.W. Imre, H. Mehrer, J.N. Mundy, Solid State Ionics 176, 1383 (2005); and: A.W. Imre, S. Voss, H. Staesche, M.D. Ingram, K. Funke, H. Mehrer, J. Phys. Chem. B, 111, 5301–5307 (2007) 15. N.L. Peterson, J. Nucl. Materials 69–70, 3 (1978) 16. H. Mehrer, J. Nucl. Materials 69–70, 38 (1978) 17. F.C. Frank, D. Turnbull, Phys. Rev. 104, 617 (1956) 18. U. Gösele, W. Frank, A. Seeger, Appl. Phys. 23, 361 (1980) 19. T.Y. Tan, U. Gösele, Diﬀusion in Semiconductors, Ch. 4 in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 20. W. Frank, U. Gösele, H. Mehrer and A. Seeger, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, 1984, p. 63 21. H. Bracht, N.A. Stolwijk, H. Mehrer, Phys. Rev. B. 52, 16542 (1995) 7 Correlation in Solid-State Diﬀusion It was not until 1951 that Bardeen1 and Herring [1, 2] drew attention to the fact that, for the vacancy mechanism, correlation exists between the directions of consecutive jumps of tracer atoms. After this pioneering work, it was soon appreciated that correlation eﬀects play an important rôle for any solid-state diﬀusion process, when point defects act as diﬀusion vehicles. In pure random-walk diﬀusion, it is assumed that the jump probabilities of atoms do not depend on the direction of the preceding jump. In real crystals, however, the jump probabilities often depend on the directions of preceding jumps. Then, successive atom jumps are correlated. Instead of following a pure random walk, each atom follows a correlated walk. This is why we have introduced the correlation factor in Chap. 4. We shall see below that the correlation factor depends on both the diﬀusion mechanism and on the lattice geometry. Clearly, an understanding of correlation eﬀects is an important topic of solid-state diﬀusion. Considerable eﬀort has gone into the study of the eﬀects of correlation on diﬀusion rates in solids. In addition, methods have been devised whereby its contribution to the diﬀusivity can be isolated and measured experimentally (see Chap. 9). Detailed calculations of correlation factors can be quite involved. It is the aim of the present chapter to explain the physical nature of correlation for some basic diﬀusion mechanisms and to describe the added understanding of diﬀusion that was achieved as a result of it. More comprehensive treatments of correlation eﬀects can be found in the literature cited at the end of this chapter. We remind the reader to the result of Chap. 4 for the correlation factor given in Eq. (4.27). For convenience, we repeat its derivation in a slightly more detailed way. Our starting point was the Einstein-Smoluchowski relation R2 = 6D∗ t , 1 (7.1) John Bardeen is one of the few scientist who received the Nobel prize twice. Schockley, Bardeen and Brattain were awarded for their studies of semiconductors and the development of the transistor in 1956. Bardeen, Cooper, and Schriefer received the 1972 price for the so-called BCS theory of superconductivity. 106 7 Correlation in Solid-State Diﬀusion which relates the diﬀusion coeﬃcient of tagged atoms, D∗ , and the mean square displacement of an ensemble of N such atoms, where R2 = N 1 2 Rk . N (7.2) k=1 It is assumed that the net displacement of the k th atom is the result of a large number of nk jumps with microscopic jump vectors ri (i=1, . . . k), so that ! nk ri . (7.3) Rk = i=1 k Thus R2 nk N 1 = ri2 N i=1 k=1 ! k ⎛ ⎞ n N k −1 n k −i 2 ⎝ + r i r i+j ⎠ . N i=1 j=1 k=1 (7.4) k For simplicity, we restrict our discussion to cases for which all jump vectors have the same length |ri | = d, i.e. to coordination lattices and nearestneighbour jumps. We then obtain ⎛ ⎞ ⎤ ⎡ ! N n N n−1 n−i 2 2 ⎝ ri2 + cos θi,i+j ⎠ ⎦ R2 = d2 n ⎣1 + N N i=1 i=1 j=1 k=1 k k=1 2 =d n f. k (7.5) Here n = N 1 nk N (7.6) k=1 is the average number of jumps per tracer atom during time t, (cos θi,i+j )k the cosine of the angle between the ith and (i + j)th jump vectors of the k th atom and f , the quantity in square brackets, the correlation factor. It is then argued that, when the ensemble average is performed and n → ∞ as t → ∞, the correlation factor can be written as n−1 n−i 2 cos θi,i+j . n→∞ n i=1 j=1 f = 1 + lim (7.7) We note that Eq. (7.7) is a rather complex expression, because the double summation contains correlation between an inﬁnite number of pairs of jumps. In what follows, we consider whether and to what extent correlation eﬀects play a rôle in some of the basic diﬀusion mechanisms catalogued in Chap. 6. 7.2 Interstitialcy Mechanism 107 7.1 Interstitial Mechanism Not all diﬀusion processes in solids entail correlation eﬀects. Let us brieﬂy address the question, why interstitial diﬀusion in crystals is usually not correlated. In a dilute interstitial solution each interstitial atom has a high probability of being surrounded by empty interstitial sites (see Fig. 6.2). All directions for jumps of an interstitial solute to neighbouring empty sites are equally probable and independent of the prior jump. Hence cos θi,i+j = 0; the jump sequence of the interstitial is uncorrelated and the correlation factor equals unity: f = 1. (7.8) This statement is correct as long as the number of interstitial atoms is much less than the number of the available sites, which is the case for many interstitial solutions of the elements boron (B), carbon (C), or nitrogen (N) in metals. A famous example is C in iron (Fe). In fcc Fe, C is incorporated in octahedral interstitial sites and in bcc iron in tetrahedral interstitial sites. The solubility of C in bcc Fe is less than 0.02 wt. % and in fcc Fe it is less than 2 wt. %. Hence the probability that neighbouring interstitial sites to a certain C atom are unoccupied is close to unity. In some systems, concentrated interstitial alloys form. Examples are hydrides, carbides, and nitrides of some metals. In such cases, some or even most sites in the H, C, or N sublattices are occupied by atoms and thus blocked for interstitial jumps. Then, the probability for a jump depends on the local arrangement of unoccupied neighbouring sites and f < 1. (7.9) For an almost ﬁlled sublattice a vacancy-type mechanism is a suitable concept. 7.2 Interstitialcy Mechanism Interstitialcy mechanisms are important for crystals in which self-interstitials are present at thermal equilibrium. One can distinguish colinear and noncolinear versions of this mechanism. For examples of non-colinear interstitialcy mechanisms, we refer to Chap. 26 and [3, 4]. The colinear interstitialcy mechanism is illustrated in Fig. 6.7. In a colinear jump-event tracer and solvent atom move in the same direction. An atom in an interstitial position migrates by ‘pushing’ an atom on a regular lattice site onto an adjacent interstitial site. During a long sequence of jumps the tracer atom changes many times between substitutional (As ) and interstitial positions (Ai ) according to (see Fig. 6.7): As → Ai → As → Ai → As . . . . (7.10) 108 7 Correlation in Solid-State Diﬀusion Let us suppose that a tracer jumps ﬁrst from an interstitial to a substitutional site and then pushes a lattice atom into an interstitial site. Immediately after this jump the tracer atom – now on a lattice site – has a self-interstitial next to it. Therefore, the second tracer jump has a greater than random probability of being the reverse of the ﬁrst one. Hence cos θ1,2 is negative. However, the third jump of the tracer – now located at an interstitial site – takes place again in random direction. Thus, alternate pairs of consecutive tracer jumps are correlated only. In other words, jumps from an interstitial site to regular sites occur in random direction, jumps from a regular site to an interstitial site are correlated. Correlation concerns the sequence Ai → As → Ai of Eq. (7.10), whereas the sequence As → Ai → As is uncorrelated. For the sequence Ai → As → Ai we have cos θi,i+1 ≡ cos θ = 0, whereas cos θ = 0 for As → Ai → As . Substituting everything in Eq. (7.7) yields f = 1 + cos θ , (7.11) where cos θ is the average of cosines of the angles between pairs of correlated, consecutive tracer jumps. 7.3 Vacancy Mechanism of Self-diﬀusion The vacancy mechanism is the most important diﬀusion mechanism in crystalline solids (see Chap. 6). In this section, we consider diﬀusion of selfatoms and of substitutional solutes via vacancies. To measure a self- or solute diﬀusion coeﬃcients one usually studies the diﬀusion of very small concentrations of ‘tracers’ labelled by their radioactivity or their isotopic mass (see Chap. 13). This ‘label’ permits to distinguish of tracer from matrix atoms. 7.3.1 A ‘Rule of Thumb’ Let us consider the motion of a tracer atom. The qualitative nature of correlation can easily be seen and a crude estimate of f is gained by considering Fig. 6.5. Vacancies migrate (in the absence of driving forces) in random directions. They approach a tracer atom with equal probabilty from any of its Z neighbouring sites. Thus, the initial vacancy-tracer exchange will occur at random in any of the possible Z directions. After a vacancy has exchanged its site with the tracer atom, the tracer-vacancy conﬁguration is no longer random but depends on the direction of the initial jump. The probability for a vacancy jump to any of its Z neighbouring sites is 1/Z, when we neglect small diﬀerences in the isotopic masses between tracer and matrix atoms. However, the probabilities for the tracer to jump to any of its Z neighbouring sites are not equal. Immediately after a ﬁrst vacancy-tracer exchange, the vacancy is in a position which permits a reverse jump. The tracer thus has 7.3 Vacancy Mechanism of Self-diﬀusion 109 a higher probability to jump backward. Consecutive pairs of tracer jumps in opposite direction lead to no net displacement of the tracer. This ‘backward correlation’ eﬀectively ‘cancels’ a pair of tracer jumps. In other words, the eﬀective number of jumps is n(1 − 2 Z1 ) rather than n. Using this hand-waving argument, the diﬀusion coeﬃcient is reduced by the factor f ≈1−2 1 . Z (7.12) An extreme example is a linear chain of atoms, for which Z = 2. Then Eq. (7.12) yields f = 0, which is in this case the correct value. Suppose that there is a vacancy in the chain and the tagged atom hops to a neighbouring site with the aid of this vacancy. The atom can only jump to and fro between two neighbouring positions. It cannot perform a long-range motion; thus f = 0. Equation (7.12) also indicates that the inﬂuence of correlation eﬀects on self-diﬀusion in three-dimensional coordination lattices should amount to not more than a factor of 2. A comparison with the exact values shows that Eq. (7.12) is indeed a reasonable estimate (see below). 7.3.2 Vacancy-tracer Encounters We now consider self-diﬀusion by a monovacancy mechanism in detail. To perform a jump the tracer atom must wait for the appearance of a vacancy on one of its neighbouring sites. At thermal equilibrium, the probability that a vacancy occupies a certain lattice site of an elemental crystal is given by eq . The total number of atomic (and the equilibrium fraction of vacancies, C1V tracer) jumps per unit time ( jump rate Γtot ), is proportional to this probability and to the rate of vacancy-atom exchanges, ω1V : eq ω1V . Γtot = ZC1V (7.13) eq The explicit form of C1V ω1V is given by Eq. (6.2). The mean residence time of the tracer atom, τ̄ , on a particular lattice site is τ̄ = 1 1 = eq . Γtot Zω1V C1V (7.14) On the other hand, the mean residence time of a vacancy, τ̄1V , on a particular lattice site is given by 1 τ̄1V = . (7.15) Zω1V eq In Chap. 5 we have seen that for metals the site fraction of vacancies, C1V , is a very small number. Even close to the melting temperature it never exceeds 10−3 to 10−4 ; in semiconductors the site fractions of point defects in equilibrium are even much smaller. Due to its Arrhenius type temperature 110 7 Correlation in Solid-State Diﬀusion Table 7.1. Return probability of a vacancy, π0 , and mean number of tracer jumps in a tracer-vacancy encounter, nenc , for various lattices according to Allnatt and Lidiard [30] Lattice π0 nenc linear chain square planar diamond imple cubic bcc fcc 1 1 0.4423 0.3405 0.2822 0.2536 ∞ ∞ 1.7929 1.5164 1.3932 1.3447 bcc, octahedral interstices bcc, tetrahedral interstices 0.4287 0.4765 1.7504 1.9102 dependence the defect fractions decrease further with decreasing temperatures. Thus, the average residence time of an atom on a given lattice site, τ̄ , is much larger than that of a vacancy: τ̄ τ̄1V . (7.16) Following a ﬁrst vacancy-tracer exchange, the vacancy will perform a random walk in the lattice. The longer this random walk continues, the less likely the vacancy returns to the tracer atom. The return probability π0 that a random walker (vacancy) starting from a particular lattice site will return to this site depends on the dimension and the type of the lattice (see Table 7.1). On a two-dimensional square lattice the vacancy will revisit its site adjacent to a tracer atom with a probability of unity. For three dimensional lattices the return probability is smaller than unity and decreases with increasing coordination number. The results for the cubic Bravais lattices were obtained by Montroll [5] (see also [6]). The calculations have been extended to nonBravais lattices by Koiwa and coworkers [7, 8], who obtained the last two entries in Table 7.1. Non-vanishing return probabilities show that correlation eﬀects for vacancy-mediated diﬀusion are unavoidable, since the same vacancy may return several times to the tracer atom. The sequence of exchanges of the tracer atom with the same vacancy is called an encounter. A ‘fresh’ vacancy will approach the tracer from a random direction and terminate the encounter with the ‘old’ vacancy. A complete encounter can develop in lattices, which contain low vacancy concentrations (e.g., metallic elements). The average number of vacancy-tracer exchanges in a complete encounter, nenc , is given by [30] 1 . (7.17) nenc = 1 − π0 Numerical values of nenc are listed in Table 7.1. For three-dimensional lattices nenc is a number not much larger than unity. 7.3 Vacancy Mechanism of Self-diﬀusion 111 Fig. 7.1. Encounter model: tracer displacement due to encounters with several diﬀerent vacancies. The numbers pertain to tracer jumps promoted by a particular vacancy A macroscopic displacement of a tracer atom is the result of many encounters with diﬀerent vacancies (Fig. 7.1). The displacements of the tracer that occur in diﬀerent encounters are uncorrelated. Only tracer jumps within the same encounter are correlated. Each encounter gives rise to a path Renc 2 and to a mean square displacement Renc . The tracer diﬀusion coeﬃcient in a cubic Bravais lattice can be written as D∗ = 2 1 Renc , 6 τenc (7.18) where τenc = τ̄ nenc . In terms of the jump length d we have D∗ = f 1 d2 . 6 τ̄ (7.19) By comparing Eq. (7.18) and Eq. (7.19) we get for the correlation factor 2 Renc f= . (7.20) nenc d2 2 and nenc can be evaluated by computer simulations The quantities Renc as functions of the number of vacancy jumps. For example, in an fcc lattice 2 = 1.0509 d2 has been obtained, when the number nenc = 1.3447 and Renc of vacancy jumps goes to inﬁnity (see, e.g., Wolf [9]). Then, Eq. (7.20) yields f = 0.7815 in agreement with the value given in Table 7.2. Computer simulations also show that sequences of more than three vacancy-tracer exchanges within one encounter are rather improbable. 112 7 Correlation in Solid-State Diﬀusion 7.3.3 Spatial and Temporal Correlation The correlation factor is also called the spatial correlation factor. The term ‘spatial’ refers to correlation between the jump directions of the tracer. Spatial correlations develop after a ﬁrst vacancy-tracer exchange, because the vacancy retains its memory with respect to the position of the tracer atom during its excursion. Correlation eﬀects between tracer jumps develop to its full extent only if Eq. (7.16) is fulﬁlled. A fresh vacancy will approach the tracer from a random direction. Its arrival destroys the chain of correlation developed in the encounter with the old vacancy. In materials with vacancy concentrations much higher than in pure metals (not considered here) encounters are no longer clearly separated and the correlation factor increases. During an encounter between vacancy and tracer, jumps occur mainly a few multiples of τ̄1V after the ﬁrst vacancy-tracer exchange. As recognised by Eisenstadt and Redfield [10], tracer jumps experience a bunching effect in time illustrated in Fig. 7.2. They form small packets of jumps following the ﬁrst tracer jump of an encounter. Such a packet is followed by a deadtime during which the tracer waits for a fresh vacancy. This bunching eﬀect is equivalent to temporal correlation of the jump events. Some microscopic techniques for diﬀusion studies such as nuclear magnetic relaxation (NMR) and Mössbauer spectroscopy (MBS) are sensitive to times between jumps. This is because these techniques have inherent time scales. In NMR experiments the Larmor frequency of the nuclear magnetic moments and in MBS the lifetime of the Mössbauer level provide such time scales. A quantitative interpretation of such experiments (see Chap. 15) must take into account temporal correlation eﬀects in addition to the spatial ones. 7.3.4 Calculation of Correlation Factors Various mathematical procedures for calculating correlation factors are available, to which references can be found at the end of this section. We refrain Fig. 7.2. Temporal correlation: bunching of tracer jumps within encounters 7.3 Vacancy Mechanism of Self-diﬀusion 113 from giving a comprehensive review of all methods. Instead we rather strive for a physical understanding of the underlying ideas: we consider explicitely low vacancy concentrations and cubic coordination lattices. Then, the averages in Eq. (7.7) refer to one complete encounter. Since for a given value of n there are (n − j) pairs of jump vectors separated by j jumps, and since all vacancy-tracer pairs immediately after their exchange are physically equivalent, we introduce the abbreviation cos θj ≡ cos θi,j and get: n−1 2 (n − j) cos θj . n→∞ n j=1 f = 1 + lim (7.21) Here cos θj is the average of the cosines of the angles between all pairs of vectors separated by j jumps in the same encounter. With increasing j the averages cos θj converge rapidly versus zero. Executing the limit n → ∞, Eq. (7.21) can be written as: f = 1+2 ∞ cos θj j=1 = 1 + 2 ( cos θ1 + cos θ2 + . . . ) . (7.22) To get further insight, we consider – for simplicity reasons – the x-displacements of a series of vacancy-tracer exchanges. For a suitable choice of the x-axis only two x-components of the jump vector need to be considered2 , which are equal in length and opposite in sign. Since then cos θj = ±1, we get from Eq. (7.22) ∞ " + # pj − p− , (7.23) f =1+2 j j=1 p+ j (p− j ) where denote the probabilities that tracer jump j occurs in the same (opposite) direction as the ﬁrst jump. If we consider two consecutive tracer jumps, say jumps 1 and 2, the probabilities fulﬁll the following equations: + + − − p+ 2 = p1 p1 + p1 p1 , − + − + p2 = p1 p1 + p− 1 p1 . (7.24) − Introducing the abbreviations tj ≡ p+ j − pj and t1 ≡ t, we get " + # −" + # − − 2 t2 = p + 1 p1 − p1 −p1 p1 − p1 = t . t (7.25) t From this we obtain by induction the recursion formula tj = tj . 2 Jumps with vanishing x-components can be omitted. (7.26) 114 7 Correlation in Solid-State Diﬀusion The three-dimensional analogue of Eq. (7.26) was derived by Compaan and Haven [20] and can be written as cos θj = ( cos θ )j , (7.27) where θ is the angle between two consecutive tracer jumps. With this recursion expression we get from Eq. (7.22) $ % 2 f = 1 + 2 cos θ cos θ + ( cos θ ) + . . . . (7.28) The expression in square brackets is a converging geometrical series with the sum 1/(1 − cos θ ). As result for the correlation factor of vacancy-mediated diﬀusion in a cubic coordination lattice, we get f= 1 + cos θ . 1 − cos θ (7.29) We note that Eq. (7.29) reduces correlation between non-consecutive pairs of tracer jumps within the same encounter to the correlation between two consecutive jumps. Equation (7.29) is valid for self- and solute diﬀusion via a vacancy mechanism. The remaining task is to calculate the average value cos θ . At this point, it may suﬃce to make a few remarks: starting from Eq. (7.29), we consider the situation immediately after a ﬁrst vacancy-tracer exchange (Fig. 7.3). The next jump of the tracer atom will lead to one of its Z neighbouring sites l in the lattice. Therefore, we have cos θ = Z Pl cos δl . (7.30) l=1 In Eq. (7.30) δl denotes the angle between the ﬁrst and the second tracer jump, which displaces the tracer to site l. Pl is the corresponding probability. A computation of Pl must take into account all vacancy trajectories in the lattice which start at site 1 and promote the tracer in its next jump to site l. An inﬁnite number of such vacancy trajectories exist in the lattice. One example for a vacancy trajectory, which starts at site 1 and ends at site 4, is illustrated in Fig. 7.3. Some trajectories are short and consist of a small number of vacancy jumps, others comprise many jumps. A crude estimate for the correlation factor can be obtained as follows: we consider the shortest vacancy trajectory, which consists of only one further vacancy jump after the ﬁrst displacement of the tracer, i.e. we disregard the inﬁnite number of all longer vacancy trajectories. Then, nothing else than the immediate back-jump of the tracer to site 1 in Fig. 7.3 can occur. Any other tracer jump requires vacancy trajectories with several vacancy jumps. For example, for a tracer jump to site 4 the vacancy needs at least 4 jumps (e.g., 7.4 Correlation Factors of Self-diﬀusion 115 Fig. 7.3. Example of a vacancy trajectory immediately after vacancy-tracer exchange in a two-dimensional lattice 1 → 2 → 3 → 4 → tracer). The probability for an immediate back-jump is Pback = 1/Z and we have cos θ ≈ Pback · cos 180◦ = − 1 . Z (7.31) Inserting this estimate in Eq. (7.29), we get f≈ Z −1 2 =1− . Z +1 Z +1 (7.32) This equation is similar to the ‘rule of thumb’, Eq. (7.12), discussed at the beginning of this section. Exact values of f are presented in the next section. 7.4 Correlation Factors of Self-diﬀusion There are a number of publications devoted to calculations of correlation factors for defect-mediated self-diﬀusion. Values of f are collected in Table 7.2 for various lattices and for several diﬀusion mechanisms (see also the reviews by Le Claire [27], Allnatt and Lidiard [30], and Murch [31]). The correlation factor depends on the type of the lattice and on the diﬀusion mechanism considered. The correlation factor decreases the tracer diﬀusion coeﬃcient with respect to its (hypothetical) ‘random-walk value’. For self-diﬀusion this eﬀect is often less than a factor of two. Nevertheless, for a complete description of the atomic diﬀusion process it is necessary to include f . There are, however, additional good reasons why a study of correlations factors is of interest. The correlation factor is quite sensitive to the diﬀusion mechanism. For example, the correlation factor for diﬀusion via divacancies is smaller than that for monovacancies. An experimental determination of f could throw considerable light on the mechanism(s) of diﬀusion. The identiﬁcation of the diﬀusion mechanism(s) is certainly of prime importance for the understanding of diﬀusion processes in solids. Unfortunately, a direct measurement of f is hardly possible. However, measurements of the isotope eﬀect 116 7 Correlation in Solid-State Diﬀusion Table 7.2. Correlation factors of self-diﬀusion in several lattices Lattice Mechanism Correlation factor f Reference 1d chain vacancy 0 see text honeycomb 2d-square 2d hexagonal vacancy vacancy vacancy 1/3 0.467 0.56006 [20] [20, 18] [20] diamond simple cubic bcc cubic fcc cubic vacancy vacancy vacancy vacancy 1/2 0.6531 0.7272, (0.72149) 0.7815 [20] [18] [18, 20] [20, 18] fcc cubic bcc cubic divacancy divacancy 0.4579 0.335 to 0.469 [19] [17] [25] fcc cubic 100 dumb-bell interstitial 0.4395 any lattice direct interstital 1 diamond colinear interstitialcy 0.727 [21] CaF2 (F ) CaF2 (Ca) CaF2 (Ca) non-colinear interstitialcy colinear interstitialcy non-colinear interstitialcy 0.9855 4/5 1 [20] [20] [20] of diﬀusion, which is closely related to f (see Chap. 9), and in some cases also measurements of the Haven ratio (see Chap. 11) can throw some light on the diﬀusion mechanism. The ‘rule of thumb’ values from Eq. (7.12) for vacancy-mediated diﬀusion are listed in Table 7.3. These values are mostly within 10 % of the correct values, indicating that a large amount of correlation results from the ﬁrst backward exchange of vacancy and tracer. For the diamond and honeycomb lattices and the 1d chain the ‘rule of thumb’ values coincide with the exact values. The exact values conﬁrm a trend suggested already by the ‘rule of thumb’: correlation becomes more important, when the coordination number Z decreases. 7.5 Vacancy-mediated Solute Diﬀusion Diﬀusion in binary alloys is more complex than self-diﬀusion in pure crystals. For dilute alloys there are two major aspects of diﬀusion: solute diﬀusion and solvent diﬀusion. In this section, we conﬁne ourselves to correlations eﬀects of solute diﬀusion in dilute alloys. Correlation eﬀects of solvent diﬀusion in dilute fcc alloys have been treated by Howard and Manning [12] on the basis of the ‘ﬁve-frequency-model’ (see below) proposed by Lidiard [13]. Here we concentrate on the more important case of solute diﬀusion. Results for correlation eﬀects of solvent diﬀusion can be found in Chap. 19. 7.5 Vacancy-mediated Solute Diﬀusion 117 Table 7.3. Comparison between ‘rule of thumb’ estimates of correlation factors based on Eq. (7.12) and exact values Lattice Z 1 − 2/Z Correlation factor fcc bcc simple cubic diamond 12 8 6 4 0.833 0.750 0.667 0.500 0.781 0.727 0.653 0.500 honeycomb 2d square 2d hexagonal 3 4 6 1/3 0.5 2/3 1/3 0.467 0.56006 1d chain 2 0 0 In a dilute alloy, isolated solute atoms are surrounded by atoms of the solvent on the host lattice. Accordingly, each solute atom can be considered to diﬀuse in a pure solvent. In Chap. 5 we have already discussed vacancies in dilute substitutional alloys. We remind the reader to the Lomer expression (5.31), which we repeat for convenience: B G eq p = C1V exp . (7.33) kB T The probability p to ﬁnd a vacancy on a nearest-neighbour site of a solute eq to ﬁnd a vacancy on an arbitrary atom is diﬀerent from the probability C1V site of the solvent. This diﬀerence is due to the Gibbs free energy of binding GB for the vacancy-solute pair. For GB > 0 (GB < 0) the probability p is eq . enhanced (reduced) with respect to C1V The presence of the solute also inﬂuences atom-vacancy exchange rates in its surroundings. The exchange rates between vacancy and solute and between vacancy and solvent atoms near a solute atom are diﬀerent from those in the pure solvent. The exchange rates enter the expression for the correlation factor. Correlation factors of solute diﬀusion in the fcc, bcc, and diamond lattices are considered in what follows. Note that it is common practice in the diﬀusion literature to use the index ‘2’ to distinguish the solute correlation factor, f2 , from the correlation factor of self-diﬀusion in the pure solvent, f , and the solute diﬀusivity, D2 , from the self-diﬀusivity in the pure solvent, D. 7.5.1 Face-Centered Cubic Solvents The inﬂuence of a solute atom on the vacancy-atom exchange rates is often described by the so-called ‘ﬁve-frequency model’ proposed by Lidiard [13, 118 7 Correlation in Solid-State Diﬀusion Table 7.4. Vacancy-atom exchange rates of the ‘ﬁve-frequency model’ ω2 : ω1 : ω3 : ω4 : ω: solute-vacancy exchange rate rotation rate of the solute-vacancy pair dissociation rate of the solute-vacancy pair association rate of the solute-vacancy pair vacancy-atom exchange rate in the solvent Fig. 7.4. Left: ‘Five-frequency model’ for diﬀusion in dilute fcc alloys. Right: ‘Energy landscape’ for vacancy jumps in the neighbourhood of a solute atom 14]3 . The ﬁve types of vacancy-atom exchange rates are illustrated in Fig. 7.4 and listed in Table 7.4. Each exchange leads to a diﬀerent local conﬁguration of solute atom, vacancy, and solvent atoms. In the framework of this model two categories of vacancies can be distinguished: vacancies located in the ﬁrst coordination shell of the solute and vacancies located on lattice sites beyond this shell. The vacancy jump with rate ω4 (ω3 ) forms (dissociates) the vacancy-solute pair. Association and dissociation rate are related to the Gibbs free energy of binding of the pair via the detailed balancing equation GB ω3 = exp − . (7.34) ω4 kT Before we discuss the correct expression for the correlation factor of solute diﬀusion, let us consider – as we did in the case of self-diﬀusion – an estimate, which may provide a better understanding of the ﬁnal result. Suppose that a ﬁrst solute-vacancy exchange has occurred. The crudest approximation for f2 takes into account only that vacancy trajectory which leads to an 3 Lidiard uses the word ‘frequency’ instead of rate. Frequency and rate have the same dimension, but they are physically diﬀerent. In the authors opinion, the term ‘rate’ is more appropriate. 7.5 Vacancy-mediated Solute Diﬀusion 119 immediate reversal of the ﬁrst solute atom jump. The pertinent probability expressed in terms of jump rates is Pback ≈ ω2 , ω2 + 4ω1 + 7ω3 (7.35) since the vacancy from its site next to the tracer can perform one ω2 jump, four ω1 jumps, and seven ω3 jumps. Herewith, we get from Eqs. (7.29) and (7.35) for the solute correlation factor f2 ≈ 2ω1 + 7ω3 /2 . ω2 + 2ω1 + 7ω3 /2 (7.36) This expression illustrates that a combination of vacancy jump rates enters the correlation factor. An exact expression for f2 was derived by Manning [15]: f2 = ω1 + 7F3 ω3 /2 . ω2 + ω1 + 7F3 ω3 /2 (7.37) It has some similarity with the approximate relation. In Eq. (7.37) F3 is the probability that, after a dissociation jump ω3 , the vacancy will not return to a neighbour site of the solute. F3 is sometimes called the escape probability. It is illustrated in Fig. 7.5 as a function of the ratio α = ω4 /ω. Manning derived the following numerical expression for the escape probability: 7F3 (α) = 7 − 10α4 + 180.5α3 + 927α2 + 1341α . 2α4 + 40.2α3 + 254α2 + 597α + 436 (7.38) When α goes to zero, no association of the vacancy-solute complex occurs and we have F3 = 1. For ω = ω4 the escape probability is F3 = 0.7357. When α goes to inﬁnity, we have F = 2/7 (see Fig. 7.5). The correlation factor f2 is a function of all vacancy-atom exchange rates. We mention several special cases: 1. For self-diﬀusion all jump rates are equal (when isotope eﬀects are neglected): ω = ω1 = ω2 = ω3 = ω4 and we get f2 = 0.7814. This value agrees (as it should) with the value listed in Table 7.2. 2. If the vacancy-solute exchange is much slower than vacancy-solvent exchanges, i.e. for ω2 ω1 , ω3 , . . ., the correlation factor tends towards unity. Frequent vacancy-solvent exchanges randomise the vacancy position before the next solute jump. Then, solute diﬀusion is practically uncorrelated. 3. If vacancy-solute exchanges occur much faster than vacancy-solvent exchanges, i.e. for ω2 ω1 , ω3 , . . ., the correlation factor tends to zero and the motion of the solute atom is highly correlated. The solute atom ‘rattles’ frequently back and forth between two adjacent lattice sites. 120 7 Correlation in Solid-State Diﬀusion Fig. 7.5. Escape probabilities F3 for the fcc, bcc, and diamond structure. For fcc and bcc lattices F3 is displayed as function of ω4 /ω. For the diamond structure F3 is a function of ω4 /ω5 . After Manning [15] 4. Dissociation jumps ω3 are very unlikely for a tightly bound solute-vacancy pair. Then, we get from Eq. (7.37) f2 ≈ ω1 . ω2 + ω1 (7.39) In this case the vacancy-solute pair can migrate as an entity via ω1 and ω2 -jumps. Such pairs are sometimes called ‘Johnson molecules’. 7.5.2 Body-Centered Cubic Solvents The simplest model for vacancy-exchange rates of solute diﬀusion in a bcc lattice is illustrated in Fig. 7.6. It distinguishes four jump rates: the solutevacancy exchange rate ω2 , the dissociation rate ω3 , the association rate ω4 , and the vacancy-solvent exchange rate ω. As in the case of the fcc lattice, the rates ω3 and ω4 are related via the detailed balancing relation Eq. (7.34). In contrast to the fcc lattice, the bcc structure has no lattice sites which are simultaneously nearest neighbours to both the solute atom and the vacancy of a solute-vacancy pair. Hence an analogue to the rotation rate in the fcc lattice 7.5 Vacancy-mediated Solute Diﬀusion 121 Fig. 7.6. ‘Four-frequency model’ of solute diﬀusion in the bcc lattice does not exist in the bcc lattice. According to Manning [15] the correlation factor for solute diﬀusion can be written as f2 = 7ω3 F3 , 2ω2 + 7ω3 F3 (7.40) where the escape probability F3 (α) is given by 7F3 (α) = 528.4 + 779.03α + 267.5α2 + 24α3 75.50 + 146.83α + 69.46α2 + 8α3 (7.41) illustrated in Fig. 7.5. The ratio α = ω4 /ω has the same meaning as for the fcc case. More sophisticated models for solute diﬀusion in bcc metals are available in the literature (see, e.g., [16]), which we will, however, not describe here. They take into account diﬀerent solute-vacancy interactions for nearest and next-nearest solute-vacancy pairs and then also several additional dissociation and association jump rates. 7.5.3 Diamond Structure Solvents In the diamond structure one usually considers the following vacancy-jump rates (see Fig. 7.7): ω2 for exchange with the solute, ω3 for vacancy jumps from ﬁrst to second-nearest neighbours of the solute, ω4 for the reverse jump of ω3 , ω5 for jumps from second- to third- or ﬁfth-nearest neighbours of the solute, and ω for jumps originating at third-nearest neighbours or further apart from the solute. Manning [15] derived the following expression for the correlation factor 3ω3 F3 f2 = (7.42) 2ω2 + 3ω3 F3 122 7 Correlation in Solid-State Diﬀusion Fig. 7.7. ‘Five frequency model’ for jump rates in the diamond structure. ω2 : jump rate of vacancy-tracer exchange, ω3 (ω4 ): jump rate of vacancy jump from ﬁrst (second) to second (ﬁrst) nearest neighbour of solute atom, ω5 : jump rate of vacancy jump from second to third nearest neighbour of tracer where the escape probability F3 (α) = 2.76 + 4.93α + 2.05α2 2.76 + 6.33α + 4.52α2 + α3 (7.43) is a function of the ratio α = ω4 /ω5 . For self-diﬀusion, all frequencies are identical, F3 = 2/3 and f2 agrees with the value 1/2 of Table 7.2. When α goes to zero, F3 goes to unity. In the other limit where α goes to inﬁnity, F3 goes to zero (see Fig.7.5). Additional complexity can arise in semiconducting solvents, when solute and vacancy carry electrical charges. In contrast to metallic solvents, where the solute-vacancy interaction is short-ranged, the Coulomb interaction can modify the vacancy behaviour over larger distances in the surroundings of a charged solute. 7.6 Concluding Remarks Nowadays, a number of methods for calculating correlation factors are available: Compaan and Haven developed an analogue simulation method based on the similarity between Fick’s and Ohm’s law [20, 21]. A matrix method was proposed by Mullen [22], generalised by Howard [23], and revisited by 7.6 Concluding Remarks 123 Bakker [24]. A rather elegant method based on Laplace and Fourier transforms was developed by Benoist et al. [25]. Koiwa [26] designed a matrix method for return probabilities. Reviews among others were provided by Le Claire [27], Mehrer [28], and in appropriate chapters of textbooks by Manning [29], Allnatt and Lidiard [30], and by Murch [31]. Monte Carlo simulations were introduced by Murch and coworkers [32, 33]. Meanwhile Monte Carlo methods and combinations between analytical schemes and Monte Carlo simulations play an important rôle in the calculations of correlation factors. For a recent example see, e.g., [34]. Correlation factors of self-diﬀusion in elements and in the sublattice of compounds are often well-deﬁned numbers. For a given lattice they are characterstic of a certain diﬀusion mechanism as indicated in Table 7.2. Often the ‘rule of thumb’ permits already a good guess. Correlation factors for substitutional solutes are temperature-dependent. The reason is that each vacancy-atom exchange rate is temperature dependent according to GM . (7.44) ωi = νi0 exp − i kB T In Eq. (7.44) the quantity GM i denotes the Gibbs free energy of activation for jump ωi and νi0 is the pertaining attempt frequency. At a ﬁrst glance, the temperature dependence of f2 looks rather complex. However, in a certain temperature interval it can always be approximated by an Arrhenius expression C 0 f2 ≈ f2 exp − , (7.45) kT where C is the ‘activation enthalpy of the correlation factor’ and f20 some temperature-independent number. The correlation factor enters the expression for the solute diﬀusivity, D2 , as a multiplier. Therefore, the activation enthalpy of the correlation factor will contribute to the total activation enthalpy of solute diﬀusion (see Chaps. 8 and 19). The correlation factors of solute diﬀusion in fcc, bcc, and diamond lattices have the following mathematical form, called ‘impurity form’, in common: f2 = u . ω2 + u (7.46) The quantity u depends on vacancy-solvent exchange rates only and not on the vacancy-solute exchange rate ω2 . This should be remembered, when we discuss isotope eﬀects of diﬀusion in Chap. 9. We stress once more that Eq. (7.29) has been derived for a vacancy mechanism in a cubic coordination lattice with one type of jumps. Equation (7.29) is valid, when the defect-tracer complex contains at least a twofold rotation axis [20]. This is indeed the case for vacancy-tracer pairs in cubic coordination lattices. These condition are, however, violated for divacancy-tracer 124 7 Correlation in Solid-State Diﬀusion complexes in cubic crystals and for monovacancy-tracer complexes in noncubic lattices. For generalisations of Eq. (7.29) to non-cubic lattices and to more complex diﬀusion mechanisms the reader should consult the literature cited at the entrance to this section. We also remind the reader that our discussion of correlation eﬀects has been limited to pure solids, very dilute alloys and to low defect concentrations. There are a number of solid compounds with high disorder in (at least) one of their sublattices. Examples are non-stoichiometric compounds with structural vacancies, certain concentrated interstitial alloys, and fast ionconductors such as silver iodide. Such compounds can be viewed as solids with high apparent defect concentrations. Then the encounter model is no longer useful. In addition ‘defects’ may interact and correlation eﬀects tend to be magniﬁed and become highly temperature dependent. In the last two decades or so intermetallic compounds have attracted considerable interest because of the substantial technological importance of some intermetallics such as aluminides and silicides. Correlation eﬀects in intermetallic compounds are complicated by the fact that at least two sublattices are involved. In addition, several diﬀusion mechanisms have been suggested. Examples are the six-jump cycles of vacancies, the triple defect mechanism in B2 lattices, migration of minority atoms as antisite atoms in the majority sublattice of L12 and D03 structures, diﬀusion by intra-sublattice jumps of vacancies (see Chap. 20). Along with the growth in computational materials science, a number of computer simulations of atomic transport in intermetallics have been performed. The progress with analytical and random walk calculations of correlation eﬀects for diﬀusion in intermetallics is reviewed by Belova and Murch [35]. Atomistic computer simulations of diﬀusion mechanisms using molecular dynamics methods are reviewed by Mishin [36]. References 1. J. Bardeen, C. Herring, in: Atom Movements A.S.M. Cleveland, 1951, p. 87. – 288 2. J. Bardeen, C. Herring, in: Imperfections in Nearly Perfect Solids, W. Shockley (Ed.), Wiley, New York, 1952, p. 262 3. R. Friauf, Phys. Rev. 105, 843 (1957) 4. R. Friauf, J. Appl. Phys. Supp. 33, 494 (1962) 5. E.G. Montroll, Symp. Appl. Math. 16, 193 (1964) 6. I. Stewart, Sci. Am. 280, 111 (1999) 7. M. Koiwa, J. Phys. Soc. Japan 45, 781 (1978) 8. M. Koiwa, S. Ishioka, Philos. Mag. A40, 625 (1979); J. Stat. Phys. 30, 477 (1983); Philos. Mag. A47, 927 (1983) 9. D. Wolf, Mass Transport in Solids, Ch. 7, (1983) p. 149 10. M. Eisenstadt, A.G. Redﬁeld, Phys. Rev. 132, 635 (1963) 11. G.E. Murch, Solid State Ionics, 7, 177 (1982) References 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 125 R.E. Howard, J.R. Manning, Phys. Rev. 154, 561 (1967) A.B. Lidiard, Philos. Mag. 46, 1218 (1955) A.B. Lidiard, Philos. Mag. 5, 1171 (1960) J. Manning, Phys. Rev. 136, A1758 (1964); see also [29] J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Crystals, Les Editions de Physique, Les Ulis, 1991 I.V. Belova, D.S. Gentle, G.E. Murch, Phil. Mag. Letters 82, 37 (2002) G. Montet, Phys. Rev. B7, 650 (1973) G.E. Murch, J. Phys. Chem. Sol. 45, 451 (1984) K. Compaan, Y. Haven, Trans. Faraday Soc. 52, 786 (1956) K. Compaan, Y. Haven, Trans. Faraday Soc. 54, 1498 (1958) J.G. Mullen, Phys. Rev. 124, 1723 (1961) R.E. Howard, Phys. Rev. 144 650 (1966) H. Bakker, Phys. Stat. Sol. 38, 167 (1970) P. Benoist, J.-L. Bocquet, P. Lafore, Acta Metall. 25, 265 (1977) M. Koiwa, Philos. Mag. 36, 893 (1977) A.D. Le Claire, Correlation Eﬀects in Diﬀusion in Solids, in: Physical Chemistry – an Advanced Treatise, Vol. X, Chap. 5, Academic Press, New York and London, 1970 H. Mehrer, Korrelation bei der Diﬀusion in kubischen Metallen, Habilitation thesis, Universität Stuttgart, 1973 J.R. Manning, Diﬀusion Kinetics for Atoms in Crystals, van Norstrand Comp., Princeton 1968 A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 G.E. Murch, Diﬀusion Kinetics in Solids, Ch.3 in: Phase Transformations in Materials, G. Kostorz (Ed.), Wiley-Vch, 2002 H.J. de Bruin, G.E. Murch, Phil. Mag. 27, 1475 (1973) G.E. Murch, R.J. Thorn, J. Phys. Chem. Sol. 38, 789 (1977) S. Divinski, M. Salamon, H. Mehrer, Philos. Mag. 84, 757 (2004) I.V. Belova, G.E. Murch, Defect and Diﬀusion Forum 237–240, 291 (2005) Y. Mishin, Atomistic Computer Simulation of Diﬀusion, in: Diﬀusion Processes in Advanced Technological Materials, D. Gupta (Ed.), William Andrews, Inc., 2005 8 Dependence of Diﬀusion on Temperature and Pressure So far, nothing has been said about the dependence of diﬀusion upon thermodynamic variables such as temperature, pressure, and composition. Diﬀusion in solids generally depends rather strongly on temperature, being low at low temperatures but appreciable at high temperatures. In an Arrhenius diagram the logarithm of the diﬀusivity is plotted versus the reciprocal absolute temperature. The wide range of diﬀusivities and activation parameters, which can occur in a solid is illustrated in the Arrhenius diagram of Fig. 8.1, where diﬀusion coeﬃcients for various elements in lead are displayed. The ‘spectrum’ of diﬀusivities covers many orders of magnitude from the very fast diﬀusion of copper to the rather slow self-diﬀusion of lead. For semiconductors, an even wider spectrum of foreign atom diﬀusivities has been reported (see Chap. 24). The variation of the diﬀusion coeﬃcient with pressure, at least for pressures accessible in laboratory devices, is far less striking than that with temperature. Usually, the diﬀusivity decreases with pressure not more than a factor of ten for pressures of 1 GPa (104 bar). The variation of the diﬀusivity with composition can range from the very slight to signiﬁcant. Examples of the inﬂuence of composition on diﬀusion can be found in Parts III to VI of this book. In this chapter, we concentrate on the dependence of the diﬀusivity on temperature and pressure. 8.1 Temperature Dependence 8.1.1 The Arrhenius Relation The temperature dependence of diﬀusion coeﬃcients is frequently, but by no means always, found to obey the Arrhenius formula ∆H 0 D = D exp − . (8.1) kB T In Eq. (8.1) D0 denotes the pre-exponential factor also called the frequency factor, ∆H the activation enthalpy of diﬀusion1 , T the absolute temperature, 1 In the literature the symbol Q is also used instead of ∆H. 128 8 Dependence of Diﬀusion on Temperature and Pressure Fig. 8.1. Arrhenius plot of diﬀusion for various elements in Pb; activation parameters from [1] and kB the Boltzmann constant. Both ∆H and D0 , are called the activation parameters of diﬀusion2 . The activation enthalpy of a diﬀusion process ∆H = −kB ∂ ln D ∂(1/T ) (8.4) corresponds to the negative slope of the Arrhenius diagram. For a temperature-independent activation enthalpy, the Arrhenius diagram is a straight line with slope −∆H/kB . The intercept of the extrapolated Arrhenius line 2 Equation (8.1) is also written as „ « ∆H D = D0 exp − , RT (8.2) where R denotes the gas constant. Then, R = NA kB = 8.3145 × 10−3 kJ mol−1 K−1 (8.3) with NA denoting the Avogadro number. The activation enthalpy ∆H is either measured in SI units kJ mol−1 K−1 or in eV per atom. Note that 1 eV per atom = 96.472 kJ mol−1 . 8.1 Temperature Dependence 129 for T −1 ⇒ 0 yields the pre-exponential factor D0 . It can usually be written as ∆S 0 0 2 D = gf ν a exp , (8.5) kB where ∆S is called the diﬀusion entropy, g is a geometrical factor, f is the correlation factor, ν 0 is the attempt frequency, and a some lattice parameter. Combining Eqs. (8.1) and (8.5) we can write ∆G ∆S ∆H exp − = gf ν 0 a2 exp − . (8.6) D = gf ν 0 a2 exp kB kB T kB T On the right-hand side of Eq. (8.6), the Gibbs free energy of activation ∆G = ∆H − T ∆S (8.7) has been introduced to combine the activation enthalpy and entropy. Thermodynamics tells us that ∂∆S ∂∆H =T . ∂T ∂T (8.8) Thus, the temperature variations of enthalpy and entropy are coupled. If ∆H is temperature independent, this must hold for ∆S as well and vice versa. Activation parameters for diﬀusion in metals and alloys can be found in the data collection edited by the present author [1] and for semiconductors and other non-metallic materials in a collection edited by Beke [2]. The physical interpretation of the activation parameters ∆H and of D0 depends on the diﬀusion mechanism, on the type of diﬀusion process, and on the lattice geometry. Simple Arrhenius behaviour should not, however, be assumed to be universal. Departures from it may arise for reasons which range from fundamental aspects of the mechanisms of atomic migration (multiple mechanisms, multiple jump vectors, . . . ) to eﬀects associated with impurities and/or with microstructural features such as grain boundaries or dislocations. In this chapter, we consider lattice diﬀusion. Diﬀusion along high-diﬀusivity paths is the subject of Chaps. 31 and 32. If several diﬀusion mechanisms with diﬀusion coeﬃcients DI , DII , . . . and 0 activation parameters ∆HI , ∆HII , . . . and DI0 , DII , . . . contribute to the total lattice diﬀusivity, D, we have ∆HI ∆HII 0 0 D = DI + DII + . . . = DI exp − + DII exp − + . . . . (8.9) kB T kB T In such cases, the Arrhenius diagram will show an upward curvature. With increasing (decreasing) temperature the contribution of the process with the highest (lowest) activation enthalpy becomes more and more important. The activation enthalpy deﬁned by Eq. (8.4) is then an eﬀective (or apparent) value 130 8 Dependence of Diﬀusion on Temperature and Pressure ∆Hef f = ∆HI DI DII + ∆HII + ... , DI + DII + . . . DI + DII + . . . (8.10) which represents a weighted average of the individual activation enthalpies. A well-studied example is self-diﬀusion in metals. Compared with divacancies (index: 2V), usually the monovacancy mechanism (index: 1V) is the dominating contribution to self-diﬀusion in fcc metals at temperatures below about 2/3 of the melting temperature since ∆H1V < ∆H2V . At higher temperatures divacancies contribute with a magnitude that varies from metal to metal (see [3, 4] and Chap. 17). 8.1.2 Activation Parameters – Examples In what follows, we consider explicitly the physical interpretation of the activation parameters for three examples, all concerning cubic lattices: interstitial diﬀusion, self-diﬀusion via vacancies, and solute diﬀusion in a dilute substitutional alloy. For direct interstitial diﬀusion (see Chap. 6) in a dilute interstitial alloy an unoccupied interstice is available next to the jumping atom. Random walk theory of Chap. 4 tells us that the diﬀusivity of solute interstitials can be written as GM D = ga2 ω = ga2 ν 0 exp − , (8.11) kB T where g is a geometrical factor, a the lattice parameter, and ω the jump rate to a neighbouring interstitial site. For octahedral interstitials in the fcc lattice we have g = 1 and in the bcc lattice g = 1/6. As discussed in Chap. 5, the Gibbs free energy of migration GM – the major parameter in the jump rate ω – can be separated according to GM = H M − T S M , (8.12) where H M denotes the enthalpy and S M the entropy of migration of the interstitial solute. Comparing Eqs. (8.1) and (8.11), the activation parameters of interstitial diﬀusion have the following meaning: ∆H ⇒ H M and ∆S ⇒ S M . (8.13) Direct interstitial diﬀusion is the simplest diﬀusion process. The enthalpy and entropy of diﬀusion are identical with the pertinent migration quantities of the interstitial. Activation enthalpies of interstitial diﬀusers, such as H, C, N, and O in metals, tend to be fairly low since no defect formation enthalpy is required. For the same reason, interstitial diﬀusion is a much faster process than self- or substitutional solute diﬀusion. Self-diﬀusion and diﬀusion of substitutional solutes (impurities) are defect-mediated. The diﬀusivity is, in essence, a product of geometrical 8.1 Temperature Dependence 131 terms ga2 , a correlation factor (f for self-diﬀusion or f2 for impurity diﬀusion) and of the atomic jump rate (Γ for self-diﬀusion or Γ2 for impurity diﬀusion): D = f ga2 Γ (self-diﬀusion), D2 = f2 ga2 Γ2 (impurity diﬀusion) . (8.14) In the case of self-diﬀusion, the defect availability equals the equilibrium eq , discussed in Chap. 5. For a monovacancy site fraction of the defect, CD eq eq ≡ C1V . The jump rate of mechanism in an elemental crystal, we have CD a self-atom can be written as GF eq D Γ = CD ω = gD exp − ω, (8.15) kB T where ω denotes the defect jump rate. On the right-hand side of Eq. (8.15), the expression for the equilibrium fraction of defects from Chap. 5 has been inserted with the Gibbs free energy of defect formation GF D . gD is a geometric factor depending on the lattice geometry and the type of the defect. For monovacancies in a monoatomic solid gD = 1. For self-interstitials in 100 dumbbell conﬁguration in an fcc crystal gD = 3. For solute diﬀusion in a very dilute substitutional alloy (often denoted as impurity diﬀusion) the Lomer relation Eq. (5.31) from Chap. 5 describes the defect-availability, p, on a site adjacent to a solute. We then ﬁnd for the jump rate of a substitutional impurity: B GF − GB G eq exp (8.16) ω2 = gD exp − D ω2 . Γ2 = pω2 = CD kB T kB T GB denotes the Gibbs free energy of binding between defect and solute and B ω2 the defect-solute exchange rate. The quantity GF D − G is the Gibbs free energy of defect formation on a site adjacent to the solute. For an attractive interaction (GB > 0) the defect availability p is enhanced whereas for a repulsive interaction (GB < 0) it is reduced compared to the equilibrium defect concentration in the pure host lattice. As usual, GB can be decomposed according to GB = H B − T S B , where H B is the binding enthalpy and S B the binding entropy (see Chap. 5). The Gibbs free energies of the defect-mediated jumps can be separated into the enthalpic and entropic terms according to: GM = H M − T S M M M (self-atom), GM 2 = H2 − T S 2 (impurity). (8.17) GM is the Gibbs free energy of motion for an exchange of the self-atom with the defect in a pure solvent. GM 2 is the barrier for an exchange-jump between impurity and defect (e.g., a vacancy). Then, the exchange jump rates read either M S GM HM ω = ν 0 exp − exp − = ν 0 exp , (8.18) kB T kB kB T 132 8 Dependence of Diﬀusion on Temperature and Pressure or M S2 GM HM ω2 = ν20 exp − 2 exp − 2 = ν20 exp , kB T kB kB T (8.19) where ν 0 , ν20 denote the corresponding attempt frequencies. Usually, the Debye frequency of the lattice is an adequate approximation for the attempt frequencies. Of course, values of the Gibbs energies, enthalpies, and entropies of motion depend on the defect involved and on the material considered. Inserting the expressions of f and Γ or f2 and Γ2 into Eq. (8.14), we arrive at the following activation parameters: – For self-diﬀusion via one type of defect (subscript D) we get F M ∆H ⇒ HD + HD – F M and ∆S ⇒ SD + SD . (8.20) The activation enthalpy (entropy) of self-diﬀusion equals the sum of the formation and migration enthalpies (entropies) of the diﬀusion-mediating F M defect. For a monovacancy we have ∆H = H1V + H1V . For solute diﬀusion in a dilute substitutional alloy the activation enthalpy is a more slightly complex quantity. Combining Eqs. (8.4), (8.14), and (8.16) we get F − H B + H2M + C . (8.21) ∆H2 ⇒ HD The correlation term C = −kB ∂ ln f2 ∂(1/T ) (8.22) arises from the temperature dependence of the correlation factor f2 of imF purity diﬀusion (see Chap. 7). The quantity HD −H B is the formation enM thalpy of the defect-impurity complex and H2 the barrier for a impuritydefect exchange. Depending on the various contributions, the activation enthalpy of substitutional impurity diﬀusion, ∆H2 , can be higher or lower than the activation enthalpy of self-diﬀusion (see Chap. 19). 8.2 Pressure Dependence The eﬀect of hydrostatic pressure p on diﬀusion can easily be recognised from the Arrhenius expression Eq. (8.6). A variation of the diﬀusivity with pressure is largely due to the fact that the Gibbs free energy of activation varies with pressure according to ∆G = ∆H − T ∆S = ∆E − T ∆S + p∆V . (8.23) Here ∆E denotes the activation energy (∆E is the change in internal energy) and ∆V the activation volume of diﬀusion. Thermodynamic tells us that ∂∆G . (8.24) ∆V = ∂p T 8.2 Pressure Dependence 133 Equation (8.24) can be considered as the deﬁnition of the activation volume. A comprehensive characterisation of a diﬀusion process requires information about three activation parameters, namely: ∆E, ∆S, and ∆V . The activation energy ∆E and the entropy ∆S are usually well appreciated in the diﬀusion literature, whereas the activation volume ∆V is often a ‘forgotten’ parameter. Activation enthalpy and activation energy are related via ∆H = ∆E + p∆V . (8.25) The term p∆V can be signiﬁcant at high pressures. At ambient pressure, it is almost negligible for solids. Then ∆E ≈ ∆H and activation energy and activation enthalpy are synonymous. Equations (8.6) and (8.24) show that the activation volume can be obtained from measurements of the pressure dependence of the diﬀusion coeﬃcient at constant temperature via # " ∂ ln f a2 ν 0 ∂ ln D + kB T · . (8.26) ∆V = −kB T · ∂p ∂p T corr. term As an example, Fig. 8.2 shows the self-diﬀusion coeﬃcient of gold as a function of pressure at constant temperature. The slope of the logarithm of D as a function of p corresponds to the ﬁrst term of Eq. (8.26). The second term on the right-hand side of Eq. (8.26) is a correction term. It can be estimated from the isothermal compressibility κT and the Grüneisen constant γG [5–7]: corr. term ≈ kB T κT γG . (8.27) Estimates for the correction terms on the basis of Eq. (8.27) lead to small corrections in the range of 0.01 to 0.03 Ω, where Ω denotes the atomic volume. Often the correction term can be neglected within the experimental accuracy. In the case of Fig. 8.2, the activation volume is ∆V = 0.76 Ω. If several mechanisms with diﬀusivities DI , DII , . . . operate simultaneously (see Eq. 8.9), measurements of the pressure dependence give an eﬀective activation volume ∆Vef f = ∆VI DI DII + ∆VII + ... , DI + DII + . . . DI + DII + . . . (8.28) which is a weighted average of the activation volumes of the individual activation volumes ∆VI , ∆VII , . . . . Since the relative contributions of several mechanisms vary with temperature (and pressure) the eﬀective activation volume is temperature (and pressure) dependent. Activation volumes of ionic conduction (see Chaps. 26 and 27) can be determined from the pressure dependence of the dc conductivity, σdc , according to 134 8 Dependence of Diﬀusion on Temperature and Pressure Fig. 8.2. Pressure dependence of 198 Au diﬀusion in Au single crystals at constant temperature according to Werner and Mehrer [11]. Ω denotes the atomic volume of Au ∆Vσ ≈ −kB T ∂ ln σdc . ∂p (8.29) The atomistic meaning of ∆Vσ depends on the type of the ion-conducting material, on the type of disorder (Frenkel or Schottky disorder), and on the temperature region studied (intrinsic or extrinsic region). Examples are discussed below. There are good reasons why the study of pressure eﬀects has consumed energies of many researcher in the past. First, a thorough understanding of diﬀusion requires knowledge about the inﬂuence of pressure on the diﬀusivity. Second, in favourable cases the value of ∆V itself, its magnitude and sign, can throw light on the mechanism(s) of diﬀusion that is (are) operating (see below). Some selected values for activation volumes are listed in Table 8.1. For elemental crystals the unit is the atomic volume Ω; for compounds the unit is the molar volume Vm . For a comprehensive collection of activation volumes for metals and alloys available until 1990 the reader is referred to Chap. 10 in [1]. A more recent review about the eﬀects of pressure on selfand solute diﬀusion in metals and semiconductors is given in [6]. The microscopic interpretation of the activation volume ∆V depends on the mechanism of diﬀusion as it also does for ∆H and ∆S. As discussed in Chap. 6, self-diﬀusion in crystalline solids is mediated by defects. In metals, monovacancies dominate self-diﬀusion at low and moderate temperatures, 8.2 Pressure Dependence 135 Table 8.1. Activation volumes of diﬀusion and ionic conduction; in units of the atomic volume Ω for elements; in units of the molar volume Vm for compounds. Diﬀusion process ∆V /Ω or ∆V /Vm Reference Cu self-diﬀusion Ag self-diﬀusion +0.93 to +1.09 +0.66 to +0.88 Au self-diﬀusion +0.72 to +0.75 Beyeler and Adda [8] Beyeler and Adda [8], Rein and Mehrer [9] Dickerson et al. [10], Beyeler and Adda [8] Werner and Mehrer [11], Rein and Mehrer [9] Mundy [12] Na self-diﬀusion +0.4 to +0.75 Ge diﬀusion in silicon -0.68 to -0.28 Södervall et al. [15], Aziz et al. [16] N in α-iron C in α-iron +0.05 -0.08 to -0.02 Bosman et al. [13] Bosman et al. [14] Al self-diﬀusion +1.29 Beyeler and Adda [8] Ge in Al Zn in Al Mn in Al Co in Al +1.16 to + 1.24 +0.74 to +1.09 +1.67 +1.64 to 1.93 Thürer et al. [17] Erdelyi et al. [18] Rummel et al. [19] Rummel et al. [19] Schottky pair formation: F VSP 1.63 2.04 1.23 1.37 0.21 0.26 0.25 0.25 1.03 1.28 0.87 0.93 Yoon and Lazarus [22] Cation migration: VVM C Intrinsic conduction: F + VSP /2 VVM C Ag ion conduction α-AgI for for for for for for for for for for for for KBr NaCl KBr NaBr KCl NaCl KBr NaBr KCl NaCl KBr NaBr ≈0 Yoon and Lazarus [22] Yoon and Lazarus [22] Mellander [23] whereas divacancies contribute to some extent as temperatures approach the melting temperature. Self-interstitials are important, for example, in silicon. In what follows, we illustrate the activation volumes for various mechanisms. 8.2.1 Activation Volumes of Self-diﬀusion For a defect mechanism of self-diﬀusion the Gibbs free energy of activation is composed of a formation (superscript F) and a migration (superscript M) term (see Sect. 8.1): 136 8 Dependence of Diﬀusion on Temperature and Pressure M ∆G = GF D + GD . (8.30) Considering Eq. (8.24) it is obvious that the activation volume is also composed of a formation volume, VDF , and a migration volume, VDM , of the diﬀusion-mediating defect according to ∆V = VDF + VDM . (8.31) The formation volume of a monovacancy is illustrated in Fig. 8.3. The left-hand side of the ﬁgure indicates a vacancy in a ‘rigid’ lattice. Without relaxation the volume of the crystal would increase by one atomic volume Ω. The situation illustrated on the right-hand side corresponds to a vacancy with some relaxation of the neighbouring atoms. This picture indicates for the formation volume of a monovacancy: F = +Ω − Vrel,1V . V1V (8.32) Usually, inward relaxation is found, which implies that the formation volume F of the vacancy V1V is somewhat smaller than Ω as the relaxation volume Vrel,1V is positive. The amount and sign of relaxation depend on the material. The formation volume of a divacancy encompasses the increase of the crystal volume due to the creation of two new lattice sites minus the relaxation volume Vrel,2V : F = +2Ω − Vrel,2V . V2V (8.33) The formation volume of the divacancy is larger than that of a monovacancy, F F i.e. V2V > V1V . For a material in which diﬀusion is mediated by monoand divacancies the total activation volume increases as the relative divacancy contribution to the total diﬀusivity increases with temperature (see Chap. 17). The formation volume of a self-interstitial is illustrated in Fig. 8.4. Without relaxation the formation of a self-interstitial would decrease the crystal volume by one atomic volume. On the other hand, the formation of a self-interstitial causes (considerable) outward relaxation of the surrounding lattice. Fig. 8.3. Schematic illustration of the formation volume of a vacancy 8.2 Pressure Dependence 137 Fig. 8.4. Illustration of the formation volume of a self-interstitial Fig. 8.5. Illustration of the migration volume. Upper part: interstitial migration. Lower part: vacancy migration VIF = −Ω + Vrel,I . VIF (8.34) Whether is positive or negative depends on the amount of outward relaxation. If the relaxation volume Vrel,I is positive and larger than one atomic volume – as is the case for close-packed metals [20] – the formation volume is positive. For a less densely packed structure such as silicon, a negative formation volume of a self-interstitial can be expected. The migration volume of an atom (or of a defect) refers to the volume change when the jumping atom is transferred from its equilibrium position to the saddle-point position. Its illustration is a somewhat ‘dangerous’ procedure. The jump event occurs in a short time interval of about 10−12 s. During this short period a complete relaxation of the saddle-point conﬁguration cannot occur because atomic displacements in a solid proceed by the velocity of sound. Nevertheless, with some precaution Fig. 8.5 may serve as an illustration of the migration volume. 138 8 Dependence of Diﬀusion on Temperature and Pressure Fig. 8.6. Activation volumes for self-diﬀusion in Au versus temperature: triangles [8], square [9], full circles [11] The migration volume of a vacancy in close-packed metals is fairly small. Experimental values around V M = 0.15 Ω have been reported for Au. These value were determined by studying the eﬀect of hydrostatic pressure on the annealing rate of vacancies, which had been produced by quenching Au wires from high temperatures [21]. Similar numbers are reported for Pt. These values suggest that the major part of the activation volume of vacancy-mediated self-diﬀusion in metallic elements (see Table 8.1) must be attributed to the formation volume. Figure 8.6 shows the activation volumes ∆V for self-diﬀusion of Au between about 600 K and the melting temperature TM . ∆V is almost independent of temperature indicating that a single mechanism dominates in the whole temperature range. For Au this is the monovacancy mechanism. Values between 0.6 and 0.9 Ω are typical for vacancy-mediated diﬀusion in close-packed metals such as Cu, Ag, and Au (see Table 8.1). For silver, an increase of the activation volume from about 0.6 to 0.9 Ω has been reported [6, 9] and taken as evidence for the simultaneous action of mono- and divacancies (see Chap. 17). A comparison between the activation volumes of self-diﬀusion of noble metals and of sodium indicates (see Table 8.1) that the relaxation around a vacancy is more pronounced for bcc metal. Negative activation volumes between about −0.6Ω and −0.3Ω have been reported for the diﬀusion of Ge in silicon (see Table 8.1). Solute diﬀusion of Ge in silicon is very similar to Si self-diﬀusion and Ge diﬀuses by the same mechanism as Si. Negative acti- 8.2 Pressure Dependence 139 vation volumes are considered as evidence (among others) for self-interstitial mediated diﬀusion in silicon (see [6, 15] and Chap. 23). 8.2.2 Activation Volumes of Solute Diﬀusion For diﬀusion of interstitial solutes no defect formation term is required. Then, from Eqs. (8.11) and (8.24) the activation volume is ∆V = V M , (8.35) where V M is the migration volume of the interstitial solute. As already mentioned, ‘small’ atoms such as C, N, and O in metals diﬀuse by this mechanism. The eﬀect of pressure was studied for C and N in α-Fe, for C in Co and for C in Ni and for N and O diﬀusion in V (for references see Chap. 10 in [1]). Interstitial diﬀusion is characterised by small values of the activation volume. For example, for C and N diﬀusion in α-iron small values between -0.08 and +0.05 Ω were reported (see Table 8.1). This implies that interstitial diﬀusion is only very weakly pressure dependent. Diﬀusion of substitutional impurities is mediated by vacancies. According to Sect. 8.1 the diﬀusivity can be written as B GF H2M 2 1V − G (8.36) exp − f2 , D2 = ga ν0 exp − kB T kB T where GB is the Gibbs ebergy of binding between solute and vacancy. H2M denotes the activation enthalpy for defect-impurity exchange and f2 the correlation factor of impurity diﬀusion. Using Eq. (8.24), we get for the activation volume of solute diﬀusion: ∂ ln f2 F − V B + V2M −kB T . ∆V2 = V1V ∂p (8.37) C2 F − V B represents the formation volume of the impurity-vacancy The term V1V pair. It is diﬀerent from the formation volume of the vacancy in the pure solvent due to the volume change V B associated with pair formation. V2M is the migration volume of the vacancy-solute exchange, which in general is M of the vacancy in the pure matrix. diﬀerent from the migration volume V1V Finally, the term C2 arises from the pressure dependence of the solute correlation factor. V2M + C2 can be interpreted as the migration volume of the solute-vacancy complex. The activation volumes for various solutes in aluminium listed in Table 8.1 show a considerable variation. As we shall see in Chap. 19, transition metal solutes are slow diﬀusers, whereas non-transition elements are normal diﬀusers in Al. Self-diﬀusion in Al has been attributed to the simultaneous action of mono- and divacancies and a similar interpretation is tenable for the 140 8 Dependence of Diﬀusion on Temperature and Pressure diﬀusion of non-transition elements such as Zn and Ge. On the other hand, transition elements in Al have high activation enthalpies and entropies of diﬀusion, which can be attributed to a repulsive interaction between vacancy and solute (see Chapt 19). The high activation volumes for the transition metals diﬀusers Mn and Co indicate large formation and/or migration volumes of the solute-vacancy complex [6]. 8.2.3 Activation Volumes of Ionic Crystals The pressure dependence of the ionic conductivity has been studied in several alkali halide crystals (KCl, NaCl, NaBr, KBr) with Schottky disorder by Yoon and Lazarus [22]. These crystals consist of sublattices of cations (index C) and anions (index A). In the intrinsic region, i.e. at high temperatures, cation and anion vacancies, VC and VA , are simultaneously present in equal numbers (Schottky pairs). In the extrinsic region of crystals, doped with divalent cations, additional vacancies in the cation sublattice are formed to maintain charge neutrality (see Chaps. 5 and 26): (i) In the intrinsic region the conductivity is due to Schottky pairs. The formation volume of Schottky pairs is F = VVFC + VVFA , VSP (8.38) where VVFC and VVFA denote the formation volumes of cation and anion vacancies, respectively. The following values for the formation volume of Schottky pairs have been reported [22] in units cm3 mol−1 : F : 61 ± 9 for KCl, 55 ± 9 for NaCl, 54 ± 9 for KBr, 44 for NaBr. VSP (ii) In the extrinsic region the conductivity is dominated by the motion of cation vacancies because anion vacancies are less mobile. Thus, from the pressure dependence of the conductivity one obtains the migration volume of the cation vacancy, VVM . The following values have been reC ported [22]: VVM :8 ± 1 for KCl, 11 ± 1 for NaCl, 11 ± 1 for KBr, 8 ± 1 for NaBr. C Due to the higher mobility of cation vacancies the activation volume of the ionic conductivity in the intrinsic region, ∆Vσ , is practically given by F ∆Vσ = VSP /2 + VVM . C (8.39) In principle, anion vacancies also contribute to the conductivity (see Chap. 26). However, as the anion component of the total conductivity is usually small this contribution has been neglected in Eq. (8.39). A comparison between activation volumes in metals and ionic crystals with Schottky disorder may be useful. In units of the molar volumes of the crystals, Vm , the activation volumes of the ionic conductivity in the intrinsic region are: 8.3 Correlations between Diﬀusion and Bulk Properties 141 ∆Vσ :1.03 Vm for KCl, 1.28 Vm for NaCl, 1.23 Vm for KBr, 1.37 Vm for NaBr. The activation volumes for intrinsic ionic conduction, which is due to the motion of vacancies, are of the order of one molar volume. These values are similar to activation volumes of self-diﬀusion in close-packed metals, where the activation volume is also an appreciable fraction of the atomic volume of the material (see above). In contrast, the migration volumes of cation vacancies are smaller: :0.21 Vm for KCl, 0.26 Vm for NaCl, 0.25 Vm for KBr, 0.25 Vm for NaBr. VVM C These values indicate a further similarity between metals and ionic crystals. In both cases, the migration volumes of vacancies are only a small fraction of the atomic (molar) volume. The α-phase of silver iodide is a typical example of a fast ion conductor (see Chap. 27). The immobile I− ions form a body-centered cubic sublattice, while no deﬁnite sites can be assigned to the Ag+ ions. In the cubic unit cell 42 sites are available for only two Ag+ ions. Because of these structural features, Ag+ ions are easily mobile and no intrinsic defect is needed to promote their migration. The pressure dependence of the dc conductivity in α-AgI was studied up to 0.9 GPa by Mellander [23]. The activation volume is 0.8 to 0.9 cm3 mol−1 . This very low value can be attributed to the migration of Ag+ ions, conﬁrming the view that migration volumes are small. 8.3 Correlations between Diﬀusion and Bulk Properties Thermodynamic properties of solids such as melting points, heats of melting, and elastic moduli reﬂect diﬀerent aspects of the lattice stability. It is thus not surprising that the diﬀusion behaviour correlates with thermodynamic properties. Despite these correlations, diﬀusion remains a kinetic property and cannot be based solely on thermodynamic considerations. In this section, we survey some correlations between self-diﬀusion parameters and bulk properties of the material. These relationships, which can be qualiﬁed as ‘enlightened empirical guesses’, have contributed signiﬁcantly to the growth of the ﬁeld of solid-state diﬀusion. The most important developments in this area were: (i) the establishment of correlations between diﬀusion and melting parameters and (ii) Zener’s hypothesis to relate the diﬀusion entropy with the temperature dependence of elastic constants. These old and useful correlations have been re-examined by Brown and Ashby [24] and by Tiwari et al. [25]. 8.3.1 Melting Properties and Diﬀusion Diﬀusivities at the Melting Point: The observation that the self-diﬀusivity of solids at the melting point, D(Tm ), roughly equals a constant is an old 142 8 Dependence of Diﬀusion on Temperature and Pressure one, dating back to the work of van Liempt from 1935 [27]. But it was not until the mid 1950s that enough data of suﬃcient precision were available to recognise that D(Tm ) is only a constant for a given structure and for a given type of bonding: the bcc structure, the close-packed structures fcc and hdp, and the diamond structured elements all diﬀer signiﬁcantly. As data became better, additional reﬁnements were added: the bcc metals were subdivided into two groups each with characteristic values of D(Tm ) [26]; also alkali halides were seen to have a characteristic value of D(Tm ) [31]. Figure 8.7 shows a comparison of self-diﬀusion coeﬃcients extrapolated to the melting point for various classes of crystalline solids according to Brown and Ashby [24]. The width of the bar is either twice the standard deviation of the geometric mean, or a factor of four, whichever is greater. Data for the solidus diﬀusivities of bcc and fcc alloys coincide with the range shown for pure metals. It is remarkable that D(Tm ) varies over about 6 orders of magnitude, being very small for semiconductors and fairly large for bcc metals. At the melting temperature Tm according to Eq. (8.6) the self-diﬀusivity is given by ∆S ∆H ∆H 0 2 0 D(Tm ) = D exp − = gf a ν exp exp − . (8.40) kB Tm kB kB Tm The constancy of the diﬀusivity at the melting point reﬂects the fact that for a given crystal structure and bond type the quantities D0 and ∆H/(kB Tm ) are roughly constant: Fig. 8.7. Self-diﬀusivities at the melting point, D(Tm ), for various classes of crystalline solids according to Brown and Ashby [24] 8.3 Correlations between Diﬀusion and Bulk Properties 143 The pre-exponential factor D0 is indeed almost a constant. According to Eq. (8.5) it contains the attempt frequency ν 0 , the lattice parameter a, geometric and correlation factors, and the diﬀusion entropy ∆S. Attempt frequencies are typically of the order of the Debye frequency, which lies in the range of 1012 to 1013 s−1 for practically all solids. The diﬀusion entropy is typically of the order of a few kB . Correlation factors and geometric terms are not grossly diﬀerent from unity. The physical arguments for a constancy of the ratio ∆H/(kB Tm ) are less clearcut. One helpful line of reasoning is to note that the formation of a vacancy, like the process of sublimation, involves breaking half the bonds that link an atom in the interior of the crystal to its neighbours; the enthalpy required to do so should scale as the heat of sublimation, Hs . The migration of a vacancy involves a temporary loss of positional order – it is somehow like local melting – and involves an energy that scales as the heat of melting (fusion), Hm . One therefore may expect ∆H Hs Hm ≈α +β , kB Tm kB Tm kB Tm (8.41) where α and β are constants. The ﬁrst term on the right-hand side contains the sublimation entropy at the melting temperature, Ss = Hs /Tm ; the second term contains the entropy of melting, Sm = Hm /Tm . These entropy changes are roughly constant for a given crystal structure and bond type; it follows that ∆H/(kB Tm ) should be approximately constant, too. Activation Enthalpy and Melting Properties: From practical considerations, correlations between melting and activation enthalpy are particularly useful. Figure 8.8 shows the ratio ∆H/(kB Tm ) for various classes of crystalline solids. It is approximately a constant for a given structure and bond type. The constants deﬁned in this way vary over a factor of about 3.5. The activation enthalpy was related to the melting point many years ago [27–29]. These correlations have been reconsidered for metals and alloys by Brown and Ashby [24] and for pure metals recently by Tiwari et al. [25]. The activation enthalpy of diﬀusion is related via ∆H ≈ K1 Tm (8.42) to the melting temperature (expressed in Kelvin) of the host crystal. This relation is called the van Liempt rule or sometimes also the Bugakov – van Liempt rule [30]. One may go further by invoking the thermochemical rule of Trouton, which relates the melting point of materials to their (nearly) constant entropy of melting, Sm . Trouton’s rule, Sm = Hm /Tm ≈ 2.3 cal/mol = 9.63 J/mol, allows one to replace the melting temperatuire in Eq. (8.42) by the enthalpy of melting, Hm . Then, the van Liempt rule may be also expressed as ∆H ≈ K1 Hm ≡ K 2 Hm . Sm (8.43) 144 8 Dependence of Diﬀusion on Temperature and Pressure Fig. 8.8. Normalised activation enthalpies of self-diﬀusion, ∆H/(kB Tm ), for classes of crystalline solids according to Brown and Ashby [24] Fig. 8.9. Activation enthalpies of self-diﬀusion in metals, ∆H, versus melting temperatures, Tm , according to Tiwari et al. [25] K1 and K2 are constants for a given class of solids. Plots of Eqs. (8.42) and (8.43) for metals are shown in Figs. 8.9 and 8.10. Values of the slopes for metals are: K1 = 146 Jmol−1 K −1 and K2 = 14.8 [25]. The validity of Eq. (8.42) has been demonstrated for alkali halides by Barr and Lidiard [31]. For inert gas solids and molecular organic solids, 8.3 Correlations between Diﬀusion and Bulk Properties 145 Fig. 8.10. Activation enthalpies of self-diﬀusion in metals, ∆H, versus melting enthalpies, Hm , according to Tiwari et al. [25] the validity of Eqs. (8.42) and (8.43) has been established by Chadwick and Sherwood [32]. The correlations above are based on self-diﬀusion, which is indeed the most basic diﬀusion process. Diﬀusion of foreign elements introduces additional complexities such as the interaction between foreign atom and vacancy and temperature-dependent correlation factors (see Chaps. 7 and 19). Correlations between the activation enthalpies of self-diﬀusion and substitutional impurity diﬀusion have been proposed by Beke et al. [33]. Activation Volume and Melting Point: The diﬀusion coeﬃcient is pressure dependent due to the term p∆V in the Gibbs free energy of activation. The activation volume of diﬀusion, ∆V , has been discussed in Sect. 8.2. Nachtrieb et al. [34, 35] observed that the diﬀusivity at the melting point is practically independent of pressure. For example, in Pb and Sn the lattice diﬀusivity, as for most metals, decreases with increasing pressure in such a way that the increased melting point resulted in a constant rate of diﬀusion at the same homologous temperature. If one postulates that D(Tm ) is independent of pressure, we have d [ln D(Tm )] = 0. dp (8.44) Then, we get from Eq. (8.6) ∆V = ∆H(p = 0) dTm Tm (p = 0) dp (8.45) 146 8 Dependence of Diﬀusion on Temperature and Pressure if the small pressure dependence of the pre-exponential factor is neglected. This equation predicts that ∆V is controlled by the sign and magnitude of dTm /dp. In fact, Brown and Asby report reasonable agreement of Eq. (8.45) with experimental data [24]. In general, dTm /dp is positive for most metals and indeed their activation volumes are positive as well. For plutonium dTm /dp is negative and, as expected from Eq. (8.45), the activation volume of Pu is negative [36]. Later, however, also remarkable exceptions have been reported, which violate Eq. (8.45). For example, dTm /dp is negative for Ge [37], but the activation volume of Ge self-diﬀusion is positive [38] (see also Chap. 23). Neither the variation of the activation volume with temperature due to varying contributions of diﬀerent point defects to self-diﬀusion nor the diﬀerences between the activation volumes of various solute diﬀusers are reﬂected by this rule. 8.3.2 Activation Parameters and Elastic Constants A correlation between the elastic constants and diﬀusion parameters was already proposed in the pioneering work of Wert and Zener [39, 40]. They suggested that the Gibbs free energy for migration (of interstitials), GM , represents the elastic work to deform the lattice during an atomic jump. Thus, the temperature variation of GM should be the same as that of an appropriate elastic modulus µ: ∂(µ/µ0 ) ∂(GM /GM 0 ) = . ∂T ∂T (8.46) The subscript 0 refers to values at absolute zero. The migration entropy S M is obtained from the thermodynamic relation SM = − ∂GM ∂T (8.47) and H M = GM + T S M yields the migration enthalpy. In the Wert-Zener picture both H M and S M are independent of T if µ varies linearly with temperature. If this is not the case, both S M and H M are temperature dependent. M in Eq. (8.46), we Substituting the thermodynamic relation and GM 0 ≈ H get: HM H M ∂(µ/µ0 ) SM ≈ − =Θ · . (8.48) Tm ∂(T /Tm ) Tm At temperatures well above the Debye temperature, elastic constants usually vary indeed linearly with temperature. The derivative Θ ≡ −∂(µ/µ0 )/ ∂(T /Tm ) is then a constant. Its values lie between −0.25 to −0.45 for most metals. Then H M and S M are proportional to each other and the model of Zener predicts a positive migration entropy. For a vacancy mechanism, Zener’s idea is strictly applicable only to the migration and not to the formation property of the defect. One can, however, References 147 always deduce a diﬀusion entropy via ∆S = kB ln[D0 /(gf a2 ν 0 )] from the measured value of D0 . Experimental observations led Zener to extend his relation to the activation properties of atoms on substitutional sites: ∆H ∆S = λΘ . (8.49) Tm Then the pre-exponential factor can be written as ∆H D0 = f ga2 ν 0 exp λΘ . (8.50) Tm λ is a constant that depends on the structure and on the diﬀusion mechanism. For self-diﬀusion in fcc metals λ ≈ 0.55 and for bcc metals λ ≈ 1. The relation Eq. (8.49) is often surprisingly well fulﬁlled. We note that this relation also suggests that the diﬀusion entropy ∆S = S M +S F is positive. This conclusion is supported by the well-known fact that the formation entropy for vacancies, S F , is positive (see Chap. 5). 8.3.3 Use of Correlations The value of the correlations discussed above is that they allow diﬀusivities to be estimated for solids for which little or no data are available. For example, when diﬀusion experiments are planned for a new material, these rules may help in choosing the experimental technique and adequate thermal treatments. The correlations should be used with clear appreciation of the possible errors involved; in some instances, the error is small. We emphasise that the correlations have been formulated for self-diﬀusion. Solute diﬀusion of substitutional solutes in most metals diﬀers by not more than a factor of 100 for many solvent metals and the activation enthalpies by less than 25 % from that of the host metal (see Chap. 19). There are, however, remarkable exceptions: examples are the very slow diﬀusion of transition metals solutes in Al and the very fast diﬀusion of noble metals in lead and other ‘open metals’ (see Chap. 19). Also diﬀusion of interstitial solutes (see Sect. 18.1), hydrogen diﬀusion (see Sect. 18.2), and fast diﬀusion of hybrid foreign elements in Si and Ge (see Chap. 25) do not follow these rules. References 1. H. Mehrer (Vol. Ed.), Diﬀusion in Solid Metals and Alloys, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Condensed Matter, Vol. 26, Springer-Verlag, 1990 2. D.L. Beke (Vol. Ed.), Diﬀusion in Semiconductors and Non-Metallic Solids, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Condensed Matter; Vol. 33, Subvolume A: Diﬀusion in Semiconductors, Springer-Verlag, 1998; Subvolume B1: Diﬀusion in Non-Metallic Solids, Springer-Verlag, 1999 148 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 8 Dependence of Diﬀusion on Temperature and Pressure N.L. Peterson, J. of Nucl. Materials 69–70, 3 (1978) H. Mehrer, J. of Nucl. Materials 69–70, 38 (1978) R.N. Jeﬀrey, D. Lazarus, J. Appl. Phys. 41, 3186 (1970) H. Mehrer, Defect and Diﬀusion Forum 129–130, 57 (1996) H. Mehrer, A. Seeger, Cryst. Lattice Defects 3, 1 (1972) M. Beyeler, Y. Adda, J. Phys. (Paris) 29, 345 (1968) G. Rein, H. Mehrer, Philos. Mag. A 45, 767 (1982) R.H. Dickerson, R.C. Lowell, C.T. Tomizuka, Phys. Rev. 137, A 613 (1965) M. Werner, H. Mehrer, in: DIMETA-82, Diﬀusion in Metals and Alloys, F.J. Kedves, D.L. Beke (Eds.), Trans Tech Publications, Diﬀusion and Defect Monograph Series No. 7, 392 (1983) J.N. Mundy, Phys. Rev. B3, 2431 (1971) A.J. Bosman, P.E. Brommer, G.W. Rathenau, Physica 23, 1001 (1957) A.J. Bosman, P.E. Brommer, L.C.H. Eickelboom, C. J. Schinkel, G.W. Rathenau, Physica 26, 533 (1960) U. Södervall, A. Lodding, W. Gust, Defect and Diﬀusion Forum 66–59, 415 (1989) E. Nygren, M.J. Aziz, D. Turnbull, J.F. Hays, J.M. Poate, D.C. Jacobson, R. Hull, Mat. Res. Soc. Symp. Proc. 86, 77 (19?8) A. Thürer, G. Rummel, Th. Zumkley, K. Freitag, H. Mehrer, Phys. Stat. Sol. (a) 143, 535 (1995) G. Erdelyi, H. Mehrer, D.L. Beke, I. Gödeny, Defect and Diﬀusion Forum 143– 147, 121 (1997) G. Rummel, Th. Zumkley, M. Eggersmann, K. Freitag, H. Mehrer, Z. Metallkd. 86, 132 (1995) H. Wollenberger, Point Defects, in: Physical Metallurgy, R.W. Cahn, P. Haasen (Eds.), North-Holland Physics Publishing, 1983, p.1139 R.M. Emrick, Phys. Rev. 122, 1720–1733 (1961) D.N. Yoon, D. Lazarus, Phys. Rev. B 5, 4935 (1972) B.E. Mellander, Phys. Rev. B 26, 5886 (1982) A.M. Brown, M.F. Ashby, Acta Metall. 28, 1085 (1980) G.P. Tiwari, R.S. Mehtrota, Y. Iijima, Solid-State Diﬀusion and Bulk Properties, in: Diﬀusion Processes in Advanced Technological Materials, D. Gupta (Ed.), William Andrew, Inc., 2005, p. 69 N.L. Peterson, Solid State Physics 22, 481 (1968) J.A.M. van Liempt, Z. Physik 96, 534 (1935) O.D. Sherby, M.T. Simnad, Trans. A.S.M. 54, 227 (1961) A.D. Le Claire, in: Diﬀusion in Body Centered Cubic Metals, J.A. Wheeler, F.R. Winslow (Eds.), A.S.M., Metals Parks, 1965, p.3 B.S. Bokstein, S.Z. Bokstein, A.A. Zhukhvitskii, Thermodynamics and Kinetics of Diﬀusion in Solids, Oxonian Press, New Dehli, 1985 L.W. Barr, A.B. Lidiard, Defects in Ionic Crystals, in: Physical Chemistry – an Advanced Treatise, Academic Press, New York, Vol. X, 1970 A.V. Chadwick, J.N. Sherwood, Self-diﬀusion in Molecular Solids, in: Diﬀusion Processes, Vol. 2, Proceedings of the Thomas Graham Memorial Symposium, University of Strathclyde, J.N. Sherwood, A.V.Chadwick, W.M. Muir, F.L. Swinton (Eds.), Gordon and Breach Science Publishers, 1971, p. 472 D. Beke, T. Geszti, G. Erdelyi, Z. Metallkd. 68, 444 (1977) N.H. Nachtrieb, H.A. Resing, S. A. Rice, J. Chem. Phys. 31, 135 (1959) References 149 35. N.H. Nachtrieb, C. Coston, in: Physics of Solids at High Pressure, C.T. Tomizuka, R.M. Emrick (Eds.), Academic Press, 1965, p. 336 36. J.A. Cornet, J. Phys. Chem. Sol. 32, 1489 (1971) 37. D.A. Young, Phase Diagrams of the Elements, University of California Press, 1991 38. M. Werner, H. Mehrer, H.D. Hochheimer, Phys. Rev. B 32, 3930 (1985) 39. C. Wert, C. Zener, Phys. Rev. 76, 1169 (1949) 40. C. Zener, J. Appl. Phys. 22, 372 (1951) 41. C. Zener, in: Imperfections in Nearly Perfect Crystals, W. Shockley et al. (Eds.), John Wiley, 1952, p. 289 9 Isotope Eﬀect of Diﬀusion In this chapter, we consider the diﬀusion of two chemically identical atoms that diﬀer in their atomic masses. Their diﬀusivities are diﬀerent and this difference is denoted as isotope eﬀect. The isotope eﬀect, sometimes also called the mass eﬀect, is of considerable interest. It provides an important experimental means of gaining access to correlation eﬀects. Correlation factors of self- and solute diﬀusion are treated in Chap.7 and values for correlation factors of self-diﬀusion in several lattices and for various diﬀusion mechanisms are listed in Table 7.2. Correlation factors of solute diﬀusion are the subject of Sect. 7.5. We shall see below that the isotope eﬀect is closely related to the correlation factor. Since correlation factors of self-diﬀusion often take values characteristic for the diﬀusion mechanism, isotope eﬀects experiments can throw light on the mechanism. 9.1 Single-jump Mechanisms Let us consider two isotopes α and β of the same element labelled by their isotopic masses mα and mβ . Because of their diﬀerent masses, the two isotopes have diﬀerent diﬀusion coeﬃcients in the same host lattice. For selfand impurity-diﬀusion in coordination lattices the tracer diﬀusivities can be written as: (9.1) Dα∗ = Aωα fα , and Dβ∗ = Aωβ fβ . The quantity A contains a geometrical factor, the lattice parameter squared, and for a defect mechanism also the equilibrium fraction of defects or the defect availability next to the solute. The atom-defect exchange rates ωα or ωβ are factors in Eq. (9.1). The correlation factors for vacancy-mediated diﬀusion in fcc, bcc, and diamond lattices according to Eq. (7.46) have the same mathematical form, sometimes called the ‘impurity form’ : fα = u , ωα + u and fβ = u . ωβ + u (9.2) The quantity u in Eq. (9.2) depends on the exchange rates between vacancy and solvent atoms but not on the vacancy-tracer exchange rate (see Chap. 7). Correlation factors of self- and impurity diﬀusion have the ‘impurity form’ 152 9 Isotope Eﬀect of Diﬀusion because tracer isotopes of the same element as the matrix itself are formally ‘solutes’, whose jump rates diﬀer slightly from those of the host atoms due to the diﬀerent masses. When the small diﬀerences between vacancy-tracer and vacancy-host atom exchange rates are neglected the correlation factor of self-diﬀusion is reduced to one of the values listed in Table 7.2. After taking the ratio Dα∗ /Dβ∗ and eliminating u and fβ using Eqs. (9.1) and (9.2), we ﬁnd Dα∗ − Dβ∗ ωα − ωβ = fα . (9.3) Dβ∗ ωβ The tracer-defect exchange rates can be written as ! GM α,β 0 ωα,β = να,β exp − kB T (9.4) 0 where να,β denote the attempt frequencies of the isotopes α and β, and GM α,β the Gibbs free migration energies of their jumps. In the following discussion we assume M M (9.5) GM α = Gβ = G . In other words, the activation enthalpies and entropies of the jump are independent of the isotopic masses of the tracers. This is usually well justiﬁed, since the barrier for an atomic jump is determined by the electronic interaction, which is identical for two isotopes of the same element, and not by the masses of the nuclei1 . Because of Eq. (9.5) the ratio of the jump rates reduces to the ratio of the attempt frequencies: ωα ν0 = α0 . ωβ νβ (9.6) In what follows, we ﬁrst mention a simple approximation to this frequency ratio: Einstein’s model for the vibration frequencies of atoms in a solid describes a crystal as a set of independent harmonic oscillators. Wert [1] has shown in 1950 that in the classical rate theory, ν 0 is the vibration frequency of an atom in its jump direction. Harmonic oscillator theory tells us that the vibration frequencies are inversely proportional to the square-root of their isotopic masses: να0 mβ ≈ . (9.7) νβ0 mα 1 Hydrogen diﬀusion is an exception. For hydrogen isotopes quantum eﬀects (see Sect. 18.2), such as zero-point vibrations and tunnelling are relevant. Both eﬀects are mass-dependent. For atoms heavier than Li, quantum eﬀects are usually negligible. 9.1 Single-jump Mechanisms 153 Inserting Eq. (9.7) into Eq. (9.3) and making use of Eq. (9.6) yields (Dα∗ − Dβ∗ )/Dβ∗ ≈ fα . mβ /mα − 1 (9.8) This result was derived by Schoen in 1958 [2]. It suggests that a measurement of the isotope eﬀect permits a determination of the correlation factor. Unfortunately the derivation of Eq. (9.8) is based on the Einstein approximation, which assumes that all atoms in the crystal vibrate independently. In other words, the Einstein model neglects many-body eﬀects. Lattice dynamics shows that the coupling between atomic vibrations is important and manifests itself, among other eﬀects, in a spectrum of phonon frequencies. Based on Vineyard’s [3] classical statistical mechanics treatment of the atomic jump process (see Chap. 4), Mullen [4] and Le Claire [5, 6] took into account the inﬂuence of many-body eﬀects. They obtain the relation mβ ωα − ωβ = ∆K −1 , (9.9) ωβ mα where ∆K is denoted as the kinetic energy factor. It is a dimensionless parameter and denotes the fraction of the kinetic energy of the jumping atom at the saddle-point with respect to the total kinetic energy, associated with the motion of all atoms in the jump direction. From Eqs. (9.3) and (9.9) we ﬁnd (Dα∗ − Dβ∗ )/Dβ∗ (9.10) = fα ∆K ≡ Eα,β , mβ /mα − 1 which replaces the approximation of Eq. (9.8). The abbreviation Eα,β introduced in Eq. (9.10) is denoted as the isotope-eﬀect parameter. In an analogous way, we arrive at (Dβ∗ − Dα∗ )/Dα∗ = fβ ∆K ≡ Eβ,α . mα /mβ − 1 (9.11) In principle, the two isotope-eﬀect parameters, Eα,β and Eβ,α , are diﬀerent because fα and fβ are also slightly diﬀerent. However, the relative mass diﬀerences between two isotope pairs are often small. Then, the diﬀerences between Eβ,α and Eα,β are usually of the order of a few percent and often smaller than the errors in a typical isotope eﬀect experiment. Therefore, it is common practice in the literature to use the following approximation: fα ≈ fβ ≈ f . (9.12) Equation (9.12) drops the distinction between fα and fβ . f is sometimes called the geometric correlation factor. f refers to a ‘hypothetical’ tracer isotope with the same jump rate as the isotopes of the solvent. Then, we may 154 9 Isotope Eﬀect of Diﬀusion drop the distinction between the two isotope eﬀect parameters (i.e. Eα,β ≈ Eβ,α ≈ E) and get E = f ∆K . (9.13) Because both f and ∆K are positive and not larger than unity we have the following limits for the isotope eﬀect parameter 0 < E ≤ 1. (9.14) Equation (9.13) expresses in compact form the relation between isotope eﬀect and correlation factor mentioned at the beginning of this chapter. If the tracer jump is completely decoupled from the motion of other atoms, we have ∆K = 1. This represents the upper limit for the kinetic energy factor. Since a certain amount of coupling between the diﬀusing atom and the surrounding atoms always exists, we expect ∆K < 1. For the interstitial mechanism we have E = ∆K (9.15) ∗ since f = 1. If several mechanisms with tracer diﬀusivities DI∗ , DII , . . . operate simultaneously (see Eq. 8.9), measurements of the isotope-eﬀect give an eﬀective isotope-eﬀect parameter, which corresponds to a weighted average Eef f = EI ∗ DI∗ DII + E II ∗ + ... ∗ + ... + ... , DI∗ + DII DI∗ + DII (9.16) of the isotope eﬀect parameters EI , EII , . . . of the individual mechanisms [7]. A measurement of the isotope eﬀect parameter may not uniquely determine f and hence the diﬀusion mechanism. Nevertheless, it is deﬁnitely useful to identify mechanisms, which are consistent with an experimental value of E, and to reject ones, which are not acceptable. We remind the reader that in the derivation of Eq. (9.13) we have made use of the mathematical form of Eq. (9.2). Chap. 7 has shown that there are indeed important mechanisms for which the correlation factor has this form. This is the case for the monovacancy mechanisms in cubic coordination lattices and also for the divacancy mechanism in an fcc lattice [8]. There are, however, mechanisms where the correlation factor does not have the impurity form (9.2). Examples are mechanisms which have several jump rates such as diﬀusion in non-cubic crystals and diﬀusion mechanisms in cubic crystals, which involve more than one tracer jump rate (e.g., for nearest-neighbour and next-nearest neighbour jumps). Sometimes it is possible to derive equations equivalent to Eq. (9.10) [6]. An example is divacancy diﬀusion in bcc crystals involving several conﬁgurations of a divacancy and transitions between these conﬁgurations [9, 10]. For a more detailed discussion of the validity of Eq. (9.13) we refer the reader to a review on isotope eﬀects in diﬀusion by Peterson [11]. 9.3 Isotope Eﬀect Experiments 155 9.2 Collective Mechanisms Equation (9.10) has been derived for single-jump mechanisms, where in a jump event only the tracer atom changes permanently its site. A more general jump process involves the simultaneous (or collective) jumping of more than one atom. A simple example is the colinear interstitialcy mechanism (see Fig. 6.7), where two atoms jump simultaneously. For a dumbbellinterstitialcy mechanism even three atoms are displaced permanently. Other examples are direct exchange, ring mechanism an chain-like motion of several atoms. All these mechanisms involve the collective motion of several atoms (see Chap. 6). For a mechanism in which n atoms move collectively during one jump event, the masses in Eq. (9.7) must be replaced by (n − 1)m + mα,β , where m denotes the average mass of the host atoms [5]. Then, & (n − 1)m + mβ να0 = (9.17) νβ0 (n − 1)m + mα and the isotope eﬀect parameter is given by [6] (Dα∗ − Dβ∗ )/Dβ∗ E= . [mβ + (n − 1)m])/[mα + (n − 1)m] − 1 (9.18) As a consequence, the isotope eﬀect is reduced. For a highly collective mechanism, a very small isotope eﬀect is plausible, due to the ‘dilution’ of the mass eﬀect by the participation of many solvent atoms in the jump event. For example, in metallic glasses, collective jump events of chains of atoms dominate, which typically involve ten to twenty atoms. Indeed the isotope eﬀect parameter is close to zero (see [15, 16] and Chap. 29). 9.3 Isotope Eﬀect Experiments Isotope eﬀects in diﬀusion are usually small eﬀects. An exception is diﬀusion of hydrogen isotopes, which is considered later in Sect. 18.2. Depending on the isotope pair (see Table 9.1), the quantity (Dα∗ −Dβ∗ )/Dβ∗ is typically of the order of a few percent. For example, for the isotope pair 105 Ag and 110m Ag the term in brackets of Eq. (9.9) is about 0.024. Thus, resolving the eﬀects of a relatively small mass diﬀerence on the diﬀusion coeﬃcient is a challenging task. Since the errors in tracer measurements are typically a few percent, it is not feasible to deduce the isotope eﬀect parameter from determinations of Dα∗ and Dβ∗ in separate experiments. Typical experimental situations for isotope eﬀect studies are illustrated in Fig. 9.1. Two isotopes of one element are diﬀused simultaneously into the same sample [11–13]. In this way, errors arising from temperature and time 156 9 Isotope Eﬀect of Diﬀusion Fig. 9.1. Schematic illustration of various isotope eﬀect experiments. Left: isotope pair A∗ /A∗∗ in a solid element A. Middle: isotope pair B ∗ /B ∗∗ in a pure solid A. Right: isotope pairs A∗ /A∗∗ or B ∗ /B ∗∗ in a binary Ax By compound measurements and from the proﬁling procedure drop out, since these errors aﬀect both isotopes in the same way. If the isotopes α and β are co-deposited in a very thin layer, the diﬀusion penetration curves of both isotopes (see also Chap. 13) are given by ! 2 x 0 , (9.19) exp − ∗ Cα,β = Cα,β 4Dα,β t where Cα,β denote their concentrations in depth x after a diﬀusion anneal 0 during time t. For a given time the quantities Cα,β are constants. By taking the logarithm of the ratio Cα /Cβ , we get from Eq. (9.19) ln x2 Cα C0 x2 + = ln α0 − ∗ Cβ Cβ 4Dα t 4Dβ∗ t x2 C0 = ln α0 + Cβ 4Dα∗ t Dα∗ −1 Dβ∗ ! . (9.20) Using Eq. (9.19) to eliminate x2 , we obtain Cα = const − ln Cβ ! Dα∗ − 1 ln Cα . Dβ∗ (9.21) Equation (9.21) shows that from the slope of a plot of ln(Cα /Cβ ) versus ln Cα the quantity (Dα∗ − Dβ∗ )/Dβ∗ can be deduced. Isotope eﬀect experiments are usually performed with radioisotope pairs. Examples of such pairs suitable for isotope eﬀect studies are listed in Table 9.1. Suppose, for example, that the radioisotopes 195 Au and 199 Au are diﬀused into a single crystal of gold. Then, the isotope eﬀect of self-diﬀusion in gold is studied. With the radioisotopes 65 Zn and 69 Zn diﬀusing in gold, the isotope eﬀect of Zn solute diﬀusion is accessible. In an isotope eﬀect experiment the speciﬁc activities (proportional to the concentrations) of both isotopes must be determined separately. Separation techniques can be based 9.3 Isotope Eﬀect Experiments 157 Table 9.1. Examples for pairs of radioisotopes suitable for isotope experiments in diﬀusion studies 12 13 C C 22 24 Na Na 55 59 Fe Fe 57 60 Co Co 65 69 Zn Zn 64 67 Cu Cu 105 110 Ag Ag 195 198 Au Au on the diﬀerent half-lives of the isotopes, on the diﬀerences in the emitted γ- or β-radiation using γ-spectroscopy, or on a combination of γ- and βcounting. Half-life separation requires a short-lived and a long-lived isotope. Scintillation spectroscopy can be used, if the γ spectra are favourable. Highresolution intrinsic Ge or Ge(Li) detectors are recommended for separation and corrections for the Compton-scattered radiation must be made. All methods require careful monitoring of radioactive impurities by either half-life measurements or by spectroscopy. Very good counting statistics is necessary to resolve the small diﬀerences between the diﬀusivities of the two isotopes. Fig. 9.2. Simultaneous diﬀusion of the radioisotope pair monocrystalline Au according to Herzig et al. [14] 199 Au and 195 Au in 158 9 Isotope Eﬀect of Diﬀusion Fig. 9.3. Isotope eﬀect parameters of self-diﬀusion in Au according to Herzig et al. [14] Further details about the experimental techniques in isotope eﬀect experiments can be found in the review of Rothman [12]. In a few experiments, stable isotope pairs were utilised as diﬀusers. Then, the separation is achieved by secondary ion mass spectroscopy (SIMS), which requires good mass resolution and careful background corrections. Figure 9.2 shows isotope eﬀect measurements for self-diﬀusion in single crystals of gold according to Herzig et al. [14]. In this experiment the isotope pair 199 Au and 195 Au was used. The proﬁle measurement was achieved by serial sectioning on a microtome. The isotope concentrations Cα and Cβ in each section were separated by combining γ spectroscopy and half-life separation. The logarithm of the ratio C(199 Au)/C(195 Au) is plotted versus the logarithm of C(199 Au), as suggested by Eq. (9.21). Isotope eﬀect parameters deduced therefrom are shown in Fig. 9.3. The correlation factor for self-diﬀusion via monovacancies in an fcc crystal is f1V = 0.78146 (see Table 7.2). The experimental results demonstrate that self-diﬀusion in gold is dominated by the monovacancy mechanism with a kinetic energy factor of ∆K ≈ 0.9, which is close to its upper limit 1. The slight decrease of the isotope eﬀect parameter with increasing temperature has been attributed to a small contribution of divacancies according to Eq. (9.16). The divacancy correlation factor (f2V = 0.458, see Table 7.2) is smaller than that of monovacanices. Near the melting temperature Tm , the divacancy contribution in Au is, however, not more than 20 % of the total diﬀusivity [14]. Reviews of isotope eﬀects in diﬀusion were given by Le Claire [6] and by Peterson [11]. A comprehensive collection of isotope eﬀect data, which were available until 1990, can be found in Chap. 10 of [13]. Diﬀusion and isotope eﬀects in metallic glasses have been reviewed by Faupel et al. [15, 16]. References 159 In metallic glasses, isotope eﬀects parameters are usually small and indicate a collective mechanism, which involve the simultaneous chain- or ring-like motion of several (10 to 20) atoms. As an example, isotope eﬀect measurements involving the isotopes 57 Co and 60 Co were carried out in the deeply supercooled liquid state of bulk metallic glasses. The isotope eﬀect parameter is very small (around 0.1) over the whole temperature range and exhibits no signiﬁcant temperature dependence (see Chap. 29) . The magnitude of the isotope eﬀect is similar to that of the isotope eﬀect found in the glassy state of conventional metallic glasses [15, 16]. This lends support to the view that the diﬀusion mechanism in metallic glasses does not change at the calorimetric glass transition temperature. Highly collective hopping processes occurring in the glassy state still determine long-range diﬀusion in a deeply undercooled melt. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. C. Wert, Phys. Rev. 79, 601 (1950) A.H. Schoen, Phys. Rev. Letters 1, 138 (1958) G.H. Vineyard, J. Phys. Chem. Sol. 3, 121 (1957) J.G. Mullen, Phys. Rev. 121, 1649 (1961) A.D. Le Claire, Philos. Mag. 14, 1271 (1966) A.D. Le Claire, Correlation Eﬀects in Diﬀusion in Solids, in: Physical Chemistry – an Advanced Treatise, Vol. X, Chap. 5, Academic Press, 1970 A. Seeger, H. Mehrer, in: Vacancies and Interstitials in Metals, A. Seeger, D. Schumacher, W. Schilling, J. Diehl (Eds.), North-Holland Publishing Company, The Netherlands, 1970, p. 1 H. Mehrer, J. Phys. F: Metal Phys. 2, L11 (1972): H. Mehrer, Korrelation bei der Diﬀusion in kubischen Metallen, Habilitation thesis, Universität Stuttgart, 1973 I.V. Belova, D.S. Gentle, G.E. Murch, Phil. Mag. Letters 82, 37 (2002) N.L. Peterson, Isotope Eﬀects in Diﬀusion, in: Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.), Academic Press 1975, p.116 S.J. Rothman, The Measurement of Tracer Diﬀusion Coeﬃcients in Solids, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, (1984), p. 1 H. Mehrer, N. Stolica, Mass and Pressure Dependence of Diﬀusion in Solid Metals and Alloys, Chap. 10, in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol.26, Springer-Verlag, 199, p.574 Chr. Herzig, H. Eckseler, W. Bussmann, D. Cardis, J. Nucl. Mater. 69/70, 61 (1978) F. Faupel, W. Frank, H.-P. Macht, H. Mehrer, V. Naundorf, K. Rätzke, H. Schober, S. Sharma, H. Teichler, Diﬀusion in Metallic Glasses and Supercooled Melts, Review of Modern Physics 75, 237 (2003) F. Faupel, K. Rätzke, Diﬀusion in Metallic Glasses and Supercooled Melts, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 10 Interdiﬀusion and Kirkendall Eﬀect Diﬀusion processes in alloys with composition gradients are of great practical interest. In the preceding chapters, we have assumed that the concentration gradient is the only cause for ﬂow of matter. Such situations can be studied using small amounts of trace elements in otherwise homogeneous materials. We will discuss the experimental procedure for tracer experiments in Chap. 13. From a general viewpoint, the diﬀusion ﬂux is proportional to the gradient of the chemical potential. The chemical potential is proportional to the concentration gradient only for dilute systems or ideal solid solutions. The gradient of the chemical potential gives rise to an ‘internal’ driving force and the intermixing of a binary A-B system can be described by a concentration-dependent chemical or interdiﬀusion coeﬃcient. In a binary alloy there is a single interdiﬀusion coeﬃcient that characterises interdiﬀusion. The interdiﬀusion coeﬃcient is usually a composition-dependent quantity. On the other hand, interdiﬀusion is due to the diﬀusive motion of A and B atoms, which in general have diﬀerent intrinsic diﬀusion coefﬁcients. This diﬀerence manifests itself in the Kirkendall eﬀect, a shift of the diﬀusion zone with respect to the ends of the diﬀusion couple. We consider ﬁrst interdiﬀusion and the Boltzmann-Matano and Sauer-Freise methods for the determination of the interdiﬀusion coeﬃcient. Further sections are devoted to intrinsic diﬀusion, Kirkendall eﬀect, and to the Darken relations. The Darken-Manning relations, the so-called vacancy-wind eﬀect, and the stability or instability of Kirkendall planes are described. A discussion of interdiﬀusion in ionic systems and the Nernst-Planck equation and its relation to the Darken equation is postponed to the end of the next chapter. 10.1 Interdiﬀusion Let us consider a binary diﬀusion couple, in which the chemical composition varies in the diﬀusion zone over a certain range. Diﬀusing atoms then experience diﬀerent chemical environments and hence have diﬀerent diﬀusion coeﬃcients. As already mentioned in Chap. 2, this situation is called interdiﬀusion or chemical diﬀusion. We use the symbol D̃ to indicate that 162 10 Interdiﬀusion and Kirkendall Eﬀect the diﬀusion coeﬃcient is concentration-dependent and call it the interdiffusion or chemical diﬀusion coeﬃcient. Fick’s second law Eq. (2.5) then reads 2 ∂ ∂C dD̃(C) ∂C ∂C ∂2C = D̃(C) . (10.1) = D̃(C) 2 + ∂t ∂x ∂x ∂x dC ∂x The second term on the right-hand side represents an ‘internal driving force’ (see also Chap. 11). Mathematically, Eq. (10.1) is a non-linear partial differential equation. For an arbitrary concentration dependence of D̃(C) it can usually be not solved analytically. In addition, theoretical models which permit the calculation of the composition-dependent diﬀusivity from deeper principles are at present not broadly available. The strategy illustrated in Chaps. 2 and 3 for calculating the concentration ﬁeld for given initial and boundary conditions is not applicable to interdiﬀusion. We shall see, however, that it is possible to determine the concentration-dependent diﬀusivity, D̃, from a measured concentration ﬁeld by using Eq. (10.1). Two methods for extracting diﬀusivities from concentration-depth proﬁles – the classical Boltzmann-Matano method and related approaches proposed by Sauer and Freise – are considered below. Boltzmann’s transformation of Fick’s second law is fundamental for both methods and is discussed ﬁrst. 10.1.1 Boltzmann Transformation In 1894 the famous Ludwig Boltzmann [1] showed that the nonlinear partial diﬀerential equation (10.1) can be transformed to a nonlinear but ordinary diﬀerential equation if D̃ is a function of C(x) alone. He introduced the variable x − xM √ , (10.2) η≡ 2 t which is a combination of the space and time variables x and t, respectively. xM refers to a special reference plane – the so-called Matano plane – to be deﬁned below. Applying chain-rule diﬀerentiation to Eq. (10.1), we get the following identity: d ∂η 1 d ∂ ≡ = √ . (10.3) ∂x dη ∂x 2 t dη The operator on the left-hand side of Eq. (10.1) is ∂ d ∂η x − xM d η d ≡ =− =− . 3/2 ∂t dη ∂t dη 2t dη 4t (10.4) The right-hand side of Eq. (10.1) can also be written in terms of η as ∂ ∂C 1 d dC d ∂η D̃(C) dC √ D̃(C) = D̃(C) = . (10.5) ∂x ∂x dη ∂x 2 t dη 4t dη dη 10.1 Interdiﬀusion 163 Fig. 10.1. Schematic illustration of the Boltzmann-Matano method for a binary diﬀusion couple with starting compositions CL and CR By recombining left- and right-hand sides and using the Boltzmann variable we get Fick’s second law as an ordinary diﬀerential equation for C(η): dC d dC −2η = D̃(C) . (10.6) dη dη dη Some authors omit the factor 2 in the deﬁnition Eq. (10.2) of η. Then, a factor of 1/2 instead of 2 appears in the equation corresponding to Eq. (10.6). However, when ﬁnally transformed in ordinary time and space coordinates, the solutions obtained are identical. 10.1.2 Boltzmann-Matano Method The Boltzmann-transformed version of Fick’s second law Eq. (10.6) is a nonlinear ordinary diﬀerential equation. This equation allows us to deduce the concentration-dependent interdiﬀusion coeﬃcient from an experimental concentration-depth proﬁle, C(x). Appropriate boundary conditions for an interdiﬀusion experiment have been suggested by the Japanese scientist Matano in 1933 [2]. He considered a binary diﬀusion couple, which consists of two semi-inﬁnite bars joined at time t = 0. The initial conditions are C = CL for (x < 0, t = 0), C = CR for (x > 0, t = 0) . (10.7) During a diﬀusion anneal of time t, a concentration proﬁle C(x) develops. This proﬁle can be measured on a cross section of the diﬀusion zone, e.g., by electron microprobe analysis (see Chap. 13). Such a proﬁle is schematically illustrated in Fig. 10.1. 164 10 Interdiﬀusion and Kirkendall Eﬀect Carrying out an integration between CL and a ﬁxed concentration C ∗ , we get from Eq. (10.6) C∗ dC dC −2 ηdC = D̃ − D̃ . (10.8) dη C ∗ dη CL CL Matano’s geometry guarantees vanishing gradients dC/dη as C ∗ approaches CL (or CR ). Using (dC/dη)CL = 0 and solving Eq. (10.8) for D̃ yields ' C∗ ηdC CL ∗ D̃(C ) = −2 . (10.9) (dC/dη)C=C ∗ We transform Eq. (10.9) back to space and time coordinates using the Boltzmann variable Eq. (10.2) and get ' C∗ 1 CL (x − xM )dC . (10.10) D̃(C ∗ ) = − 2t (dC/dx)C ∗ This relation is called the Boltzmann-Matano equation. It permits us to determine D̃ for any C ∗ from an experimental concentration-distance proﬁle. For the analysis, the position of the Matano plane, xM , must be known. Carrying out the integration between the limits CL and CR , we get from Eq. (10.6) CR ηdC = 0 . (10.11) CL Equation (10.11) can be considered as the deﬁnition of the Matano plane. xM must be chosen in such a way that Eq. (10.11) is fulﬁlled. In order to determine the Matano plane, we have to remember that at the beginning of the experiment the concentration of the diﬀusing species was CL (CR ) on the left-hand (right-hand) side. Let us suppose, for example, CL < CR . Then, at the end of the experiment, the surplus of the diﬀusing species found on the left-hand side must have arrived by diﬀusion from the right-hand side. The location of the Matano plane can be determined from the conservation condition ∞ xM [C(x) − CL ] dx = −∞ [CR − C(x)] dx . xM gain (10.12) loss When integrated by parts, the integrals in Eq. (10.12) transform to integrals with C as the running variable instead of x. If we apply the Matano boundary conditions Eq. (10.7), we get CM (CL − CR )xM + CR xdC + CL xdC = 0 , CM (10.13) 10.1 Interdiﬀusion 165 where CM denotes the concentration at the Matano plane. If we choose the Matano plane as origin of the x-axis (xM = 0), the ﬁrst term in Eq. (10.13) vanishes. Then, the following integrals balance across the Matano plane: CM CL xdC + CR xdC = 0 . (10.14) CM Although the location of the Matano plane is not known a priori, it can be found from experimental concentration-distance data by balancing the horizontally hatched areas in Fig. 10.1. In summary, the determination of interdiﬀusion coeﬃcients from an experimental concentration-distance proﬁle via the Boltzmann-Matano method requires the following steps: 1. Determine the position of the Matano plane from Eq. (10.11) and use this position as the origin of the x-axis. ' C∗ 2. Choose C ∗ and determine the integral CL xdC from the experimental concentration-distance data. The integral corresponds to the doublehatched area A∗ in Fig. 10.1. 3. Determine the concentration gradient S = (dC/dx)C ∗ . S corresponds to the slope of the concentration-distance curve at the position x∗ . 4. Determine the interdiﬀusion coeﬃcient D̃ for C = C ∗ from the Boltzmann-Metano equation (10.10) as: D̃(C ∗ ) = −A∗ /(2tS). We draw the readers attention to the following points: (i) The Boltzmann-Matano equation (10.10) refers to an ‘inﬁnite’ system. Its application to an experiment requires that the concentration changes must not have reached the boundaries of the system. (ii) Close to the end-member compositions, the Boltzmann-Matano procedure may incur relatively large errors in D̃ because far away from the Matano plane both the integral A∗ and the slope S become very small. (iii) The initial interface of a diﬀusion couple can be tagged by inert diﬀusion markers (e.g., ThO2 particles, thin Mo or W wires). The plane of the markers in the diﬀusion couple is denoted as the Kirkendall plane. Usually, for t = 0 the positions of the Matano plane and of the Kirkendall plane will be diﬀerent. This is called the Kirkendall eﬀect and is discussed in Sect. 10.2. (iv) This method is applicable when the volume of the diﬀusion couple does not change during interdiﬀusion. The Boltzmann-Matano method has been modiﬁed by Sauer and Freise [3] and later by den Broeder [4]. These authors introduce a normalised concentration variable Y deﬁned by: Y = C − CR . CL − CR (10.15) 166 10 Interdiﬀusion and Kirkendall Eﬀect If no volume change occurs upon interdiﬀusion, the Sauer-Freise solution can be written in the following way: ⎡ ⎤ ∞ x∗ 1 ⎣(1 − Y )) (C ∗ − CR )dx + Y D̃(C ∗ ) = (CL − C ∗ )dx⎦ . 2t(dC/dx)x∗ x∗ −∞ (10.16) Here C ∗ is the concentration at the position x∗ . The Sauer-Freise approach circumvents the need to locate the Matano plane. In this way, errors associated with ﬁnding its position are eliminated. On the other hand, application of Eq. (10.16) to the analysis of an experimental interdiﬀusion proﬁle, like the Boltzmann-Matano method, requires the computation of two integrals and of one slope. 10.1.3 Sauer-Freise Method When the volume of a diﬀusion couple changes during interdiﬀusion neither the Boltzmann-Matano equation (10.10) nor Eq. (10.16) can be used. Fick’s law then needs a correction term [5, 6]. Volume changes in a binary diﬀusion couple occur whenever the total molar volume Vm of an A-B alloy deviates from Vegard’s rule, which states that the total molar volume of the alloy is obtained from Vm = VA NA + VB NB , where VA , VB denote the molar volumes of the pure components and NA , NB the molar fractions of A and B in the alloy. Vegard’s rule is illustrated by the dashed line in Fig. 10.2. Non-ideal solid solution alloys exhibit deviations from Vegard’s rule, as indicated by the solid line in Fig. 10.2. Diﬀusion couples of such alloys change their volume during interdiﬀusion. Couples with positive deviations from Vegard’s rule swell, couples with negative deviations shrink. The partial molar volumes of the components A and B, ṼA ≡ ∂Vm /∂NA and ṼB ≡ ∂Vm /∂NB , are related to the total molar volume via: Vm = ṼA NA + ṼB NB . (10.17) As indicated in Fig. 10.2, the partial molar volumes can be obtained graphically as intersections of the relevant tangent with the ordinate. Sauer and Freise [3] deduced a solution for interdiﬀusion with volume changes. Instead of Eq. (10.15), they introduced the ratio of the mole fractions Y = Ni − NiR , NiL − NiR (10.18) with NiL and NiR being the unreacted mole fractions of component i at the left-hand or right-hand side of the diﬀusion couple. The interdiﬀusion coeﬃcient D̃ is then obtained from 10.1 Interdiﬀusion 167 Fig. 10.2. Molar volume of an A-B solid solution alloy (solid line) versus composition. The dashed line repesents the Vegard rule. The partial molar volumes, ṼA and ṼB , and the molar volumes of the pure components, VA and VB , are also indicated ⎡ V m ⎣(1 − Y ∗ ) D̃(Y ∗ ) = 2t(dY /dx)x∗ x∗ −∞ +∞ Y dx + Y ∗ Vm x∗ ⎤ 1−Y ⎦ dx . (10.19) Vm In order to evaluate Eq. (10.19), it is convenient to construct from the experimental composition-distance proﬁle and from the Vm data two graphs, namely the integrands Y /Vm and (1 − Y )/Vm versus x, as illustrated in Fig. 10.3. The two integrals in Eq. (10.19) correspond to the hatched areas. Equations (10.19) and (10.16) contain two inﬁnite integrals in the running variable. Their application to the analysis of an experimental concentrationdepth proﬁle requires accurate computation of a gradient and of two integrals. Fig. 10.3. Composition proﬁles constructed according to the Sauer-Freise method. Vm,L and Vm,R are the molar volumes of the left-hand and right-hand end-members of the diﬀusion couple 168 10 Interdiﬀusion and Kirkendall Eﬀect 10.2 Intrinsic Diﬀusion and Kirkendall Eﬀect So far, we have described diﬀusion of a two-component system by a single interdiﬀusion coeﬃcient, which depends on composition. In general, the rate of transfer of A atoms is greater/smaller than that of B atoms. Thus, there I I and DB , which are denoted as the intrinsic are two diﬀusion coeﬃcients, DA diﬀusion coeﬃcients of the components. They are concentration dependent as well. On the other hand, there is only one diﬀusion process, namely the intermixing of A and B. These two apparently contradictory facts are closely related to the question of how we specify the reference frame for the diﬀusion process. We know that the atoms in a crystalline solid are held in a lattice structure and we shall therefore retain the form of Fick’s ﬁrst law for the diﬀusion ﬂuxes relative to a frame ﬁxed in the local crystal lattice (intrinsic diﬀusion ﬂuxes): ∂CA I ∂CB , jB = −DB . (10.20) ∂x ∂x The inequality of these ﬂuxes leads to a net mass ﬂow accompanying the interdiﬀusion process, which causes the diﬀusion couple to shrink on one side and to swell on the other side. This observation is called the Kirkendall effect. It was discovered by Kirkendall and coworkers in a copper-brass diﬀusion couple in the 1940s [7, 8]. The Kirkendall shift can be observed by incorporating inert inclusions, called markers (e.g., Mo or W wires, ThO2 particles), at the interface where the diﬀusion couple is initially joined. The original Kirkendall experiment is illustrated in Fig. 10.4. It showed that Zn I I > DCu ) causing atoms diﬀused faster outwards than Cu atoms inward (DZn the inner brass core to shrink. This in turn resulted in the movement of the inert Mo wires. In the period since, it has been demonstrated that the Kirkendall eﬀect is a widespread phenomenon of interdiﬀusion in substitutional alloys. I jA = −DA Fig. 10.4. Schematic illustration of a cross section of a diﬀusion couple composed of pure Cu and brass (Cu-Zn) prepared by Smigelskas and Kirkendall [8] before and after heat treatment. The Mo markers placed at the original contact surface moved towards each other. It was concluded that Zn atoms diﬀused faster outwards I I > DCu ) than Cu atoms move inwards (DZn 10.2 Intrinsic Diﬀusion and Kirkendall Eﬀect 169 The Kirkendall eﬀect was received by contemporary scientists with much surprise. Before the 1940s it was commonly believed that diﬀusion in solids takes place via direct exchange or ring mechanism (see Chap. 6), which imply that the diﬀusivities of both components of a binary alloy are equal. The fact that in a solid-state diﬀusion process the species diﬀuse at diﬀerent rates changed the existing atomistic models on solid-state diﬀusion completely. The Kirkendall eﬀect lended much support to the vacancy mechanism of diﬀusion1 . The position of the Kirkendall plane, xK , moves parabolically in time with respect to the laboratory-ﬁxed frame: √ xK = K t . (10.21) Here K is a (temperature-dependent) constant. The parabolic shift indicates that we are dealing with a diﬀusion-controlled process. We also note that the Kirkendall plane is the only marker plane that starts moving from the beginning. The Kirkendall velocity vK is given by xK dxK = (10.22) dt 2t From the position of the Kirkendall plane one can deduce information about the intrinsic diﬀusivities. Van Loo showed that their ratio is given by [10]: ⎡ ⎤ x'K '∞ 1 1 R L L R N (N − N )dx − N (N − N )dx A A A A A A Vm Vm ⎥ I DA ṼA ⎢ −∞ xK ⎢ ⎥ = ⎢ ⎥. x ∞ I DB ṼB ⎣ −(N R ) 'K 1 (N − N L )dx + N L ' 1 (N R − N )dx ⎦ A A B A B A Vm Vm vK ≡ −∞ xK (10.23) Ni is the mole fraction of component i, with NiL and NiR the unreacted lefthand (x → −∞) and right-hand (x → −∞) ends of the couple, respectively. Since the discovery of the Kirkendall eﬀect by Smigelskas and Kirkendall [8] and its analysis by Darken [9], this eﬀect assumed a prominent rôle in the diﬀusion theory of metals. It was considered as evidence for vacancy-mediated diﬀusion in solids. There are also technological ﬁelds in which the Kirkendall eﬀect is of great interest. Examples are composite materials, coating technologies, microelectronic devices, etc. The interactions accompanying the Kirkendall eﬀect between constituents of such structures can, for example, induce stress and even deformation on a macroscopic scale. It can also cause migration of microscopic inclusions inside a reaction zone and Kirkendall porosity. 1 Nowadays, we know that the Kirkendall eﬀect can manifest itself in many phenomena such as the development of diﬀusional porosity (Kirkendall voids), generation of internal stresses [13, 14], and even by deformation of the material on a macroscopic scale [15]. These diﬀusion-induced processes are of concern in a wide variety of structures including composite materials, coatings, welded components, and thin-ﬁlm electronic devices. 170 10 Interdiﬀusion and Kirkendall Eﬀect 10.3 Darken Equations The ﬁrst theoretical desciption of interdiﬀusion and Kirkendall eﬀect was attempted by Darken in 1948 [9]. For a binary substitutional alloy he used the two intrinsic diﬀusivities introduced above to describe the interdiﬀusion process. The Kirkendall velocity vK can be expressed in terms of the intrinsic ﬂuxes, jA and jB , and partial molar volumes, ṼA and ṼB , as vK = −(ṼA jA + ṼB jB ) . (10.24) Given the fact that dCA = −(ṼB /ṼA )dCB , we can write for the Kirkendall velocity I I ∂CB , (10.25) − DA ) vK = ṼB (DB ∂x where ∂CB /∂x denotes the concentration gradient at the Kirkendall plane. Following Darken’s approach, the laboratory-ﬁxed interdiﬀusion ﬂux J (at the Kirkendall plane) can be written as the sum of an intrinsic diﬀusion ﬂux of one of the components i plus (or minus) a Kirkendall drift term vK Ci : J = −DiI ∂Ci ± vK Ci ∂x i = A, B . (10.26) Substituting Eq. (10.25) in Eq. (10.26) one arrives at a general expression for the interdiﬀusion coeﬃcient: I I D̃ = CB ṼB DA + CA ṼA DB . (10.27) Equations (10.25) and (10.27) provide a description of isothermal diﬀusion in a binary substitutional alloy. They also provide a possibility to determine the intrinsic diﬀusivities from measurements of the interdiﬀusion coeﬃcient and the Kirkendall velocity. From a fundamental point of view, the assumption that the concentration gradients are the driving forces of diﬀusion as given by Fick’s laws is not correct. Instead, as already stated at the beginning of this chapter, the gradient of the chemical potential µi of component i is the real driving force. The ﬂux of component i (i = A, B) in a binary alloy can be written as [16, 17] ji = −Bi Ci ∂µi , ∂x (10.28) where Bi denotes the mobility of component i. The chemical potential can be expressed in terms of the thermodynamic activity, ai , via µi = µ0i + RT ln ai , (10.29) where µ0i is the standard chemical potential (at 298 K and 1 bar) and R is the ideal gas constant (R = 8.3143 J mol−1 K−1 ). The atomic mobility Bi 10.3 Darken Equations 171 is connected to the tracer diﬀusion coeﬃcient Di∗ of component i via the Nernst-Einstein relation (see Chap. 11): Di∗ = Bi RT . (10.30) Substituting Eqs. (10.30) and (10.28) in Eq. (10.20) and knowing that CA = NA /Vm and dNA = (Vm2 /ṼA )dCA one obtains relations between the intrinsic and the tracer diﬀusion coeﬃcients: I ∗ = DA DA Vm ∂ ln aA ṼB ∂ ln NA I ∗ and DB = DB Vm ∂ ln aB . ṼA ∂ ln NB (10.31) The quantity Φ ≡ ∂ ln ai /∂ ln Ni is denoted as the thermodynamic factor. The thermodynamics of binary systems tells us that the thermodynamic factor can also be expressed as follows [21]: Φ= ∂ln ai ∂ln γi NA NB d2 G = =1+ , 2 R T dNi ∂ln Ni ∂ln Ni (10.32) Here G denotes the Gibbs free energy and γi ≡ ai /Ni the coeﬃcient of thermodynamic activity of species i ( = A or B). In addition, as a consequence of the Gibbs-Duhem relation there is only one thermodynamic factor for a binary alloy: ∂ ln aB ∂ ln aA = (10.33) Φ= ∂ ln NA ∂ ln NB Substiting Eq. (10.31) in Eq. (10.27) and knowing the relation Ci ≡ Ni (CA + CB ) = Ni /Vm between concentrations and mole fractions, we obtain for the interdiﬀusion coeﬃcient ∗ ∗ D̃Darken = (NA DB + N B DA ) Φ. (10.34) Equations (10.31) and (10.34) are called the Darken equations. Sometimes the name Darken-Dehlinger equations is used. These relations are widely used in practice for substitutional binary alloys. Their simplicity provides an obvious convenience. We shall assess its accuracy below and also in Chap. 12. If thermodynamic data are available, either from activity measurements or from theoretical models, Eqs. (10.31) or (10.34) allow to relate the intrinsic diﬀusivities and the interdiﬀusion coeﬃcient to the tracer diﬀusivities. For an ideal solid solution alloy we have γi = 1 and ai = Ni and hence Φ = 1 (Raoult’s law). For non-ideal solutions Φ deviates from unity. It is larger than unity for phases with negative deviations of G from ideality and smaller than unity in the opposite case. Negative deviations are expected for systems with order. Therefore, thermodynamic factors of intermetallic compounds are often larger, sometimes even considerably larger than unity due to the attractive interaction between the constituents of the intermetallic phase. As a consequence, interdiﬀusion coeﬃcients are often larger than the term in paranthesis of Eq. (10.34). 172 10 Interdiﬀusion and Kirkendall Eﬀect 10.4 Darken-Manning Equations Soon after the detection of the Kirkendall eﬀect and its phenomenological description via the Darken equations, Seitz in 1948 [11] and Bardeen in 1949 [12] recognised that the original Darken equations are approximations. From an atomistic point of view, interdiﬀusion in substitutional alloys is mediated by vacancies. It was shown that the Darken equations are obtained if the concentration of vacancies is in thermal equilibrium during the interdiﬀusion process. For the Kirkendall eﬀect to occur, vacancies must be created at one site and annihilated on the other side of the interdiﬀusion zone so that a vacancy ﬂux is created to maintain local equilibrium. This implies that sources and sinks for vacancies are abundant in the diﬀusion couple. The vacancy ﬂux causes the so-called vacancy-wind eﬀect – a correction term that must be added to the original Darken equations to obtain the Darken-Manning relations. The relations between tracer diﬀusivities and intrinsic diﬀusivities and the interdiﬀusion coeﬃcient discussed in the previous section are incomplete for a vacancy mechanism, because of correlation eﬀects. The exact expressions are similar to those discussed above but with vacancy-wind factors (see, e.g., [17, 21, 22]). The intrinsic diﬀusion coeﬃcients Eq. (10.31) with vacancywind corrections, rA and rB , can be written as I ∗ DA = DA Vm ΦrA ṼB I ∗ and DB = DB Vm ΦrB . ṼA (10.35) The vacancy-wind factors can be expressed in terms of the tracer and collective correlation factors: (A) rA = fAA − NA fAB /NB fA (B) and rB = fBB − NA fAB /NA . fA (10.36) The fi are the tracer correlation factors and fij the collective correlation factors sometimes also called correlations functions [22] (see also Chap. 12). Perhaps the best-known vacancy-wind factor is the total vacancy-wind factor, S, occuring in the generalised Darken equation: ∗ ∗ D̃ = (NA DB + N B DA ) ΦS = D̃Darken S . (10.37) Equation (10.37) is also called the Darken-Manning equation and S is also denoted as the Manning factor. It can be expressed as S= ∗ ∗ rB + NB DA rA NA DB . ∗ ∗ NA DB + NB DA (10.38) Manning [18, 19] developed approximate expressions for vacancy-wind factors in the framework of a model called the random alloy model. The term random alloy implies that vacancies and A and B atoms are distributed at 10.5 Microstructural Stability of the Kirkendall Plane 173 random on the same lattice, although the rates at which atoms exchange with vacancies are allowed to be diﬀerent. For a random alloy, the individual vacancy-wind factors are rA = 1 + ∗ ∗ − DB ) (1 − f ) NA (DA ∗ ∗) f (NA DA + NB DB rB = 1 + ∗ ∗ − DA ) (1 − f ) NA (DB ∗ ∗) , f (NA DA + NB DB and (10.39) where f is the tracer correlation factor for self-diﬀusion. A transparent derivation of Eq. (10.39) can be found in [20]. For convenience let us assume that ∗ ∗ DA ≥ DB . Then, from these expressions we see that the factors rA and rB take the limits 1 and 0.0 ≤ rB ≤ 1.0 . 1.0 ≤ rA ≤ (10.40) f There is also a ‘forbidden region’ NA ≤ 1 − f , where rB can take negative ∗ ∗ values (unphysical for this model) if DA /DB > NB /(NB −f ). In other words, there is a concentration-dependent upper limit for the ratio of the tracer diﬀusivities in this region. Manning also provides an expression for the total vacancy-wind factor: S =1+ ∗ ∗ 2 NA NB (DA − DB ) (1 − f ) ∗ ∗ ∗ + N D∗ ) . f (NA DA + NB DB )(NA DB B A (10.41) From Eq. (10.41) it is seen that S varies within narrow limits: 1 ≤ S ≤ 1/f . (10.42) Thus, in the framework of the random alloy model the total vacancy-wind factor S is not much diﬀerent from unity. The Manning expressions for the vacancy-wind factors have been used for some 30 years. Extensive computer simulations studies in simple cubic, fcc, and bcc random alloys by Belova and Murch [23] have shown that the Manning formalism is not as accurate as commonly thought. It is, however, a reasonable approximation when the ratio of the atom vacancy exchange rates are not too far from unity. Vacancy-wind corrections for chemical diﬀusion in intermetallic compounds depend on the structure, the type of disorder and on the diﬀusion mechanism. Belova and Murch have also contributed signiﬁcantly to chemical diﬀusion in ordered alloys by considering among others L12 structured compounds [24], D03 and A15 structured alloys [26], and B2 structured compounds [25]. 10.5 Microstructural Stability of the Kirkendall Plane Kirkendall eﬀect induced migration of inert markers inside the diﬀusion zone and the uniqueness of the Kirkendall plane have not been questioned for 174 10 Interdiﬀusion and Kirkendall Eﬀect quite a long time. In recent years, the elucidation of the Kirkendall eﬀect accompanying interdiﬀusion has taken an additional direction. Cornet and Calais [29] were the ﬁrst to describe hypothetical diﬀusion couples in which more than one ‘Kirkendall marker plane’ can emerge. Experimental discoveries also revealed a more complex behaviour of inert markers situated at the original interface of a diﬀusion couple in both spatial and temporal domains. Systematic studies of the microstructural stability of the Kirkendall plane were undertaken by van Loo and coworkers [30–35]. Clear evidence for the ideas of Cornet and Calais was found and led to further developments in the understanding of the Kirkendall eﬀect. In particular, it was found that the Kirkendall plane, under predictable circumstances, can be multiple, stable, or unstable. The diﬀusion process in a binary A-B alloy can best be visualised by considering the intrinsic ﬂuxes, jA and jB , of the components in Eq. (10.20) with respect to an array of inert markers positioned prior to annealing along the anticipated diﬀusion zone. According to Eq. (10.25) the sum of the oppositely directed ﬂuxes of the components is equal to the velocity of the inert markers, v, with respect to the laboratory-ﬁxed frame of reference: I I − DA ) v = ṼB (DB ∂CB , ∂x (10.43) with ṼB being the partial molar volume of component B. Multifoil experiments, in which a diﬀusion couple is composed of many thin foils with markers at each interface, permit a determination of v at many positions inside a diﬀusion couple. Thus a v versus x curve (marker-velocity curve) can be determined experimentally. In a diﬀusion-controlled intermixing process, those inert markers placed at the interface where the concentration step is located in the diﬀusion couple is the Kirkendall plane. The markers in the Kirkendall plane are the only ones that stay at a constant composition and move parabolically with a velocity given by Eq. (10.22), which we repeat for convenience: vK = xK dx = . dt 2t (10.44) xK is the position of the Kirkendall plane at time t. The location of the Kirkendall plane(s) in the diﬀusion zone can be found graphically at the point(s) of intersection(s) between the marker-velocity curve and the straight line given by Eq. (10.44) (see Fig. 10.5). In order to draw the line vK = xK /2t, one needs to know the position in the diﬀusion zone where the ‘Kirkendall markers’ were located at time t = 0. If the total volume does not change during interdiﬀusion this position can be determined via the usual Boltzmann-Matano analysis. If the partial molar volumes are composition dependent, the Sauer-Freise method should be used. The nature of the Kirkendall plane(s) in a diﬀusion couple depends on the gradient of the marker-velocity curve at the point of intersection with the 10.5 Microstructural Stability of the Kirkendall Plane 175 straight line xK /2t. For illustration, let us consider a hypothetical diﬀusion couple of A-B alloys with the end-members Ay B1−y and Az B1−z where y > z. Let us suppose that on the A-rich side of the diﬀusion zone A is the faster diﬀusing species, whereas on the B-rich side B is the faster diﬀusing species. Figure 10.5 shows schematic representations of the marker-velocity curves in diﬀerent situations. For some diﬀusion couples the straight line, vK = x/2t, may intersect the marker-velocity curve in the diﬀusion zone once at a point with a negative gradient (upper part). At this point of intersection one can expect one stable Kirkendall plane. Markers, which by some perturbation Fig. 10.5. Schematic velocity diagrams, pertaining to diﬀusion couples between the end-members Ay B1−y and Az B1−z for y > z. On the A-rich side A diﬀuses faster and on the B-rich side B diﬀuses faster. Diﬀerent situations are shown, which pertain to one stable Kirkendall plane (upper part), to an unstable plane (middle part), and to two stable Kirkendall planes, K1 and K3 , and an unstable plane K2 176 10 Interdiﬀusion and Kirkendall Eﬀect move ahead of the Kirkendall plane, will slow down, because of the lower velocity; markers behind this plane will move faster. The stable Kirkendall plane acts as an ‘attractor for inert markers’. By changing the end-member compositions the straight line, vK = x/2t, may intersect the marker-velocity curve at a point with a positive velocity gradient (middle part). Markers slightly ahead of this plan will move faster, whereas markers behind this plane will move slower. This will result in scatter of the markers and there will be no unique plane acting as the Kirkendall plane (unstable Kirkendall plane). The lower part of Fig. 10.5 illustrates a situation where the straight line intersects the marker-velocity curve three times at K1 , K2 , and K3 . In this case one might expect that three Kirkendall planes will be present in the sample. In reality, one ﬁnds two stable Kirkendall planes, K1 and K3 . An unstable plane, K2 , is located between two stable Kirkendall planes and the stable planes will accumulate the markers during the initial stage of interdiﬀusion. The presence of stable and unstable Kirkendall planes has been veriﬁed, for example, in Ni-Pd and Fe-Pd diﬀusion couples [31]. The marker-velocity curves over the whole homogeneity range have been determined in multifoil experiments. It was indeed found that for Ni-Pd a stable Kirkendall plane is present and the straight line, vK = x/2t, intersects the marker-velocity curve at a point with a negative gradient. An unstable Kirkendall plane is found in Fe-Pd and the gradient of the marker-velocity curve is positive at the intersection point. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. L. Boltzmann, Wiedemanns Ann. Phys. 53 (1894) 959 C. Matano, Japan. J. Phys. 8 (1933) 109 F. Sauer and V. Freise, Z. Elektrochem. 66 (1962) 353 F.J.A. den Broeder, Scr. Metall. 3 (1969) 321 K. Wagner, Acta Metall. 17 (1969) 99 F.F.J. van Loo, Acta Metall. 18 (1970) 1107 E.O. Kirkendall, Trans. AIME 147, 104 (1942) A.D. Smigelskas, E.O. Kirkendall, Trans. AIME 171, 130 (1947) L.S. Darken, Transactions AIME 175, 184 (1948) F.J.J. van Loo, Progr. Solid State Chemistry 20, 47 (1990) F. Seitz, Phys. Rev. 74, 1513 (1948) J. Bardeen, Phys. Rev. 76, 1403 (1949) G.B. Stephenson, Acta Metall. 36, 2663 (1988) D.L. Beke, I.A. Szabo (Eds.), Proc. of Int. Workshop on Diﬀusion and Stresses, Balatonfüred, Hungary, May 1995; also: Defect and Diﬀusion Forum 129–130 (1996) 15. I. Daruka, I.A. Szabo, D.L. Beke, C. Cerhati, A.A. Kodentsov, F.J.J. van Loo, Acta Mater. 44, 4981 (1996) 16. S. Prager, J. Chem. Phys. 21 1344–1347 (1953) References 177 17. A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge Univerity Press, 1993 18. J.R. Manning, Diﬀusion Kinetics for Atoms in Crystals, van Norstrand, Princeton, 1968 19. J.R. Manning, Acta Metall. 15, 817 (1967) 20. R.E. Howard, A.B. Lidiard, Matter Transport in Solids, in: Reports on Progress in Physics, Vol. XXVII, The Institute of Physics and the Physical Society, London, 1964, pp. 161–240 21. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 22. G.E. Murch, Z. Qin, Defect and Diﬀusion Forum 109, 1 (1994) 23. I.V. Belova, G.E. Murch, Philos. Mag. A 80, 1469–1479 (2000); Philos. Mag. A 81, 1749–1758 (2001) 24. I.V. Belova, G.E. Murch, Philos. Mag, A 78, 1085–1092 (1998) 25. I.V. Belova, G.E. Murch, Philos. Mag, A 79, 193–202 (1999) 26. I.V. Belova, G.E. Murch, J. Phys. Chem. Sol. 60, 2023–2029 (1998) 27. I.V. Belova, G.E. Murch, Philos. Mag, A 81, 83–94 (2001) 28. I.V. Belova, G.E. Murch, Defect and Diﬀusion Forum 194–199, 533–540 (2001) 29. J.-F. Cornet, D. Calais, J. Phys. Chem. Sol. 33, 1675 (1972) 30. F.J.J. van Loo, B. Pieragi, R.A. Rapp, Acta Metall. Mater. 38, 1769 (1990) 31. M.J.H. van Dal, M.C.I.P. Pleumeckers, A. A. Kodentsov, F.J.J. van Loo, Acta Mater. 48, 385 (2000) 32. M.J.H. van Dal, A.M. Gusak, C. Cerhati, A. A. Kodentsov, F.J.J. van Loo, Phys. Rev. Lett. 86, 3352 (2001) 33. M.J.H. van Dal, A.M. Gusak, C. Cerhati, A. A. Kodentsov, F.J.J. van Loo, Philos. Mag. A 82, 943 (2002) 34. A. Paul, M.J.H. van Dal, A. A. Kodentsov, F.J.J. van Loo, Acta Mater. 52, 623 (2004) 35. A. Paul, A.A. Kodentsov, F.J.J. van Loo, Defect and Diﬀusion Forum 237– 240, 813 (2005) 11 Diﬀusion and External Driving Forces 11.1 Overview Diﬀusing particles experience a drift motion in addition to random diﬀusion, when an external driving force is applied. Table 11.1 lists examples of driving forces. An electric ﬁeld is the most common example of an external force and is treated in detail below. Another example is the gradient of the nonideal part of the chemical potential, which we have considered already in the previous chapter on interdiﬀusion. The nature of and analytic expressions for the driving forces can be deduced from the thermodynamics of irreversible processes (see Chap. 12 and [1, 2]). For many ionic solids (see Chaps. 26 and 27) the electrical conductivity results from the transport of ions rather than electrons as is the case in metals and semiconductors. When the charge carriers are ions in an electronically insulating crystal or glass, the ionic motion under the inﬂuence of an electric ﬁeld is described by the ionic conductivity. The dc conductivity, σdc , relates the electrical current density, j e , via Ohm’s law to the applied electric ﬁeld E: j e = σdc E . (11.1) If the ions in the material are labelled i (= 1, 2, . . .), the conductivity can be written in terms of mobilities ui and charges qi as σdc = Ci | qi | ui , (11.2) i where Ci is the number density of ions of kind i. An appropriate comparison between mobility and diﬀusivity of ions is obtained via the Nernst-Einstein relation discussed below. The interplay of electron currents and atomic ﬂuxes is necessary in the consideration of electromigration in metals [5, 6]. In metals ions are screened by the conduction electrons. Then, the eﬀective charge of an ion can be very diﬀerent from the charge of the ionic cores. An electronic current also exerts a force on the atomic species. The origin of this force is the scattering of electrons at the ion cores and the associated momentum transfer. The coupling between electronic and atomic current in metals at elevated temperatures is of considerable technical relevance, because it is the origin of electromigration. 180 11 Diﬀusion and External Driving Forces Table 11.1. Examples of driving forces for drift motion of atoms Force Expression Remarks Gradient of electrical potential E = −∇U Gradient of chemical potential (non-ideal part) Temperature gradient ∇T q∗ E q ∗ : eﬀective electric charge −∇µ µ: chemical potential −(Q∗ /T )∇T or −S∇T Q∗ : heat of transport S: Soret coeﬃcient Stress gradient −∇Uel Uel : elastic interaction energy due to stress ﬁeld Gravitational force mgz Centrifugal force m∗ ω 2 r m: particle mass g: acceleration due to gravity m∗ : eﬀective atomic mass ω: angular velocity r: distance from rotation axis The latter is a major reason for the degradation of metallic interconnects in microelectronic devices. Temperature gradients in a material can also act as driving force on diffusing atoms. The resulting eﬀect is called thermotransport (also thermomigration). If there are simultaneous gradients of temperature and of concentration, we can combine Fick’s ﬁrst law and thermotransport to give j = −D ∂T ∂C −S . ∂x ∂x (11.3) A steady state (index ss) can be established for j = 0. We then have ∂C S ∂T =− . (11.4) ∂x ss D ∂x ss This equation describes the concentration gradient established by thermotransport. This eﬀect is called the Ludwig-Soret eﬀect or often just the Soret eﬀect. The Soret coeﬃcient, S, and the heat of transport, Q∗ ≡ S/T , may be of either sign, whereas D is always positive. Thermotransport is a relatively complex phenomenon since the system is, per se, not isothermal. For a more detailed discussion the reader is referred to [3–5]. In the case of non-ideal alloys the gradient of the chemical potential gives rise to a driving force. The gradient of the chemical potential can be expressed as a sum of two terms: the ﬁrst term contains the concentration gradient and the second term the gradient of the activity coeﬃcient. This case is discussed in detail in Chaps. 10 and 12. A uniform stress ﬁeld cannot generate a particle ﬂux. However, a driving force can arise from the stress gradient. Its eﬀects must be considered 11.2 Fick’s Equations with Drift 181 whenever the interaction energy of the particle with the stress ﬁeld is large enough. Examples are the Gorski eﬀect, which can be observed for hydrogen diﬀusion in metals (see Chap. 14), and the formation of Cottrell atmospheres in the stress ﬁeld of dislocations [7]. Gravitational forces are weak and accordingly play no rôle in solid-state diﬀusion. In gases and liquids, however, gravitational forces can cause sedimentation eﬀects. The experimental observation of eﬀects of centrifugal forces requires rapid rotation. Equilibrium sedimentation of Au in solid sodium and lead has been studied in centrifuge experiments [8]. The results have been discussed to demonstrate the interstitial nature of fast diﬀusers. 11.2 Fick’s Equations with Drift Suppose that an external driving force F acts on diﬀusing particles. After a short transition period, a steady state particle ﬂux develops. The drift velocity v̄ of the particles under the action of the driving force is v̄ = uF . (11.5) u is called the mobility. The mobility is the drift velocity for a unit driving force, i.e. for F = 1. The particle ﬂux is C v̄ = CuF . The total ﬂux due to diﬀusion plus the action of the driving force is j = −D ∂C + v̄C . ∂x (11.6) The ﬁrst term is the well-known Fickian term and the second term is the drift term. Thermodynamics of irreversible processes shows that the distinction between these two terms is more practical than fundamental (see Chap. 12). Formally, the second term in Eq. (11.6) is also a ﬂux which is proportional to a gradient. In the case of an electrical driving force, this is the electrical potential gradient. If we combine Eq. (11.6) with the continuity equation (2.4), we get ∂ ∂C ∂ ∂C = (v̄C). (11.7) D − ∂t ∂x ∂x ∂x If the driving force and, consequently, the drift velocity v̄ and the diﬀusion coeﬃcient are independent of x, Eq. (11.7) reduces to ∂ 2C ∂C ∂C = D 2 − v̄ . ∂t ∂x ∂x (11.8) Then, it is possible to reduce the problem of solving the diﬀerential equation (11.8) by applying the following transformation [9, 10] v̄ v̄ 2 t x− C = C ∗ exp . (11.9) 2D 4D 182 11 Diﬀusion and External Driving Forces Fig. 11.1. Schematic illustration of diﬀusion and drift Substitution of Eq. (11.9) in Eq. (11.8) yields a linear diﬀerential equation for C ∗ ∂C ∗ = D∆C ∗ . (11.10) ∂t Hence solutions for Eq. (11.8) are available, if Eq. (11.10) can be solved for the given boundary condition. The concentration ﬁeld C(x, t) originating from a thin-ﬁlm diﬀusion source is modiﬁed by a constant driving force. The appropriate diﬀusion equation is Eq. (11.8). Its solution can be obtained by inserting the thin-ﬁlm solution without drift, Eq. (3.9), into Eq. (11.9). We get (x − v̄t)2 N exp − . C(x, t) = √ 4Dt 2 πDt (11.11) This corresponds to a Gaussian distribution, the center of which shifts with the velocity v̄. Equation (11.11) somehow justiﬁes the distinction between the Fickian term and the drift term in Eq. (11.6). The ﬁrst term leads to a broadening of the distribution of diﬀusing particles and the second term causes a translation of the whole distribution (Fig.11.1). The fact that diﬀusion leads to a Gaussian distribution of the diﬀusing particles reveals their underlying random movement, whereas under the inﬂuence of an external force an additional directed motion occurs. On the other hand, both processes involve the same elementary jumps of the particles. This indicates that D and v̄ must be related to each other. This relation is known as the Nernst-Einstein relation. Its derivation and some of its implications are considered in the following. 11.3 Nernst-Einstein Relation We consider a system with one mobile component, where the ﬂux resulting from an external driving force exactly counterbalances the diﬀusion ﬂux. The combined eﬀect of a concentration gradient and of a driving force can lead 11.3 Nernst-Einstein Relation 183 to a steady state, if the corresponding ﬂuxes are equal and opposite in sign, i.e. if the total ﬂux vanishes. Then, we get from Eq. (11.6) 0 = −D̃ ∂C + v̄C . ∂x (11.12) The diﬀusion coeﬃcient D̃ in Eq. (11.12) refers to a chemical composition gradient as will become evident below. It is deﬁnitely conceived as a chemical diﬀusion coeﬃcient not as a tracer diﬀusion coeﬃcient. Lack of appreciation of this fact leads to misunderstandings and inconsistencies. Let the diﬀusing substance be contained in a cylinder and let us suppose that v̄ = uF is the stationary velocity in negative x-direction due to an external ﬁeld. Then, the solution of Eq. (11.12) is v̄ C = C0 exp − x , (11.13) D̃ where C0 denotes the stationary concentration at x = 0. Let us further assume that the external force is the derivative of a potential U : F =− ∂U . ∂x (11.14) At thermodynamic equilibrium, the distribution of non-interacting particles must also follow the Boltzmann distribution 1 U C(x) = α exp − , (11.16) kB T where kB denotes the Boltzmann constant, T absolute temperature, and α a constant. Diﬀerentiation with respect to x yields C ∂U CF ∂C =− = . ∂x kB T ∂x kB T (11.17) Substituting this equation in Eq. (11.12), we get D̃ = v̄ RT kB T = ukB T = u . F NA (11.18) R = kB NA denotes the gas constant and NA the Avogadro number. Equation (11.18) relates the chemical coeﬃcient D̃ and the mobility u of the diﬀusing particles. This relation is called the Nernst-Einstein relation. 1 For a gas in the gravitational ﬁeld of the earth the potential acting on gas molecules is U = mgz, where m is their mass, g the acceleration in the gravitational ﬁeld, and z the height. Then we get « „ mgz . (11.15) C = C0 exp − kB T This is the well-known formula for the decrease of gas concentration in the atmosphere with increasing height. 184 11 Diﬀusion and External Driving Forces 11.4 Nernst-Einstein Relation for Ionic Conductors and Haven Ratio Let us now suppose that the external driving force is the result of an electric ﬁeld E acting on ions with charge q. Then we have F = qE . (11.19) Using Eq. (11.18) the ﬂux of ions in the electric ﬁeld can be written as j = v̄C = qC D̃ E. kB T (11.20) The associated electric current density is je = qj = q 2 C D̃ E. kB T (11.21) This equation is Ohm’s law, je = σdc E, with the ionic d.c. conductivity σdc = q 2 C D̃ . kB T (11.22) caused by the mobile ions. In the solid-state diﬀusion literature this relation is often called in a rather misleading way the Nernst-Einstein relation. However, we remind the reader that we used in its derivation Eq. (11.16) – an equation which holds for non-interacting particles only. More generally, interactions are present between the particles. For this case, Murch [11] showed that the general form of the Nernst-Einstein relation is q 2 C D̃ ∂ ln N σdc = , (11.23) kB T ∂µ where µ is the chemical potential of the particles and N their site fraction. When the distribution of particles is completely ideal (no interaction, not even site blocking eﬀects), the thermodynamic factor is unity and Eq. (11.23) reduces to Eq. (11.22). In this special case, the diﬀusion coeﬃcient D̃ equals the tracer diﬀusion coeﬃcient D∗ , so that σdc = q 2 CD∗ . kB T (11.24) When the particles are ideally distributed but subject to site blocking eﬀects, Eq. (11.23) can be written as [11] σdc = q 2 CD∗ , f kB T (11.25) 11.4 Nernst-Einstein Relation for Ionic Conductors and Haven Ratio 185 where f is the tracer correlation factor (see Chap. 4). This equation is appropriate to very dilute solutions. Ionic crystals having a virtually perfect lattice of ions fall into this category. Charge diﬀusion coeﬃcient: In the solid-state diﬀusion literature Eq. (11.22) is often used to calculate another ‘diﬀusion coeﬃcient’ called the charge diﬀusion coeﬃcient (sometimes denoted also as the conductivity diﬀusion coeﬃcient or the electrical diﬀusion coeﬃcient) via: Dσ = kB T σdc RT σdc = . Cq 2 NA Cq 2 (11.26) R denotes the gas constant and NA the Avogadro number. Dσ has indeed the dimensions of a diﬀusion coeﬃcient. However, it does not correspond to any diﬀusion coeﬃcient that can be measured by way of Fick’s laws. The identiﬁcation of Dσ with a diﬀusion coeﬃcient is only adequate for noninteracting particles. What can be done is to use Eq. (11.26) as a deﬁnition of Dσ , recognising that at the same time Dσ has no Fickian meaning. It is, however, misleading in these circumstances to call Eq. (11.26) the Nernst-Einstein equation. Equation (11.26) is then used purely as a means of changing the d.c. conductivity σdc to a quantity that has the dimensions of a diﬀusion coeﬃcient. Haven ratio: It is common practice in solid-state ionics to deﬁne the socalled Haven ratio HR , which is simply the ratio of the tracer diﬀusion coefﬁcient, D∗ , and the charge diﬀusion coeﬃcient, Dσ : HR ≡ D∗ . Dσ (11.27) In view of the remarks about Dσ , it is appropriate to ask whether the Haven ratio has a straightforward physical meaning. Apart from some simple models (mentioned below) a general theory of HR is not yet available. For a hopping model of ionic conduction, provided that the ionic jumps are mediated by low concentrations of vacancies like in NaCl (see Chap. 26), one gets [11, 13] f HR = . (11.28) fAA Here f is the tracer correlation factor of the atoms and fAA the physical or collective correlation factor (see Chap. 12). If one can neglect collective correlations, which is justiﬁed for an almost full or empty lattice of charge carriers, the interpretation of the Haven ratio is straightforward. This is the case for diﬀusion mechanisms such as the vacancy mechanism. Then, the Haven ratio simply equals the tracer correlation factor: HR ≈ f . (11.29) 186 11 Diﬀusion and External Driving Forces In such a case, from a measurement of the Haven ratio the correlation factor and then the mechanism of diﬀusion can be exposed (see Chap. 7). For a collective mechanism, such as the interstitialcy mechanism, the displacement of the charge is diﬀerent from the displacement of the tracer atom. For a colinear interstitialcy mechanism the charge moves two jump distances whereas the tracer moves only one (see Chap. 6). The Haven ratio then becomes f d2 , (11.30) HR = fAA d2q where d and dq are the jump distances of the tracer and of the charge, respectively. A classic example for identifying the mechanism using experimental Haven ratios is the work of Friauf [12] on the motion of Ag in AgBr. It was observed that the Haven ratio varies from 0.5 at low temperatures to 0.65 at high temperatures. This behaviour of the Haven ratio was attributed to the simultaneous action of colinear and non-colinear interstitialcy jumps (see Chap. 26). Much less satisfactorily interpreted are Haven ratios for fast ion conductors with highly disordered sublattices and for ion-conducting glasses. Haven ratios in such materials have been reviewed by Murch [13] and by Jain and Kanert [14]. Further comments on the subject of correlations eﬀects and ionic diﬀusion can be found in the review by Murch [11] and the literature cited therein, as well as in a paper on Monte Carlo simulations of the Haven ratio of alkali ions in oxide glasses [15]. Pressure-dependent diﬀusivities and Haven ratios in alkali borate glasses are considered by Imre et al. [18]. 11.5 Nernst-Planck Equation – Interdiﬀusion in Ionic Crystals Let us now consider two ionic system AX and BX with two ionic species A and B, which share the same sublattice of a crystal. Let us assume that only the species A and B are mobile, the X sublattice being ﬁxed. During interdiﬀusion the two mobile species compete for vacancies on the common sublattice of A and B. Let us ﬁrst consider the case of an ideal solution and the absence of an electric driving force. Then ﬂuxes jA and jB are connected to the concentration gradients via ∗ jA = −DA with ∂CA ∂x ∗ and jB = −DB ∂CB ∂CA =− . ∂x ∂x ∂CB ∂x (11.31) (11.32) 11.5 Nernst-Planck Equation – Interdiﬀusion in Ionic Crystals 187 ∗ ∗ Since DA and DB are not equal, a net ﬂux of electric charge jA = jB would develop. However, the condition of electrical neutrality requires that this net ﬂux must be zero. Any electrical ﬁeld E gives rise to drift ﬂuxes. More general, the ﬂux equations should then be written as ∗ jA = −DA ∗ qCA DA ∂CA + E ∂x kB T ∗ and jB = −DB ∗ qCB DB ∂CB + E . (11.33) ∂x kB T Here we have introduced the drift term from the Nernst-Einstein equation and q denotes the (identical) charges of ions A and B. The condition of electrical neutrality requires (11.34) jA + jB = 0 . It follows that E= ∗ ∗ DA − DB ∂CA kB T . ∗ ∗ q CA DA + CB DB ∂x (11.35) We now recall the intrinsic diﬀusivities of Eq. (10.20), which we repeat for convenience: I ∂CA I ∂CA jA = −DA and jB = −DB . (11.36) ∂x ∂x Inserting Eqs. (11.33) and (11.35), we arrive at: I I DA = DB = ∗ ∗ DB DA ∗ + N D∗ . NA DA B B (11.37) This equation is called the Nernst-Planck equation for ideal solutions. For interdiﬀusion between ionic crystals AX and BX, there is no Kirkendall eﬀect because there is no separation of charge and therefore no net vacancy ﬂow. Equation (11.37) can also be written as 1 1 NA NB + I = ∗ + ∗ . I DB DA DA DB (11.38) For a non-ideal solution Eq. (11.37) must be multiplied by the thermodynamic factor Φ: I I DA = DB = ∗ ∗ DA DB ∗ ∗ Φ ≡ D̃N ernst−P lanck . NA DA + N B DB (11.39) We mention without prove that in terms of the transport coeﬃcients discussed in Chap. 12 one gets: D̃N ernst−P lanck = 2f LAB . 1 − f NA NB (11.40) This equation shows that interdiﬀusion in ionic crystals is completely due to the oﬀ-diagonal term LAB of the Onsager matrix. 188 11 Diﬀusion and External Driving Forces 11.6 Nernst-Planck Equation versus Darken Equation The Nernst-Planck equation (11.39) and the Darken equation (10.34) diﬀer signiﬁcantly if the ratio of the tracer diﬀusivities is far from unity: D̃N ernst−P lanck = D̃Darken . (11.41) We have seen above that the interdiﬀusion coeﬃcient described by the NernstPlanck equation corresponds to a consecutive connection of the two diﬀusivities; it is controlled by the slower diﬀusing component. By contrast, the Darken expression is analogous to the paralled connection of the two diﬀusivities, which is controlled by the faster diﬀusing component. In addition, we note that the Nernst-Planck and the Darken equations represent two limiting cases of interdiﬀusion in a binary metallic alloy: We recall that the Darken equation has been derived under the assumption that vacancies are practically at thermal equilibrium during the interdiﬀusion process and that the vacancy ﬂux compensates the unequal ﬂuxes of the atomic species A and B. Usually, this is justiﬁed for a macroscopic diﬀusion sample, when suﬃcient sinks and sources for vacancies (e.g., dislocations) keep the vacancy concentration close to equilibrium in spite of non-vanishing vacancy ﬂuxes. Non-equilibrium vacancy distributions can be generated by the diﬀerence of the intrinsic ﬂuxes of atoms, if the density and/or eﬃciency of vacancy sources/sinks are insuﬃcient. Nazarov and Gurov have performed an analysis of interdiﬀusion in binary alloys taking into account non-equilibrium vacancies [16]. They have shown that the evolution of an interdiﬀusion proﬁle is then governed by D̃N azarov−Gurov = ∗ ∗ DA DB ∗ + N D ∗ Φ ≡ D̃N ernst−P lanck . NA DA B B (11.42) The Nernst-Planck expression for interdiﬀusion in ionic crystals and the Nazarov-Gurov expression for interdiﬀusion in a binary alloy with nonequilibrium vacancies are identical. Furthermore, the interdiﬀusion coeﬃcients of Darken and of NazarovGurov correspond to diﬀerent space and time regimes. This has been pointed out by Gusak and coworkers (see, e.g., [17]): – The Darken expression, Eq. (10.34), governs the interdiﬀusion process for long diﬀusion times τV . (11.43) t CV Here τV is the mean life-time of vacancies between their creation at vacancy sources and their annilhilation at vacancy sinks. CV denotes the References 189 vacancy concetration. This condition is fulﬁlled when the average dis√ tance between vacancy sources and sinks, DV τV , is small as compared to the width of the interdiﬀusion zone, i.e. for D̃Darken t DV τV , – (11.44) DV denotes the vacancy diﬀusivity. The Nazarov-Gurov equation governs the interdiﬀusion process for short diﬀusion times τV . (11.45) t CV This corresponds to D̃N azarov−Gurov t DV τV , (11.46) Then, the width of the interdiﬀusion zone is much smaller than the average distance between vacancy sources and sinks. Loosely speaking, non-equilibrium vacancies and the Nazarov-Gurov equation are important on ‘nanoscopic scales’, whereas the Darken equation is relevant for interdiﬀusion on ‘macroscopic scales’. References 1. S.R. de Groot, P. Mazur, Thermodynamics of Irreversible Processes, NorthHolland Publ. Comp., 1952 2. R.E. Howard, A.B. Lidiard, Matter Transport in Solids, in: Reports on Progress in Physics Vol. XXVII, The Institute of Physics and the Physical Society, London, 1964, pp. 161–240 3. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 4. A.R. Allnatt. A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 5. H. Wever, Elektro- und Thermotransport in Metallen, Barth-Verlag, Leipzig, 1973 6. H.B. Huntington, Electromigration in Metals, in: Diﬀusion in Solids – Recent Developments, A. S. Nowick, J.J. Burton (Eds.), Academic Press, 1975, p. 303 7. J. Völkl, G. Alefeld, Hydrogen Diﬀusion in Metals, in: Diﬀusion in Solids – Recent Developments, A. S. Nowick, J.J. Burton (Eds.), Academic Press, 1975, p. 303 8. L.W. Barr, A.D. Le Claire, Philos. Mag, 20, 1289–1291 (1969) 9. R. Fürth, Diﬀusion, in: Handbuch physikalisch, technische Mechanik, F. Auerbach, W. Hort (Eds.), Vol. 7, Leipzig, 1932 10. W. Jost, Diﬀusion in Solids, Liquids, Gases, Academic Press, Inc., New York, 1960 11. G.E. Murch, Diﬀusion Kinetics in Solids, Chap. 3 in: Phase Transformations in Materials, G. Kostorz (Ed.), Wiley-VCh Verlag GmbH, Weinheim, Germany, 2001 190 11 Diﬀusion and External Driving Forces 12. R.J. Friauf, Phys. Rev. 105, 843 (1957) 13. G.E. Murch, Solid State Ionics 7, 177 (1982) 14. H. Jain, O. Kanert, in: Defects in Insulating Materials, O. Kanert, J.-M. Spaeth (Eds.), World Scientiﬁc Publishing Comp., Ltd., Singapore, 1993 15. S. Voss, S.V. Divinski, A.W. Imre, H. Mehrer, J.N. Mundy, Solid State Ionics 176, 1383 (2005) 16. A.V. Nazarov, K.P. Gurov, Fizika Metallov Metallovedenie 37, 496 (1974); 38, 689 (1974); 45, 855 (1978) 17. A.M. Gusak, S.V. Kornienko, G.V. Lutsenko, presented at Int. Workshop on Diﬀusion and Stresses (DS 2006), Lillafüred, Hungary, 2006 18. A.W. Imre, S. Voss, H. Staesche, M.D. Ingram, K. Funke, H. Mehrer, J. Phys. Chem. B, 111, 5301–5307 (2007) 12 Irreversible Thermodynamics and Diﬀusion 12.1 General Remarks So far, we have discussed the usual descriptions of atomic transport in solids such as diﬀusion and ionic conduction. Fick’s ﬁrst law was introduced as a postulate describing a linear relationship between the ﬂux of a diﬀusing species i and its concentration gradient. Ohm’s law describes a linear relation between the ﬂux of charged species and the gradient of the electric potential. Fourier’s law is a linear relation between the ﬂux of heat and the temperature gradient. However, these simple laws may not be suﬃcient even within the stated limitation of linear eﬀects. For example, Fick’s ﬁrst law is sometimes insuﬃcient for attaining equilibrium of species i because it does not recognise all driving forces, direct or indirect, acting on i. It may be necessary to allow that a concentration gradient in one species gives rise to a ﬂux of another. Diﬀusion, electrical conduction, and heat ﬂow are examples of irreversible processes. Non-equilibrium thermodynamics provides a general phenomenological theory of such processes. In this chapter, we brieﬂy introduce the macroscopic equations of this theory suggested for the ﬁrst time by Lars Onsager (1903–1976), the Norwegian Nobel laureate of 1968. Wide-ranging treatments, especially of macroscopic formulations of this theory can be found in textbooks of de Groot and Mazur [1] and Haase [2]. A treatment with emphasis on the foundations of irreversible thermodynamics by statistical mechanics has been provided by Kreuzer [3]. Non-equilibrium thermodynamics is based on three major assumptions: 1. The Onsager transport equations of atoms, heat, and electrons are linear relations between the ﬂuxes J i and the so-called generalised thermodynamic forces X i . The phenomenological response for the complete set of n ﬂuxes assumes a linear form Ji = n Lij X j , (12.1) j=1 where Lij are called the phenomenological coeﬃcients or transport coefﬁcients. The matrix of coeﬃcients is also called the Onsager matrix or simply the L matrix. The great importance of the phenomenological coeﬃcients stems from their independence of driving forces. For example, 192 12 Irreversible Thermodynamics and Diﬀusion in solid-state diﬀusion problems the coeﬃcients Lij are functions of temperature and pressure, but they do not depend on the gradient of the chemical potential. 2. The Onsager matrix is composed in part of diagonal terms, Lii , connecting each generalised force with its conjugate ﬂux. For example, a gradient of the chemical potential causes a generalised diﬀusion ‘force’, and the associated diﬀusion response is determined by the material’s diﬀusivity. Similarly, an applied temperature gradient creates a generalised force associated with heat ﬂow. In this case, the amount of heat ﬂow is determined by the thermal conductivity. The Onsager matrix also contains oﬀ-diagonal coeﬃcients, Lij . Each oﬀdiagonal coeﬃcient determines the inﬂuence of a generalised force on a non-conjugate ﬂux. For example, a concentration gradient of one species can give rise to a ﬂux of another species. The electric ﬁeld, which exerts a force on electrons in metals to produce an electric current has a crossinﬂuence on the ﬂow of heat, known as the Peltier eﬀect. Conversely, the thermal force (temperature gradient) that normally causes heat ﬂow, also has a cross-inﬂuence on the distribution of electrons – known as the Thomson eﬀect. The Thomson and Peltier eﬀects combine and provide the basis for thermoelectric devices: thermopiles can be used to convert heat ﬂow into electric current; in thermocouples a voltage is produced by a temperature diﬀerence. Another example is that an electronic current and the associated ‘electron wind’ causes a ﬂow of matter called electromigration (see also Chap. 11). Electromigration can be a major cause for the failure of interconnects in microelectronic devices. The Onsager matrix is symmetric, provided that no magnetic ﬁeld is present. The relationship (12.2) Lij = Lji is known as the Onsager reciprocity theorem. 3. The central idea of non-equilibrium thermodynamics is that each of the thermodynamic forces acting with its ﬂux response dissipates free energy and produces entropy. The characteristic feature of an irreversible process is the generation of entropy. The rate of entropy production, σ, is basic to the theory. It can be written as: Tσ = n J iX i + J q X q . (12.3) i J i denotes the ﬂux of atoms i and J q the ﬂux of heat. The thermodynamic forces require some explanation: X i and X q are measures for the imbalance generating the pertinent ﬂuxes. The thermal force X q 1 (12.4) X q = − ∇T T 12.2 Phenomenological Equations of Isothermal Diﬀusion 193 is determined by the temperature gradient ∇T . When only external forces are acting, the X i are identical with these forces. If, for example, an ionic system with ions of charge qi is subject to an electric ﬁeld E, each ion of type i experiences a mechanical force F i = qi E. In the presence of a composition gradient the appropriate force is related to the gradient of chemical potential ∇µi . Then, the thermodynamic force Xi is the sum of the external force exerted by the electric ﬁeld and the gradient of the chemical potential of species i: µ i = F i − ∇µi . (12.5) Xi = F i − T ∇ T Here the gradient of the chemical potential is that part due to gradients in concentration, but not to temperature. Thermodynamic equilibrium is achieved when the entropy production vanishes: σ = 0. (12.6) Then, there are no irreversible processes any longer and the thermodynamic forces and the ﬂuxes vanish. 12.2 Phenomenological Equations of Isothermal Diﬀusion In this section, we apply the phenomenological transport equations to solidstate diﬀusion problems. We give a brief account of some major aspects relevant for transport of matter, which are treated in more detail in [4–6]. The phenomenological equations are on the one hand very powerful. On the other hand, they lead quickly to cumbersome expressions. Therefore, only a few examples will be given. Detailed expressions for the phenomenological coefﬁcients in terms of the elementary jump characteristics must be provided by atomistic models. Here, we consider the consequences of phenomenological equations for isothermal diﬀusion. In a binary system we have 3 transport coeﬃcients – two diagonal ones and one oﬀ-diagonal coeﬃcient. For a ternary system six transport coeﬃcients must be taken into account. One of the crucial questions is, whether the oﬀ-diagonal terms are suﬃciently diﬀerent from zero to be important for data analysis. If they are negligible, the analysis can be largely simpliﬁed. This assumption in made in some models for diﬀusion, e.g., in the derivation of the Darken equations for a binary system (see Chap. 10). We shall see below, however, that neglecting oﬀ-diagonal terms is not always justiﬁed. 12.2.1 Tracer Self-Diﬀusion in Element Crystals Fundamental mobilities of atoms in solids can be obtained by monitoring radioactive isotopes (‘tracers’) (see Chap. 13). Let us consider the diﬀusion 194 12 Irreversible Thermodynamics and Diﬀusion of an isotope A∗ in a solid A, where A∗ and A are chemically identical. Let us further suppose that diﬀusion occurs via vacancies (index V ). Taking into account the reciprocity relations, the Onsager ﬂux equations can be written as1 : JA∗ = LA∗ A∗ XA∗ + LA∗ A XA + LA∗ V XV , JA = LA∗ A XA∗ + LAA XA + LAV XV , JV = LA∗ V XA∗ + LAV XA + LV V XV . (12.7) Let us now suppose that in an isothermal experiment vacancies are always maintained at thermal equilibrium. This is possible if sources and sinks of vacancies such as dislocations are suﬃciently numerous and active during the diﬀusion process. Under such conditions, the chemical potential of vacancies is constant everywhere and hence XV = 0. Then, the ﬂux equations for the components apply directly in the laboratory reference frame: JA∗ = LA∗ A∗ XA∗ + LA∗ A XA JA = LA∗ A XA∗ + LAA XA . (12.8) ∗ Tracer atoms A and matrix atoms A form an ideal (isotopic) solution. Let CA∗ and CA denote their concentrations and µA∗ and µA their chemical potentials, respectively. These are: µA∗ = µ0A∗ (p, T ) + kB T ln CA∗ , µA = µ0A (p, T ) + kB T ln CA . (12.9) The reference potentials µ0A∗ (p, T ) and µ0A (p, T ) depend on pressure and temperature but not on concentration. The corresponding forces are 1 ∂CA∗ , CA∗ ∂x 1 ∂CA XA = −kB T . CA ∂x For tracer self-diﬀusion in an element crystal we have XA∗ = −kB T JA∗ + JA = 0 , (12.10) (12.11) i.e. the ﬂuxes are equal in magnitude and opposite in sign. Furthermore, since CA∗ +CA is constant, the concentration gradients are equal in magnitude and opposite in sign, i.e. ∂CA∗ /∂x = −∂CA /∂x. We then have L A∗ A∗ L A∗ A ∂CA∗ , (12.12) − JA∗ = − kB T CA∗ CA ∂x ∗ JA = − 1 A DA LAA L A∗ A − CA CA∗ kB T ∂CA . ∂x (12.13) For simplicity reasons we consider unidirectional ﬂow (in x direction) and omit the vector notation. 12.2 Phenomenological Equations of Isothermal Diﬀusion 195 Since JA∗ = −JA we get: L A∗ A∗ L A∗ A LAA LA∗ A − = − ∗ . CA∗ CA CA CA (12.14) Recalling that the diﬀusivity of a tracer is deﬁned through Fick’s law A JA∗ = −DA ∗ ∂CA∗ , ∂x we obtain by comparison with Eqs. (12.12): L A∗ A∗ LAA L A∗ A L A∗ A A∗ − − kB T = kB T DA = CA∗ CA CA CA∗ Since for tracer diﬀusion always CA∗ CA , we also have LAA L A∗ A∗ L A∗ A A∗ DA = kB T = − kB T . CA∗ CA CA∗ (12.15) (12.16) (12.17) The ﬁrst term on the right-hand side of Eq. (12.17) is sometimes denoted A A as the ‘true’ self-diﬀusion coeﬃcient, DA ≡ kB T LAA /CA . The quantity DA denotes self-diﬀusion in the absence of a tracer – a quantity that is diﬃcult to measure directly2 . We then get LA∗ A CA A∗ A DA = 1 − DA , (12.18) LAA CA∗ f where f is the correlation factor of tracer self-diﬀusion (see Chap. 7). This equation shows that the coupling between the ﬂuxes is the origin of correlation eﬀects. For LA∗ A = 0 the correlation factor would be unity. We also note that in addition to the defect two atomic species (here A∗ and A) must be present to obtain correlation. This is a rule that we have already stated in Chap. 4. 12.2.2 Diﬀusion in Binary Alloys In this section, we discuss the Onsager equations for solid-state diﬀusion via vacancies in a substitutional binary alloy and the structure and physical meaning of the pertinent phenomenological coeﬃcients. We suppose that the system is isothermal and that external forces are absent, i.e. Xq = 0 and Fi = 0. We then have a system of two atomic components A and B and vacancies (index V) on a single lattice. Taking into account the reciprocity relations the Onsager ﬂux equations can be written as: 2 In favourable cases, PFG-NMR (see Chap. 13) can be applied to measure this quantity. 196 12 Irreversible Thermodynamics and Diﬀusion JA = LAA XA + LAB XB + LAV XV , JB = LAB XA + LBB XB + LBV XV , JV = LAV XA + LBV XB + LV V XV . (12.19) To promote atomic diﬀusion, either A or B atoms exchange with vacancies on the same lattice. Therefore, the ﬂuxes deﬁned relative to that lattice (in regions outside the diﬀusion zone) necessarily must obey JV = −(JA + JB ) . (12.20) In other words, the ﬂux of vacancies is equal and opposite in sign to the total ﬂux of atoms3 . In view of the constraint imposed by Eq. (12.20), each term on the right-hand side of Eq. (12.19) must vanish column by column. We get: (LAA + LAB + LAV )XA = 0, (LAB + LBB + LBV )XB = 0, (LAV + LBV + LV V )XV = 0 . (12.21) These equations must hold for arbitrary values of the forces Xi . Hence each bracket term must vanish separately: −LAV = LAA + LAB , −LBV = LAB + LBB , −LV V = LAV + LBV . (12.22) These equations show that the kinetic coeﬃcients of the vacancy ﬂux are related to those of the atomic species. If Eq. (12.22) is combined with the ﬂux equations (12.19), the following expressions for the ﬂuxes of the atomic species are obtained: JA = LAA (XA − XV ) + LAB (XB − XV ), JB = LAB (XA − XV ) + LBB (XB − XV ) . (12.23) The vacancy ﬂux may be written as JV = LAV (XA − XV ) + LBV (XB − XV ) . (12.24) Let us now assume that vacancies are always maintained close to their thermal equilibrium concentration. Then, the chemical potential of vacancies is constant everywhere and XV = 0. Equations (12.23) then reduce to JA = LAA XA + LAB XB , JB = LAB XA + LBB XB . 3 (12.25) In this context the reader should also see the discussion of the ‘vacancy wind’ in Chap. 10. 12.2 Phenomenological Equations of Isothermal Diﬀusion 197 The chemical potential of a real solid solution is given by µi = µ0i (p, T ) + kB T ln(Ni γi ) , (12.26) where γi is the activity coeﬃcient and Ni mole fractions of species i. Using NA + NB ≈ 1, i.e. CV CA + CB , we obtain: LAA ∂NA LAB JA = − , − kB T Φ NA NB ∂x JB = − I DA LBB LAB − NB NA I DB ∂NB . kB T Φ ∂x (12.27) Here we have used that the Gibbs-Duhem relation of thermodynamics provides an additional constraint: the factors (1 + ∂ ln γA /∂ ln NA ) and (1 + ∂ ln γB /∂ ln NB ) are equal to each other. This common factor is abbreviated by Φ and denoted as the thermodynamic factor (see Chap. 10). We note that one common thermodynamic factor exists for binary alloys. For ternary or higher order systems several thermodynamic factors are necessary. Equations (12.27) have the form of Fick’s ﬁrst law with diﬀusion coeﬃI I and DB , denoted as the intrinsic diﬀusion coeﬃcients: cients, DA LAA LAB NA I = DA 1− kB T Φ, NA LAA NB LBB LAB NB I = (12.28) DB 1− kB T Φ . NB LBB NA The intrinsic diﬀusivities are in general diﬀerent and can be determined separately. The two quantities that are usually measured to obtain the intrinsic diﬀusivities are (i) the chemical interdiﬀusion coeﬃcient D̃, and (ii) the Kirkendall velocity vK (see Chap. 10): In interdiﬀusion plus Kirkendall experiments, diﬀusion couples (either AB or Ax B1−x -Ay B1−y ) are studied and the initial interfaces contain inert markers. The ﬂuxes JA and JB relative to the local crystal lattice are generally such that their sum is non-zero, which according to Eq. (12.20) implies that the vacancy ﬂux is also non-zero. Since the ﬂuxes vary with position one also has: (12.29) divJV = div(−JA − JB ) = 0 . This condition requires vacancies to disappear or to be created at inner sources or sinks (e.g., dislocations) in the diﬀusion zone of the sample. When this occurs, regions where diﬀusion ﬂuxes are large will move relative to regions where ﬂuxes are small. The concentration distribution after an interdiﬀusion experiment, analysed with respect to the unaﬀected ends of the 198 12 Irreversible Thermodynamics and Diﬀusion couple, links the concentration gradients to the ﬂuxes of atoms relative to the ﬁxed parts of the sample. In the simplest case these ﬂuxes are JA = JA − NA (JA + JB ) , = JB − NB (JA + JB ) . JB (12.30) Here we have assumed that the velocity v of the local lattice relative to the non-diﬀusing parts of the sample is −v(JA + JB ). This implies that there is no change in the cross-section or shape of the sample, i.e. that the vacancies condense on lattice planes perpendicular to the diﬀusion ﬂow. It also implies that the volume per lattice site remains constant. From Eqs. (12.27), (12.30), and NA + NB = 1, because the vacancy site fraction is very small, it also follows I I JA = −(NB DA + N A DB ) ∂NA , ∂x I I JB = −(NB DA + N A DB ) ∂NB . ∂x (12.31) The quantity I I + N A DB . D̃ = NB DA (12.32) is the interdiﬀusion coeﬃcient introduced already in Chap. 10. It is the same for both components. The Kirkendall velocity vK characterises the motion of the diﬀusion zone relative to the ﬁxed end of the sample and can be observed by inserting inert markers (see Chap. 10). Since ∂NA /∂x = −∂NB /∂x it is given by: I I ∂NA . (12.33) − DB ) vK = (DA ∂x The Kirkendall eﬀect is a consequence of unequal intrinsic diﬀusivities and results from the non-zero vacancy ﬂux in the diﬀusion zone. We now have convinced ourselves that the equations of Darken and Manning discussed in Chap. 10 have a basis in the phenomenological equations. We note, however, that although measurements of interdiﬀusion and the Kirkendall shift have been made on a number of alloy systems it is clear that only I I two quantities, DA and DB , can be obtained. This is insuﬃcient to deduce the three independent phenomenological coeﬃcients LAA , LAB , and LBB for a binary alloy system. Such a situation, in which the number of experimentally accessible quantities is less than the number of the independent Onsager coeﬃcients, is not uncommon. This is one reason for the theoretical interest in these coeﬃcients. It is also the reason for the interest in relations between the phenomenological coeﬃcients. Such relations are called ‘sum rules’. Sum rules have been identiﬁed in several cases [6] and some of them are discussed in Sect. 12.3.2. 12.3 The Phenomenological Coeﬃcients 199 12.3 The Phenomenological Coeﬃcients The physical meaning of diﬀusion coeﬃcients is well appreciated. However, this is less so for the phenomenological coeﬃcients. The purpose of this section is to provide some insight into the phenomenological coeﬃcients, their structure, relations between phenomenological coeﬃcients and diﬀusion coefﬁcients, and relations among phenomenological coeﬃcients. An introduction for non-specialists in this area, which we follow in parts below, has been given by Murch and Belova [6]. Consider, for example, diﬀusion in a binary alloy. We have eliminated the vacancies as a third component because we have made the assumption that vacancies are maintained at their equilibrium concentration. Then, it suﬃces to introduce the phenomenological coeﬃcients LAA , LAB , and LBB as we have done in the previous section. According to the Onsager reciprocity theorem the L matrix is symmetric, i.e. LAB = LBA . We simply have three independent coeﬃcients, two diagonal ones and one oﬀ-diagonal coeﬃcient. Let us now consider a ‘thought experiment’: suppose that A atoms in a binary AB alloy can respond to an external electric ﬁeld E but the B atoms cannot. This is expressed by writing the driving force on A with charge qA as XA = qA E, whereas the driving force on B is XB = 0. One might ﬁrst expect that the A atoms would simply drift in the ﬁeld and the B atoms would be unaﬀected. The Onsager ﬂux equations show indeed that the ﬂux of A atoms is given by JA = LAA qA E. But the Onsager ﬂux equations also show that the ﬂux of B atoms is not zero but given by JB = LAB qA E. This equation says that the B atoms should also drift in the ﬁeld, although the B atoms do not feel the ﬁeld directly. The drifting A atoms appear to drag the B atoms along with them, thereby giving rise to a ﬂux of B atoms. In principle, the oﬀ-diagonal coeﬃcient LAB can be either positive or negative depending on the type of interaction. If LAB were to be negative, it would mean that the B atoms would drift up-ﬁeld whilst the A atoms drift down-ﬁeld. This example may suﬃce to illustrate that the oﬀ-diagonal coeﬃcient can be responsible not only for an atomic ﬂux but also that it can change the magnitude and even the direction of an atom ﬂux. As discussed in Chap. 4, the tracer diﬀusion coeﬃcient is related to the mean square of the displacement R of a particle during time t as [8]: D∗ = R2 , 6t (12.34) where the brackets indicate an average over an ensemble of a large number of particles. This relation is called the Einstein relation or sometimes also the Einstein-Smoluchowski relation. The diﬀusion coeﬃcient is understood to be a tracer diﬀusion coeﬃcient indicated by the superscript * placed on D. The implication is that in principle we can follow each particle explicitly. 200 12 Irreversible Thermodynamics and Diﬀusion The Einstein expression for tracer diﬀusion coeﬃcient is usually expanded for solid-state diﬀusion according to ‘hopping models’, in which atoms jump from one site to another in a lattice with a long residence time at lattice sites between the jumps. For the simplest case, diﬀusion on a cubic Bravais lattice with jump distance d and jump rate Γ , we have (see Chap. 6) D∗ = 1 2 d Γf 6 (12.35) where f is the tracer correlation factor. This equation shows that the tracer diﬀusion coeﬃcient is the product of two parts: a correlated part embodied in the tracer correlation factor and an uncorrelated part that contains the jump distance squared and the jump rate. We remember that according to Eq. (7.22) the tracer correlation factor can be expanded as f =1+2 ∞ cos θ(j) . (12.36) j=1 cos θ(j) is the average of the cosine of the angle between the ﬁrst and the j’s succeeding tracer jump. In vacancy-mediated solid-state diﬀusion cos θ(1) is invariably negative because the ﬁrst jump is more likely to be reversed, either as the result of the vacancy being still present at the nearest-neighbour site to the tracer, or perhaps as a result of re-ordering jump immediately following a disordering one, or a combination of both. For a vacancy mechanism the values of cos θ(j) also alternate in sign. The phenomenon of tracer correlation has been the subject of an extensive literature over several decades and is discussed in Chap. 7. In 1982 Allnatt [7] showed on the basis of a linear response theory that the phenomenological coeﬃcients for isothermal diﬀusion in solids can be expressed via generalised Einstein formulae, similar in character to the Einstein-Smoluchowski relation. These relations can be written as: Ri · Ri , 6V kB T t Ri · Rj , = 6V kB T t Lii = Lij (12.37) where Ri and Rj are the collective displacements of atoms i and j, V is the volume of the system. The collective displacement of a species in each case can be thought of as the displacement of the centre of mass of that species. Imagine in a ‘thought experiment’ a volume V containing N lattice sites on which two species A and B are randomly distributed. This might represent a binary alloy. Let diﬀusion occur for some time t. Then, we calculate the displacements of the centres of mass of A atoms, RA , and of B atoms, RB , and repeat the experiment a large number of times in order to produce the ensemble average. In this way, we would be able to calculate the 12.3 The Phenomenological Coeﬃcients 201 phenomenological coeﬃcients LAA , LBB , and LAB from Eqs. (12.37). This provides indeed a convenient route for the evaluation of the phenomenological coeﬃcients in Monte Carlo computations (see, e.g., [9, 10]). Similar to the tracer diﬀusion coeﬃcient the phenomenological coeﬃcients can be decomposed into correlated and into non-correlated parts Lii = fii d2 Ci ni , 6kB T t (12.38) (i) Lij fij d2 Ci ni , = 6kB T t or alternatively (12.39) (j) Lij = fij d2 Cj nj . 6kB T t (12.40) ni denotes the number of jumps of species i during the time t. Ci = Ni N/V with Ni denoting the fraction of species i and N the total number of sites in volume V . The correlated parts of the phenomenological coeﬃcients, the fij , are denoted as the correlation functions or collective correlation factors. In very much the same way that the tracer correlation factors can be expressed in terms of the average cosines of the angles between a given jump of the tracer and its succeeding jumps via Eq. (12.36), the diagonal and oﬀ-diagonal collective correlation factors can also be expressed in terms of the average of the cosines of the angle between a given jump of a species and the subsequent jump of the same (diagonal) or another (oﬀ-diagonal) species. The diagonal correlation factors are given by fii = 1 + 2 ∞ (k) cos θii , (12.41) k=1 (k) where cos θii is the average of the cosine of the angle between some jump of an atom of species i and the k’th succeeding jump of the same or another atom of species i. The expressions for the oﬀ-diagonal collective correlation factors are a bit more complicated in notation, but they are structurally related to Eq. (12.41). For simplicity, the following expression are given only for a binary system: (A) fAB = ∞ (k) cos θAB + k=1 (B) fAB = ∞ CA nA (k) cos θAB + CB nB k=1 (k) ∞ CB nB (k) cos θBA , CA nA k=1 ∞ (k) cos θBA , (12.42) (12.43) k=1 where cos θij is the average cosine of the angle between any given jump of the i species and the k’th succeeding jump of the j species. 202 12 Irreversible Thermodynamics and Diﬀusion 12.3.1 Phenomenological Coeﬃcients, Tracer Diﬀusivities, and Jump Models Tracer diﬀusion coeﬃcients are directly accessible from experiments (see Chap. 13). On the other hand, direct measurements of phenomenological coeﬃcients are diﬃcult. Accordingly, there is interest in relations between the tracer diﬀusivities and phenomenological coeﬃcients. There are also expressions for phenomenological coeﬃcients in terms of atomistic hopping models. In what follows, we consider examples of such relations and expressions. Relations for Self-diﬀusion: In the previous section, we obtained equations which related kinetic coeﬃcients for an element crystal to the tracer self-diﬀusion coeﬃcient. After some algebra we get L A∗ A∗ ≈ and A CA∗ DA kB T ∗ (12.44) ∗ LAA∗ = LA∗ A A (1 − f ) CA∗ DA . = kB T f (12.45) The oﬀ-diagonal transport coeﬃcient is related to tracer correlation. For uncorrelated diﬀusion, i.e. for f = 1, it vanishes. Relations for Dilute Binary Alloys: For a dilute alloy of solute B in solvent A, i.e. for NB → 0 we have Φ → 1. It can be shown that L BB /NB approaches a ﬁnite value, whereas LAB /NA goes to zero. Then, we get from the second equation (12.28): I DB (0) = kB T LBB B∗ = DA (0) , NB (12.46) ∗ B (0) is the solute diﬀusion coeﬃcient at inﬁnite dilution. It is meawhere DA surable, e.g. by using tracer B ∗ . From the ﬁrst equation (12.28) we have LAA LAA LAB NA I DA (0) = kB T . (12.47) 1− kB T = CA LBB NB NA In this case the oﬀ-diagonal term LAB cannot be neglected. It may be of some interest to consider in a very dilute alloy the phenomenological coeﬃcients in the framework of the ﬁve-frequency model of diﬀusion suggested by Lidiard. This model is described in Chap. 7. It is very useful for describing solute and solvent diﬀusion in a very dilute binary alloy. We remind the reader that in this model ﬁve exchange jump-rates between vacancies and A or B atoms are speciﬁed, namely: ω2 for solutevacancy exchange, ω1 for rotation of the vacancy-solute complex, ω3 (ω4 ) for dissociation (association) of the vacancy-solute complex, and ω for vacancy jumps in the solvent. According to [4] the phenomenological coeﬃcients are: 12.3 The Phenomenological Coeﬃcients LAA LBB LAB 203 ω4 d2 ωCV = ω 1 − 12NB kB T ω3 7ω3 ω d2 CV NB ω4 40ω1 ω3 + 40ω32 + 14ω2 ω3 + 4ω1 ω2 + − kB T ω3 ω1 + ω2 + 7ω3 /2 ω4 2 d CV NB ω4 ω2 (ω1 + 7ω3 /2) = kB T ω3 ω1 + ω2 + 7ω3 /2 2 d CV NB ω4 ω2 (−2ω1 + 7ω3 ) = (12.48) kB T ω3 ω1 + ω2 + 7ω3 /2 The so-called Heumann relation [18] was also derived on the basis of the ﬁve-frequency model. It can be shown that in the limit CB → 0, the ratio of LAB (0)/LBB (0) is given by: ∗ I DA (0) 1 DA LAB (0) (0) , (12.49) = A − ∗ ∗ B (0) f A (0) LBB (0) DA DA ∗ ∗ A B I where DA (0), DA (0) are the tracer diﬀusivities of A and B and DA (0) the intrinsic diﬀusion coeﬃcient of A in the limit CB → 0. Relations for Concentrated Binary Alloys: Let us ﬁrst brieﬂy consider relations based on the original Darken equations [11]. In essence, Darken neglects the oﬀ-diagonal coeﬃcients entirely. If this is assumed, the diagonal phenomenological coeﬃcients can be related to the corresponding tracer diﬀusion coeﬃcient in a binary alloy: ∗ LAA A NA DA , ≈ kB T ∗ LBB B NB DB , ≈ kB T LAB = 0 . (12.50) The Darken equations neglect all correlation information as embodied in tracer correlation factors, collective correlation factors, and vacancy-wind factors [24]. The neglect of the oﬀ-diagonal phenomenological coeﬃcients can be dangerous. However, in most cases, it is reasonable as a ﬁrst approximation. The random alloy model with the vacancy mechanism introduced by Manning is probably the most important model for dealing with diﬀusion in concentrated alloys that are disordered [12, 13]. The atomic species A and B exchange sites with vacancies with the jump rates ωA or ωB , respectively. Then, the Darken relation is replaced by the Darken-Manning relation which includes the vacancy wind corrections (see Chap. 10). In the random alloy model, the phenomenological coeﬃcients are directly related to the tracer diﬀusion coeﬃcients via the Manning relations: ∗ ∗ Ni Dii Ni Dii (1 − f ) Lii = , 1+ A∗ + N D B ∗ kB T f NA DA B B ∗ LAB = ∗ A B NA DA NB DB (1 − f ) . ∗ A + N DB∗ ) f kB T (NA DA B B (12.51) 204 12 Irreversible Thermodynamics and Diﬀusion f is the tracer correlation factor: e.g., f = 0.781 for the fcc lattice and f = 0.732 for the bcc lattice. The random alloy model seems to have more general validity. Computer simulations by Murch and coworkers have shown that the Manning relations are quite good approximations, even for ordered alloys, at least at low levels of order [14–16]. The Manning relations have also been re-derived for ordered alloys [17]. 12.3.2 Sum Rules – Relations between Phenomenological Coeﬃcients Various relations usually called sum rules have been identiﬁed between the phenomenological coeﬃcients in randomly mixed systems. Sum rules reduce the number of independent phenomenological coeﬃcients. As an example, we consider the sum rules between the phenomenological coeﬃcients in the random alloy model with a vacancy mechanism. The atomvacancy exchange rates ωi can be considered in two rather diﬀerent ways. In the ﬁrst way, one can consider them as explicit jump rates that depend only on the species i and not on the surroundings. For example, ωA in the binary random alloy then simpls represents the average jump rate of a given A atom at all compositions and environments. In the second more general way, one considers that the ωi represent an average jump rate of species i as it migrates through the lattice sampling the various environments. Since the average environment of an atom will change with composition, the ωi can also be expected to change with composition. Moleko and Allnatt [19] identiﬁed the following sum rules for an n-component random alloy for diﬀusion via a vacancy mechanism: n i=1 Lij ωj Zd2 CV ωj Nj , = ωi 6kB T j = 1, . . . , n . (12.52) Here Z is the coordination number and d the jump distance. Equations (12.52) relate the phenomenological coeﬃcients to the vacancy-atom exchange rates and reduce the number of independent phenomenological coeﬃcients. In addition, we mention that the sum rules can be restated in terms of collective correlation factors as: n i=1 (j) ωj fij ωi = 1, j = 1, . . . n . (12.53) For a binary random alloy the sum rule relations (12.52) reduce to two equations: References 205 LAA + LAB ωA Zd2 CV ωA NA , = ωB 6kB T (12.54) LBB + LAB ωB Zd2 CV ωB NB . = ωA 6kB T (12.55) Hence there is only one independent coeﬃcient and not three. In a ternary random alloy, the number of independent coeﬃcients is reduced from six to three. On the other hand, the reader should keep in mind that the random alloy model introduces two vacancy jump rates for a binary alloy and three jump rates for a ternary alloy. For the derivation of sum rules we refer the reader to the original papers. The sum rules introduced by Moleko and Allnatt for the random alloy model were the ﬁrst ones that were discovered. In the meantime, various sum rules have been identiﬁed for a number of other mechanisms and situations by Murch and coworkers. Such situations include the dumb-bell interstitial mechanism in the binary random alloy [20], the divacancy mechanism in the fcc random alloy [21], the vacancy-pair mechanism in ionic materials with randomly mixed cations [22], and for an intermetallic compound with randomly mixed sublattices [23]. Interdiﬀusion data in multicomponent alloys as a source of quantitative fundamental diﬀusion information are summarised in [24]. References 1. S.R. de Groot, P. Mazur, Non-equilibrium Thermodynamics, North-Holland, Amsterdam, 1962 2. R. Haase, Thermodynamics of Irreversible Processes, Addison Wesley, Reading, 1969 3. J.H. Kreuzer, Non-equilibrium Thermodynamics and its Statistical Foundations, Clarendon Press, Oxford, 1981 4. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 5. A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 6. G.E. Murch, I.V. Belova, Phenomenological Coeﬃcients in Solid-State Diﬀusion: an Introduction, in: Diﬀusion Fundamentals, p. 105; J. Kärger, F. Grinberg, P. Heitjans (Eds.), Universitätsverlag Leipzig, 2005 7. A.R. Allnatt, J. Phys. C: Solid State Phys. 15, 5605 (1982) 8. A. Einstein, Annalen der Physik 17, 549 (1905) 9. A.R. Allnatt, E.L. Allnatt, Philos. Mag. A 49, 625 (1984) 10. I.V. Belova, G.E. Murch, Philos. Mag. A 49, 625 (2000) 11. L.S. Darken, Trans-Am. Inst. Min. Metall. Engrs. 175, 184 (1948) 12. J.R. Manning, Diﬀusion Kinetics for Atoms in Crystals, van Norstrand, Princeton, 1968 13. J.R. Manning, Phys. Rev. B4, 1111 (1971) 14. L. Zhang, W.A. Oates, G.E. Murch, Philos. Mag. 60, 277 (1989) 206 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 12 Irreversible Thermodynamics and Diﬀusion I.V. Belova, G.E. Murch, J. Phys. Chem. Solids 60, 2023 (1999): I.V. Belova, G.E. Murch, Philos. Mag. A 78, 1085 (1998) I.V. Belova, G.E. Murch, Philos. Mag. A 75, 1715 (1997) Th. Heumann, J. Phys. F: Metal Physics 9, 1997 (1979) L.K. Moleko, A.R. Allnatt, Philos. Mag. A 59, 141 (1989) S. Sharma, D.K. Chatuvedi, I.V. Belova, G. E. Murch, Philos. Mag. A 81, 431 (2001) I.V. Belova, G.E. Murch, Philos. Mag. Lett. 81, 101 (2001) I.V. Belova, G.E. Murch, Philos. Mag. Lett. 84, 3637 (2004) I.V. Belova, G.E. Murch, Defect and Diﬀusion Forum 194–199, 547 (2001) I.V. Belova, G.E. Murch, Defect and Diﬀusion Forum 263, 1 (2007) Part II Experimental Methods 13 Direct Diﬀusion Studies 13.1 Direct versus Indirect Methods There are numerous experimental methods for studying diﬀusion in solids. They can be grouped roughly into two major categories (see Table 13.1). Direct methods are based on the laws of Fick and the phenomenological deﬁnition of the diﬀusion coeﬃcient therein. They are sensitive to long-range diﬀusion and in this sense they are macroscopic. The radiotracer method is the standard technique for the study of selfand solute diﬀusion, if radioisotopes with suitable half-lives are available. The tracer method is element-selective and due to the use of nuclear counting facilities highly sensitive. It can cover a large range of diﬀusivities provided that both mechanical and sputter sectioning techniques are used for depth proﬁling. Further proﬁling techniques for diﬀusion studies are secondary ion mass Table 13.1. Survey of experimental methods for direct and indirect diﬀusion studies in solids Direct methods Tracer diﬀusion plus depth proﬁling Indirect methods Mechanical spectroscopy (after eﬀect, internal friction, Gorski eﬀect) Chemical diﬀusion plus proﬁling Magnetic relaxation Proﬁling techniques: (for ferromagnetc materials) - Mechanical and sputter proﬁling Nuclear magnetic relaxation (NMR): - Secondary ion mass spectrometry (SIMS) - Line-shape spectroscopy - Electron microprobe analysis (EMPA) - Spin lattice relaxation spectroscopy - Auger electron spectroscopy (AES) - Spin alignment experiments (SAE) Spreading resistance proﬁling (SRP) Impedance spectroscopy (IS) for semiconductors for ion conductors Rutherford backscattering (RBS) Mössbauer spectroscopy (MBS) Nuclear reaction analysis (NRA) Quasielastic neutron scattering (QENS) Field gradient NMR (FG-NMR) Pulsed ﬁeldgradient NMR (PFG-NMR) 210 13 Direct Diﬀusion Studies spectrometry (SIMS), electron microprobe analysis (EMPA), Auger electron spectroscopy (AES). SIMS and AES both utilise sputter proﬁling and are appropriate for small diﬀusion distances and low diﬀusivities. AES is applicable for diﬀusion of foreign atoms, since it discriminates between diﬀerent elements but not between isotopes of the same element. EMPA is the major tool for the study of chemical diﬀusion (interdiﬀusion) and suitable for relatively large diﬀusion coeﬃcients, since the size of the specimen volume excited by the electron beam limits the depth resolution. Rutherford back scattering (RBS) or nuclear reaction analysis (NRA) are both nuclear techniques, which use ion beams of several MeV energy for proﬁle analysis. RBS is particular suitable for heavy solutes in a light solvent whereas NRA is appropriate for some light solutes including hydrogen. A prerequisite for NRA studies is a nuclear reaction with a narrow resonance. The penetration depth and energy straggling of the ion beam limit RBS and NRA to small diffusivities. Spreading resistance proﬁling (SRP) of dopant diﬀusion proﬁles in semiconductors is direct in the sense that it provides a depth proﬁle of the spreading resistance. However, some transformation is needed to convert spreading resistance to dopant concentration. Usually, NMR techniques are indirect (see below). However, ﬁeld-gradient NMR, either with static ﬁeld gradients (FG-NMR) or with pulsed ﬁeld gradients (PFG-NMR), are methods that permit diﬀusivity measurements without referring to a microscopic model. Indirect methods are not directly based on the laws of Fick. Indirect methods usually study phenomena which are inﬂuenced by the diﬀusion jumps of atoms. Some of these methods are sensitive to one or a few atomic jumps only. Quantities such as relaxation times, relaxation rates, or line-widths are measured and the mean residence time of the diﬀusing atoms, τ̄ , is deduced therefrom. A microscopic model of the atomic jump process is needed to deduce the diﬀusivity via the Einstein-Smoluchowski relation (see Chap. 4). In simple cases, the (uncorrelated) diﬀusivity DE is given by DE = d2 , 6τ̄ (13.1) where d denotes the length of an atomic jump. The numbers of atomic jumps performed by the diﬀusing species during anelastic or magnetic after-eﬀect measurements (e.g., Snoek or Zener eﬀect) are typically of the order of one. Internal friction studies are particularly sensitive to diﬀusion processes, when the atomic jump rate, 1/τ̄ , is comparable with the vibration frequency of the internal friction device. When applicable, these techniques can monitor very small to small diﬀusion coeﬃcients. The Gorski eﬀect is an anelastic after-eﬀect, which can be observed in hydrogenmetal systems. Its origin is the hydrogen redistribution in a strained sample. The associated after-eﬀect can be monitored because hydrogen diﬀusion is a very fast process. 13.1 Direct versus Indirect Methods 211 Among the nuclear methods, nuclear magnetic relaxation (NMR) covers the widest range of diﬀusivities. Spin-alignment experiments (SAE), lineshape spectroscopy, and spin-lattice relaxation spectroscopy can be used. Favourable are materials with large gyromagnetic ratios and small nondiﬀusive contributions to line-width or relaxation rates. Mössbauer spectroscopy (MBS) requires a suitable Mössbauer isotope. The usual workhorse of MBS is 57 Fe, which permits studies of Fe diﬀusion. There is a short list of further Mössbauer probes such as 119 Sn, 151 Eu, and 161 Dy. Quasielastic neutron scattering (QENS) is applicable to isotopes with large enough quasielastic scattering cross sections. Both techniques are limited to relatively fast diﬀusion processes. The main virtues of MBS and QENS are that these techniques can unravel microscopic information such as jump length and jump direction of the diﬀusing atoms. Impedance spectroscopy (IS) measures the complex conductivity of ionconducting materials as a function of the frequency. For materials in which only one type of ion contributes to the dc conductivity, Eq. (11.26) can be used to ‘translate’ the dc conductivity, σdc , into a charge diﬀusion coeﬃcient of the ions, Dσ (see Chap. 11). Fig. 13.1. Typical ranges of the diﬀusivity D and the mean residence time τ̄ of direct and indirect methods for diﬀusion studies 212 13 Direct Diﬀusion Studies Figure 13.1 shows typical ranges of diﬀusivity (D: upper abscissa) and mean residence time (τ̄ : lower abscissa) for direct and indirect methods, respectively. D and τ̄ have been converted via Eq. (13.1), adopting a typical jump length d in solids of some tenths of a nanometer. The length scale for the diﬀusion processes which are probed by IS and NMR varies with the applied measuring frequency. Thus a combination of various techniques and/or experimental devices may be desirable. The present chapter is devoted to direct methods. Diﬀusion of atoms in a certain direction x is described by one of the following versions of Fick’s second law (see Chaps. 2 and 10) ∂2C ∂ ∂C ∂C ∂C = D 2 or = D̃(C) . (13.2) ∂t ∂x ∂t ∂x ∂x The ﬁrst version corresponds to a concentration-independent diﬀusivity. As outlined below, in experiments with trace elements very tiny amounts of the diﬀusing species can be studied and the chemical composition of the sample is unchanged. The second version is applicable for a concentration-dependent diﬀusion coeﬃcient, D̃(c), denoted as the interdiﬀusion- or chemical diﬀusion coeﬃcient (see Chap. 10). We discuss relaxation and internal friction methods based on the anelastic behaviour of materials in Chap. 14, the nuclear methods NMR, MBS, and QENS in Chap. 15, and the electrical methods IS and SRP in Chap. 16. For further details the reader may consult textbooks [1–3], reviews [4, 5], and conference proceedings [6–9]. 13.2 The Various Diﬀusion Coeﬃcients Before discussing experimental methods in detail, we describe situations which entail various types of diﬀusion coeﬃcients. In this section, we distinguish the various diﬀusion coeﬃcients by lower and upper indices. We drop the indices in the following text again, whenever it is clear which diﬀusion coeﬃcient is meant. We concentrate on lattice (bulk) diﬀusion in unary and binary systems. Diﬀusion in ternary systems produces complexities, which are not treated in this book. We focus on lattice diﬀusion since diﬀusion along grain boundaries and dislocations is considered separately in Chaps. 32 and 33. 13.2.1 Tracer Diﬀusion Coeﬃcients In diﬀusion studies with trace elements (labelled by their radioactivity or by their isotopic mass) tiny amounts of the diﬀusing species (in the ppm range or even less) can be used. Although in a diﬀusion experiment a concentration gradient of the trace element is necessary, the total tracer concentration can be kept so small that the overall composition of the sample during the 13.2 The Various Diﬀusion Coeﬃcients 213 investigation practically does not change. From an atomistic viewpoint this implies that a tracer atom is not inﬂuenced by other tracer atoms. The analysis of such a diﬀusion experiment yields a tracer diﬀusion coeﬃcient, which is independent of tracer concentration. Tracers are appropriate to study selfdiﬀusion of matrix atoms. They can also be used to study diﬀusion of foreign atoms under very dilute conditions. The latter phenomenon is called impurity diﬀusion. The expressions foreign diﬀusion or solute diﬀusion are also used. Self-diﬀusion: The diﬀusion of A atoms in a solid element A is called selfdiﬀusion. Studies of self-diﬀusion with tracers utilise an isotope A∗ of the same element. A typical initial conﬁguration for a tracer self-diﬀusion experA∗ iment is illustrated in Fig. 13.2a. The tracer self-diﬀusion coeﬃcient DA is obtained from the diﬀusion broadening of a narrow initial distribution. The connection between the macroscopically deﬁned tracer self-diﬀusion coeﬃcient and the atomistic picture of diﬀusion is the Einstein-Smoluchowski relation discussed in Chap. 4. In simple cases, it reads ∗ A = f DE DA with DE = d2 , 6τ̄ (13.3) where d denotes the jump length and τ̄ the mean residence time of an atom on a particular but arbitrary site of the crystal. Equation (13.3) is applicable for cubic structures when only jumps to nearest-neighbour sites occur. f is the tracer correlation factor discussed in Chap. 7. For self-diﬀusion in cubic crystals f is usually a known numeric factor, which depends on the lattice geometry and the diﬀusion mechanism. In some textbooks the quantity DE is denoted as the Einstein diﬀusion coeﬃcient. In the author’s opinion, the notation Einstein diﬀusion coeﬃcient is misleading, since the original Einstein-Smoluchowski equation relates the total macroscopic mean square displacement of atoms to the diﬀusion coeﬃcient (see Chap. 4), in which correlation eﬀects are included. In a homogeneous binary AX B1−X alloy or compound two tracer selfdiﬀusion coeﬃcients for A∗ and B ∗ tracer atoms can be measured using the initial conﬁguration displayed in Fig. 13.2b. We denote the corresponding A∗ B∗ and DA . In general, the two tracer diﬀusion coeﬃcients by DA X B1−X X B1−X tracer diﬀusivities are not equal: ∗ ∗ A B DA = DA . X B1−X X B1−X Depending on the speciﬁc alloy system one component will be more mobile than the other. The diﬀerence depends on the crystal structure of the material, on the atomic mechanisms which mediate diﬀusion, and on the constituents themselves. For example, in B2 structured intermetallic compounds the tracer diﬀusivities of the constituents are usually similar, whereas in L12 or DO3 structured compounds the component diﬀusivities can be very diﬀerent (see [10–12] and Chap. 20). In ionic crystals and ceramics the diﬀusivities of the components also can diﬀer signiﬁcantly (see Chaps. 26 and 27). Of 214 13 Direct Diﬀusion Studies Fig. 13.2a–f Initial conﬁgurations for direct diﬀusion studies: a) Thin layer of A∗ on solid A: tracer self-diﬀusion in pure elements. b) Thin layer of A∗ or B ∗ on homogeneous A-B alloy: tracer self-diﬀusion of alloy components. c) Thin layer of C ∗ on solid A or on a homogeneous alloy: Impurity diﬀusion. d) Diﬀusion couple between metal-hydrogen alloy and a pure metal. e) Diﬀusion couple between pure end-members. f ) Diﬀusion couple between two homogeneous alloys course, both component diﬀusivities are also functions of the thermodynamic variables temperature and pressure and in general also depend on the composition. Impurity Diﬀusion: When the diﬀusion of a trace solute C ∗ in a monoatomic solvent A or in a homogeneous binary solvent AX B1−X (Fig. 13.2c) is measured, the tracer diﬀusion coeﬃcients ∗ ∗ C C and DA DA X B1−X are obtained. These diﬀusion coeﬃcients are denoted as the impurity diﬀusion coeﬃcients or sometimes also as the foreign diﬀusion coeﬃcients. 13.2.2 Interdiﬀusion and Intrinsic Diﬀusion Coeﬃcients For interdiﬀusion studies on binary alloys, diﬀusion couples are formed consisting either of two elements from a continuous solid solution alloy or of two homo-phase alloys with diﬀerent compositions (AX B1−X and AY B1−Y ) within the same phase ﬁeld (Fig. 13.2 e and f). Usually the thicknesses of the couple members are chosen large as compared to the average diﬀusion length. Then, each couple member can be considered to be semi-inﬁnite. Some typical examples are: – Pure end-member diﬀusion couples consisting of two slices of pure elements joined together (Ni|Pd, Au|Ag, Si|Ge, . . . ). 13.3 Tracer Diﬀusion Experiments – – 215 Incremental diﬀusion couples consisting of two slices of homogenous alloys joined together (Fe75 Al25 |Fe60 Al40 , Ni50 Pd50 |Ni70 Pd30 , Ni|Ni70 Pd30 , . . . ). Diﬀusion couples which involve solutions of hydrogen (Pd-H|Pd, Ag1−X HX |Ag1−Y HY , . . . ). During hydrogen interdiﬀusion the metal atoms are practically immobile. Then the intrinsic diﬀusion coeﬃcient and the chemical diﬀusion coeﬃcient of hydrogen are identical. Interdiﬀusion: The phenomenon of interdiﬀusion or chemical diﬀusion has been discussed in Chap. 10. We have seen that the interdiﬀusion coeﬃcient D̃ can be deduced either by a Boltzmann-Matano analysis for systems without volume change or for systems with volume changes from a Sauer-Freise type analysis of the experimental concentration-distance proﬁle. Using one of these methods, an interdiﬀusion coeﬃcient D̃ = D̃(C) for each composition C in the diﬀusion zone is obtained (see Chap. 10). D̃ characterises the intermixing of A and B atoms. I I Intrinsic Diﬀusion: The intrinsic diﬀusion coeﬃcients DA and DB describe diﬀusion of the components A and B of a binary alloy relative to the lattice planes. As discussed in Chap. 10, a determination the intrinsic diﬀusivities requires two measurements. The Kirkendall velocity, vK , and the interdiffusion coeﬃcient, D̃, permit to deduce intrinsic diﬀusivities as described in Chap. 10. Either the Darken equations or the more precise Darken-Manning equations can be used. 13.3 Tracer Diﬀusion Experiments Many of the reliable diﬀusion studies on solids have been performed by radiotracer techniques as evidenced in textbooks [1–3], reviews [4, 5, 10–12] and conference proceedings [6–9]. Due to the high sensitivity of nuclear counting facilities, radiotracer studies are often superior to other techniques. A very important advantage is the fact that self-diﬀusion – the most basic diﬀusion process in a solid material – can be studied in a straightforward manner using radioisotopes of matrix atoms. Then, the tracer self-diﬀusion coeﬃcient is obtained. Foreign atom diﬀusion studies can also be performed with tiny amounts of tracer. Typical tracer concentrations are less or even much less than a ppm, if radioisotopes with high speciﬁc activity are used. In this way, diﬀusion in a chemically homogeneous solid can be investigated. Complications due to chemical gradients play no rôle and the thermodynamic factor equals unity. In a tracer diﬀusion experiment atoms are usually labelled by their radioactivity. When stable isotopes are used as tracers the ‘label’ is 216 13 Direct Diﬀusion Studies Fig. 13.3. Schematic illustration of the tracer method: The major steps – deposition of the tracer, diﬀusion anneal, serial sectioning, and evaluation of the penetration proﬁle – are indicated the isotopic mass. Sometimes, in the case of impurity diﬀusion atoms are labelled just by their chemical nature. The major steps of a tracer diﬀusion experiment are indicated in Fig. 13.3. Preparation of a diﬀusion sample usually involves preparation of a ﬂat, strain-free surface. Polishing of metals, intermetallics, semiconductors, and glasses is usually performed by standard metallographic procedures. Soft materials such as organic crystals or polymers can be cut with a microtome. Mechanical methods produce the best ﬂatness but introduce strain. Etching or electropolishing and/or a pre-diﬀusion anneal should be used to remove cold-worked material. The tracer is deposited onto the polished, ﬂat surface of the diﬀusion sample. Evaporation, dripping of a liquid solution, and electrodeposition of the radiotracer onto the surface are the major deposition techniques. Complete homogeneity of the deposit is not necessary as long as iregularties in its thickness are small as compared to the mean diﬀusion length and as long as the same sample area is counted in each section [13]. Implantation of the radioisotope is more laborious but oﬀers sometimes advantages [4, 14]: for example, tracer hold-up by surface oxide layers can be avoided by implantation. Following the tracer deposition, an isothermal diﬀusion anneal is performed at temperature T for some diﬀusion time t. During the diﬀusion anneal the sample is usually encapsulated in a quartz ampoule under vacuum or inert atmosphere (e.g., Ar). For temperatures below 1500 K quartz ampoules and resistance furnaces are frequently used. For higher temperatures more sophisticated annealing techniques (e.g., electron-beam heating) are necessary. Suppose that a thin layer of tracer atoms (M atoms per unit area) has been deposited at the surface x = 0 of a semi-inﬁnite sample. Let us further suppose that tracer losses and tracer hold-up at the surface can be avoided. Then, the concentration distribution after a diﬀusion anneal is described by (see Chap. 3) 13.3 Tracer Diﬀusion Experiments 217 x2 M exp − . (13.4) C(x, t) = √ 4Dt πDt We recall that Eq. (13.4) is the thin-ﬁlm √ solution (Gaussian solution) of Fick’s second law and that the quantity Dt is a typical diﬀusion length. An alternative possibility of tracer deposition is ion-implantation using an accelerator. Implantation can be a very suitable deposition technique for materials like Al, which readily form a thin oxide layer when exposed to air. After implantation the tracer atoms form a buried layer. For a ﬁxed implantation energy their distribution as a function of range x is given by1 $ (x − R )2 % M p . (13.5) C(x, 0) = exp − 4Dt 2π∆Rp Rp denotes the mean projected range of implantation and ∆Rp the standard deviation of the projected range. Both quantities depend on the implantation energy, on the tracer, and on the matrix. Typical values of Rp lie in the range 20 to 100 nm for implantation energies of 50 keV. A layer buried in great depth broadens during diﬀusion annealing to $ (x − Rp )2 % M . (13.6) exp − C(x, t) = 2∆Rp + 4Dt 2π∆Rp + 4Dt However, after implantation the tracer layer will usually be close to the sample surface. Then, Eq. (13.6) must be modiﬁed. If the surface acts either as a ‘perfect mirror’ or as a ‘perfect sink’ for tracer atoms the solution of Fick’s second equation can be written as $ $ M (x + Rp )2 % (x − Rp )2 % C(x, t) = ± exp − . exp − 2∆Rp + 4Dt 2∆Rp + 4Dt 2π∆Rp + 4Dt (13.7) The minus-sign stands for a perfect sink and the plus-sign for a perfect reﬂection at x = 0. Both boundary conditions are approximations and may not always hold in practical cases. If this is the case, numerical solutions of Fick’s equation should be used. 13.3.1 Proﬁle Analysis by Serial Sectioning The major task of a diﬀusion experiment is to study the concentration-depth proﬁle and to deduce the diﬀusion coeﬃcient by comparison with the corresponding solution of Fick’s second law. Let us assume that the experimental conditions were chosen in such√a way that the deposited layer is thin compared with the diﬀusion length Dt. Then, the distribution after the diﬀusion anneal is described by Eq. (13.4). 1 For simplicity reasons we neglect channelling eﬀects. Channeling can be neglected if the direction of the implntation beam avoids directions of high crystal symmetry, 218 13 Direct Diﬀusion Studies The best way to determine the resulting concentration-depth proﬁle is serial sectioning of the sample and subsequent determination of the amount of tracer per section. To understand sectioning the reader should think in terms of isoconcentration contours. For lattice diﬀusion these are parallel to the original surface, on which the thin layer is deposited, and perpendicular to the diﬀusion direction. The most important criterion of sectioning is the parallelness of sections to the isococentration contours. For radioactive tracers the speciﬁc activity per section, A(x), is proportional to the tracer concentration: A(x) = kC(x) . (13.8) Here k is a constant, which depends on the nature and energy of the nuclear radiation and on the eﬃciency of the counting device. The speciﬁc activity is obtained from the section mass and the count rate. The latter can be measured in nuclear counting facilities such as γ- or β-counting devices. Usually, the count-rate must be corrected for the background count-rate of the counting device. For short-lived radioisotopes half-life corrections are also necessary. According to Eq. (13.4) a diagram of the logarithm of the speciﬁc activity versus the penetration distance squared is linear. From its slope, (4Dt)−1 , and the diﬀusion time the tracer diﬀusivity D is obtained. In an ordinary thin-layer sectioning experiment, one wishes to measure diﬀusion over a drop of about three orders of magnitude in concentration. About twenty sections suﬃce to deﬁne a penetration proﬁle. The section thickness ∆x required to get a concentration decrease of three orders of mag√ nitude over 20 sections is ∆x ≈ Dt/3.8. Thicker sections should be avoided for the following reason: in a diﬀusion penetration proﬁle the average concentrations (speciﬁc activities) per section are plotted versus the position of the distance of the center of each section from the surface. Errors caused by this procedure are only negligible if the sections are thin enough. The radiotracer deposited on the front face of a sample may rapidly reach the side surfaces of a sample by surface diﬀusion or via transport in the vapour phase and then diﬀuse √ inward. To eliminate lateral diﬀusion eﬀects, one usually removes about 6 Dt from the sample sides before sectioning. For studies of bulk diﬀusion, single crystalline samples rather than polycrystalline ones should be used to eliminate the eﬀects of grain-boundary diﬀusion, which is discussed in Chap. 31. If no single crystals are available coarse-grained polycrystals should be used. The following serial-sectioning techniques are frequently used for the determination of diﬀusion proﬁles: √ Mechanical sectioning: For diﬀusion lengths, Dt, of at least several micrometers mechanical techniques are applicable (for a review see [4]). Lathes and microtomes are appropriate for ductile samples such as some pure metals (Na, Al, Cu, Ag, Au, . . . ) or polymers. For brittle materials such as intermetallics, semiconductors, ionic crystals, ceramics, and inorganic glasses grinding is a suitable technique. 13.3 Tracer Diﬀusion Experiments 219 Fig. 13.4. Penetration proﬁle of the radioisotope 59 Fe in Fe3 Si obtained by grinder sectioning [15]. The solid line represents a ﬁt of the thin-ﬁlm solution of Fick’s second law For extended diﬀusion anneals and large enough diﬀusivities, D > 10−15 m2 s−1 , lathe sectioning can be used. Diﬀusivities D > 10−17 m2 s−1 are accessible via microtome sectioning. In cases where the half-life of the isotope permits diﬀusion anneals of several weeks, grinder sectioning can be used for diﬀusivities down to 10−18 m2 s−1 . Figure 13.4 shows a penetration proﬁle of the radioisotope 59 Fe in the intermetallic Fe3 Si, obtained by grinder sectioning [15]. Gaussian behaviour as stated by Eq. (13.4) is observed over several orders of magnitude in concentration. Ion-beam Sputter Sectioning (IBS): Diﬀusion studies at lower temperatures often require measurements of very small diﬀusivities. Measurements of diﬀusion proﬁles with diﬀusion lengths in the micrometer or sub-micrometer range are possible using sputtering techniques. Devices for serial sectioning of radioactive diﬀusion samples by ion-beam sputtering (IBS) are described in [16, 17]. Figure 13.6 shows a schematic drawing of such a device. Oblique incidence of the ion beam and low ion energies between 500 and 1000 eV are used to minimise knock-on and surface roughening eﬀects. The sample (typically several mm in diameter) is rotated to achieve a homogeneous lateral sputtering rate. The sputter process is discussed in some detail below and 220 13 Direct Diﬀusion Studies Fig. 13.5. Penetration proﬁle of the radioisotope 59 Fe in Fe3 Al obtained by sputter sectioning [18]. The solid line represents a ﬁt of the thin-ﬁlm solution of Fick’s second law illustrated in Fig. 13.8, in connection with secondary ion mass spectroscopy (SIMS). An advantage of IBS devices lies in the fact that neutral atoms are collected, which comprise by far the largest amount (about 95 to 99 %) of the oﬀ-sputtered particles. In contrast, SIMS devices (see below) analyse the small percentage of secondary ions, which depends strongly on sputter- and surface conditions. Sectioning of shallow diﬀusion zones, which correspond to average diﬀusion lengths between several ten nm and 10 µm, is possible using IBS devices. For a reasonable range of annealing times up to about 106 s, a diﬀusivity range between 10−23 m2 s−1 and 10−16 m2 s−1 can be examined. Depth calibration can be performed by measuring the weight loss during the sputtering process or by determining the depth of the sputter crater by interference microscopy or by proﬁlometer techniques. The depth resolution of IBS and SIMS is limited by surface roughening and atomic mixing processes to about several nm. A penetration proﬁle of 59 Fe in the intermetallic Fe3 Al [18], obtained with the sputtering device described in [17] is displayed in Fig. 13.5. From diﬀusion proﬁles of the quality of Figs. 13.4 and 13.5, diﬀusion coeﬃcients can be determined with an accuracy of a few percent. A determi- 13.3 Tracer Diﬀusion Experiments 221 Fig. 13.6. Ion-beam sputtering device for serial sectioning of diﬀusion samples nation of the absolute tracer concentration is not necessary since the diﬀusion coeﬃcient is obtained from the slope, −1/(4Dt), of such proﬁles. Deviations from Gaussian behaviour in experimental penetration proﬁles (not observed in Figs. 13.4 and 13.5) may occur for several reasons: 1. Grain-boundary diﬀusion: Grain boundaries in a polycrystalline sample act as diﬀusion short-circuits with enhanced mobility of atoms. Grain boundaries usually cause a ‘grain-boundary tail’ in the deeper penetrating part of the proﬁle (see Chap. 32 and [19]). In the ‘tail’ region the concentration of the diﬀuser is enhanced with respect to lattice diﬀusion. Then, one should analyse the diﬀusion penetration proﬁle in terms of lattice diﬀusion and short-circuit diﬀusion terms: x2 M exp − + C0 exp(−A x6/5 ) . (13.9) C(x, t) = √ 4Dt πDt Here C0 is constant, which depends on the density of grain boundaries. The quantity A is related to the grain-boundary diﬀusivity, the grain-boundary width, and to the lattice diﬀusivity. The grain-boundary tails can be used for a systematic study of grain-boundary diﬀusion in bi- or polycrystalline samples. Grain-boundary diﬀusion is discussed in Chap. 32. 2. Evaporation losses of tracer : A tracer with high vapour pressure will simultaneously evaporate from the surface and diﬀuse into the sample. Then, the thin-ﬁlm solution (13.4) is no longer valid. The outward ﬂux of the tracer will be proportional to the tracer concentration at the surface: D ∂C ∂x x=0 = −KC(0) . (13.10) 222 13 Direct Diﬀusion Studies K is the rate constant for evaporation. The solution for Fick’s second equation for this boundary condition is [1] 2 K 1 x2 K K exp − exp C(x, t) = M √ Dt + x − 4Dt D D2 D πDt x K√ √ erfc Dt . (13.11) + 2 Dt D Evaporation losses of the tracer cause negative deviations from Gaussian behaviour in the near-surface region. 3. Evaporation losses of the matrix : For a matrix material with a high vapour pressure the surface of the sample may recede due to evaporation. A solution for continuous matrix removal at a rate v and simultaneous in-diﬀusion of the tracer has been given by [20] 1 v exp(−η 2 ) − erfc(η) , (13.12) C(x , t) = M √ 2D πDt where√x is the distance from the surface after diﬀusion and η = (x + vt)/2 Dt. 13.3.2 Residual Activity Method Gruzin has suggested a radiotracer technique, which is called the residual activity method [21]. Instead of analysing the activity in each removed section, the activity remaining in the sample after removing a section is measured. This method is applicable if the radiation being detected is absorbed exponentially. The residual activity A(xn ) after removing a length xn from the sample is then given by ∞ A(xn ) = k C(x) exp[−µ(x − xn )]dx , (13.13) xn where k is a constant and µ is the absorption coeﬃcient. According to Seibel [22] the general solution of Eq. (13.13) – independent of the functional form of C(x) – is given by d ln A(xn ) C(xn ) = kA(xn ) µ − . (13.14) dxn If the two bracket terms in Eq. (13.14) are comparable, the absorption coeﬃcient must be measured accurately in the same geometry in which the sample is counted. Thus, the Gruzin method is less desirable than counting the sections, except for two limiting cases: 1. Strongly absorbed radiation: Suppose that the radiation is so weak that it is absorbed in one section, i.e. µ d ln A(xn )/dxn . Isotopes such as 63 Ni, 13.4 Isotopically Controlled Heterostructures 223 14 C, or 3 H emit weak β-radiation. Their radiation is readily absorbed and Eq. (13.14) reduces to (13.15) C(xn ) = µkA(xn ) and the residual activity A(xn ) follows the same functional form as C(xn ). In this case, the Gruzin technique has the advantage that it obviates the tedious preparation of sections for counting. 2. Slightly absorbed radiation: For µ d ln A(xn )/dxn the radiation is so energetic that absorption is negligible. Then, the activity An in section n is obtained by subtracting two subsequent residual activities: An = A(xn ) − A(xn+1 ) . (13.16) The Gruzin technique is useful, when the specimen can be moved to the counter repeatedly without loosing alignment in the sectioning device. In general, this method is not as reliable as sectioning and straightforward measurement of the section activity. 13.4 Isotopically Controlled Heterostructures The use of enriched stable isotopes combined with modern epitaxial growth techniques enables the preparation of isotopically controlled heterostructures. Either chemical vapour deposition (CVD) or molecular beam epitaxy (MBE) are used to produce the desired heterostructures. After diﬀusion annealing, the diﬀusion proﬁles can be studied using, for example, conventional SIMS or TOF-SIMS techniques (see the next section). We illustrate the beneﬁts of this method with an example of Si selfdiﬀusion. In the past, self-diﬀusion experiments were carried out using the radiotracer 31 Si with a half-life of 2.6 hours. However, this short-lived radiotracer limits such studies to a narrow high-temperature range near the melting temperature of Si. Other self-diﬀusion experiments utilising the stable isotope 30 Si (natural abundance in Si is about 3.1 %) in conjunction with neutron activation analysis, SIMS proﬁling and nuclear reaction analysis (NRA) overcame this diﬀuculty (see also Chap. 23). However, these methods have the disadvantage that the 30 Si background concentration is high. Figure 13.7 illustrates the technique of isotopically controlled heterostructures for Si self-diﬀusion studies. The sample consists of a Si-isotope heterostructure, which was grown by chemical vapour deposition on a natural ﬂoating-zone Si substrate. A 0.7 µm thick 28 Si layer was covered by a layer of natural Si (92.2 % 28 Si, 4.7 % 29 Si, 3.1 % 30 Si). The 28 Si proﬁle in the asgrown state (dashed line), after a diﬀusion anneal (crosses), and the best ﬁt to the data (solid line) are shown. Diﬀusion studies on isotopically controlled heterostructures have been used by Bracht and Haller and their associates mainly for self- and dopant diﬀusion studies in elemental [24, 25] and compound semiconductors [26–28]. 224 13 Direct Diﬀusion Studies Fig. 13.7. SIMS depth proﬁles of 30 Si measured before and after annealing at 925 ◦ C for 10 days of a 28 Si isotope heterostructure. The initial structure consisted of a layer of 28 Si embedded in natural Si 13.5 Secondary Ion Mass Spectrometry (SIMS) Secondary ion mass spectroscopy (SIMS) is an analytical technique whereby layers of atoms are sputtered oﬀ from the surface of a solid, mainly as neutral atoms and a small fraction as ions. Only the latter can be analysed in a mass spectrometer. Several aspects of the sputtering process are illustrated in Fig. 13.8. The primary ions (typically energies of a few keV) decelerate during impact with the target by partitioning their kinetic energy through a series of collisions with target atoms. The penetration depth of the primary ions depends on their energy, on the types of projectile and target atoms and their atomic masses, and on the angle of incidence. Each primary ion initiates a ‘collision cascade’ of displaced target atoms, where momentum vectors can be in any direction. An atom is ejected after the sum of phonon and collisional energies focused on a target atom exceeds some threshold energy. The rest of the energy dissipates into atomic mixing and heating of the target. The sputtering yield of atomic and molecular species from a surface depends strongly on the target atoms, on the primary ions and their energy. Typical yields vary between 0.1 to 10 atoms per primary ion. The great majority of emitted atoms are neutral. For noble gas primaries the percentage of secondary ions is below 1 %. If one uses reactive primary ions (e.g., oxygenor alkali-ions) the percentage of secondary ions can be enhanced through the interaction of a chemically reactive species with the sputtered species by exchanging electrons. In a SIMS instrument, schematically illustrated in Fig. 13.9, a primary ion beam hits the sample. The emitted secondary ions are extracted from the surface by imposing an electrical bias of a few kV between the sample 13.5 Secondary Ion Mass Spectrometry (SIMS) 225 Fig. 13.8. Sputtering process at a surface of a solid and the extraction electrode. The secondary ions are then transferred to the spectrometer via a series of electrostatic and magnetic lenses. The spectrometer ﬁlters out all but those ions with the chosen mass/charge ratios, which are then delivered to the detector for counting. The classical types of mass spectrometers are equipped either with quadrupole ﬁlters, or electric and magnetic sector ﬁelds. Time-of-ﬂight (TOF) spectrometers are used in TOF-SIMS instruments. The TOF-SIMS technique developed mainly by Benninghoven [35] combines high lateral resolution (< 60 nm) with high depth resolution (< 1 nm). It is nowadays acknowledged as one of the major techniques for the surface characterisation of solids. In diﬀerent operational modes - surface spectrometry, surface imaging, depth proﬁling - this technique oﬀers several features: the mass resolution is high; in principle all elements and isotopes can be detected and also chemical information can be obtained; detection limits in the range of ppm of a monolayer can be achieved. For details of the construction of SIMS devices we refer to [33, 34, 36, 37]. When SIMS is applied for diﬀusion proﬁle measurements, the mass spectrum is scanned and the ion current for tracer and host atoms can be recorded simultaneously. In conventional SIMS, the ion beam is swept over the sample and, in eﬀect, digs a crater. An aperture prevents ions from the crater edges from reaching the mass spectrometer. The diﬀusion proﬁle is constructed from the plots of instantaneous tracer/host atom ratio versus sputtering time. The distance is deduced from a measurement of the total crater depth, assuming that the material is removed uniformly as a function of time. Large changes of the chemical composition along the diﬀusion direction can invalidate this assumption. 226 13 Direct Diﬀusion Studies Fig. 13.9. SIMS technique (schematic illustration) One must keep in mind that the relationship between measured secondaryion signals and the composition of the target is complex. It involves all aspects of the sputtering process. These include the atomic properties of the sputtered ions such as ionisation potentials, electron aﬃnities, the matrix composition of the target, the environmental conditions during the sputtering process such as the residual gas components in the vacuum chamber, and instrumental factors. Diﬀusion analysis by SIMS also depends on the accuracy of measuring the depth of the eroded crater and the resolution of the detected concentration proﬁle. A discussion of problems related to quantiﬁcation and standardisation of composition and distance in SIMS experiments can be found in [34, 39]. SIMS, like the IBS technique discussed above, enables the measurement of very small diﬀusion coeﬃcients, which are not attainable with mechanical sectioning techniques. The very good depth resolution and the high sensitivity of mass spectrometry allows the resolution of penetration proﬁles of solutes in the 10 nm range and at ppm level. Several perturbing eﬀects, inherent to the method and limiting its sensitivity are: degradation of depth resolution by surface roughening, atomic mixing, and near surface distortion of proﬁles by transient sputtering eﬀects. SIMS has mainly been applied for diﬀusion of foreign atoms although the high mass resolution especially of TOF-SIMS also permits separation of stable isotopes of the same element. SIMS has found particularly widespread use in studies of implantation- and diﬀusion proﬁles in semiconductors. However, SIMS is applicable to all kinds of solids. As an example, Fig. 13.10 shows diﬀusion proﬁles for both stable isotopes 69 Ga and 71 Ga of natural Ga in a ternary Al-Pd-Mn alloy (with a quasicrystalline structure) according to [38]. For metals, the relatively high impurity content of so-called ‘pure metals’ as compared to semiconductors can limit the dynamic range of SIMS proﬁles. 13.6 Electron Microprobe Analysis (EMPA) 227 Fig. 13.10. Diﬀusion proﬁles for both stable isotopes 69 Ga and 71 Ga of natural Ga in AlPdMn (icosahedral quasicrystalline alloy) according to [38]. The solid lines represent ﬁts of the thin-ﬁlm solution SIMS has in few cases also been applied to self-diﬀusion. This requires that highly enriched stable isotopes are available as tracers. Contrary to selfdiﬀusion studies by radiotracer experiments, in the case of stable tracers diﬀused into a matrix with a natural abundance of stable isotopes the latter limits the concentration range of the diﬀusion proﬁle. A ﬁne example of this technique can be found in a study of Ni self-diﬀusion in the intermetallic compound Ni3 Al, in which the highly enriched stable 64 Ni isotope was used [40]. The limitation due to the natural abundance of a stable isotope in the host has been avoided in some SIMS studies of self-diﬀusion on amorphous Nicontaining alloys by using the radioisotope 63 Ni as tracer [42, 43]. An elegant possibility to overcome the limits posed by the natural abundance of stable isotopes are isotopically controlled heterostructures. This method is discussed in the previous section and illustrated in Fig. 13.7. 13.6 Electron Microprobe Analysis (EMPA) The basic concepts of electron microprobe analysis (EMPA) can be found already in the PhD thesis of Castaing [44]. The major components of an 228 13 Direct Diﬀusion Studies Fig. 13.11. Schematic view of an electron microprobe analyser (EMPA) EMPA equipment are illustrated in Fig. 13.11. An electron-optical column containing an electron gun, magnetic lenses, a specimen chamber, and various detectors is maintained under high vacuum. The electron-optical column produces a ﬁnely focused electron beam, with energies ranging between 10 and 50 keV. Scanning coils and/or a mechanical scanning device for the specimen permit microanalysis at various sample positions. When the beam hits the specimen it stimulates X-rays of the elements present in the sample. The X-rays are detected and characterised either by means of an energy dispersive X-ray spectrometer (EDX) or a crystal diﬀraction spectrometer. The latter is also referred to as a wave-length dispersive spectrometer (WDX). The ability to perform a chemical analysis is the result of a simple and unique relationship between the wavelength of the characteristic X-rays, λ, emitted from an element and its atomic number Z. It was ﬁrst observed by Moseley [45] in 1913. He showed that for K radiation 1 Z ∝ √ . λ (13.17) The origin of the characteristic X-ray emission is illustrated schematically in Fig. 13.12. An incident electron with suﬃcient energy ejects a core electron from its parent atom leaving behind an orbital vacancy. The atom is then in an excited state. Orbital vacancies are quickly ﬁlled by electronic relaxations accompanied by the release of a discrete energy corresponding to the diﬀerence between two orbital energy levels. This energy can be emitted as an X-ray photon or it can be transferred to another orbital electron, called 13.6 Electron Microprobe Analysis (EMPA) 229 Fig. 13.12. Characteristic X-ray and Auger-electron production an Auger electron, which is ejected from the atom. The fraction of electronic relaxations which result in X-ray emission rather than Auger emission depends strongly on the atomic number. It is low for small atomic numbers and high for large atomic numbers. The characteristic radiation is superimposed to the continuous radiation also denoted as ‘Bremsstrahlung’. The continuum is the major source of the background and the principal factor limiting the X-ray sensitivity. For details about EMPA, the reader may consult, e.g., the reviews of Hunger [46] and Lifshin [47]. A diﬀusion proﬁle is obtained by examining on a polished cross-section of a diﬀusion sample the intensity of the characteristic radiation of the element(s) involved in the diﬀusion process along the diﬀusion direction. The detection limit in terms of atomic fractions is about 10−3 to 10−4 , depending on the selected element. It decreases with decreasing atomic number. Light elements such as C or N are diﬃcult to study because their ﬂuorescence yield is low. The diameter of the electron beam is typically 1 µm or larger depending on the instrument’s operating conditions. Accordingly, the volume of X-ray generation is of the order of several µm3 . This limits the spatial resolution to above 1 to 2 µm. Thus, only relatively large diﬀusion coeﬃcients D > 10−15 m2 s−1 can be measured (Fig. 13.1). Because of its detection limit, EMPA is mainly appropriate for interdiﬀusion- and multiphasediﬀusion studies. An example of a single-phase interdiﬀusion proﬁle for an Al50 Fe50 –Al30 Fe70 couple is shown in Fig. 13.13 [23]. The Boltzmann-Matano method [29, 30] is usually employed to evaluate interdiﬀusion coeﬃcients D̃ from an experimental proﬁle. Related procedures for non-constant volume have been developed by Sauer and Freise and den Broeder [31, 32]. These methods for deducing the interdiﬀusion coeﬃcient, D̃(c), from experimental concentration-depth proﬁles are described in Chap. 10. 230 13 Direct Diﬀusion Studies Fig. 13.13. Interdiﬀusion proﬁle of a Fe70 Al30 –Fe50 Al50 couple measured by EMPA according to Salamon et al. [23]. Dashed line: composition distribution before the diﬀusion anneal 13.7 Auger-Electron Spectroscopy (AES) Auger-electron spectroscopy (AES) is named after Pierre Auger, who discovered and explained the Auger eﬀect in experiments with cloud chambers in the mid 1920s (see [48]). An Auger electron is generated by transitions within the electron orbitals of an atom following an excitation an electron from one of the inner levels (see Fig. 13.12). Auger-electron spectroscopy (AES) was introduced in the 1960s. In AES instruments the excitation is performed by a primary electron beam. The kinetic energy of the Auger electron is independent of the primary beam but is characteristic of the atom and electronic shells involved in its production. The probability that an Auger electron escapes from the surface region decreases with decreasing kinetic energy. The range of analytical depth in AES is typically between 1 and 5 nm. AES is one of the major techniques for surface analysis. When a primary electron beam strikes a surface, Auger electrons are only a fraction of the total electron yield. Most of the electrons emitted from the surface are either secondary electrons or backward scattered electrons. These and the inelastically scattered Auger electrons constitute the background in an Auger spectrum. Auger-electron emission and X-ray ﬂuorescence after creation of a core hole are competing processes and the emission probability depends on the atomic number. The probability for Auger-electron emission 13.8 Ion-beam Analysis: RBS and NRA 231 Fig. 13.14. Schematic representation of Rutherford backscattering (RBS) and of nuclear reaction analysis (NRA) decreases with increasing atomic number whereas the probability for X-ray ﬂuorescence increases with atomic number. AES is thus particularly well suited for light elements. The combined operation of an AES spectrometer for chemical surface analysis and an ion sputtering device can be used for depth proﬁling. Information with regard to the quantiﬁcation and to factors aﬀecting their resolution can be found, e.g., in [49, 50]. AES is applicable to diﬀusion of foreign atoms, since AES only discriminates between diﬀerent elements. It has, for example, been used to measure Au and Ag diﬀusion in amorphous Cu-Zr [41] and Cu and Al diﬀusion in amorphous Zr61 Ni39 -alloys [51]. 13.8 Ion-beam Analysis: RBS and NRA High-energy ion-beam analysis has several desirable features for depth proﬁling of diﬀusion samples. The technique is largely non-destructive, it oﬀers good depth resolution, and measurements of both concentration and depth can be achieved. The depth resolution is in the range from about 0.01 to 1 µm. This is inferior to the depth resolution achieved in IBS or SIMS devices but substantially better than the resolution of mechanical sectioning techniques. Atomic species are identiﬁed in ion-beam analysis by detecting the products of nuclear interactions, which are created by the incident MeV ions. There are several diﬀerent techniques. The two more important ones are Rutherford backscattering (RBS) and nuclear reaction analysis (NRA). These two are depicted schematically in Fig. 13.14. 232 13 Direct Diﬀusion Studies Rutherford Backscattering (RBS): The ﬁrst scattering experiment was performed by Rutherford in 1911 [53] and his students Geiger and Marsden [54] for veriﬁcations of the atomic model. A radioactive source of α-particles was used to provide energetic probing ions and the particles scattered from a gold foil were observed with a zinc blende scintillation screen. Nowadays, elastic backscattering analysis also denoted as Rutherford backscattering (RBS) is probably the most frequently used ion-beam analytical technique among the surface analysis tools. In RBS experiments a high-energy beam of monoenergetic ions (usually α-particles) with energies of some MeV is used for depth proﬁling. The sample is bombarded along the diﬀusion direction with ions and one studies the number of elastically backscattered ions as a function of their energy. The particles of the analysing beam are scattered by the nuclei in the sample and the energy spectrum of scattered particles is used to determine the concentration proﬁle of scattering nuclei. The signals from diﬀerent nuclei can be separated in the energy spectrum, because of the diﬀerent kinematic factors K of the scattering process. K is related to the masses of analysing particles and scattering nuclei. It is a monotonically decreasing function of the mass of the target nuclei. The backscattered particles re-emerge unchanged except for a reduction in energy. The depth information comes from the continuous energy loss of the ions in the sample. The yield of the backscattered ions is proportional to the concentration of the scattering nuclei. RBS is illustrated schematically in Fig. 13.15 for a layer of heavy atoms (mass M ) deposited on a substrate of light atoms (Mass m). Yield and energy of the backscattered ions are monitored by an energy-sensitive particle detector and a multichannel analyser. The high energy end of the spectrum (M -signal) corresponds to ions backscattered from heavy atoms at the sample surface. The low energy end of the M -signal corresponds to ions backscattered from the heavy atoms near the interface. The signals from the heavy and light nuclei are separated in the spectrum due to the diﬀerent kinematic factors for heavy and light nuclei. Although widely applicable, RBS has two inherent limitations for diﬀusion studies: First, the element of interest must diﬀer in mass suﬃciently – at least several atomic masses – from other constituents of the sample. Second, adequate sensitivity is achieved only when the solutes are heavier than the majority constituents of the matrix. Then, the backscattering yield from the diﬀuser appears at higher energies than the yield from the majority nuclei. Therefore, RBS is particular suitable for detecting heavy elements in a matrix of substantially lower atomic weight. Because of the limited penetration range of ions (several micrometers) and the associated energy straggling in a solid, only relatively small diﬀusion coeﬃcients are accessible. Nuclear Reaction Analysis (NRA): In a NRA proﬁling experiment monoenergetic high-energy particles (protons, α-particles, . . . ) are used as in RBS. NRA is applicable if the analysing particles undergo a suitable nu- 13.8 Ion-beam Analysis: RBS and NRA 233 Fig. 13.15. Rutherford backscattering spectrometry: high-energy ion beam, electronics for particle detection and a schematic example of a RBS spectrum. The technique is illustrated for a thin layer of atoms with mass M deposited on a substrate of lower mass m clear reaction with narrow resonance with the atoms of interest. The yield of out-going reaction products is measured as a function of the energy of the incident beam. From the yield versus energy curve the concentration proﬁle can be deduced. As shown schematically in Fig. 13.14, the analysis-beam particles undergo an inelastic, exothermic nuclear reaction with the target nuclei thus producing two or more new particles. Depending on the conditions it may be preferable to detect either charged reaction products, neutrons or γ-rays from the reaction. This method distinguishes speciﬁc isotopes and is therefore free from the mass-related restrictions of RBS. Suitable resonant nuclear reactions occur for at least one readily available isotope of all elements from hydrogen to ﬂuorine and for beam energies below 2 MeV. NRA can mainly be used to investigate the diﬀusion of light solutes in a heavier matrix. Concluding Remarks: Depth proﬁling is possible in RBS and NRA because the charged particles continuously loose energy as they traverse the specimen. Usually, this loss is almost entirely due to electronic excitations, although there is some additional contribution from small-angle nuclear scattering. The consequences may be appreciated by considering the RBS experiment illustrated in Fig. 13.15. In RBS the energy of the analysis-beam particle decreases during both inward and outward passages. When the particle is detected, the accumulated energy loss is superimposed on the recoil 234 13 Direct Diﬀusion Studies loss via the kinematic factor. Hence the measured energy decreases monotonically with the depth of the scattering nucleus. In NRA the situations are analogous but more varied. For example, the relevant energy loss may occur only during the inward or outward passage. Nevertheless, depth resolution is always a consequence of the charged-particle energy loss in the sample. For example, the diﬀusion of ion-implanted boron in amorphous Ni59.5 Nb40.5 was measured by irradiating the amorphous alloy with high energy protons and detecting α-particles emitted from the nuclear reaction 11 B + p → 8 B + α, and determining the concentration proﬁle of 11 B from the number and energy of emitted α-particles as a function of the incident proton energy [52]. In NRA and in RBS the penetration range of ions is not more than several micrometer. This limits the diﬀusion depth. Diﬀusion coeﬃcients between about 10−17 and 10−23 m2 s−1 are accessible (see also Fig. 13.1). Both RBS and NRA methods need a depth calibration, which is based on not always very accurate data of the stopping power in the matrix for the relevant particles. Also the depth resolution is usually inferior to that achievable in careful IBS radiotracer and SIMS proﬁling studies. For a comprehensive discussion of ionbeam techniques the reader may consult reviews by Myers [55], Lanford et al. [56], and Chu et al. [57]. References 1. J. Crank, The Mathematics of Diﬀusion, Oxford University Press, 2nd ed., 1975 2. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 3. Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, Berlin, 1992 4. S.J. Rothman, The Measurement of Tracer Diﬀusion Coeﬃcients in Solids, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, 1984, p. 1 5. H. Mehrer (Vol. Ed.), Sect. 1.6 in: Diﬀusion in Solid Metals and Alloys, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 6. Proc. Int. Conf. on Diﬀusion in Materials – DIMAT-92, Kyoto, Japan, 1992, M. Koiwa, H. Nakajima, K.-I. Hirano (Eds.); also: Defect and Diﬀusion Forum 95–98 (1993) 7. Proc. Int. Conf. on Diﬀusion in Materials – DIMAT-96, Nordkirchen, Germany, 1996, H. Mehrer, Chr. Herzig, N.A. Stolwijk, H. Bracht (Eds.); also: Defect and Diﬀusion Forum 143–147 (1997) 8. Proc. Int. Conf. on Diﬀusion in Materials – DIMAT-2000, Paris, France, 2000, Y. Limoge, J.L. Bocquet (Eds.); also: Defect and Diﬀusion Forum 194–199 (2001) 9. Proc. Int. Conf. on Diﬀusion in Materials – DIMAT-2004, Cracow, Poland, 2004, M. Danielewski, R. Filipek, R. Kozubski, W. Kucza, P. Zieba, Z. Zurek (Eds.); also: Defect and Diﬀusion Forum 237–240 (2005) 10. H. Mehrer, Materials Transactions, JIM, 37, 1259 (1996) References 235 11. H. Mehrer, F. Wenwer, Diﬀusion in Metals, in: Diﬀusion in Condensed Matter, J. Kärger, R. Haberlandt, P. Heitjans (Eds.), Vieweg Verlag, 1998 12. H. Mehrer, Diﬀusion: Introduction and Case Studies in Metals and Binary Alloys, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 13. D. Tannhauser, J. Appl. Phys. 27, 662 (1956) 14. H. Mehrer, Phys. Stat. Sol. (a) 104, 247 (1987) 15. A. Gude, H. Mehrer, Philos. Mag. A 76, 1 (1996) 16. F. Faupel, P.W. Hüppe, K. Rätzke, R. Willecke. T. Hehenkamp, J. Vac. Sci. Technol. a 10, 92 (1992) 17. F. Wenwer, A. Gude, G. Rummel, M. Eggersmann, Th. Zumkley, N.A. Stolwijk, H. Mehrer, Meas. Sci. Technol. 7, 632 (1996) 18. M. Eggersmann, B. Sepiol, G. Vogl, H. Mehrer, Defect and Diﬀusion Forum 143–147, 339 (1997) 19. I. Kaur, Y. Mishin, W. Gust, Fundamentals of Grain and Interphase Boundary Diﬀusion, John Wiley & Sons Ltd., 1995 20. R.N. Ghoshtagore, Phys. Stat. Sol. 19, 123 (1967) 21. P.L. Gruzin, Dokl. Akad. Nauk. SSSR 86, 289 (1952) 22. G. Seibel, Int. J. Appl. Radiat. Isot. 15, 679 (1964) 23. M. Salamon, S. Dorfman, D. Fuks, G. Inden, H. Mehrer, Defect and Diﬀusion Forum 194–199, 553 (2001) 24. H.D. Fuchs, W. Walukiewicz, E.E. Haller, W. Dondl, R. Schorer, G. Abstreiter, A.I. Rudnev, A.V. Tikomirov, V.I. Ozhogin, Phys. Rev. B 51, 16817 (1995) 25. H. Bracht, E.E. Haller, R. Clark-Phelps, Phys. Rev. Lett. 81 393 (1998) 26. L. Wang, L. Hsu, E.E. Haller, J.W. Erickson, A. Fisher, K. Eberl, M. Cardona, Phys. Rev. Lett. 76, 2342 (1996) 27. L. Wang, J.A. Wolk, L. Hsu, E.E. Haller, J. W. Erickson, M. Cardona, T. Ruf, J.P. Silveira, F. Briones, Appl. Phys. Lett. 70, 1831 (1997) 28. H. Bracht, E.E. Haller, K. Eberl, M. Cardona, R. Clark-Phelps, Mat. Res. Soc. Symp. 527, 335 (1998) 29. L. Boltzmann, Wiedemanns Ann. Physik 53, 959 (1894) 30. C. Matano, Jap. J. Phys. 8, 109–113 (1933) 31. F. Sauer, V. Freise, Z. Elektrochem. 66, 353 (1962) 32. F.J.A. den Broeder, Scr. Metall. 3, 321 (1969) 33. C.-E. Richter, Sekundärionen-Massenspektroskopie und Ionenstrahl-Mikroanalyse, in: Ausgewählte Untersuchungsverfahren der Metallkunde, H.-J. Hunger et al. (Eds.), VEB Verlag, 1983, p. 197 34. W.T. Petuskey, Diﬀusion Analysis using Secondary Ion Mass Spectroscopy, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p. 179 35. A. Benninghoven, The History of Static SIMS: a Personal Perspective, in: TOFSIMS – Surface Analysis by Mass Spectrometry, J.C. Vickerman, D. Briggs (Eds.), IM Publications and Surface Spectra Limited, 2001 36. A. Benninghoven, F.G. Rüdenauer, H.W. Werner, Secondary Ion Mass Spectrometry – Basic Concepts, Instrumental Aspects, Applications and Trends, John Wiley and Sons, Inc., 1987 37. J.C. Vickerman, D. Briggs (Eds.), TOF-SIMS – Surface Analysis by Mass Spectrometry, IM Publications and Surface Spectra Limited, 2001 236 13 Direct Diﬀusion Studies 38. H. Mehrer, R. Galler, W. Frank, R. Blüher, T. Strohm, Diﬀusion in Quasicrystals, in: Quasicrystals: Structure and Physical Properties, H.-R. Trebin (Ed.), J. Wiley VCH, 2003 39. M.-P. Macht, V. Naundorf, J. Appl. Phys. 53, 7551 (1982) 40. S. Frank, U. Södervall, Chr. Herzig, Phys. Stat. Sol. (b) 191, 45 (1995) 41. E.C. Stelter, D. Lazarus, Phys. Rev. B 36, 9545 (1987) 42. A.K. Tyagi, M.-P. Macht, V. Naundorf, Scripta Metall. et Mater. 24, 2369 (1999) 43. A.K. Tyagi, M.-P. Macht, V. Naundorf, Acta Metall. et Mater. 39, 609 (1991) 44. R. Castaing, Ph.D. thesis, Univ. of Paris, 1951 45. H.G.J. Moseley, Philos. Mag. 26, 1024 (1913) 46. H.-J. Hunger, Elektronenstrahl-Mikroanalyse und Rasterelektronen-Mikroskopie, in: Ausgewählte Untersuchungsverfahren der Metallkunde, H.-J. Hunger et al. (Eds.), VEB Deutscher Verlag für Grundstoﬃndustrie, Leipzig, 1983, p.175 47. E. Lifshin, Electron Microprobe Analysis, in: Materials Science and Technology, R.W. Cahn, P. Haasen, E.J. Kramer (Eds.), Vol. 2B: Characterisation of Materials, VCH, 1994, p. 351 48. P. Auger, Surf. Sci 1, 48 (1975) 49. S. Hofmann, Surf. Interface Anal. 9, 3 (1986) 50. A. Zalar, S. Hofmann, Surf. Interface Anal. 12, 83 (1988) 51. S.K. Sharma, P. Mukhopadhyay, Acta Metall. 38, 129 (1990) 52. M.M. Kijek, D.W. Palmer, B. Cantor, Acta Metall. 34, 1455 (1986) 53. E. Rutherford, Philos. Mag. 21, 669 (1911) 54. H. Geiger, E. Marsden, Philos. Mag. 25, 206 (1913) 55. S.M. Myers, Ion-beam Analysis and Ion Implantation in the Study of Diﬀusion, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p. 137 56. W.A. Lanford, R. Benenson, C. Burman, L. Wielunski, Nuclear Reaction Analysis for Diﬀusion Studies, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p. 155 57. W.K. Chu, J. Liu, Z. Zhang, K.B. Ma, High Energy Ion Beam Analysis Techniques, in: Materials Science and Technology, R.W. Cahn, P. Haasen, E.J. Cramer (Eds.), Vol. 2B: Characterisation of Materials, VCH Weinheim, 1994, p. 423 14 Mechanical Spectroscopy 14.1 General Remarks The discoveries of thermally-activated anelastic relaxation processes in solids by Snoek [1], Zener [2, 3] and Gorski [4] were made more than half a century ago. Since then, anelastic measurements have become an established tool for the study of atomic movements in solids. Relaxation methods and the closely related internal friction (or damping) methods make use of the fact that atomic motion in a solid can be induced by the application of constant or oscillating mechanical stress. Nowadays, anelastic measurements are also denoted by the title mechanical spectroscopy. Under the inﬂuence of an applied stress or strain, an instantaneous elastic eﬀect (Hooke’s law) is observed, followed by strain or stress which varies with time. The latter eﬀect is called anelasticity or anelastic relaxation. Anelastic behaviour is reversible. If stress (strain) is removed the sample will return – after some time – to its initial shape. This distinguishes anelastic from plastic behaviour. Light interstitials, such as H, C, N, and O as well as substitutional solutes and solute-defect complexes are accompanied by local straining of the surrounding lattice. The presence of microstrains surrounding a diﬀusing atom allows interaction between a macroscopic stress ﬁeld arising from external forces applied to the material. This interaction generates a rich variety of stress-assisted diﬀusion eﬀects. Stress-mediated motion can cause time-dependent anelastic (recoverable) strains that result in several types of internal friction processes encountered in many materials. Sometimes, anelastic relaxation involves the reorientation of point defects which act as elastic dipoles as illustrated in Fig. 14.1. Reorientation relaxations are short-range processes, which in some cases involve only one or few atomic jump(s). However, only in some special cases, exempliﬁed by Snoek relaxation, the same jump produces both reorientation and diﬀusion. Only then, a simple relationship exists between the relaxation time and the long-range diﬀusion coeﬃcient. Long-range diﬀusion controls the so-called Gorski relaxation illustrated in Fig. 14.2. Gorsky relaxation can be produced by bending a sample containing defects, which act as dilatation centers. In practice, the only experimentally known example of Gorski relaxation is due to hydrogen diﬀusion metals. It can be observed because hydrogen diﬀusion is very fast. 238 14 Mechanical Spectroscopy Fig. 14.1. Schematic illustration of anelastic relaxation caused by reorientation of elastic dipoles (represented by grey ellipses) Fig. 14.2. Schematic illustration of Gorski-eﬀect One should, however, keep in mind that mechanical relaxation and internal friction may arise from various sources. These can range from pointdefect reorientations, long-range diﬀusion, dislocation eﬀects, grain-boundary processes, and phase transformations to visco-elastic behaviour and plastic deformation. Some point-defect relaxations are diﬀusion-related, some are not. For point-defect relaxations of trapped and paired defects, the nature and the activation enthalpy of the reorientation jump can be signiﬁcantly diﬀerent from those associated with long-range diﬀusion. A review of the substantial body of work that has been accumulated on the study of atomic movement by anelastic methods is beyond the scope of this chapter. Several textbooks, e.g., those of Zener [3] and Nowick and Berry [5] and reviews by Berry and Pritchet [6, 7] are available for the interested reader. A review about the potential of mechanical loss spectroscopy for inorganic glasses and glass ceramics has been given by Roling [8]. A comprehensive treatment of magnetic relaxation eﬀects can be found in a textbook of Kronmüller [9]. In the present chapter, we ﬁrst mention the basic concepts of mechanical loss spectroscopy, i.e. of anelastic behaviour and internal friction. Then, we describe some examples of diﬀusion-related anelasticity such as the Snoek eﬀect, the Zener eﬀect, the Gorski eﬀect, and give an example of a mechanical loss spectrum of glasses. 14.2 Anelasticity and Internal Friction 239 14.2 Anelasticity and Internal Friction From the viewpoint of mechanical stress-strain behaviour, we may regard an ideal solid as one which obeys Hooke’s law and thus behaves in an ideally elastic manner. Such a solid would always recover completely and instantaneously on removal of an applied stress. If set into vibration, the solid would vibrate forever with undiminished amplitude if totally isolated from its surroundings. The mechanical behaviour of real solids at low stress levels (below the yield stress) is modiﬁed by the appearance of anelasticity, which develops at a rate controlled by the atomic movements. It can often be traced back to the presence of mobile atoms or point defects. A quantitative description of the anelastic behaviour of materials can be found by analysing a model having the name standard linear solid, which was originally proposed by Voigt [10] and by Poynting and Thomson [11]. In this model, stress σ, strain , and their respective time derivatives, σ̇ and , ˙ are related through a linear response equation: ˙ . σ + τ σ̇ = MR ( + τσ ) (14.1) This anelastic equation of state is a generalisation of Hooke’s law of linear elasticity. Equation (14.1) contains three material parameters: the strain relaxation time τ , the stress relaxation time τσ (sometimes also denoted as the stress retardation time), and the relaxed elastic modulus MR . Figure 14.3 illustrates in its left part the strain response of a standard linear solid induced by an instantaneous application and subsequent removal of a constant stress. The continued relaxation of the strain after removal of the stress is also termed the elastic aftereﬀect. The stress response induced by instantaneous application and removal of strain is illustrated in the right part. Note that τσ and τ are diﬀerent. It is obvious from Eq. (14.1) that for vanishing time derivatives Eq. (14.1) reduces to Hooke’s law. Under uniaxial stress MR is termed the Young modulus, whereas under applied shear MR is termed the shear modulus. Periodic Stress and Strain: Let us now suppose that a uniaxial, periodic stress-time function of frequency ω and amplitude σ0 of the form σ = σ0 exp [iωt] (14.2) is imposed on the material. The time-dependent strain response of an anelastic solid then is = 0 exp [i(ωt − δ)] , (14.3) where δ is the phase shift between σ and . For a completely elastic material, σ and are in phase and the phase shift is zero for all frequencies. The stressstrain behaviour for an anelastic material under periodic stress is illustrated in Fig. 14.4. For an anelastic material a hysteresis loop is obtained. The area 240 14 Mechanical Spectroscopy Fig. 14.3. Schematic illustration of anelastic behaviour. The strain response for an instantaneous stress-time function is shown in the left half. The stress response for an instantaneous strain-time function corresponds to the right half Fig. 14.4. Stress-strain relations for a periodically driven anelastic material at three diﬀerent frequencies inside the hysteresis represents the dissipated energy per unit volume and per cycle (see below). It is convenient to introduce a complex elastic modulus M̂ via σ = M̂ , (14.4) which can be split up according to M̂ = M + iM , (14.5) i.e. into real and imaginary parts M and M , respectively. Assuming periodic strain with a frequency ω and substituting Eqs. (14.4) and (14.5) into Eq. (14.1) yields after a few steps of algebra M̂ = MR 1 + τσ iω . 1 + τ iω (14.6) 14.2 Anelasticity and Internal Friction 241 After separation into real and imaginary parts we get M (ω) = MR 1 + τ τσ ω 2 ω 2 τ2 = M + ∆M R 1 + ω 2 τ2 1 + ω 2 τ2 (14.7) (τσ − τ )ω ωτ = ∆M , 1 + ω 2 τ2 1 + ω 2 τ2 (14.8) and M (ω) = MR where the abbreviations ∆M ≡ MU − MR and ∆ ≡ ∆M/MR (14.9) have been introduced. At high frequencies, the time scale for stress and strain removals becomes small compared to the relaxation times. Then M approaches an unrelaxed elastic modulus MU = MR τσ , τ (14.10) which denotes the stress increment per unit strain at high frequency. Note that MU and MR are diﬀerent because τσ and τ are diﬀerent. The tangent of the loss angle δ is given by tan δ ≡ M /M = ∆M ωτ ω(τσ − τ ) ≡ ∆ . MR + MU ω 2 τ2 1 + τσ τ ω 2 (14.11) Internal Friction: Internal friction is the dissipation of mechanical energy caused by anelastic processes occurring in a strained solid. The internal friction, usually called Q−1 , in a cyclically driven anelastic solid is deﬁned as Q−1 ≡ ∆Edissipated , Estored (14.12) where ∆Edissipated is the energy dissipated as heat per unit volume of the material over one cycle. Estored denotes the peak elastic energy stored per unit volume. For a periodically strained solid subject to sinusoidal stress, the internal friction is given by the following ratio of energy integrals: ' 2π σ(ωt)(ωt) ˙ out−of −phase d(ωt) −1 . (14.13) Q = 0 ' 2π ˙ in−phase d(ωt) 0 σ(ωt)(ωt) Substituting the out-of-phase and in-phase components of the strain rate ˙ yields after some algebra the following relation between internal friction and the tangent of the loss angle: Q−1 = π tan δ . (14.14) 242 14 Mechanical Spectroscopy It is convenient to combine the stress and strain relaxation times to a mean relaxation time τ , which is deﬁned as the geometric mean of the two fundamental times: √ (14.15) τ ≡ τσ τ . We will see later that τ sometimes can be associated with atomic jump processes occurring in the strained solid, having a well-deﬁned activation enthalpy. It is also convenient to combine the relaxed and the unrelaxed moduli to a mean modulus M via τσ τ MR = MU . (14.16) M ≡ MR MU = τ τσ Using the deﬁnitions of the mean modulus Eq. (14.16), the mean relaxation time Eq. (14.15) and Eq. (14.11), yields a basic expression for internal friction: Q−1 = π tan δ = π ωτ ∆M . M 1 + ω2τ 2 (14.17) The term π∆M/M is called the relaxation strength. The second term describes the frequency dependence of internal friction. Figure 14.5 shows a diagram of Q−1 versus the logarithm of ωτ . The frequency-dependent modulus M is also shown, which varies between the relaxed modulus MR at low frequencies and the unrelaxed modulus MU at high frequencies. The maximum of internal friction occurs when ωτ = 1 (14.18) is fulﬁlled. This relation is an important condition for the analysis of anelasticity. If an anelastic solid is strained periodically with a frequency ω the maximum energy loss occurs, when the imposed frequency and relaxation time of the process match. 14.3 Techniques of Mechanical Spectroscopy Usually, the relaxation time τ is thermally activated according to ∆H τ ∝ exp , kB T (14.19) where ∆H denotes some activation enthalpy. Thus, by varying the temperature at constant frequency ω a maximum of internal friction occurs on the temperature scale. This is the usual way of measuring internal friction peaks, as temperature is easier to vary than frequency. The latter is often more or less ﬁxed by the internal friction device. By using diﬀerent experimental techniques, the mechanical loss can be determined at frequencies roughly between 10−5 and 5 × 1010 Hz. It is convenient to perform temperature-dependent measurements at ﬁxed frequencies. 14.3 Techniques of Mechanical Spectroscopy 243 Fig. 14.5. Internal friction, Q−1 = π tan δ, and frequency dependent modulus, M , as functions of ωτ In this case, a thermally activated process manifests itself in a loss peak, which shifts to higher temperatures as the frequency is increased. Information on the activation enthalpy is then obtained from the peak temperatures, Tpeak , shifting with frequencies ω by using the equation: ∆H = −kB d ln ω . d(1/Tpeak ) (14.20) In the Hz regime torsional pendulums operating at their natural frequencies can be used. A major disadvantage of this technique is that the range of available frequencies is very narrow, often less than half a decade. This makes it diﬃcult to determine accurate values of the activation enthalpies and to analyse frequency-temperature relations in detail. In order to overcome this limitation devices with forced oscillations are in use. The frequency window of this technique ranges approximately from 30 Hz up to 105 Hz. At higher frequencies, the mechanical loss of solids can be studied by resonance methods [14, 15]. At even higher frequencies, in the MHz and GHz regimes, ultrasonic absorption and Brillouin light scattering can be used. However, most mechanical loss studies have been done and are still done with the help of low-frequency methods. Starting in the 1990s, there have been eﬀorts to make use of commercially available instrumentation for dynamic mechanical thermal analysis (DMTA) These devices usually operate in the three-point-bending mode. Among other systems, this technique has been applied to study relaxation processes in oxide glasses [16–18]. 244 14 Mechanical Spectroscopy Fig. 14.6. Octahedral interstitial sites in the bcc lattice 14.4 Examples of Diﬀusion-related Anelasticty 14.4.1 Snoek Eﬀect (Snoek Relaxation) The Snoek eﬀect is the stress-induced migration of interstitials such as C, N, or O in bcc metals. Although eﬀects of internal friction in bcc iron were reported as early as the late 19th century, this phenomenon was ﬁrst carefully studied and analysed by the Dutch scientist Snoek [1]. Interstitial solutes in bcc crystals usually occupy octahedral interstitial sites illustrated in Fig. 14.6. Octahedral sites in the bcc lattice have tetragonal symmetry inasmuch the distance from an interstitial site to neighbouring lattice atoms is shorter along 100 than along 110 directions. The microstrains surrounding interstitial solutes have tetragonal symmetry as well, which is lower than the cubic symmetry of the matrix. Another way of expressing this is to say that interstitial solutes give rise to permanent elastic dipoles. Figure 14.6 illustrates the three possible orientations of octahedral sites denoted as X-, Y-, and Z-sites. Without external stress all sites are energetically equivalent, i.e. EX = EY = EZ , and the population n0j of interstitial sites by solutes is n0X = n0Y = n0Z = n0 /3. n0 denotes the total number of interstitials. If an external stress is applied this degeneracy is partly or completely removed, depending on the orientation of the external stress. For example, with uniaxial stress in the Z-direction Z-sites are energetically slightly diﬀerent from X- and Y-sites, i.e. EZ = EX = EY . In contrast, uniaxial stress in 111 direction does not not remove the energetic degeneracy, because all sites are energetically equivalent. In thermodynamic equilibrium the distribution of interstitial solutes on the X-, Y-, and Z-sites is given by 0 neq i = n exp(−Ei /kB T ) . j=X,Y,Z exp(−Ej /kB T ) (14.21) In general, under the inﬂuence of a suitable oriented external stress the ‘solute dipoles’ reorient, if the interstitial atoms have enough mobility. This redistribution gives rise to a strain relaxation and/or to an internal friction peak. 14.4 Examples of Diﬀusion-related Anelasticty 245 The relaxation time or the frequency/temperature position of the internal friction peak can be used to deduce information about the mean residence time of a solute on a certain site. In order to deduce this information, we consider the temporal development of interstitial subpopulations nX , nY , nZ on X-, Y-, and Z-sites. Suppose that uniaxial stress is suddenly applied in Z-direction. This stress disturbs the initial equipartition of interstitials on the various types of sites and redistribution will start. Fig 14.6 shows that every X-site interstitial that performs a single jump ends either on a Y- or on a Z-site. Interstitials on Y- and Z-sites jump with equal probabilities to X-sites. The rate of change of the interstitial subpopulations can be expressed in terms of the interstitial jump rate, Γint , as follows: dnX (14.22) = −2Γint nX + Γint (nY + nZ ) . dt The ﬁrst term on the right-hand side in Eq. (14.22) represents the loss of interstitials located at X-sites due to hops to either Y- or Z-sites. The second term on the right-hand side represents the gain of interstitials at X-sites from other interstitials jumping from either Y- or Z-sites. Corresponding equations are obtained for nY and nZ by cyclic permutation of the indices. Since the total number of interstitials, n0 , is conserved, we have n0 = nX + nY + nZ . (14.23) Substitution of Eq. (14.23) into Eq. (14.22) yields " # Γint 0 3 dnX 0 = −Γint nX + (n − neq X ) = − Γint nX − n /3 . dt 2 2 (14.24) Equation (14.24) is an ordinary diﬀerential equation for the population dynamics of interstitial solutes. Its solution can be written in the form " 0 t eq # exp − nX (t) = neq + n − n , (14.25) X X X τR where the relaxation time τR is given by τR = 2 . 3Γint (14.26) The relaxation time is closely related to the mean residence time, τ̄ , of an interstitial solute on a given site. Because an interstitial solute on an octahedral site can leave its site in four directions with jump rate Γint , we have τ̄ = 1 . 4Γint (14.27) 246 14 Mechanical Spectroscopy The solute jump rate can be written in the form M Hint 0 Γint = ν exp − , kB T (14.28) M denote attempt frequency and activation enthalpy of a sowhere ν 0 and Hint lute jump. Then, the relaxation time of the Snoek eﬀect is M 1 4 Hint . (14.29) τR = τ̄ = 0 exp 3 6ν kB T The jump of an interstitial solute which causes Snoek relaxation and the elementary diﬀusion step (jump length d = a/2, a = lattice parameter) are identical. The diﬀusion coeﬃcient developed from random walk theory for octahedral interstitials in the bcc lattice is given by D= 1 1 Γint d2 = Γint a2 . 6 24 (14.30) Substituting Eqs. (14.27) and (14.29) into Eq. (14.30) yields D= 1 a2 . 36 τR (14.31) This equation shows that Snoek relaxation can be used to study diﬀusion of interstitial solutes in bcc metals by measuring the relaxation time. It is also applicable to interstitial solutes in hcp metals since the non-ideality of the c/a-ratio gives rise to an asymmetry in the octahedral sites. Very pure and very dilute interstitial alloys must be used, if the Snoek eﬀect of isolated interstitials is in focus. Otherwise, solute-solute or solute-impurity interactions could cause complications such as broadening or shifts of the internal friction peak. Figure 14.7 shows an Arrhenius diagram of carbon diﬀusion in α-iron. For references the reader may consult Le Claire’s collection of data for interstitial diﬀusion [12] and/or a paper by da Silva and McLellan [13]. The data above about 700 K have been obtained with various direct methods including diﬀusion-couple methods, in- and out-diﬀusion, or thin layer techniques. The data below about 450 K were determined with indirect methods, including internal friction, elastic after-eﬀect, or magnetic after-eﬀect measurements. The data cover an impressive range of about 14 orders of magnitude in the carbon diﬀusivity. Extremely small diﬀusivities around 10−24 m2 s−1 are accessible with the indirect methods, illustrating the potential of these techniques. The Arrhenius plot of C diﬀusion is linear over a wide range at lower temperatures. There is some small positive curvature at higher temperatures. One possible origin of this curvature could be an inﬂuence the magnetic transition, which takes place at the Curie temperature TC . In the case of self-diﬀusion of iron this inﬂuence is well-studied (see Chap. 17). 14.4 Examples of Diﬀusion-related Anelasticty 247 Fig. 14.7. Diﬀusion coeﬃcient for C diﬀusion in α-Fe obtained by direct and indirect methods: DIFF = in- and out-diﬀusion or diﬀusion-couple methods; IF = internal friction; EAE = elastic after eﬀect, MAE = magnetic after eﬀect It is interesting to note that the Snoek eﬀect cannot be used to study interstitial solutes in fcc metals. Interstitial solutes in fcc metals are also incorporated in octahedral sites. In contrast to octahedral sites in the bcc lattice, which have tetragonal symmetry, octahedral sites in the fcc lattice and the microstrains associated with an interstitial solute in such sites have cubic symmetry. Interstitial solutes produce some lattice dilation but no elastic dipoles. Therefore, an external stress will not result in changes of the interstitial populations in an fcc matrix. 14.4.2 Zener Eﬀect (Zener Relaxation) The Zener eﬀect, like the Snoek eﬀect, is a stress-induced reorientation of elastic dipoles by atomic jumps. Atom pairs in substitutional alloys, pairs of interstitial atoms, solute-vacancy pairs possessing lower symmetry than the lattice can form dipoles responsible for Zener relaxation. For example, in strain-free dilute substitutional fcc alloys solute atoms are distributed ran- 248 14 Mechanical Spectroscopy domly and isotropically. Solute-solute pairs on nearest-neighbour sites are uniformly distributed among the six 110 directions. The size diﬀerence between solute and solvent atoms causes pairs to create microstrains with strain ﬁelds of lower symmetry than that of the cubic host crystal. A well-studied example of solute-solute pair reorientation in fcc materials was reported already by Zener [2]. He observed a strong internal friction peak in Cu-Zn alloys (α-brass) around 570 K. The stress-mediated reorientation of random Zn-Zn pairs along 110 in fcc crystals is somewhat analogous to the Snoek eﬀect. Le Claire and Lomer interpreted this relaxation on the basis of changing directional short-range order under the inﬂuence of external stress. In reality, the Zener eﬀect in dilute substitutional fcc alloys depends on several exchange jump frequencies between solute atoms and vacancies. Therefore, it is diﬃcult to relate the eﬀect to the diﬀusion of solute atoms in a quantitative manner. A satisfactory model, such as is available for the Snoek eﬀect of dilute interstitial bcc alloys, is not straightforward. The activation enthalpy of the process can be determined. However, in a pair model for low solute concentrations the activation energy is more characteristic of the rotation of the dipoles than of long-range diﬀusion. 14.4.3 Gorski Eﬀect (Gorski Relaxation) In contrast to reorientation relaxations discussed above, the Gorski eﬀect is due to the long-range diﬀusion of solutes B which produce a lattice dilatation in a solvent A. This eﬀect is named after the Russian scientist Gorski [4]. Relaxation is initiated, for example, by bending a sample to introduce a macroscopic strain gradient. This gradient induces a gradient in the chemical potential of the solute, which involves the size-factor of the solute and the gradient of the dilatational component of the stress. Solutes redistribute by ‘up-hill’ diﬀusion and develop a concentration gradient, as indicated in Fig. 14.2. This transport produces a relaxation of elastic stresses, by the migration of solutes from the regions in compression to those in dilatation. The associated anelastic relaxation is ﬁnished when the concentration gradient equalises with the chemical potential gradient across the sample. For a strip of thickness d, the Gorski relaxation time, τG , is given by τG = d2 π 2 ΦD , (14.32) B where DB is the diﬀusion coeﬃcient of solute B and Φ is the thermodynamic factor. A thermodynamic factor is involved, because Gorski relaxation establishes a chemical gardient. Equation (14.32) shows that with the Gorski eﬀect one measures the time required for diﬀusion of B atoms across the sample. The Gorski relaxation time is a macroscopic one, in contrast to the relaxation time of the Snoek relaxation. If the sample dimensions are known, an absolute value of the 14.4 Examples of Diﬀusion-related Anelasticty 249 Fig. 14.8. Mechanical loss spectrum of a Na2 O4SiO4 at a frequency of 1 Hz according to Roling and Ingram [18, 19] diﬀusivity is obtained. For a derivation of Eq. (14.32) we refer the reader to the review by Völkl [20]. The Gorski eﬀect is detectable if the diﬀusion coeﬃcient of the solute is high enough. Gorski eﬀect measurements have been widely used for studies of hydrogen diﬀusion in metals [6, 20–22]. 14.4.4 Mechanical Loss in Ion-conducting Glasses Diﬀusion and ionic conduction in ion-conducting glasses is the subject of Chap. 30. Mechanical loss spectroscopy is also applicable for the characterisation of dynamic processes in glasses and glass ceramics. This method can provide information on the motion of mobile charge carriers, such as ions and polarons, as well as on the motion of network forming entities. Mixed mobile ion eﬀects in diﬀerent types of mixed-alkali glasses, mixed alkali-alkaline earth glasses, mixed alkaline earth glasses, and mixed cation anion glasses. For references see, e.g., a review of Roling [8]. Let us consider an example: Fig. 14.8 shows the loss spectrum of a sodium silicate glass according to Roling and Ingram [18, 19]. Such a spectrum is typical for ion conducting glasses. The low-temperature peak near 0 ◦ C is attributed to the hopping motion of sodium ions, which can be studied by conductivity measurements in impedance spectroscopy and by tracer diﬀusion techniques as well (for examples see Chap. 30). The activation enthalpy of the loss peak is practically identical to the activation enthalpy of the dc conductivity, which is due to the long-range motion of sodium ions [19]. The intermediate-temperature peak at 235 ◦ C is attributed to the presence of water in the glass. The increase of tan δ near 350 ◦ C is caused by the onset of the glass transition. 250 14 Mechanical Spectroscopy 14.5 Magnetic Relaxation In ferromagnetic materials, the interaction between the magnetic moment and local order can give rise to various relaxation phenomena similar to those observed in anelasticity. Their origin lies in the induced magnetic anisotropy energy, the theory of which was developed by the French Nobel laureate Neel [24]. An example, which is closely related to the Snoek eﬀect, was reported for the ﬁrst time in 1937 by Richter [23] for α-Fe containing carbon. The direction of easy magnetisation in α-iron within a ferromagnetic domain is one of the three 100 directions. Therefore, the octahedral X-, Y-, and Z-positions for carbon interstitials are energetically not equivalent. A repopulation among these sites takes place when the magnetisation direction changes. This can happen when a magnetic ﬁeld is applied. Suppose that the magnetic susceptibility χ is measured by applying a weak alternating magnetic ﬁeld. Beginning with a uniform population of the interstitials, after demagnetisation a redistribution into the energetically favoured sites will occur. This stabilises the magnetic domain structure and reduces the mobility of the Bloch walls. As a consequence, a temporal decrease of the susceptibility χ is observed, which can be described by t χ(t) = χ0 − ∆χs 1 − exp − , (14.33) τR where ∆χs = χ0 − χ(∞) is denoted as the stabilisation susceptibility, t is the time elapsed since demagnitisation, and τR is the relaxation time. The relationship between jump frequency, relaxation time, and diﬀusion coeﬃcient is the same as for anelastic Snoek relaxation. The magnetic analogue to the Zener eﬀect is directional ordering of ferromagnetic alloys in a magnetic ﬁeld, which produces an induced magnetic anisotropy. The kinetics of the establishment of magnetic anisotropy after a thermomagnetic treatment can yield information about the activation energy of the associated diﬀusion process. The link between the relaxation time and diﬀusion coeﬃcient is as diﬃcult to establish as in the case of the Zener eﬀect. A magnetic analogue to the Gorski eﬀect is also known. In a magnetic domain wall, the interaction between magnetostrictive stresses and the strain ﬁeld of a defect (such as interstitials in octahedral sites of the bcc lattice, divacancies, etc.) can be minimised by diﬀusional redistribution in the wall. This diﬀusion gives rise to a magnetic after-eﬀect. The relaxation time is larger by a factor δB /a (δB = thickness of the Bloch wall, a = lattice parameter) than for magnetic Snoek relaxation. The variation of the susceptibility with time is more complex than in Eq. (14.33). A comprehensive treatment of magnetic relaxation eﬀects can be found in the textbook of Kronmüller [9]. Obviously, magnetic methods are applicable to ferromagnetic materials at temperatures below the Curie point only. References 251 References 1. J.L. Snoek, Physica 8, 711 (1941) 2. C. Zener, Trans. AIME 152, 122 (1943) 3. C. Zener, Elasticity and Anelasticicty of Metals, University of Chicago Press, Chicago, 1948 4. W.S. Gorski, Z. Phys. Sowjetunion 8, 457 (1935) 5. A.S. Nowick, B.S. Berry, Anelastic Relaxation in Crystalline Solids, Academic Press, New York, 1972 6. B.S. Berry, W.C. Pritchet, Anelasticity and Diﬀusion of Hydrogen in Glassy and Crystalline Metals, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p.83 7. R.D. Batist, Mechanical Spectroscopy, in: Materials Science and Technology, Vol. 2B: Characterisation of Materials, R.W. Cahn, P. Haasen, E.J. Cramer (Eds.), VCH, Weinheim, 1994. p. 159 8. B. Roling, Mechanical Loss Spectroscopy on Inorganic Glasses and Glass Ceramics, Current Opinion in Solid State Materials Science 5, 203–210 (2001) 9. H. Kronmüller, Nachwirkung in Ferromagnetika, Springer Tracts in Natural Philosophy, Springer-Verlag, 1968 10. W. Voigt, Ann. Phys. 67, 671 (1882) 11. J.H. Poynting, W. Thomson, Properties of Matter, C. Griﬃn & Co., London, 1902 12. A.D. Le Claire, Diﬀusion of C, N, and O in Metals, Chap. 8 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol.Ed,), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 13. J.R.G. da Silva. R.B. McLellan, Materials Science and Engineering 26, 83 (1976) 14. J. Woirgard, Y. Sarrazin, H. Chaumet, Rev. Sci. Instrum. 48, 1322 (1977) 15. S. Etienne, J.Y. Cavaille, J. Perez, R. Point, M. Salvia, Rev. Sci. Instrum. 53, 1261 (1982) 16. P.F. Green, D.L. Sidebottom, R.K. Brown, J. Non-cryst. Solids 172–174, 1353 (1994) 17. P.F. Green, D.L. Sidebottom, R.K. Brown, J.H. Hudgens, J. Non-cryst. Solids 231, 89 (1998) 18. B. Roling, M.D. Ingram, Phys. Rev. B 57, 14192 (1998) 19. B. Roling, M.D. Ingram, Solid State Ionics 105, 47 (1998) 20. J. Völkl, Ber. Bunsengesellschaft 76, 797 (1972) 21. J. Völkl, G. Alefeld, in: Hydrogen in Metals I, G. Alefeld, J. Völkl (Eds.), Topics in Applied Physics 28, 321 (1978) 22. H. Wipf, Diﬀusion of Hydrogen in Metals, in: Hydrogen in Metals III, H. Wipf (Ed.), Topics in Applied Physics 73, 51 (1995) 23. G. Richter, Ann. d. Physik 29, 605 (1937) 24. L. Neel, J. Phys. Rad. 12, 339 (1951); J. Phys. Rad. 13, 249 (1952); J. Phys. Rad. 14, 225 (1954) 15 Nuclear Methods 15.1 General Remarks Several nuclear methods are important for diﬀusion studies in solids. They are listed in Table 13.1 and their potentials are illustrated in Fig. 13.1. The ﬁrst of these methods is nuclear magnetic resonance or nuclear magnetic relaxation (NMR). NMR methods are mainly appropriate for self-diﬀusion measurements on solid or liquid metals. In favourable cases self-diﬀusion coeﬃcients between about 10−20 and 10−10 m2 s−1 are accessible. In the case of foreign atom diﬀusion, NMR studies suﬀer from the fact that a signal from nuclear spins of the minority component must be detected. Mössbauer spectroscopy (MBS) and quasielastic neutron scattering (QENS) are techniques, which have considerable potential for understanding diﬀusion processes on a microscopic level. The linewidths ∆Γ in MBS and in QENS have contributions which are due to the diﬀusive motion of atoms. This diﬀusion broadening is observed only in systems with fairly high diﬀusivities since ∆Γ must be comparable with or larger than the natural linewidth in MBS experiments or with the energy resolution of the neutron spectrometer in QENS experiments. Usually, the workhorse of MBS is the isotope 57 Fe although there are a few other, less favourable Mössbauer isotopes such as 119 Sn,115 Eu, and 161 Dy. QENS experiments are suitable for fast diﬀusing elements with a large incoherent scattering cross section for neutrons. Examples are Na self-diﬀusion in sodium metal, Na diﬀusion in ion-conducting rotor phases, and hydrogen diﬀusion in metals. Neither MBS nor QENS are routine methods for diﬀusion measurements. The most interesting aspect is that these methods can provide microscopic information about the elementary jump process of atoms. The linewidth for single crystals depends on the atomic jump frequency and on the crystal orientation. This orientation dependence allows the deduction of the jump direction and the jump length of atoms, information which is not accessible to conventional diﬀusion studies. 15.2 Nuclear Magnetic Relaxation (NMR) The technique of nuclear magnetic relaxation has been widely used for many years to give detailed information about condensed matter, especially about 254 15 Nuclear Methods its atomic and electronic structure. It was recognised in 1948 by Bloembergen, Purcell and Pound [1] that NMR measurements can provide information on diﬀusion through the inﬂuence of atomic movement on the width of nuclear resonance lines and on relaxation times. Atomic diﬀusion causes ﬂuctuations of the local ﬁelds, which arise from the interaction of nuclear magnetic moments with their local environment. The ﬂuctuating ﬁelds either can be due to magnetic dipole interactions of the magnetic moments or due to the interaction of nuclear electric quadrupole moments (for nuclei with spins I > 1/2) with internal electrical ﬁeld gradients. In addition, external magnetic ﬁeld gradients can be used for a direct determination of diﬀusion coeﬃcients. We consider below some basic principles of NMR. Our prime aim is an understanding of how diﬀusion inﬂuences NMR. Solid state NMR is a very broad ﬁeld. For a comprehensive treatment the reader is referred to textbooks of Abragam [2], Slichter[3], Mehring [4] and to chapters in monographs and textbooks [5–9]. In addition, detailed descriptions of NMR relaxation techniques are available, e.g., in [10]). Corresponding pulse programs are nowadays implemented in commercial NMR spectrometers. 15.2.1 Fundamentals of NMR NMR methods are applicable to atoms with non-vanishing nuclear spin moment, I, and an associated magnetic moment µ = γI , (15.1) where γ is the gyromagnetic ratio, I the nuclear spin, and the Planck constant divided by 2π. In a static magnetic ﬁeld B0 in z-direction, a nuclear magnetic moment µ performs a precession motion around the z-axis governed by the equation dµ = µ ⊗ B0 . (15.2) dt The precession frequency is the Larmor frequency ω0 = γB0 . (15.3) The degeneracy of the 2I +1 energy levels is raised due to the nuclear Zeeman eﬀect. The energies of the nuclear magnetic dipoles are quantised according to (15.4) Um = −mγB0 , where the allowed values correspond to m = −I, −I + 1, . . . , I − 1, I. For example, for nuclei with I = 1/2 there are only two energy levels with the energy diﬀerence ω0 . At thermal equilibrium, the spins are distributed according to the Boltzmann statistics on the various levels. Since the energy diﬀerence between 15.2 Nuclear Magnetic Relaxation (NMR) 255 Fig. 15.1. Set-up for a NMR experiment (schematic) levels for typical magnetic ﬁelds (0.1 to 1 Tesla) is very small, the population diﬀerence of the levels is also small. A macroscopic sample in a static magnetic ﬁeld B 0 in the z-direction displays a magnetisation M eq along the z-direction and a transverse magnetisation M⊥ = 0. The equilibrium magnetisation of an ensemble of nuclei (number density N ) is given by M eq = N γ 2 2 I(I + 1) B0 . 3kB T (15.5) A typical experimental set-up for NMR experiments (Fig. 15.1) consists of a sample placed in a strong, homogeneous magnetic ﬁeld B 0 of the order of a few Tesla. A coil wound around the sample permits the application of an alternating magnetic ﬁeld B 1 perpendicular to the z-direction with frequency ω. Typically, these ﬁelds are radio-frequency (r.f.) ﬁelds. If the frequency ω of the transverse r.f. ﬁeld B 1 is close to the Larmor frequency, this ﬁeld will induce transitions between the Zeeman levels of the nuclear spins. In NMR-spectrometers the coil around the sample is used for several steps of the experiment, such as irradiation of r.f. pulses and detection of the free induction decay of the ensemble of nuclei (see below). The analysis of NMR experiments proceeds via a consideration of detailed interactions among nuclear moments and between them and other components of the solid such as electrons, point defects, and paramagnetic impurities. This theory has been developed over the past decades and can be found, e.g., in the textbooks of Abragam [2] and Slichter [3]. Although this demands the use of quantum mechanics, much can be represented by semi-classical equations proposed originally by Bloch. The eﬀect of rf-pulse sequences on the time evolution of the total magnetisation M in an external ﬁeld (15.6) B = B0 + B1 256 15 Nuclear Methods is given by the Bloch equation [2, 3]: dM M⊥ Mz − Mzeq = γM ⊗ B − − + ∇ [D∇(M − M eq )] . dt T2 T1 (15.7) The ﬁrst term in Eq. (15.7) describes the precession of the spins around the magnetic ﬁeld B. The second and third terms give the rate of relaxation of the magnetisation and deﬁne two phenomenological constants, T1 and T2 , denoted as relaxation times. They pertain to the longitudinal and transverse components of the magnetisation. In the absence of any transverse ﬁeld, T1 determines the rate at which Mz returns to its equilibrium value Mzeq . This relaxation corresponds to an energy transfer between the spin-system and the so-called ‘lattice’, where the ‘lattice’ represents all degrees of freedom of the material with the exception of those of the spin-system. Therefore, T1 is denoted as the spin-lattice relaxation time. T2 refers to the transverse part of the nuclear magnetisation and is called the spin-spin relaxation time. Nuclear spins can be brought to a state of quasi-thermal equilibrium among themselves without being in thermal equilibrium with the lattice. T2 describes relaxation to such a state. It follows that T2 ≤ T1 . T2 is closely related to the width of the NMR signal. The last term in Eq. (15.7) was introduced by Torrey [11] and describes the time evolution of the magnetisation M , when the sample is also put into a magnetic ﬁeld gradient. M eq is the equilibrium value of the magnetic moment in ﬁeld B0 and D the diﬀusion coeﬃcient. Equation (15.7) shows that various NMR techniques can be used to deduce information about atomic diﬀusion. Elegant pulse techniques of radiofrequency spectroscopy permit the direct determination of D and of the relaxation times T1 and T2 (see, e.g., Gerstein and Dybowski [10]). 15.2.2 Direct Diﬀusion Measurement by Field-Gradient NMR When a sample is placed deliberately in a magnetic ﬁeld gradient, G = ∂B/∂z, in addition to a static magnetic ﬁeld, a direct determination of diﬀusion coeﬃcients is possible. The basis of such NMR experiments in an inhomogeneous magnetic ﬁeld is the last term of the Bloch equation. In a magnetic ﬁeld gradient the Larmor frequency of a nuclear moment depends on its positions. Field-gradient NMR (FG-NMR) utilises the fact that nuclear spins that diﬀuse in a magnetic ﬁeld-gradient experience an irreversible phase shift, which leads to a decrease in transversal magnetisation. This decay can be observed in so-called spin-echo experiments [12, 13]. The amplitude of the spin-echo is given by ⎤ ⎡ ! t techo MG (techo ) = M0 (techo ) exp ⎣−γ 2 D 2 G(t ) dt 0 0 dt ⎦ , (15.8) 15.2 Nuclear Magnetic Relaxation (NMR) where techo M0 (techo ) = M0 (0) exp − . T2 257 (15.9) techo denotes the time of the spin echo. MG (techo ) and M0 (techo ) are the echo amplitudes with and without ﬁeld-gradient G(t). M0 (0) is the equilibrium magnetisation of the spin system. For a 90-τ -180-τ spin-echo pulse sequence we have techo = 2τ . In a constant magnetic ﬁeld gradient G0 the solution of Eq. (15.8) is proportional to the transversal magnetisation M⊥ , which is given by 2τ 2 2 2 3 MG (2τ ) = M0 (0) exp − exp − γ DG0 τ . (15.10) T2 3 By varying τ or G0 the diﬀusion coeﬃcient can be determined from the measured spin-echo amplitude. The diﬀusion of spins is followed directly by FG-NMR. Thus, FG-NMR is comparable to tracer diﬀusion. For a known G0 value a measurement of the diﬀusion-related part of the spin echo versus time can provide the diﬀusion coeﬃcient without any further hypothesis. In contrast to tracer diﬀusion, the FG-NMR technique permits diﬀusion measurements in isotopically pure systems. Equation (15.10) shows that the FG-NMR technique is applicable when the spin-spin relaxation time T2 of the sample is large enough. A signiﬁcant diﬀusion-related decay of the spin-echo amplitude must occur within T2 . For ﬁxed values of T2 and G0 this requires D-values that are large enough. The measurement of small D-values requires high ﬁeld-gradients. This can be achieved by using pulsed magnetic ﬁeld-gradients (PFG) as suggested by McCall [14]. The ﬁrst experiments with PFG-NMR were performed by Stejskal and Tanner [13] for diﬀusion studies in aqueous solutions. For a comprehensive review of PFG-NMR spectroscopy the reader is referred, for example, to the reviews of Stilbs [15], Kärger et al. [16], and Majer [7]. PFG-NMR has been widely applied to study diﬀusion of hydrogen in metals and intermetallic compounds [7]. Applications to anomalous diﬀusion processes such as diﬀusion in porous materials and polymeric matrices can be found in [16]. Diﬀusion of hydrogen in solids is a relatively fast process and the proton is particularly suited for NMR studies due to its high gyromagnetic ratio. Diﬀusivities of hydrogen between 10−10 and 10−13 have been studied by PFG-NMR [7]. A ﬁne example for the application of PFG-NMR are measurements of self-diﬀusion of liquid lithium and sodium [17]. Figure 15.2 displays selfdiﬀusivities in liquid and solid Li obtained by PFG-NMR according to Feinauer and Majer [18]. At the melting point, the diﬀusivity in liquid Li is almost three orders of magnitude faster than in the solid state. Also visible is the isotope eﬀect of Li diﬀusion. The diﬀusivity of 6 Li is slightly faster than that of 7 Li. 258 15 Nuclear Methods Fig. 15.2. Self-diﬀusion of 6 Li and 7 Li in liquid and solid Li studied by PFG-NMR according to Feinauer and Majer [18] 15.2.3 NMR Relaxation Methods Indirect NMR methods for diﬀusion studies measure either the relaxation times T1 and T2 , or the linewidth of the absorption line. In addition, other relaxation times not contained in the Bloch equation can be operationally deﬁned. The best known of these is the spin-lattice relaxation time in the rotating frame, T1ρ . This relaxation time characterises the decay of the magnetisation when it is ‘locked’ parallel to B1 in a frame of reference rotating around B0 with the Larmor frequency ω0 = γB0 . In such an experiment, M starts from M eq and decays to B1 M eq /B0 . Since T1ρ is shorter than T1 , measurements of T1ρ permit the detection of slower atomic motion than T1 . Let us consider a measurement of the spin-lattice relaxation time T1 . If a magnetic ﬁeld is applied in the z-direction, T1 describes the evolution of the magnetisation Mz towards equilibrium according to dMz M eq − Mz = z . dt T1 (15.11) A measurement of T1 proceeds in two steps. (i) At ﬁrst, the nuclear magnetisation is inverted by the application of an ‘inversion pulse’. (ii) Then, the magnetisation Mz (t) is observed by a ‘detection pulse’ as it relaxes back to the equilibrium magnetisation. The eﬀect of r.f. pulses can be discussed on the basis of the Bloch equation (15.7). If the resonance condition, ω0 = γB0 , is fulﬁlled for the alternating B 1 ﬁeld, the magnetisation will precess in the y-z plane with a precession 15.2 Nuclear Magnetic Relaxation (NMR) 259 Fig. 15.3. Schematic iluustration of a T1 measurement with an inversion-recovery (π-τ -π/2) pulse sequence frequency γB1 . The application of a pulse of the r.f. ﬁeld B1 with a duration tp will result in the precession of the magnetisation to the angle Θp = γB1 tp . By suitable choice of the pulse length the magnetisation can be inverted (Θp = π) or tilted into the x-y plane (Θp = π/2). During precession in the x-y plane the magnetisation will induce a voltage in the coil (Fig. 15.1). This signal is called the free induction decay (FID). If, for example, an initial π-pulse is applied, Mz (t) can be monitored by the amplitude of FID after a π/2-reading pulse at the evolution time t, which is varied in the experiment1 . This widely used pulse sequence for the measurement of T1 is illustrated in Fig. 15.3. NMR is sensitive to interactions of nuclear moments with ﬁelds produced by their local environment. The relaxation times and the linewidth are determined by the interaction between nuclear moments either directly or via electrons. Apart from coupling to the spins of conduction electrons in metals or of paramagnetic impurities in non-metals, two basic mechanisms of interaction must be considered in relation to atomic movements. The ﬁrst interaction is dipole-dipole coupling among the nuclear magnetic moments. The second interaction is due to nuclear electric quadrupole moments with internal electric ﬁeld gradients. Nonzero quadrupolar moments are present for nuclei with nuclear spins I > 1/2. The diﬀusion of nuclear moments causes variations in both of these interactions. Therefore, the width of the resonance line and the relaxation times have contributions which are due to the thermally activated jumps of atoms. 1 Without discussing further details, we mention that more complex pulse sequences have been tailored to overcome limitations of the simple sequence, which suﬀers from the dead-time of the detection system after the strong r.f. pulse. 260 15 Nuclear Methods Fig. 15.4. Temporal ﬂuctuations of the local ﬁeld – the origin of motional narrowing Spin-Spin Relaxation and Motional Narrowing: Let us suppose for the moment that we need to consider only magnetic dipole interactions, which is indeed the case for nuclei with I = 1/2. Each nuclear spin precesses, in fact, in a magnetic ﬁeld B = B 0 + B local , where B local is the local ﬁeld created by the magnetic moments of neighbouring nuclei. The local ﬁeld experienced by a particular nucleus is dominated by the dipole ﬁelds created by the nuclei in its immediate neighbourhood, because dipolar ﬁelds vary as 1/r3 with the distance r between the nuclei. Since the nuclear moments are randomly oriented, the local ﬁeld varies from one nucleus to another. This leads to a dispersion of the Larmor frequency and to a broadening of the resonance line according to 1 ∆ω0 = ∝ γ∆Blocal . (15.12) T2 ∆Blocal is an average of the local ﬁelds in the sample. In solids without internal motion, local ﬁelds are often quite large and give rise to rather short T2 values. Typical values without motion of the nuclei are the following: ∆Blocal ≈ 2×10−4 Tesla, T2 ≈ 100µs and ∆ω0 ≈ 104 rad s−1 . Such values are characteristic of a ‘rigid lattice’ regime. The pertaining spin-spin relaxation time is denoted as T2 (rigid lattice). Let us now consider how diﬀusion aﬀects the spin-spin relaxation time and the linewidth of the resonance line. Diﬀusion comes about by jumps of individual atoms from one site to another. The mean residence time of an atom, τ̄ , is temperature dependent via ∆H τ̄ = τ0 exp (15.13) kB T with an activation enthalpy ∆H and a pre-factor τ0 . Each time when an atom jumps into a new site, its nuclear moment will ﬁnd itself in another local ﬁeld. As a consequence, the local ﬁeld sensed by a nucleus will ﬂuctuate between ±Blocal on a time-scale characterised by the mean residence time (Fig. 15.4). If the mean residence time of an atom is much shorter than the spin-spin relaxation time of the rigid lattice, i.e. for τ̄ T2 (rigid lattice), 15.2 Nuclear Magnetic Relaxation (NMR) 261 Fig. 15.5. Schematic illustration of diﬀusional contributions (random jumps) to spin-lattice relaxation rates, 1/T1 and 1/T1ρ , and to the spin-spin relaxation rate 1/T2 a nuclear moment will sample many diﬀerent local ﬁelds. The nuclear moment will behave as though it were in some new eﬀective local ﬁeld, which is given by the average of all the local ﬁelds sampled. If the sampled local ﬁelds vary randomly in direction and magnitude this average will be quite small, depending on how many are sampled. The dephasing between the spins grows more slowly with time than in a ﬁxed local ﬁeld. The eﬀective local ﬁelds of all the nuclear moments will be small, and the nuclear moments will precess at nearly the same frequency. Thus, the nuclear moments will not lose their coherence as rapidly during a FID, and T2 will be longer. A longer FID is equivalent to a narrower resonance line. If the diﬀusion rate is increased, it can be shown by statistical considerations that the width of the resonance line becomes ∆ω = 1 = ∆ω02 τ̄ . T2 (15.14) This phenomenon is called motional narrowing. A schematic illustration of the temperature dependence the spin-spin relaxation rate 1/T2 is displayed in Fig. 15.5: at low temperatures the relaxation rate of the rigid lattice is observed, since diﬀusion is so slow that an atom does not even jump once during the FID; as τ̄ gets shorter with increasing temperature 1/T2 decreases and the width of the resonance line gets narrower. Spin-Lattice Relaxation: When discussing the Bloch equations we have seen that the spin-lattice relaxation time T1 is the characteristic time during 262 15 Nuclear Methods which the nuclear magnetisation returns to its equilibrium value. We could also say the nuclear spin system comes to equilibrium with its environment, called ‘lattice’. In contrast to spin-spin relaxation, this process requires an exchange of energy with the ‘lattice’. Spin-lattice relaxation either takes place by the absorption or emission of phonons or by coupling of the spins to conduction electrons (via hyperﬁne interaction) in metals. The relaxation rate due to the coupling of nuclear spins with conduction electrons is approximately given by the Koringa relation 1 = const × T, (15.15) T1 e where T denotes the absolute temperature. The relaxation rate due to dipolar interactions, (1/T1 )dip , and due to quadrupolar interactions, (1/T1 )Q , is added to that of electrons, so that the total spin-lattice relaxation rate is 1 1 1 1 = + + . (15.16) T1 T1 e T1 dip T1 Q For systems with nuclear spins I = 1/2, quadrupolar contributions are absent. The ﬂuctuating ﬁelds can be described by a correlation function G(t), which contains the temporal information about the atomic diﬀusion process [2, 3]. Let us assume as in the original paper by Bloembergen, Purcell and Pound [1] that the correlation function decays exponentially with the correlation time τc , i.e. as |t| G(t) = G(0) exp − . (15.17) τc This behaviour is characteristic of jump diﬀusion in a three dimensional system and τc is closely related to the mean residence time between successive jumps. The Fourier transform of Eq. (15.17), which is called the spectral density function J(ω), is a Lorentzian given by J(ω) = G(0) 2τc . 1 + ω 2 τc2 (15.18) Transitions between the energy levels of the spin-system can be induced, i.e. spin-lattice relaxation becomes eﬀective, when J(ω) has components at the transition frequency. The spin-lattice relaxation rate is then approximately given by 1 3 ≈ γ 4 2 I(I + 1)J(ω0 ) . (15.19) T1 dip 2 Detailed expressions for the relaxation rates e.g., in [2, 6]. 1 1 T1 , T2 and 1 T1ρ can be found, 15.2 Nuclear Magnetic Relaxation (NMR) 263 Fig. 15.6. Diﬀusion-induced spin-lattice relaxation rate, (1/T1 )dip , of 8 Li in solid Li as a function of temperature according to Heitjans et al. [8]. The B0 values correspond to Larmor frequencies ω0 /2π of 4.32 MHz, 2.14 MHz, 334 kHz, and 53 kHz The correlation time τc , like the mean residence time τ̄ , will usually obey an Arrhenius relation ∆H τc = τc0 exp , (15.20) kB T where ∆H is the activation enthalpy of the diﬀusion process. Since the movement of either atom of a pair will change the correlation function we may identify τc with one half of the mean residence time τ̄ of an atom at a lattice site. The diﬀusion-induced spin-lattice relaxation rate, (1/T1 )dip , is shown in Fig. 15.6 for self-diﬀusion of 8 Li in lithium according to Heitjans et al. [8]. In a representation of the logarithm of the relaxation rate as function of the reciprocal temperature, a symmetric peak is observed with a maximum at ω0 τc ≈ 1. At temperatures well above or below the maximum, which correspond to the cases ω0 τc 1 or ω0 τc 1, the slopes yield ∆H/kB or −∆H/kB . The work of Bloembergen, Purcell and Pound [1] is based on the assumption of the exponential correlation function of Eq. (15.17), which is appropriate for diﬀusion in liquids. Later on, the theory was extended to random walk diﬀusion in lattices by Torrey [19]. Based on the encounter model (see Chap. 7) the inﬂuence of defect mechanisms of diﬀusion and the associated correlation eﬀects have been included into the theory by Wolf [20] and MacGillivray and Sholl [21]. These reﬁnements lead to results that 264 15 Nuclear Methods Fig. 15.7. Comparison of self-diﬀusivities for 6 Li in solid Li determined by PFGNMR with spin-lattice relaxation results assuming a vacancy mechanism (solid line) and an interstitial mechanism (dashed line) according to Majer [22] are broadly similar to those of [1]. However, the reﬁnements are relevant for a quantitative interpretation of NMR results in terms of diﬀusion coeﬃcients. We illustrate this by an example: Figure 15.7 shows a comparison of diﬀusion data of 6 Li in solid lithium obtained with PFG-NMR and data deduced from relaxation measurements. PFG-NMR yields directly 6 Li self-diﬀusion coeﬃcients in solid lithium. No assumption about the elementary diﬀusion steps is needed for these data. The dashed and solid lines are deduced from (1/T1 )dip data, assuming two diﬀerent atomic mechanisms. Good coincidence of diﬀusivities from spinlattice relaxation and the PFG-NMR data is obtained with the assumption that Li diﬀusion is mediated by vacancies. Direct interstitial diﬀusion clearly can be excluded [22]. 15.3 Mössbauer Spectroscopy (MBS) The Mössbauer eﬀect has been detected by the 1961 Nobel laureate in physics R. Mössbauer [23]. The Mössbauer eﬀect is the recoil-free emission and absorption of γ-radiation by atomic nuclei. Among many other applications, Mössbauer spectroscopy can be used to deduce information about the movements of atoms for which suitable Mössbauer isotopes exist. There are only 15.3 Mössbauer Spectroscopy (MBS) 265 Fig. 15.8. Mössbauer spectroscopy. Top: moving source experiment; bottom: principles a few nuclei, 57 Fe, 119 Sn, 151 Eu, and 161 Dy, for which Mössbauer spectroscopy can be used. 57 Fe is the major ‘workhorse’ of this technique Information about atomic motion is obtained from the broadening of the otherwise very narrow γ-line. Thermally activated diﬀusion of Mössbauer atoms contributes to the linewidth in a way ﬁrst recognised by Singwi and Sjölander in 1960 [24] soon after the detection of the Mössbauer eﬀect. Mössbauer spectroscopy uses two samples, one playing the rôle of the source, the other one the rôle of an absorber of γ-radiation as indicated in Fig. 15.8. In the source the nuclei emit γ-rays, some of which are absorbed without atomic recoil in the absorber. The radioisotope 57 Co is frequently used in the source. It decays with a half-life time of 271 days into an excited state of the Mössbauer isotope 57 Fe. The Mössbauer level is an excited level of 57 Fe with lifetime τN = 98 ns. It decays by emission of γ-radiation of the energy Eγ = 14.4 keV to the ground state of 57 Fe, which is a stable isotope with a 2.2% natural abundance. If the Mössbauer isotope is incorporated in a crystal, the recoil energy of the decay is transferred to the whole crystal. Then, the width of the emitted γ-line becomes extremely narrow. This is the eﬀect for which Mössbauer received the Nobel price. The absorber also contains the Mössbauer isotope. A fraction f of the emitted γ-rays is absorbed without atomic recoil in the absorber. In the experiment, the source is usually moved relative to the absorber with a velocity v. Experimantal set-ups with static source and a moving absorber are also possible. This motion causes a Doppler shift v (15.21) ∆E = Eγ c of the source radiation, where c denotes the velocity of light. The linewidth in the absorber is then recorded as a function of the relative velocity or as a function of the Doppler shift ∆E. 266 15 Nuclear Methods Fig. 15.9. Simpliﬁed, semi-classical explanation of the diﬀusional line-broadening of a Mössbauer spectrum. Q denotes the wave vector of the γ-rays Diﬀusion in a solid, if fast enough, leads to a diﬀusional broadening of the Mössbauer spectrum. This can be understood in a simpliﬁed picture as illustrated in Fig. 15.9 [25]: at low temperatures, the Mössbauer nuclei stay on their lattice sites during the emission process. Without diﬀusion the natural linewidth Γ0 is observed, which is related to the lifetime of the excited Mössbauer level, τN , via the Heisenberg uncertainty relation: Γ0 τN ≥ . (15.22) At elevated temperatures, the atoms become mobile. A diﬀusing atom resides on one lattice site only for a time τ̄ between two successive jumps. If τ̄ is of the same order or smaller than τN , the Mössbauer atom changes its position during the emission process. When an atom is jumping the wave packet emitted by the atom is ‘cut’ into several shorter wave packets. This leads to a broadening of the linewidth Γ , in addition to its natural width Γo . If τ̄ τN , the broadening, ∆Γ = Γ − Γ0 , is of the order of ∆Γ ≈ /τ̄ . (15.23) Neglecting correlation eﬀects (see, however, below) and considering diﬀusion on a Bravais lattice with a jump length d the diﬀusion coeﬃcient is related to the diﬀusional broadening via D≈ d2 ∆Γ . 12 (15.24) Experimental examples for Mössbauer spectra of 57 Fe in iron are shown in Fig. 15.10 according to Vogl and Petry [27]. The Mössbauer source was 57 Co. The linewidth increases with increasing temperature due to the diﬀusional motion of Fe atoms. Figure 15.11 shows an Arrhenius diagram of self-diﬀusion for γ- and δ-iron, in which the Mössbauer data are compared with tracer results [27]. The jump length d in Eq. (15.24) was assumed to be the nearest neighbour distance of Fe. It can be seen that 15.3 Mössbauer Spectroscopy (MBS) 267 Fig. 15.10. Mössbauer spectra for self-diﬀusion in polycrystalline Fe from a review of Vogl and Petry [27]. FWHM denotes the full-width of half maximum of the Mössbauer line. The spectrum at 1623 K pertains to γ-iron and the spectra at higher temperatures to δ-iron the diﬀusivities determined from the Mössbauer study agree within error bars with diﬀusivities from tracer studies. Equation (15.24) is an approximation and follows from the more general Eq. (15.27). For this aim Eq. (15.27) is speciﬁed to polycrystalline samples and considered for Q 1/d. For 14.4 keV γ-radiation we have Q = 73 nm−1 , which is indeed much larger than 1/d. The broadening is more pronounced in the hightemperature δ-phase of iron with the bcc structure as compared to the fcc γ-phase of iron. This is in accordance with the fact that self-diﬀusion increases by about one order of magnitude, when γ-iron transforms to δ-iron (see Chap. 17). 268 15 Nuclear Methods Fig. 15.11. Self-diﬀusion in γ- and δ-iron: comparison of Mössbauer (symbols) and tracer results (solid lines) according to Vogl and Petry [27] Diﬀusional Broadening of MBS Signals: A quantitative analysis of diﬀusional line-broadening uses the fact that according to van Hove [28] the displacement of atoms in space and time can be described by the selfcorrelation function Gs (r, t). This is the probability density to ﬁnd an atom displaced by the vector r within a time interval t. We are interested in the selfcorrelation function because the Mössbauer absorption spectrum, σ(Q, ω), is related to the double Fourier transform of Gs in space and time via σ(Q, ω) ∝ Re Gs (r, t) exp [i(Q · r − ωt) − Γ0 | t | /2]drdt , (15.25) where Γ0 is the natural linewidth of the Mössbauer transition. The self-correlation function contains both diﬀusional motion as well as lattice vibrations. Usually, these two contributions can be separated. The vibrational part leads to the so-called Debye-Waller factor, fDW , which governs the intensity of the resonantly absorbed radiation. The diﬀusional part determines the shape of the Mössbauer spectrum. As the wave packets are emitted by the same nucleus, they are coherent. The interference between these packets depends on the orientation between the jump vector of the atom and the wave vector (see Fig. 15.9). If a single-crystal specimen is used, in certain crystal directions the linewidth is small and in other directions it is larger. To exploit Eq. (15.25) a diﬀusion model is necessary to calculate σ(Q, ω). For random jumps on a Bravais lattice (Markov process) the shape of the 15.4 Quasielastic Neutron Scattering (QENS) 269 resulting Mössbauer spectrum is a Lorentzian [25, 26] σ(Q, ω) ∝ fDW ∆Γ (Q)/2 , [∆Γ (Q)/2]2 + (ω)2 (15.26) where ∆Γ (Q) is the full peak-width at half maximum. This diﬀusional broadening depends on the relative orientation between radiation and crystal: ⎛ ⎞ Nj 1 2 ⎝ Wj Ej ⎠ where Ej = exp(iQ · rk ) . 1− ∆Γ (Q) = τ̄ Nj j k=1 (15.27) Wj is the probability for a displacement to coordination shell j, Ej the corresponding structure factor, Nj denotes the number of sites in the coordination shell j, and rk are the displacement vectors to sites in shell j. For diﬀusion mediated by vacancies, successive jumps of an atom are correlated. An extension of Eq. (15.27) for correlated diﬀusion has been developed by Wolf [20] on the basis of the so-called encounter model (see Chap. 7). The mean time between encounters is τenc = τ̄ Zenc , (15.28) where Zenc is the average number of jumps performed by a Mössbauer atom in one encounter. Each complete encounter is treated as an eﬀective displacement not correlated to the previous or following encounter. Wolf showed that the line broadening can be expressed as ⎛ ⎞ 2 ⎝ 1− (15.29) Wjenc Ej ⎠ , ∆Γ (Q) = τ̄ Zenc j where Wjenc is the probability for a displacement of r j by an encounter with a defect. For further details and for an extension to non-Bravais lattices the reader is referred to [25, 29]. An important consequence of Eq. (15.26) and of Eq. (15.29) is that both σ(Q, ω) and ∆Γ depend on the relative orientation between Q and the jump vector r and hence on the orientation of the crystal lattice. This can be exploited by measurements on monocrystals. By varying the crystal orientation, information about the length and direction of the jump vector is obtained. In that respect MBS and QENS are analogous. Examples for the deduction of elementary diﬀusion jumps will be given in the next section. 15.4 Quasielastic Neutron Scattering (QENS) The scattering of beams of slow neutrons obtained from nuclear reactors or other high-intensity neutron sources can be used to study structural and dynamic properties of condensed matter. Why neutron scattering is a tool with 270 15 Nuclear Methods Fig. 15.12. Comparison between the dispersion relations of electromagnetic waves (EM waves) and neutrons unique properties can be seen from Fig. 15.12, which shows a comparison of the dispersion relations of electromagnetic waves (EM waves) and neutrons. For EM waves the frequency ν and the wavelength λ are related via ν = c/λ, where c is the velocity of light. For (non-relativistic) neutrons of mass mn the dispersion relation is ν = h/(2mn λ2 ). Typical atomic vibration frequencies in a solid, νatomic , match with far infrared and microwave frequencies of EM waves. On the other hand, typical interatomic distances, ratomic , match with wavelengths of X-rays. Slow and thermal neutrons have the unique feature that their wavelengths and frequencies match atomic frequencies and interatomic distances simultaneously. Neutrons are uncharged probes and interact with nuclei. In contrast to photons, neutrons have only a weak interaction with matter. This means that neutron probes permit easy access to bulk properties. Since neutrons can penetrate suitable sample containers easily. One can also use sophisticated sample environments, such as wide temperature ranges and high magnetic ﬁelds. The scattering cross section for neutrons is determined by the sample nuclei. The distribution of scattering cross sections in the periodic table is somehow irregular. For example, protons have very high scattering cross sections and are mainly incoherent scatterers. For deuterons the coherent cross section is larger than the incoherent scattering cross section. Carbon, nitrogen, and oxygen have very small incoherent scattering cross sections and are mainly coherent scatterers. For sodium, coherent and incoherent scattering cross sections are similar in magnitude. 15.4 Quasielastic Neutron Scattering (QENS) 271 Fig. 15.13. Neutron scattering geometry: in real space (left); in momentum space (right) Neutron scattering leads to a spectrum of energy and momentum transfers (Fig. 15.13). The energy transfer is ω = E1 − E0 , (15.30) where E1 and E0 denote the neutron energies after and before the scattering process, respectively. The corresponding momentum transfer is Q. The scattering vector is (15.31) Q = k 1 − k0 , where k0 and k1 are the neutron wave vectors before and after the scattering event. The corresponding neutron wavelenghts are λ1 = 2π/k1 and λ0 = 2π/k0 . The values of 4π Q= sin(Θ/2) (15.32) λ0 (Θ = scattering angle Q = modulus of the scattering vector) vary typically between 1 and 50 nm−1 . Therefore, 1/Q can match interatomic distances. The scattered intensity in such an experiment is proportional to the so-called scattering function or dynamic structure factor, S(Q, ω), which can be calculated for diﬀusion processes (see below). A schematic energy spectrum for neutron scattering with elastic, quasielastic, and inelastic contributions is illustrated in Fig. 15.14. Inelastic peaks are observed, due to the absorption and emission of phonons. Quasielastic Scattering: Quasielastic scattering must be distinguished from the study of periodic modes such as phonons or magnons by inelastic scattering, which usually occurs at higher energy transfers. For samples with suitable scattering cross sections, diﬀusion of atoms in solids can be studied by quasielastic neutron scattering (QENS), if a highresolution neutron spectrometer is used. QENS, like MBS, is a technique which has considerable potential for elucidating diﬀusion steps on a microscopic level. Both techniques are applicable to relatively fast diﬀusion processes only (see Fig. 13.1). QENS explores the diﬀusive motion in space for a range comparable to the neutron wavelength. Typical jump distances and 272 15 Nuclear Methods Fig. 15.14. Energy spectrum of neutron scattering (schematic) diﬀusion paths between 10−8 and 10−10 m can be studied. Let us brieﬂy anticipate major virtues of QENS. The full peak-width at half maximum of a Lorentzian shaped quasielastic line is given for small values of Q by ∆Γ = 2DQ2 , (15.33) where D is the self-diﬀusion coeﬃcient [31, 32]. Quasielastic line broadening is due to the diﬀusive motion of atoms. The pertinent energy transfers ω typically range from 10−3 to 10−7 eV. For larger scattering vectors, ∆Γ is periodic in reciprocal space and hence depends on the atomic jump vector like in MBS. For a particle at rest, we have ∆Γ = 0 and a sharp line at ω = 0 is observed. This elastic line (Bragg peak) results from a scattering process in which the neutron transmits the momentum Q to the sample as a whole, without energy transfer. For resonance absorption of γ−rays this corresponds to the well-known Mössbauer line (see above). We have already seen that in MBS a diﬀusing particle produces a line broadening. QENS is described by similar theoretical concepts as used in MBS [25, 30–32]. Figure 15.15 shows an example of a quasielastic neutron spectrum measured on a monocrystal of sodium according to Göltz et al. [33]. The number of scattered neutrons N is plotted as a function of the energy transfer ω for a ﬁxed scattering vector with Q = 1.3×10−10 m−1 . The dashed line represents the resolution function of the neutron spectrometer. The observed line is broadened due to the diﬀusive motion of Na atoms. The quasielastic linewidth depends on the orientation of the momentum transfer and hence of the crystallographic orientation of the crystal (see below). The Dynamic Structure Factor (Scattering Functions): Let us now recall some theoretical aspects of QENS. The quantity measured in neutron scattering experiments is the intensity of neutrons, ∆Is , scattered from a collimated mono-energetic neutron beam with a current density I0 . The intensity 15.4 Quasielastic Neutron Scattering (QENS) 273 Fig. 15.15. QENS spectrum of a Na monocrystal at 367.5 K according to Göltz et al. [33]. Dashed line: resolution functionof the neutron spectrometer of neutrons scattered into a solid angle element, ∆Ω, and an interval, ∆ω, from a sample with volume V and number density of scattering atoms, N , (see Fig. 15.13) is given by [31] 2 d σ ∆Is = I0 N V ∆Ω∆ω , (15.34) dΩdω where the double diﬀerential scattering cross section is k1 σ d2 σ = S(Q, ω) . dΩdω k0 4π (15.35) The cross section is factorised into three components: the ratio of the wave numbers k1 /k0 ; the cross section for a rigidly bound nucleus, σ = 4πb2 , where b is the corresponding scattering length of the nucleus; the scattering intensity is proportional to the dynamical structure factor S(Q, ω). The dynamical structure factor depends on the scattering vector and on the energy transfer deﬁned in Eqs. (15.30) and (15.31). It describes structural and dynamical properties of the sample which do not depend on the interaction between neutron and nuclei. The interaction of a neutron with a scattering nucleus depends on the chemical species, the isotope, and its nuclear spin. In a mono-isotopic sample, all nuclei have the same scattering length. Then, only coherent scattering will be observed. In general, however, several isotopes are present according to their natural abundance. Each isotope i is characterised by its scattering length bi . The presence of diﬀerent isotopes distributed randomly in the sample means that the total scattering cross section is made up of two parts, called coherent and incoherent. 274 15 Nuclear Methods The theory of neutron scattering is well developed and can be found, e.g., in reviews by Zabel [30], Springer [31, 32] and in textbooks of Squires [37], Lovesey [38], Bee [36], and Hempelmann [39]. Theory shows that the diﬀerential scattering cross section can be written as the sum of a coherent and an incoherent part 2 2 d σ d σ d2 σ + = dΩdω dΩdω coh dΩdω inc % k1 $ σcoh σinc Scoh (Q, ω) + Sinc (Q, ω) . = (15.36) k0 4π 4π Coherent (index: coh) and incoherent (index: inc) contributions depend on the composition and the scattering cross sections of the nuclei in the sample. The coherent scattering cross section σcoh is due to the average scattering from diﬀerent isotopes σcoh = 4π b̄2 with b̄ = Σci bi . (15.37) The incoherent scattering is proportional to the deviations of the individual scattering lengths from the mean value # " with b¯2 = Σci b2i . (15.38) σinc = 4π b¯2 − b̄2 The bars indicate ensemble averages over the various isotopes present and their possible spin states. The ci are the fractions of nuclei i. Coherent scattering is due to interference of partial neutron waves originating at the positions of diﬀerent nuclei. The coherent scattering function, Scoh (Q, ω), is proportional to the Fourier transform of the correlation function of any nuclei. Coherent scattering leads to interference eﬀects and collective properties can be studied. Among other things, this term gives rise to Bragg diﬀraction peaks. Incoherent scattering monitors the fate of individual nuclei and interference eﬀects are absent. The incoherent scattering function, Sinc (Q, ω), is proportional to the Fourier transform of the correlation function of individual nuclei. Only a mono-isotopic ensemble of atoms with spin I = 0 would scatter neutrons in a totally coherent manner. Incoherent scattering is connected to isotopic disorder and to nuclear spin disorder. We emphasise that it is the theory of neutron scattering that leads to the separation into coherent and incoherent terms. The direct experimental determination of two separate functions, Scoh (Q, ω) and Sinc (Q, ω), is usually not straightforward, unless samples with diﬀerent isotopic composition are available. However, sometimes the two contributions can be separated without the luxury of major changes in the isotopic composition. The coherent and incoherent length bi of nuclei are known and can be found in tables [40]. For example, the incoherent cross section of hydrogen is 40 times larger than the coherent cross section. Then, coherent scattering can be disregarded. 15.4 Quasielastic Neutron Scattering (QENS) 275 Incoherent Scattering and Diﬀusional Broadening of QENS Signals: Incoherent quasielastic neutron scattering is particularly useful for diﬀusion studies. The incoherent scattering function can be calculated for a given diﬀusion mechanism. Let us ﬁrst consider the inﬂuence of diﬀusion on the scattered neutron wave in a simpliﬁed, semi-classical way: in an ensemble of incoherent scatterers, only the waves scattered by the same nucleus can interfere. At low temperatures the atoms stay on their sites during the scattering process; this contributes to the elastic peak. The width of the elastic peak is then determined by the energy resolution of the neutron spectrometer. At high temperatures the atoms are in motion. Then the wave packets emitted by diﬀusing atoms are ‘cut’ to several shorter ‘packets’, which leads to diﬀusional broadening of the elastic line. This is denoted as incoherent quasielastic scattering. Like in MBS the interference between wave packets emitted by the same nucleus depends on the relative orientation between the jump vector of the atom and the scattering direction. Therefore, in certain crystal direction the linewidth will be small while in other directions it will be large. For a quantitative description of the incoherent scattering function the van Hove self-correlation function Gs (r, t) is used as a measure of diﬀusive motion. The incoherent scattering function is proportional to the Fourier transform of the self-correlation function Sinc (Q, ω) = 1 2π Gs (r, t) exp [i(Qr − ωt)]drdt . (15.39) When atomic motion can simply be described by continuous translational diﬀusion in three dimensions, the self-correlation function Gs (r, t) takes the form of a Gaussian (see Chap. 3) 1 r2 exp − Gs (r, t) = , (15.40) 4Dt (4πDt)3/2 with D denoting the self-diﬀusion coeﬃcient of atoms. Its Fourier transform in space # " (15.41) S(Q, t) = exp −Q2 Dt is an exponential function of time, the time Fourier transform of which is a Lorentzian: DQ2 1 Sinc (Q, ω) = . (15.42) π (DQ2 )2 + ω 2 This equation shows that for small Q values the linewidth of the quasielastic line is indeed given by Eq. (15.33). It is thus possible to determine the diffusion coeﬃcient from a measurement of the linewidth as a function of small scattering vectors. In the derivation of Eq. (15.42) the continuum theory of diﬀusion was used for the self-correlation function. This assumption is only valid for small scattering vectors |Q| << 1/d, where d is the length of the jump vectors in the 276 15 Nuclear Methods Fig. 15.16. Top: Self-correlation function Gs for a one-dimensional lattice. Top: The height of the solid lines represents the probability of occupancy per site. Asymptotically, the envelope approaches a Gaussian. Bottom: Incoherent contribution Sinc (Q, ω) to the dynamical structure factor and quasi-elastic linewidth ∆Γ versus scattering vector Q. According to [32] lattice. For jump diﬀusion of atoms on a Bravais lattice the self-correlation function Gs can be obtained according to Chudley and Elliot [41]. The probability P (r n , t) to ﬁnd a diﬀusing atom on a site r n at time t is calculated using the master equation for P (rn , t): Z 1 1 ∂P (rn , t) = − P (rn , t) + P (r n + li , t) . ∂t τ̄ Z τ̄ i=1 (15.43) li (i =1, 2, . . . Z) is a set of jump vectors connecting a certain site with its Z neighbours. τ̄ denotes the mean residence time. The two terms in Eq. (15.43) correspond to loss and gain rates due to jumps to and from adjacent sites respectively. With the initial condition P (r n , 0) = δ(r n ), the probability P (r, t) becomes equivalent to the self-correlation function Gs (r n , t). A detailed theory of the master equation can be found in [42, 43]. If P (r n , t) is known the incoherent scattering function is obtained by Fourier transformation in space and time according to Eq. (15.39). For a one-dimensional lattice Gs is illustrated in Fig. 15.16. The classical model for random jump diﬀusion on Bravais lattices via nearest-neighbour jumps was derived by Chudley and Elliot in 1961 [35] (see also [36]). The incoherent scattering function for random jump motion on a Bravais lattice is given by 15.4 Quasielastic Neutron Scattering (QENS) Sinc (Q, ω) = ∆Γ (Q) 2 . π ∆Γ (Q)2 + ω 2 277 (15.44) The function ∆Γ (Q) is determined by the lattice structure, the jumps which are possible, and the jump rate with which they occur. For the scattering of neutrons in a particular direction Q, the variation with change in energy ω is Lorentzian in shape with a linewidth given by ∆Γ . In the case of polycrystalline samples, the scattering depends on the modulus Q = |Q| only, but still consists of a single Lorentian line with linewidth 2 sin(Qd) ∆Γ = 1− . (15.45) τ̄ Qd Here τ̄ is the mean residence time for an atom on a lattice site and d the length of the jump vector. For a monocrystal with a simple cubic Bravais lattice one gets for the orientation dependent linewidth ∆Γ (Q) = 2 [3 − cos(Qx d) − cos(Qy d) − cos(Qz d)] , 3τ̄ (15.46) where Qx , Qy , Qz are the components of Q and d is the length of the jump vector. The linewidth is a periodic function in reciprocal space. It has a maximum at the boundary of the Brillouin zone and it is zero if a reciprocal lattice point G is reached. This line narrowing is a remarkable consequence of quantum mechanics. For vacancy-mediated diﬀusion successive jumps of atoms are correlated. Like in the case of MBS, the so-called encounter model can be used for low vacancy concentrations (see Chap. 7). A vacancy can initiate several correlated jumps of the same atom, such that one encounter comprises Zenc atomic jumps. As we have seen in Chap. 7, the time intervals between subsequent atomic jumps within the same encounter are very short as compared to the time between encounters. As a consequence, the quasielastic spectrum can be calculated within the framework of the Chudley and Elliot model, where the rapid jumps within the encounters are treated as instantaneous. The linewidth of the quasielastic spectrum is described by [33] 2 Wenc (r m ) cos(Qrm ) , (15.47) 1− ∆Γ = τ̄ Zenc r m where Wenc (r m ) denotes the probability that, during an encounter, an atom originally at r m = 0 has been displaced to lattice site rm by one or several jumps. The probabilities can be obtained, e.g., by computer simulations. A detailed treatment based on the encounter model can be found in a paper by Wolf [46]. Equation (15.47) is equivalent to Eq. (15.29) already discussed in the section about Mössbauer spectroscopy. 278 15 Nuclear Methods Fig. 15.17. Quasielastic linewidth as a function of the modulus Q = |Q| for polycrystalline Na2 PO4 according to Wilmer and Combet [47]. Solid lines: ﬁts of the Chudley-Elliot model 15.4.1 Examples of QENS studies Let us now consider examples of QENS studies, which illustrate the potential of the technique for polycrystalline material and for monocrystals. Na self-diﬀusion in ion-conducting rotor phases: Sodium diﬀusion in solid solutions of sodium orthophosphate and sodium sulfate, xNa2 SO4 (1-x)Na3 PO4 , has been studied by Wilmer and Combet [47]. These materials belong to a group of high-temperature modiﬁcations with both fast cation conductivity and anion rotational disorder and are thus termed as fast ion-conducting rotor phases. The quasielastic linewidth of polycrystalline samples has been measured as a function of the momentum transfer. In the case of polycrystalline samples, the scattering depends on the modulus of Q = |Q| only, but still consist of a single Lorentzian line with linewidth Eq. (15.45). The Q-dependent linebroadening is shown for Na2 PO4 at various temperatures in Fig. 15.17. The linewidth parameters τ̄ and d have been deduced. Obviously, the jump rates τ̄ −1 incresase with increasing temperature. Much more interesting is that the jump distance could be determined. It turned out that sodium diﬀusion is dominated by jumps between neighbouring tetrahedrally coordinated sites on an fcc lattice, the jump distance being half of the lattice constant. At very low values of Q, quasielastic broadening does no longer depend on details of the jump geometry since the linewidth is dominated by the long-range diﬀusion via Eq. (15.33). The linebroadening at the two lowest accessible Q values (1.9 and 2.9 nm−1 ) was used to determine the sodium self-diﬀusivites [47]. An Arrhenius plot of the sodium diﬀusivities is shown in 15.4 Quasielastic Neutron Scattering (QENS) 279 Fig. 15.18. Self-diﬀusion of Na in three xNa2 SO4 (1-x)Na3 PO4 rotor phases according to Wilmer and Combet [47] Fig. 15.18. The activation enthalpies decrease from 0.64 eV for pure Na3 PO4 to 0.3 eV for a sulphate content of 50%: Na self-diﬀusion in Na single-crystals: Quasielastic scattering of sodium single crystals has been investigated by Göltz et al. [33] and Ait-Salem et al. [34] and analysed in terms of Eq. (15.47). It was demonstrated that self-diﬀusion of sodium occurs by nearest-neighbour jumps in the bcc lattice. Figure 15.19 shows the linebroadening as a function of the momentrum transfer Q in directions parallel to 111 , 110 , and 100 at 362.2 K. Model calculations are also shown, assuming a monovacancy mechnaism with nearest-neighbour jumps on with a 111 jumps. The results show that diffusion proceeds via nearest-neighbour jumps. H diﬀusion in palladium: QENS measurements have been widely used to study diﬀusion of H-atoms in interstitial solutions of hydrogen in palladium. Interstitial diﬀusion is uncorrelated (see Chap. 7). It was shown, for example, that H-atoms jump between nearest-neighbour octahedral sites of the interstitial lattice of fcc Pd [44, 45]. 15.4.2 Advantages and Limitations of MBS and QENS For MBS diﬀusion studies it is necessary to heat the sample to suﬃciently high temperatures that the mean residence time of an atom on a lattice site, τ̄ , is comparable to or less than the half-life of the Mössbauer level τN . For metals, this implies temperatures not much below the melting temperature. Mössbauer spectroscopy is sensitive to the elementary steps of diﬀusion on a microscopic scale. A direct determination of jump vectors and jump rates 280 15 Nuclear Methods Fig. 15.19. Self-diﬀusion of Na metal. Dependence of the QENS line broadening in three major crystallographic directions. Theoretical curves have been calculated for a monovacancy mechanism assuming nearest-neighbour junps (solid lines) and a111 jumps (dotted line). From Vogl and Petry [27] according to [33, 34] is possible, when single-crystal samples are used and the line-broadening is measured as a function of crystal orientation. In addition, one can deduce the diﬀusion coeﬃcient and compare it with data obtained, e.g., by tracer diﬀusion studies. However, this is not the main virtue of a microscopic method. The nuclei studied in MBS must have a large value of the recoilless fraction, which limits the number of good isotopes to a few species. As already mentioned the major ‘workhorse’ of Mössbauer spectroscopy is 57 Fe. The isotopes 119 Sn, 151 Eu, and 161 Dy are less favourable but still useful isotopes for diﬀusion studies. Mössbauer diﬀusion studies in practice require a diﬀusional line-broadening that is comparable or larger than the natural linewidth of the Mössbauer transition. Only relatively large diﬀusion coeﬃcients can be measured. For example, 57 Fe diﬀusion coeﬃcients in the range 10−14 to 10−10 m2 s−1 are accessible. For diﬀusion studies by quasielastic neutron scattering (QENS) it is necessary to keep the sample at temperatures where the mean residence time of atoms on a lattice site, τ̄ , is short enough to produce a diﬀusional broadening, which exceeds the energy resolution of the neutron spectrometer. For timeof-ﬂight spectrometry the resolution is in the range of µeV to 0.1 meV. This allows a range of diﬀusion coeﬃcients between about 10−12 and 10−8 m2 s−1 to be covered. Diﬀusion coeﬃcients can be determined directly from the Q2 dependence of the linewidth. QENS has mainly been used to study hydrogen and sodium diﬀusion in solids. A prerequisite of QENS is that the element of interest has a large enough incoherent scattering cross section as compared to the coherent scattering cross section. Only few elements such as hydrogen, sodium, and vanadium fulﬁll this condition. In these cases QENS is unique, since there are no Mössbauer isotopes for these elements. Otherwise, in luxury experiments dif- References 281 ferent mixtures of isotopes can be used to separate coherent and incoherent contributions to scattering. The major merits of QENS and MBS are that both permit the investigation of the elementary steps of diﬀusion in solids on a scale of atomic dimensions and times. Both techniques are applicable to fast diﬀusion processes (see Fig. 13.1). References 1. N. Bloembergen, E.M. Purcell, R.V. Pound, Phys. Rev. 73, 679 (1948) 2. A. Abragam, The Priciples of Nuclear Magnetism, University Press, Oxford, 1973 3. C.P. Slichter, Principles of Magnetic Resonance, Springer-Verlag, Berlin, 1989 4. M. Mehring, High Resolution NMR Spectroscopy in Solids, Springer-Verlag, Berlin, 1983 5. H.T. Stokes, Study of Diﬀusion in Solids by Pulsed Nuclear Magnetic Resonance, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984. p. 39 6. A.R. Allnatt, A.B. Lidiard, Atomic Transport in Solids, Cambridge University Press, 1993 7. G. Majer, Die Methoden der Kernspinresonanz zum Studium der Diﬀusion von Wasserstoﬀ in Metallen und intermetallischen Verbindungen, Cuvillier Verlag, Göttingen, 2000 8. P. Heitjans, A. Schirmer, S. Indris, NMR and β-NMR Studies of Diﬀusion in Interface-Dominated and Disordered Solids, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), SpringerVerlag, 2005 9. P. Heitjans, S. Indris, M. Wilkening, Solid-State Diﬀusion and NMR, in Diﬀusion Fundamentals – Leipzig 2005, J. Kärger, F. Grinberg, P. Heitjans (Eds.), Leipziger Universitätsverlag, 2005 10. B.C. Gerstein, C.R. Dybowski, Transient Techniques in NMR of Solids, Academic Press, New York, 1985 11. H.C. Torrey, Phys. Rev. 104, 563 (1956) 12. E.L. Hahn, Phys. Rev. 80, 580 (1950) 13. E.O. Stejskal, J.E. Tanner, J. Chem. Phys. 42 288 (1965) 14. D.W. McCall, D.C. Douglas, E.W. Anderson, Ber. Bunsenges. 67, 336 (1963) 15. P. Stilbs, in: Progress in NMR Spectroscopy, J.W. Emsley, J. Feeney, L.H. Sutcliﬀe (Eds.), Pergamon Press, Oxford, 19, 1988 16. J. Kärger, G. Fleischer, U. Roland, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Vieweg-Verlag, 1998, p. 144 17. A. Feinauer, G. Majer, A. Seeger, Defect and Diﬀusion Forum 143–147, 881 (1997) 18. A. Feinauer, G. Majer, Phys. Rev. B 64,134302 (2001) 19. H.C. Torrey, Phys. Rev. 96, 690 (1954) 20. D. Wolf, Spin Temperature and Nuclear Spin Relaxation in Matter, Clarendon Press, Oxford, 1979 21. I.R. MacGillivray, C.A. Sholl, J. Phys. C 19, 4771 (1986); C.A. Sholl, J. Phys. C 21, 319 (1988) 282 15 Nuclear Methods 22. G. Majer, presented at: International Max Planck Research School for Advanced Materials, April 2006 23. R.L. Mössbauer, Z. Physik 151, 124 (1958) 24. K.S. Singwi, A. Sjölander, Phys. Rev. 120 1093 (1960) 25. G. Vogl, R. Feldwisch, The Elementary Diﬀusion Step in Metals Studied by Methods from Nuclear Solid-State Physics, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Vieweg-Verlag, 1998, p. 40 26. G. Vogl, B. Sepiol, The Elementary Diﬀusion Step in Metals Studied by the Interference of γ-Rays, X-Rays and Neutrons, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 27. G. Vogl, W. Petry, Diﬀusion in Metals studied by Mössbauer Spectroscopy and Quasielastic Neutron Scattering, in: Festkörperprobleme XXV (Advances in Solid State Physics), P. Grosse (Ed.), Braunschweig, F. Vieweg und Sohn, 1985, P. 655 28. L. van Hove, Phys. Rev. 95, 249 (1954) 29. J.G. Mullen, Mössbauier Diﬀusion Studies, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p.59 30. H. Zabel, Quasi-Elastic Neutron Scattering: a Powerful Tool for Investigating Diﬀusion in Solids, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984. p. 1 31. T. Springer, Diﬀusion Studies of Solids by Quasielastic Neutron Scattering, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Vieweg-Verlag, 1998., p. 59 32. T. Springer, R.E. Lechner, Diﬀusion Studies of Solids by Quasielastic Neutron Scattering, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 33. G. Göltz, A. Heidemann, H. Mehrer, A. Seeger, D. Wolf, Philos. Mag. A 41, 723 (1980) 34. M. Ait-Salem, T. Springer, A. Heidemann, B. Alefeld, Philos. Mag. A 39, 797 (1979) 35. C.T. Chudley, R.J. Elliiot. Proc. Phys. Soc. 77, 353 (1961) 36. M. Bee, Quasielastic Scattering, Adam Hilger, Bristol, 1988 37. G.L. Squires, Introduction to the Theory of Thermal Neutron Scattering, Cambridge University Press, 1978 38. S.W. Lovesey, Theory of Neutron Scattering from Condensed Matter, Clarendon Press, Oxford, 1986 39. R. Hempelmann, Quasielastic Neutron Scattering and Solid-State Diﬀusion, Oxford Science Publication, 2000 40. L. Koester, H. Rauch, E. Seyman, Atomic Data and Nuclear Data Tables 49, 65 (1991) 41. C.T. Chudley, R.J. Elliot, Proc. Phys. Soc. 77, 353 (1961) (see [35]) 42. K.W. Kehr, K. Mussawisade, Th. Wichmann, Diﬀusion of Particles on Lattices, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Vieweg-Verlag, 1998, p. 265 43. K.W. Kehr, K. Mussawisade, G. M. Schütz, G. Th. Wichmann, Diﬀusion of Particles on Lattices, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 References 283 44. K. Sköld, G. Nelin, J. Phys. Chem. Solids 28, 2369 (1967) 45. J.M. Rowe, J.J. Rush, L.A. de Graaf, G.A. Ferguson, Phys. Rev. Lett 29, 1250 (1972) 46. D. Wolf, Appl. Phys. Letters 30, 617 (1977) 47. D. Wilmer, J. Combet, Chemical Physics 292, 143 (2003) 16 Electrical Methods Measurements of electrical properties of materials are of interest for diﬀusion experiments in several areas of materials science. Impedance spectroscopy plays an important rôle for ion-conducting materials. With the availability of commercially made impedance bridges covering wide frequency ranges impedance studies became popular among electrochemists and materials scientists. For an introduction to the ﬁeld of impedance spectroscopy the reader may consult the textbook of Macdonald [1]. In semiconducting materials electrically active foreign atoms have a strong inﬂuence on the electrical conductivity. For diﬀusion studies in semiconductors electrical measurements are useful. In particular spreading resistance proﬁling, introduced by Mazur and Dickey in the 1960s [2], has become a powerful tool for measuring spatial distributions of electrically active atoms in semiconductors. Electrical resistivity measurements on metals have sometimes also been used to study diﬀusion. These studies utilise the resistivity change that occurs upon in- or out-diﬀusion of foreign elements. This method is fairl¡y indirect and diﬀusion proﬁles cannot be obtained. Therfore, we refrain from discussing such experiments. 16.1 Impedance Spectroscopy In ion-conducting materials with negligible electronic conduction such as ionic crystals, ion-conducting glasses, and oxides the conductivity results from the hopping motion of ions. For such materials the measurement of the electrical conductivity is an indispensable complement to that of tracer diﬀusion. As discussed in Chap. 11, the dc conductivity, σdc , is related to the charge or diﬀusivity, Dσ , via σdc kB T Dσ = . (16.1) Nion q 2 Nion denotes the number density of mobile ions and q the electrical charge per ion. Measurements of the ionic conductivity are carried out with an ac bridge to avoid polarisation eﬀects at the electrodes. An experimental set-up is illustrated in Fig. 16.1. The measurements are usually made with cells which have 286 16 Electrical Methods Fig. 16.1. Schematic illustration of an impedance bridge with sample and electrodes two identical electrodes applied to the faces of a sample in the form of a circular cylinder or rectangular parallelepiped. The general approach is to apply an electrical ac stimulus of frequency ν (a known voltage or current) and to observe the resulting response (current or voltage). Usually, impedance spectroscopy can cover a frequency range from about 10−3 Hz to several MHz. The experimental set-up requires a variable frequency generator and a vector ammeter and volt-meter for current and voltage measurements including the ˆ phase-shift between current I(ν) and voltage V̂ (ν). The complex impedance is deﬁned as V̂ (ν) . (16.2) Ẑ(ν) ≡ ˆ I(ν) It is composed according to Ẑ(ν) = Z − iZ (16.3) of real and imaginary parts, Z and Z . i denotes the imaginary unit. The complex conductivity σ̂(ν) = σ (ν) + iσ (ν) (16.4) is also composed of a real part, σ , and an imaginary part, σ . Conductivity and complex impedance are related via σ̂(ν) = d0 , Ẑ(ν) A 1 (16.5) where d0 and A denote the thickness and the electrode area of the sample, respectively. 16.1 Impedance Spectroscopy 287 For a discussion of impedance measurements, it is convenient to recall that the complex impedance of a circuit formed by an ohmic resistance R and a capacitance C parallel to it is given by Ẑ = R , 1 + iωCR (16.6) where ω = 2πν denotes the angular frequency. Then, the real and imaginary parts of the impedance can be written as Z = R 1 + ω 2 R2 C 2 and Z = ωCR2 . 1 + ω 2 R2 C 2 (16.7) The representation of the impedance in the complex Z − Z plane is denoted as the Cole diagram. For a RC-circuit the values of Ẑ(ω) plotted in the Z versus −Z plane fall on a semicircle of diameter R, passing through the origin for ω → ∞, through (R, 0) for ω = 0, and through (R/2, R/2) for ω = (RC)−1 . When several circuits of this type are connected in series, the graphic representation is a series of semicircles as illustrated in Fig. 16.2. An ensemble of three RC circuits in series can represent a measurement cell. The cell may consist of a polycrstalline sample plus electrodes. Each circuit represents a conductivity process: RV and CV volume conduction, Rb and Cb boundary conduction, and Re and Ce the electrode process. One should, however, keep in mind that the representation of the total impedance of an experimental set-up by RC-circuits can be oversimpliﬁed. Sometimes other equivalent circuits may better represent the actual processes. Furthermore, sometimes the centers of the arcs are below the Z -axis. As a simple experimental example, Fig. 16.3 shows the Cole diagram for an ion-conducting alkali-borate glass according to Imre et al. [3]. The semicircles represent the volume conduction process at various temperatures. Grain boundaries are absent in a glass and the electrode process is located at lower frequencies not displayed in the ﬁgure. The dc resistance of the sample is given by the intercept of the arcs with the Z -axis. It decreases with increasing temperature. The dc conductivity can be deduced from the ohmic resistance observed at the intersection of the ‘semicircle’ with the Z axis of Fig. 16.3. The real part of the conductivity times temperature (σ ×T ) of the same material is shown in Fig. 16.4 as a function of the frequency ν for various temperatures. The low frequency plateau in Fig. 16.4 corresponds to the dc conductivity. This plateau reﬂects the long-range transport of ions. The dc-conductivity increases with temperature Arrhenius activated. Using relation Eq. (16.1), the charge diﬀusivity, Dσ , can be deduced (see Chap. 11). This quantity is displayed in the Arrhenius diagram of Fig 16.5 together with the tracer diﬀusivity of 22 Na measured on the same material according to [4]. As discussed in Chap. 11 the ratio between tracer diﬀusivity D∗ and the conductivity diﬀusivity is denoted as the Haven ratio, HR ≡ 288 16 Electrical Methods Fig. 16.2. Circuits for the complex impedance and Cole diagram Fig. 16.3. Complex impedance (Cole diagram) for three temperatures representing volume conduction of a sodium-borate glass [3] D∗ /Dσ , which is usually less than unity. A measurement of the Haven ratio can provide useful information about the atomic mechanism of diﬀusion and the correlation eﬀects involved. In the illustrated case, the Haven ratio is temperature-independent indicating that the mechanism of ionic motion does not change with temperature. The increase of the conductivity at higher frequencies is called dispersion. The conductivity dispersion reﬂects the fact that ionic jumps are correlated (see, e.g., [5]). An onset frequency of dispersion, νonset , may be deﬁned by the condition σ (ν) = 2σdc . The fact that the onset frequencies in Fig. 16.4 lie on a straight line with a slope of unity shows that σdc × T and νonset are thermally activated with the same activation enthalpy. This behaviour is sometimes denoted as Summerﬁeld scaling [6]. Microscopically, it implies 16.1 Impedance Spectroscopy 289 Fig. 16.4. Conductivity spectra of a sodium borate glass in a diagram of logarithm σ × T versus logarithm of the frequency ν. The onset frequencies of dispersion for various temperatures are connected by a straight line Fig. 16.5. Arrhenius diagram of the charge diﬀusivity Dσ and the tracer diﬀusivity D∗ of 22 N a for a sodium borate glass that the same jump processes occur at diﬀerent temperatures. Of course, their jump rate is higher at higher temperatures. Summerﬁeld scaling is observed for several materials but by no means in all ion conducting materials. For more information about conduction in disordered ionic materials the reader may consult Chap. 30 and reviews, e.g., by Ingram [7], Dieterich and Maas [8], Funke and coworkers [9], and by Bunde et al. [10]. 290 16 Electrical Methods 16.2 Spreading Resistance Proﬁling In semiconductors, the resistivity in the extrinsic domain is related to the concentration of electrically active foreign atoms. The concentration distribution of such atoms can be deduced by measuring the spreading resistance Rs (see below). Spreading resistance proﬁling (SRP) [2] has become a useful tool for measuring spatial distributions of electrically active atoms in semiconducting samples. SRP is widely used in silicon technology to monitor depth proﬁles of dopants after processing steps and to check the lateral uniformity in the resistivity of virgin Si wafers. In addition, SRP has been successfully applied in basic studies of diﬀusion processes in Si (see, e.g., [11, 12]), in Ge [13] and to a lesser extent in GaAs [14]. SRP is a two-point-probe technique, which measures the electrical resistance on semiconductor surfaces with a much higher spatial resolution than the traditional four-point-probe technique. The concentration-depth proﬁle for foreign atoms can be established by measuring the resistance of the sample between two ‘points’ as indicated in Fig. 16.6. The probe tips, usually made of a tungsten-osmium alloy, are separated by a distance of typically 100 µm or less. The current between the probes spreads over a small space region near the semiconductor surface, which explains the notion ‘spreading resistance’. A SRP device is commonly operated in an automatic-stepping mode with probe-tip steps varying from 5 to 25 µm. The measurements can be either performed on a cross section of the sample or for shallow proﬁles on a bevelled section as indicated in Fig. 16.6. An example for an experimental spreading resistance proﬁle is displayed in the left part of Fig. 16.7. The right part shows the concentration-depth proﬁle deduced from the spreading resistance proﬁle. The employed procedure is described below. Fig. 16.6. Spreading resistance proﬁling (schematic) 16.2 Spreading Resistance Proﬁling 291 Fig. 16.7. Spreading resistance proﬁle of Se in Si (left) and concentration depth proﬁle of Se deduced therefrom (right) The SRP technique relies on the fact that the ideal resistance of a smalldiameter metal probe in perfect contact with the plane surface of a semiinﬁnite semiconductor is given by Rs = ρ , 4a (16.8) where ρ denotes the resistivity of the semiconductor and a the radius of the contact area. The spreading resistance, Rs , originates from the radial ﬂow of the current from the probe tip into the semiconductor. Due to the special conﬁguration, about 80 % of the potential drop occurs within a distance of 5a. In practice, the SRP contact radius can be made as small as a few µm, which leads to a corresponding small sampling volume. Theoretically, the twoprobe arrangement doubles Rs with regard to Eq. (16.8), provided that the probe-tip separation is much larger than the contact radius. In reality, the contacts are not planar circles but irregularly shaped microcontacts. This gives rise to substantial contact resistance, which cannot be derived with suﬃcient accuracy from theory. Therefore, in SRP analysis the relationship between ρ and Rs is established by calibration using homogeneously doped samples of the same material, conductivity type, and surface orientation as the test sample under consideration. Standard semiconductor theory is used to establish the relation between the resistivity and the concentration of the electrically active foreign atoms. We illustrate this procedure for a singly ionizable donor atom X in an otherwise undoped semiconductor. For a given Fermi energy EF , the electron concentration n is obtained as EF − EC n = NC exp , (16.9) kB T 292 16 Electrical Methods where EC denotes the energy of the conduction band edge and NC the eﬀective density of states in the conduction band. The latter quantity is closely related to the eﬀective electron mass mn according to 3/2 2πmn kB T NC = 2 , (16.10) h2 where h is the Planck constant. The hole concentration p follows from EG (T ) 2 np = ni = NC NV exp − (16.11) kB T with the intrinsic carrier density ni , the temperature-dependent band gap energy, EG (T ), and the eﬀective density of states, NV , in the valence band. Having obtained electron and hole concentrations, the charge neutrality condition ion +p (16.12) n = CX ion ion yields the concentration CX of ionized foreign atoms. Values of CX dis−16 −3 tinctly above 10 cm lead to enhanced scattering of charge carriers, which may be taken into account by expressions for the carrier mobilities of elecion ion , T ) and holes µn = µn (CX , T ). Empirical expressions trons µn = µn (CX of this kind can be found in the literature [15]. In a subsequent step the resistivity is obtained from 1 = qµn n + qµp p , ρ (16.13) where q denote the charge per carrier. For singly ionizable donor atoms the second term on the right hand side of Eq. (16.13) can be neglected for ion ni . Once the calculated resistivity ρ(EF , T ) value has converged to CX ion the experimental one, EF and CX (EF , T ) are known. Then, the electrically 0 , results from neutral foreign atom concentration, CX ion EX − EF CX . (16.14) 0 = gX exp CX kB T This equation accounts for the electron occupation probability of a foreign atom with a donor level, EX , and a degeneration factor, gX . The latter equals 2 for common group-V dopants such as P in silicon. Finally, the total foreign atom concentration follows from ion 0 + CX . CX = CX (16.15) Background doping can be taken into account by including additional terms in the charge neutrality Eq. (16.12). The alternative case in which the foreign atom X has acceptor character can be treated in a similar set of equations reﬂecting the reversed rôle of holes and electrons as majority and minority charge carriers. For further details about SRP the reader may consult a paper by Voss et al. [16]. References 293 References 1. J.R. Macdonald (Ed.), Impedance Spectroscopy – Emphasizing Solid Materials and Systems, John Wiley and Sons, 1987 2. R.G. Mazur, D.H. Dickey, J. Electrochem. Soc. 113, 255 (1966) 3. A.W. Imre, S. Voss, H. Mehrer, Phys. Chem. Chem. Phys. 4, 3219 (2002) 4. H. Mehrer, A.W. Imre, S. Voss, in: Mass and Charge Transport in Inorganic Materials II, Proc. of CIMTEC 2002–10th Int. Ceramics Congress and 3rd Forum on New Materials, Florence, Italy, 2002;, P. Vincenzini, V. Buscaglia (Eds.), Techna, Faenza, 2003, p.127 5. K. Funke, R.D. Banhatti, S. Brückner, C. Cramer, C. Krieger, A. Mandanici, C. Martiny, I. Ross, Phys. Chem. Chem. Phys. 4, 3155 (2002) 6. S. Summerﬁeld, Philos. Mag. B 52, 9 (1985) 7. M.D. Ingram, Phys. Chem of Glasses 28, 215 (1987) 8. W. Dieterich, P. Maass, Chem. Physics 284 439 (2002) 9. K. Funke, C. Cramer, D. Wilmer, Concept of Mismatch and Relaxation for Self-Diﬀusion and Conduction in Ionic Materials with Disordered Structures, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 10. A. Bunde, W. Dieterich, Ph. Maass, M. Mayer, Ionic Transport in Disordered Materials, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 11. D.A. Antoniadis, A.G. Gonzales, R.W. Dutton, J. Electrochem. Soc. 125, 813 (1978) 12. N.A. Stolwijk, J. Hölzl, W. Frank, Appl. Phys. A: Solid surf. 39, 37 (1966) 13. H. Bracht, N.A. Stolwijk, H. Mehrer, Phys. Rev. B 43, 14465 (1991) 14. G. Bösker, N.A. Stolwijk, U. Södervall, W. Jäger, H. Mehrer, J. Appl. Phys. 86, 791 (1999) 15. C. Jacobini, C. Canali, G. Ottaviani, A. Alberigi Quaranta, Solid State Electron. 20, 77 (1977) 16. S. Voss, N.A. Stolwijk, H. Bracht, J. Applied Physics 92, 4809 (2002) Part III Diﬀusion in Metallic Materials 17 Self-diﬀusion in Metals 17.1 General Remarks Self-diﬀusion is the most fundamental diﬀusion process in a solid. This is the major reason in addition to application-oriented motives why self-diﬀusion studies have consumed energies of many researchers. Self-diﬀusion in a metallic element A is the diﬀusion of A atoms. In practice, in most cases tagged atoms A∗ – either radioactive or stable isotopes – are used as tracers (see Chap. 13), which are chemically identical to the atoms of the base metal. As already mentioned in Chap. 8, the temperature dependence of the tracer self-diﬀusion coeﬃcient, D∗ , is often, but by no means always, described by an Arrhenius relation1 ∆H , D∗ = D0 exp − kB T (17.1) with a pre-exponential factor D0 and an activation enthalpy ∆H. The preexponential factor can usually be written as D0 = gf ν 0 a2 exp ∆S , kB (17.2) where ∆S is called the diﬀusion entropy, g is a geometrical factor of the order of unity (e.g., g = 1 for the vacancy mechanism in cubic metals), f the tracer correlation factor, ν 0 an attempt frequency of the order of the Debye frequency, and a the lattice parameter. For a diﬀusion process with a temperature-independent activation enthalpy, the Arrhenius diagram is a straight line with slope −∆H/kB . From its intercept – for T −1 =⇒ 0 – the pre-exponential factor D0 is obtained. The physical meaning of the activation parameters of diﬀusion depends on the diﬀusion mechanism and on the lattice geometry (see also Chap. 8) . Self-diﬀusion in metals is mediated by vacancy-type defects [1–6]. Strong evidence for this interpretation comes from the following observations: 1. The Kirkendall eﬀect has shown that the diﬀusivities of diﬀerent kinds of atoms in a substitutional metallic alloy diﬀuse at diﬀerent rates (see also 1 We use in this chapter again the upper index * to indicate tracer diﬀusivities. 298 2. 3. 4. 5. 17 Self-diﬀusion in Metals Chaps. 1 and 10). Neither the direct exchange nor the ring mechanism can explain this observation. It became evident that vacancies are responsible for self-diﬀusion and diﬀusion of substitutional solutes in metals in practically all cases. Vacant lattice sites are the dominating defect in metals at thermal equilibrium. Studies which permit the determination of vacancy properties were discussed in Chap. 5. These studies are based mainly on diﬀerential dilatometry, positron-annihilation spectroscopy, and quenching experiments. Isotope-eﬀect experiments of self-diﬀusion (see Chap. 9) are in accordance with correlation factors which are typical for vacancy-type mechanisms [5, 6]. Values and signs of activation volumes of self-diﬀusion deduced from high-pressure experiments (see Chap. 8) are in favour of vacancy-type mechanisms [7]. Formation and migration enthalpies of vacancy-type defects add up to the activation enthalpies observed for self-diﬀusion (see, e.g., [5, 6, 8–10]). Self-diﬀusion of many metallic elements has been studied over wide temperature ranges by the techniques described in Chap. 13. As an example, Fig. 17.1 displays the tracer diﬀusion coeﬃcient of the radioisotope 63 Ni in Ni singlecrystals. A diﬀusivity range of about 9 orders of magnitude is covered by Fig. 17.1. Diﬀusion of 63 Ni in monocrystalline Ni. T > 1200 K: data from grinder sectioning [11]; T < 1200 K: data from sputter sectioning [12] 17.2 Cubic Metals 299 the combination of mechanical sectioning [11] and sputter-sectioning techniques [12]. The investigated temperature interval ranges from about 0.47 Tm to temperatures close the melting temperature Tm . For some metals, data have been deduced by additional techniques. For example, nuclear magnetic relaxation proved to be very useful for aluminium and lithium, where no suitable radioisotopes for diﬀusion studies are available. A collection of selfdiﬀusion data for pure metals and information about the method(s) employed can be found in [8]. A convex curvature of the Arrhenius plot – i.e. deviations from Eq. (17.1) – may arise for several reasons such as contributions of more than one diﬀusion mechanism (e.g., mono- and divacancies), impurity eﬀects, grain-boundary or dislocation-pipe diﬀusion (see Chaps. 31–33). Impurity eﬀects on solvent diﬀusion are discussed in Chap. 19. Grain-boundary inﬂuences are completely avoided, if mono-crystalline samples are used. Dislocation inﬂuences can be eliminated in careful experiments on well-annealed crystals. 17.2 Cubic Metals Self-diﬀusion in metallic elements is perhaps the best studied area of solidstate diﬀusion. Some useful empirical correlations between diﬀusion and bulk properties for various classes of materials are already discussed in Chap. 8. Here we consider self-diﬀusivities of cubic metals and their activation parameters in greater detail. 17.2.1 FCC Metals – Empirical Facts Self-diﬀusion coeﬃcients of some fcc metals are shown in Fig. 17.2 as Arrhenius lines in a plot which is normalised to the respective melting temperatures (homologous temperature scale). The activation parameters listed in Table 17.1 were obtained from a ﬁt of Eq. (17.1) to experimental data. The following empirical correlations are evident: – – 2 Diﬀusivities near the melting temperature are similar for most fcc metals and lie between about 10−12 m2 s−1 and 10−13 m2 s−1 . An exception is self-diﬀusion in the group-IV metal lead, where the diﬀusivity is about one order of magnitude lower and the activation enthalpy higher2 . The diﬀusivities of most fcc metals, when plotted in a homologous temperature scale, lie within a relatively narrow band (again Pb provides an exception). This implies that the Arrhenius lines in the normalised plot have approximately the same slope. Since this slope equals −∆H/(kB Tm ) The group-IV semiconductors Si and Ge have even lower diﬀusivities than Pb at the melting point (see Chap. 23). 300 17 Self-diﬀusion in Metals Fig. 17.2. Self-diﬀusion of fcc metals: noble metals Cu, Ag, Au; nickel group metals Ni, Pd, Pt; group IV metal Pb. The temperature scale is normalised to the respective melting temperature Tm Table 17.1. Activation parameters D0 and ∆H for self-diﬀusion of some fcc metals ∆H [kJ mol−1 ] D0 [10−4 m2 s−1 ] ∆H/kB Tm Cu [14] Ag [16] Au [18] Ni [12] Pd [19] Pt [20] Pb [23] 211 0.78 18.7 170 0.041 16.5 165 0.027 14.8 281 1.33 19.5 266 0.205 17.5 257 0.05 15.2 107 0.887 21.4 a correlation between the activation enthalpy ∆H and the melting temperature Tm exists (see also Table 17.1). This correlation can be stated as follows: (17.3) ∆H ≈ (15 to 19) kB Tm (Tm in K) . – Relations like Eq. (17.3) are sometimes referred to as the rule of van Liempt [13] (see also Chap. 8). The pre-exponential factors lie within the following interval: several 10−6 m2 s−1 < D0 < several 10−4 m2 s−1 . – (17.4) The factor gf ν 0 a2 in Eq. (17.2) is typically about 10−6 m2 s−1 . Hence the range of D0 values corresponds to diﬀusion entropies ∆S between about 1 kB and 5 kB . Within one column of the periodic table, the diﬀusivity in homologous temperature scale is lowest for the lightest element and highest for the heaviest element. For example, in the group of noble metals Au self- 17.2 Cubic Metals 301 diﬀusion is fastest and Cu self-diﬀusion is slowest. In the Ni group, Pt self-diﬀusionm is fastest and Ni self-diﬀusion is slowest. 17.2.2 BCC Metals – Empirical Facts Self-diﬀusion of bcc metals is shown in Fig. 17.3 on a homologous temperature scale. A comparison between fcc and bcc metals (Figs. 17.2 and 17.3) reveals the following features: – – – – Diﬀusivities for bcc metals near the melting temperature lie between about 10−11 m2 s−1 and 10−12 m2 s−1 . Diﬀusivities of fcc metals near their melting temperatures are about one order of magnitude lower. The ‘spectrum’ of self-diﬀusivities as a function of temperature is much wider for bcc than for fcc metals. For example, at 0.5 Tm the diﬀerence between the self-diﬀusion of Na and of Cr is about 6 orders of magnitude, whereas the diﬀerence between self-diﬀusion of Au and of Ni is only about 3 orders of magnitude. Self-diﬀusion is slowest for group-VI transition metals and fastest for alkali metals. The Arrhenius diagram of some bcc metals shows clear convex (upward) curvature (see, e.g., Na in Fig. 17.3). Fig. 17.3. Self-diﬀusion of bcc metals: alkali metals Li, Na, K (solid lines); group-V metals V, Nb, Ta (dashed lines); group-VI metals Cr, Mo, W (solid lines). The temperature scale is normalised to the respective melting temperature Tm 302 – 17 Self-diﬀusion in Metals A common feature of fcc and bcc metals is that within one group of the periodic table self-diﬀusion at homologous temperatures is usually slowest for the lightest and fastest for the heaviest element of the group. Potassium appears to be an exception. Group-IV transition metals (discussed below) are not shown in Fig. 17.3, because they undergo a structural phase transition from a hcp low-temperature to a bcc high-temperature phase. The self-diﬀusivities in the bcc phases β-Ti, β-Zr and β-Hf are on a homologous scale even higher than those of the alkali metals. On a homologous scale self-diﬀusion of β-Ti – the lightest group-IV transition element – is slowest; self-diﬀusion of the heaviest group-IV transition element β-Hf is fastest. In addition, β-Ti and β-Zr show upward curvature in the Arrhenius diagram. β-Hf exists in a narrow temperature interval, which is too small to detect curvature. 17.2.3 Monovacancy Interpretation Self-diﬀusion in most metallic elements is dominated by the monovacancy mechanism (see Fig. 6.5) at least at temperatures below 23 Tm . At higher temperatures, a certain divacancy contribution, which varies from metal to metal, may play an additional rôle (see below). Let us ﬁrst consider the monovacancy contribution: Using Eqs. (4.29) and (6.2) the diﬀusion coeﬃcient of tracer atoms due to monovacancies in cubic metals can be written as eq ∗ = g1V f1V a2 C1V ω1V . D1V (17.5) g1V is a geometric factor (g1V = 1 for cubic Bravais lattices), a the lattice parameter, and f1V the tracer correlation factor for monovacancies. The atomic eq fraction of vacant lattice sites at thermal equilibrium C1V (see Chap. 5) is given by F F GF H1V S1V eq 1V C1V = exp − exp − = exp , (17.6) kB T kB kB T F where the Gibbs free energy of vacancy formation is related via GF 1V = H1V − F T S1V to the pertinent formation enthalpy and entropy. The exchange rate between vacancy and tracer atom is M S1V GM HM 0 0 ω1V = ν1V exp − 1V = ν1V exp exp − 1V , (17.7) kB T kB kB T M M where GM 1V , H1V , and S1V denote the Gibbs free energy, the enthalpy and 0 the entropy of vacancy migration, respectively. ν1V is the attempt frequency of the vacancy jump. 17.2 Cubic Metals 303 The standard interpretation of tracer self-diﬀusion attributes the total diﬀusivity to monovacancies: M H F + H1V ∗ 0 = D1V exp − 1V D∗ ≈ D1V . (17.8) kB T In the standard interpretation, the Arrhenius parameters of Eq. (17.1) have the following meaning: F M + H1V ∆H ≈ ∆H1V = H1V and 0 0 = f1V g1V a2 ν1V exp D0 ≈ D1V F M S1V + S1V kB (17.9) . (17.10) Then, according to Eq. (17.9) the activation enthalpy ∆H1V equals the sum of formation and migration enthalpies of the vacancy. The diﬀusion entropy F M + S1V ∆S ≈ ∆S1V = S1V (17.11) equals the sum of formation and migration entropies of the vacancy. Typical values for ∆S are of the order of a few kB . As discussed in Chap. 7, the correlation factor f1V accounts for the fact that for a vacancy mechanism the tracer atom experiences some ‘backward correlation’, whereas the vacancy performs a random walk. The tracer correlation factors are temperatureindependent quantities (fcc: f1V = 0.781; bcc: f1V = 0.727; see Table 7.2). 17.2.4 Mono- and Divacancy Interpretation In thermal equilibrium, the concentration of divacancies increases more rapidly than that of monovacancies (see Fig. 5.2 in Chap. 5). Even more important, individual divacancies, once formed, will avoid dissociating and thereby exhibit extended lifetimes in the crystal. In addition, divacancies in fcc metals are more eﬀective diﬀusion vehicles than monovacancies since their mobility is considerably higher than that of monovacancies [2, 9]. At temperatures above about 2/3 of the melting temperature, a contribution of divacancies to self-diﬀusion can no longer be neglected (see, e.g., the review by Seeger and Mehrer [2] and the textbooks of Philibert [3] and Heumann [4]). The total diﬀusivity of tracer atoms then is the sum of monoand divacancy contributions ∆H1V ∆H2V 0 0 exp − + D2V exp − . (17.12) D∗ = D1V kB T kB T ∗ D1V ∗ D2V The activation enthalpy of the divacancy contribution can be written as F B M ∆H2V = 2H1V − H2V + H2V . (17.13) 304 17 Self-diﬀusion in Metals M B Here H2V and H2V denote the migration and binding enthalpies of the divacancy. For fcc metals the pre-exponential factor of divacancy diﬀusion is 0 0 = g2V f2V a2 ν2V exp D2V F B M − S2V + S2V 2S1V . kB (17.14) 0 f2V is the divacancy tracer correlation factor, g2V a geometry factor, ν2V the M B attempt frequency, S2V and S2V denote migration and binding entropies of the divacancy. Measurements of the temperature, mass, and pressure dependence of the tracer self-diﬀusion coeﬃcient have proved to be useful to elucidate monoand divacancy contributions in a quantitative manner. As an example of divacancy-assisted diﬀusion in an fcc metal, Fig. 17.4 shows the Arrhenius daigram of silver self-diﬀusion according to [15–17]. A ﬁt of Eq. (17.12) to the data, performed by Backus et al. [17], resulted in the mono- and divacancy contributions displayed in Fig. 17.4. Near the melting temperature both contributions in Ag are about equal. With decreasing temperature the divacancy contribution decreases more rapidly than the monovacancy contribution. Near 2/3 Tm the divacancy contribution is not more than 10 % of the total diﬀusivity and below about 0.5 Tm it is negligible. As a consequence, the Arrhenius diagram shows a slight upward curvature and a well-deﬁned single value of the activation enthalpy no longer exists. Fig. 17.4. Self-diﬀusion in single-crystals of Ag: squares [15], circles [16], triangles [17]. Mono- and divacancy contributions to the total diﬀusivity are shown as 0 = 0.046 × dotted and dashed lines with the following Arrhenius parameters: D1V 0 = 2.24 × 10−4 m2 s−1 , ∆H2V = 2.24 eV 10−4 m2 s−1 , ∆H1V = 1.76 eV and D2V according to an analysis of Backus et al. [17] 17.2 Cubic Metals 305 Instead an eﬀective activation enthalpy, ∆Hef f , can be deﬁned (see Chap. 8), which reads for the simultaneous action of mono- and divacancies ∆Hef f = ∆H1V ∗ D1V D∗ + ∆H2V ∗ 2V ∗ . ∗ + D2V D1V + D2V ∗ D1V (17.15) Equation (17.15) is a weighted average of the individual activation enthalpies of mono- and divacancies. Additional support for the monovacancy-divacancy interpretation comes from measurements of the pressure dependence of self-diﬀusion (see Chap. 8), from which an eﬀective activation volume, ∆Vef f , is obtained. For the simultaneous contribution of the two mechanisms we have ∆Vef f = ∆V1V ∗ D1V D∗ + ∆V2V ∗ 2V ∗ , ∗ + D2V D1V + D2V ∗ D1V (17.16) which is a weighted average of the activation volumes of the individual activation volumes of monovacancies, ∆V1V , and divacancies, ∆V2V . Since ∆V1V < ∆V2V and since the divacancy contribution increases with temperature, the eﬀective activation volume increases with temperature as well. Figure 17.5 displays eﬀective activation volumes for Ag self-diﬀusion. An increase from about 0.67 Ω at 600 K to 0.88 Ω (Ω = atomic volume) near the melting temperature has been observed by Beyeler and Adda [21] and Rein and Mehrer [22]. Fig. 17.5. Eﬀective activation volumes, ∆Vef f , of Ag self-diﬀusion versus temperature in units of the atomic volume Ω of Ag: triangle, square [21], circles [22] 306 17 Self-diﬀusion in Metals Fig. 17.6. Experimental isotope-eﬀect parameters of Ag self-diﬀusion: full circles [15], triangles [25], full square [26], triangles on top [27], open circles [28] Isotope-eﬀect measurements can throw also light on the diﬀusion mechanism, because the isotope-eﬀect parameter is closely related to the corresponding tracer correlation factor (see Chap. 9). If mono- and divacancies operate simultaneously, measurements of the isotope-eﬀect yield an eﬀective isotope-eﬀect parameter: Eef f = E1V ∗ D1V D∗ + E2V ∗ 2V ∗ . ∗ + D2V D1V + D2V ∗ D1V (17.17) Eef f is a weighted average of the isotope-eﬀect parameters for monovacancies, E1V , and divacancies, E2V . The individual isotope eﬀect parameter are related via E1V = f1V ∆K1V and E2V = f2V ∆K2V to the tracer correlation factors and kinetic energy factors of mono- and divacancy diﬀusion (see Chap. 9). Fig 17.6 shows measurements of the isotope-eﬀect parameter for Ag self-diﬀusion. According to Table 7.2, we have f1V = 0.781 and f2V = 0.458. The decrease of the eﬀective isotope-eﬀect parameter with increasing temperature has been attributed to the simultaneous contribution of mono- and divacancies in accordance with Fig. 17.4. 17.3 Hexagonal Close-Packed and Tetragonal Metals Several metallic elements such as Zn, Cd, Mg, and Be crystallise in the hexagonal close-packed structure. A few others such as In and Sn are tetragonal. 17.3 Hexagonal Close-Packed and Tetragonal Metals 307 Fig. 17.7. Self-diﬀusion in single crystals of Zn, In, and Sn parallel and perpendicular to their unique axes According to Chap. 2, the diﬀusion coeﬃcient in a hexagonal or tetragonal single-crystal has two principal components: ∗ D⊥ : tracer diﬀusivity perpendicular to the axis , D∗ : tracer diﬀusivity parallel to the axis . Figure 17.7 shows self-diﬀusion in single-crystals of Zn, In, and Sn for both ∗ principal directions. In hexagonal Zn we have D∗ > D⊥ ; i.e. diﬀusion parallel to the hexagonal axis is slightly faster. For the tetragonal materials In and Sn ∗ ∗ holds true. For all of these materials the anisotropy ratio D⊥ /D∗ D ∗ < D⊥ is small; it lies in the interval between about 1/2 and 2 in the temperature ranges investigated. Diﬀusivity values in hcp Zn, Cd, and Mg reach about 10−12 m2 s−1 near the melting temperature. Such values are similar to those of fcc metals. This is not very surprising, since both lattices are close-packed structures. Let us recall the atomistic expressions for self-diﬀusion in hcp metals. The hcp unit cell is shown in Fig. 17.8. Vacancy-mediated diﬀusion can be expressed in terms of two vacancy-atom exchange rates. The rate ωa accounts for jumps within the basal plane and ωb for jumps oblique to the basal plane. The two principal diﬀusion coeﬃcients can be written as a2 eq C (3ωa fa⊥ + ωb fb⊥ ) , 2 V 3 D∗ = c2 CVeq ωb fb . 4 ∗ D⊥ = (17.18) 308 17 Self-diﬀusion in Metals Fig. 17.8. Hexagonal close-packed unit cell with lattice paranmeters a and c. Indicated are the vacancy jump rates: ωa is within the basal plane and ωb oblique to it Here a denotes the lattice parameter within the basal plane and c the lattice parameter in the hexagonal direction. fa⊥ , fb⊥ and fb are correlation factors. The anisotropy ratio is then: A ≡ ∗ D⊥ 2 a2 (3ωa fa⊥ + ωb fb⊥ ) = . ∗ D 3 c2 ωb fb (17.19) If correlation eﬀects are negelected, i.e. for fa⊥ = fb⊥ = fb = 1, we get from Eq. (17.19) 2 a2 ωa A ≈ +1 . (17.20) 3 3 c2 ωb For the ideal ratio c/a = 8/3 and ωa = ωb , one ﬁnds A = 1; this remains correct if correlation is included. The correlation factors and A vary with the ratio ωa /ωb . For details the reader is referred to a paper by Mullen [29]. 17.4 Metals with Phase Transitions Many metallic elements undergo allotropic transformations and reveal different crystalline structures in diﬀerent temperature ranges. Such changes are found in about twenty metallic elements. Allotropic transitions are ﬁrstorder phase transitions, which are accompanied by abrupt changes in physical properties including the diﬀusivity. Some metals undergo second-order phase transitions, which are accompanied by continuous changes in physical properties. A well known example is the magnetic transition from the ferromagnetic to paramagnetic state of iron. In intermetallic compounds (considered in Chap. 20) also order-disorder transitions occur, which can be second order. In what follows we consider two examples, which illustrate the eﬀects of phase transitions on self-diﬀusion: 17.4 Metals with Phase Transitions 309 Self-diﬀusion in iron: Iron undergoes allotropic transitions from a bcc, to an fcc, and once more to a bcc structure, when the temperature varies according to the following scheme: 1183 K 1653 K 1809 K α-Fe (bcc) ⇐⇒ γ-Fe (fcc) ⇐⇒ δ-Fe (bcc) ⇐⇒ Fe melt. Numerous heat treatments of steels beneﬁt from these phase transformations, which are of ﬁrst-order. They are associated with abrupt changes of the diﬀusion coeﬃcient (see Fig. 17.9). It is interesting to note that the transition from bcc iron to close-packed fcc iron is accompanied by a decrease in the diﬀusivity of about one order of magnitude. This is in accordance with the observation that self-diﬀusion in fcc metals (Fig 17.2) is slower than self-diﬀusion in bcc metals (Fig. 17.3) at the same homologous temperature. Magnetic phase transitions are prototypes of second-order phase transitions. In such transitions an order parameter passes through the transition temperature in continuos manner. Second-order transitions are associated with continuous changes of physical properties. Below the Curie temperature, TC = 1043 K, iron is ferromagnetic, above TC it is paramagnetic. Figure 17.9 shows that self-diﬀusion is indeed a continuous function of temperature around TC . However, below TC it is clearly slower that an Arrhenius extrapolation from the paramagnetic bcc region would suggest. In the literature several models have been discussed, which describe the inﬂuence of Fig. 17.9. Self-diﬀusion in the α-, γ- and δ-phases of Fe: full circles [30]; open circles [31]; triagles [32]; squares [33] 310 17 Self-diﬀusion in Metals ferromagnetic order on diﬀusion. The simplest one correlates the variation of the activation enthalpy according to ∆Hp (1 + αS 2 ) ∗ 0 D = Dp exp − (17.21) kB T with some ferromagnetic order parameter S. The long-range order parameter is connected via S ≡ MS (T )/MS (0) to the spontaneous magnetisation MS (T ) at temperature T . ∆Hp and Dp0 are the activation enthalpy and the preexponential factor in the paramagnetic state; α is a ﬁtting parameter. Self-diﬀusion in group-IV transition metals: These metals undergo transformations from a hcp low-temperature phase (α−phase) to a bcc hightemperature phase (β-phase). The transition temperatures, Tα,β , are 1155 K for Ti, 1136 K for Zr, and 2013 K for Hf. As an example, Fig. 17.10 shows self-diﬀusion in hcp and bcc titanium according to [34–36]. We note that upon the transformation from the hcp to the bcc structure the diﬀusivity increases by almost three orders of magnitude. Very similar behaviour is reported for zirconium and hafnium (see, [8] for references). Self-diﬀusion in the close-packed hcp structure is relatively slow, whereas we have already seen in Fig. 17.3 that self-diﬀusion in the less densely packed bcc phases metals is relatively fast. Fig. 17.10. Self-diﬀusion in α- und β-phases of titanium: circles [34]; tiangles [35]; squares [36] References 311 The very fast self-diﬀusion of bcc high-temperature phases and the wide spectrum of diﬀusivities of bcc metals has been attributed to special features of the lattice dynamics in the bcc structure by Köhler and Herzig [37] and also by Vogl and Petry [38]. A nearest-neighbour jump of an atom in the bcc lattice is a jump in a 111 direction. For bcc metals the longitudinal phonon branch shows a minimum for 2/3 111 phonons. This minimum is most pronounced for group-IV metals. The associated low phonon frequencies indicate a small activation barrier for nearest-neighbour exchange jumps between atom and vacancy. References 1. Y. Adda, J. Philibert, La Diﬀusion dans les Solides, Presses Universitaires de France, 1966 2. A. Seeger, H. Mehrer, in: Vacancies and Interstitials in Metals, A. Seeger, D. Schumacher, J. Diehl, W. Schilling (Eds.), North-Holland, Amsterdam, 1970, p.1 3. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 4. Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, Berlin, 1992 5. N.L. Peterson, J. Nucl. Mat. 69/70, 3 (1978) 6. H. Mehrer, J. Nucl. Mat. 69/70, 38 (1978) 7. H. Mehrer, Defect and Diﬀusion Forum 129–130, 57 (1996) 8. H. Mehrer, N. Stolica, N.A. Stolwijk, Self-diﬀusion in Solid Metallic Elements, Chap. 2 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol.-Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 9. H.J. Wollenberger, Point Defects, in: Physical Metallurgy, R.W. Cahn, P. Haasen (Eds.), North-Holland Publishing Company, 1983, p. 1139 10. H. Ullmaier (Vol.Ed.), Atomic Defects in Metals, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Condensed Matter, Vol. 25, Springer-Verlag, 1991 11. H. Bakker, Phys. Stat. Sol. 28, 569 (1968) 12. K. Maier, H. Mehrer, E. Lessmann, W. Schüle, Phys. Stat. Sol. (b) 78, 689 (1976) 13. B.S. Bokstein, S.Z. Bokstein, A.A. Zhukhovitskii, Thermodynamics and Kinetics of Diﬀusion in Solids, Oxonian Press, New Dehli, 1985 14. S.J. Rothman, N.L. Peterson, Phys. Stat. Sol. 35, 305 (1969) 15. S.J. Rothman, N.L. Peterson, J.T. Robinson, Phys. Stat. Sol. 39, 635 (1970) 16. N.Q. Lam, S.J. Rothman, H. Mehrer, L.J. Nowicki, Phys. Stat. Sol. (b) 57, 225 (1973) 17. J.G.E.M. Backus, H. Bakker, H. Mehrer, Phys. Stat. Sol. (b) 64, 151 (1974) 18. M. Werner, H. Mehrer, in: DIMETA 82 – Diﬀusion in Metals and Alloys, F.J. Kedves, D.L. Beke (Eds.), Trans Tech Publications, Switzerland, 1983, p. 393 19. N.L. Peterson, Phys. Rev. A 136, 568 (1964) 20. G. Rein, H. Mehrer, K. Maier, Phys. Stat. Sol. (a) 45, 253 (1978) 312 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 17 Self-diﬀusion in Metals M. Beyeler, Y. Adda, J. Phys. (Paris) 29, 345 (1968) G. Rein, H. Mehrer, Philos. Mag. A 45,767 (1982) J.W. Miller, Phys. Rev. 181, 10905 (1969) R.H. Dickerson, R.C. Lowell, C.T. Tomizuka, Phys. Rev. A 137, 613 (1965) P. Reimers, D. Bartdorﬀ, Phys. Stat. Sol. (b9 50, 305 (1972) N.L. Peterson, L.W. Barr, A.D. Le Claire, J. Phys, C6, 2020 (1973) Chr. Herzig, D. Wolter, Z. Metallkd. 65, 273 (1974) H. Mehrer, F. Hutter, in: Point Defects and Defect Interactions in Metals, J.I. Takamura, M. Doyama, M. Kiritani (Eds.), University of Tokyo Press, 1982, p. 558 J. Mullen, Phys. Rev. 124 (1961) 1723 M. Lübbehusen, H. Mehrer, Acta Metall. Mater. 38, 283 (1990) Y. Iijima, K. Kimura, K. Hirano, Acta Metall. 36, 2811 (1988) F.S. Buﬃngton, K.I. Hirano, M. Cohen, Acta Metall. 9, 434 (1961) C.M. Walter, N.L. Peterson, Phys. Rev. 178, 922 (1969) J.F. Murdock, T.S. Lundy, E.E. Stansbury, Acta Metall. 12 1033 (1964) F. Dyment, Proc. 4th Int. Conf. on Titanium, H. Kimura, O. Izumi (Eds.), Kyoto, Japan, 1980, p. 519 U. Köhler, Chr. Herzig, Phys. Stat. Sol. (b) 144, 243 (1987) U. Köhler, Chr. Herzig, Philos. Mag. A 28, 769 (1988) G. Vogl, W. Petry, Physik. Blätter 50, 925 (1994) 18 Diﬀusion of Interstitial Solutes in Metals Solute atoms which are considerably smaller than the atoms of the host lattice are incorporated in interstitial sites and form interstitial solid solutions. This is the case for hydrogen (H), carbon (C), nitrogen (N) and oxygen (O) in metals. Interstitial sites are deﬁned by the geometry of the host lattice. For example, in fcc, bcc and hcp host metals interstitials occupy either tetrahedral or octahedral sites and diﬀuse by jumps from one interstitial site to neighbouring ones (see Chap. 6). No defect is necessary to mediate their diffusion jumps, no defect-formation term enters the expression for the diﬀusion coeﬃcient and no defect-formation enthalpy contributes to the activation enthalpy of diﬀusion (see Chap. 6). In the present chapter we consider ﬁrst the ‘heavy’ interstitial diﬀusers C, N and O in Sect. 18.1. Hydrogen is the smallest and lightest atom in the periodic table. Hydrogen diﬀusion in metals is treated separately in Sect. 18.2. Whereas non-classical isotope eﬀects and quantum eﬀects are usually negligible for heavier diﬀusers, such eﬀects play a rôle for diﬀusion of hydrogen. 18.1 ‘Heavy’ Interstitial Solutes C, N, and O 18.1.1 General Remarks Interstitial atoms diﬀuse much faster than atoms of the host lattice or substitutional solutes, because the small sizes of the interstitial solutes permit rather free jumping between interstices. Typical examples are shown in Fig. 18.1, where the diﬀusion coeﬃcients of C, N, and O in niobium (Nb) are displayed together with Nb self-diﬀusion. The corresponding activation Table 18.1. Activation parameters of interstitial diﬀusants in Nb. For comparison self-diﬀusion paramters of Nb are also listed (for references see [1]) −1 ∆H/kJ mol D0 /m2 s−1 C N O Nb 142 1 × 10−6 161 6.3 × 10−6 107 4.2 × 10−7 395 5.2 × 10−5 314 18 Diﬀusion of Interstitial Solutes in Metals Fig. 18.1. Diﬀusion of interstitial solutes C, N, and O in Nb. For comparison Nb self-diﬀusion is also shown enthalpies and pre-exponential factors are collected in Table 18.1. The activation enthalpies of interstitital diﬀusers are much smaller than those of Nb self-diﬀusion with the result that the diﬀusion coeﬃcients for interstitial diﬀusion are many orders of magnitude larger than those for self-diﬀusion of lattice atoms. Interstitial diﬀusivities can be as high as diﬀusivities in liquids, which near the melting temperature are typically between 10−8 m2 s−1 and 10−9 m2 s−1 (see, e.g., Fig. 15.2). 18.1.2 Experimental Methods The fast diﬀusion of C, N, and O and the fact that nitrogen and oxygen are gases, or, in the case of carbon, readily available in gas or vapour form (CO, CO2 , CH4 ,. . . ) have an impact on the choice of methods used to measure their diﬀusion coeﬃcients (see also Part II of this book). In the following, we summarise the most important experimental methods: – Steady-state methods are particularly appropriate for fast diﬀusers such as C, N, and O. The steady-state concentration gradient may be measured directly or calculated from solubility data. The ﬂux can be 18.1 ‘Heavy’ Interstitial Solutes C, N, and O – – – – – – – 315 measured by standard gas-ﬂow methods. With suitable electrodes supplying and removing diﬀusant in an electrochemical cell, which can be sometimes devised, the ﬂux can be deduced from measurements of the electrical current. A suitable carbon isotope for the radiotracer method, viz. 14 C, is available. Because of its weak β-radiation the residual activity method (Gruzin-Seibel method, see Chap. 13) is adequate. Enriched stable isotopes (28 O, 12 N) in combination with SIMS proﬁling can be used to study O and N diﬀusion. Diﬀusion-couple methods are sometimes used, although not so commonly as with substitutional alloys. Both the simple error-function solution and the Boltzmann-Matano method of analysis are applied (see Chaps. 3 and 10). Nuclear reaction analysis (NRA) for the determination of diﬀusion proﬁles (see Chap. 15) is a natural complement for ion implantation of sample preparation. Both techniques are frequently applied together. Out-diﬀusion methods utilise outgassing for N or O and decarburisation for C. These processes usually entail samples containing the diﬀuser in primary solid solution. Often error-function type solutions apply for the analysis of the results. In-diﬀusion experiments often include reaction diﬀusion situations. Reaction of the diﬀuser can occur leading, in addition to the always present primary solid solution, to the growth of one or more outer layers of other phases, corresponding to the intermediate phases at the diﬀusion temperature. For example, carbide, oxide, or nitride phase layers may form on samples into which C, N, or O is being diﬀused. If the concentrationdepth proﬁle is measured, the interdiﬀusion coeﬃcient can be determined, e.g., by the Boltzmann-Matano method (see Chap. 10). For the diﬀusion of C, N, and O in bcc metals by far the most commonly employed indirect methods are those based on Snoek-eﬀect – internal friction methods and, at the lower temperatures, measurements of the anelastic stress or strain relaxation (for details see Chap. 14 and the reviews by Nowick and Berry [2] and Batist [3]). The latter techniques provide values of D at temperatures that may extend down to ambient and even below. With all the indirect methods, the deduced D-values are model-sensitive. For the interpretation of Snoek-eﬀect based measurements on bcc metals it is usually assumed that the solute atoms occupy octahedral interstitial sites. Occasionally measurements of magnetic relaxation have been used in the study of C, N, and O diﬀusion. For details see Chap. 14 and the textbook of Kronmüller [4]. 316 18 Diﬀusion of Interstitial Solutes in Metals 18.1.3 Interstitial Diﬀusion in Dilute Interstial Alloys Diﬀusivities of interstitial diﬀusers have sometimes been measured over an exceptionally wide range of temperatures by combining direct measuring techniques at high temperatures and indirect techniques, which monitor a few atomic jumps only, at low temperatures. Such measurements can provide materials for tests of the linearity of the Arrhenius relation. For example, N diﬀusion in bcc α-Fe and δ-Fe covers a range from 10−8 m2 s−1 to about 10−24 m2 s−1 without signiﬁcant deviation from linearity (for references see [1]). For N and O diﬀusion in Ta and Nb, linear Arrhenius behaviour has been reported over wide temperature ranges as well. Diﬀusion coeﬃcients, for C diﬀusion in α-Fe are assembled in Fig. 14.7. In this ﬁgure data from direct diﬀusion measurements at high temperatures and data deduced from indirect techniques such as internal friction, elastic after eﬀect, and magnetic after eﬀect have been included (see also Chap. 14). Interstitial solutes migrate by the direct interstitial mechanism discussed already in Chap. 6. For cubic host lattices, the diﬀusion coeﬃcient of interstitial solutes can be written as M S HM exp − . (18.1) D = ga2 ν 0 exp R kB T Here a is the cubic lattice parameter and g a geometric factor, which depends on the lattice geometry and on the type of interstitial sites (octahedral or tetrahedral) occupied by the solute. For jumps between neighbouring octahedral sites (see Fig. 6.1) g = 1 for the fcc and g = 1/6 for the bcc lattice. The Arrhenius parameters of Eq. (8.1) have the following simple meaning for diﬀusion of interstitial solutes: ∆H ≡ H M and D0 ≡ ga2 ν 0 exp (18.2) SM kB , (18.3) where H M and S M denote the migration enthalpy and entropy of the intertitial. With reasonable values for the migration entropy (between zero and several kB ) and the attempt frequency ν 0 (between 1012 and 1013 s−1 ), Eq. (18.3) yields the following limits for the pre-exponential factors of interstitial solutes: (18.4) 10−7 m2 s−1 ≤ D0 ≤ 10−4 m2 s−1 . The experimental values of D0 for C, N, and O from Table 18.1 indeed lie in the expected range. Measurements of the isotope eﬀect of 12 C/13 C diﬀusion in α-Fe yielded an isotope eﬀect parameter near unity [7]. This isotope eﬀect is well compatible with a correlation factor of f = 1, which is expected for a direct interstitial mechanism (see Chap. 9). 18.2 Hydrogen Diﬀusion in Metals 317 Slight upward curvatures in the Arrhenius diagram were observed, e.g., for C diﬀusion in Mo and in α-Fe (see Fig. 14.7) in the high-temperature region [1]. Several suggestions have been discussed in the literature to explain this curvature [5, 6]. These suggestions include formation of interstitialvacancy pairs, formation of di-interstitials and interstitial jumps between octahedral and tetrahedral sites in addition to jumps between neighbouring octahedral sites, and in the case of iron the magnetic transition. The simple picture developed above describes diﬀusion in very dilute interstitial solutions. For diﬀusion in interstitial alloys with higher concentration the interaction between interstitial solutes comes into play. For carbon in austenite, tracer data are available from the work of Parris and McLellan [8] and chemical diﬀusion and activity data from the work of Smith [9]. According to Belova and Murch [10] paired carbon interstititals play a rôle in diﬀusion. 18.2 Hydrogen Diﬀusion in Metals 18.2.1 General Remarks The ﬁeld of hydrogen in metals originates from the work of Thomas Graham – one of the pioneers of diﬀusion in Great Britain (see Chap. 1). In 1866 he discovered the ability of Pd to absorb large amounts of hydrogen. He also observed that hydrogen can permeate Pd-membranes at an appreciable rate [11] and he introduced the concept of metal-hydrogen alloys without deﬁnite stoichiometry, in contrast to stoichiometric nonmetallic hydrides. In 1914 Sieverts found that the concentration of hydrogen in solution (at small concentrations) is proportional to the square root of hydrogen pressure [12]. The observation of Sieverts can be considered as direct evidence for the dissociation of the H2 molecule, when hydrogen enters a metal-hydrogen solution. Inside the metal crystal, hydrogen atoms occupy interstices. Since Graham and Sieverts, many scientists have devoted much of their scientiﬁc work to metal-hydrogen systems. Hydrogen in metals provides a large and fascinating topic of materials science, which has been the subject of many international conferences. Hydrogen in metals has also attracted considerable interest from the viewpoint of applications. For example, hydrogen storage in metals is based on the high solubility and fast diﬀusion of hydrogen in metal-hydrogen systems. Pd membranes for hydrogen puriﬁcation provide an old and well-known application based on the very fast diﬀusion. Such membranes can be used either to extract hydrogen from a gas stream or to purify it. Nowadays, an enormous body of knowledge about hydrogen in metals is available. In this chapter, we can only provide a brief survey of some of the striking features of H-diﬀusion. For more comprehensive treatments we refer the reader to books edited by Alefeld and Völkl [13, 14], Wipf [15] and 318 18 Diﬀusion of Interstitial Solutes in Metals to reviews of the ﬁeld [16–18]. A data collection for H diﬀusion in metals can be found in [19] and for diﬀusion in metal hydrides in [20]. 18.2.2 Experimental Methods The very fast diﬀusion and the often high solubility of hydrogen have consequences for the experimental techniques used in hydrogen diﬀusion studies: In addition to concentration-proﬁle methods, permeation methods based on Fick’s ﬁrst law, absorption and desorption methods, electrochemical methods, and relaxation methods are in use. Due to the favourable gyromagnetic ratio of the proton and due its large quasielastic scattering cross section for neutrons, nuclear magnetic resonance (NMR) and quasielastic neutron scattering (QENS) are specially suited for hydrogen diﬀusion studies. Here, we mention the major experimental methods brieﬂy and refer for details to Part II of this book: – – – The radiotracer method can be applied using the isotope tritium (3 H). Its half-life is t1/2 = 12.3 years and it decays by emitting weak β-radiation. Nuclear reaction analysis (NRA) can be used to measure concentration proﬁles (see Chap. 15). For example, the 15 N resonant nuclear reaction H(15 N, αγ)12 C has been used to determine H concentration proﬁles. In steady-state permeation usually the stationary rate of permeation of hydrogen through a thin foil is studied. If the steady-state concentration on the entry and exit surface are maintained at ﬁxed partial pressures of molecular hydrogen gas, pm1 and pm2 , respectively, the ﬂux per unit are through a membrane of thickness ∆x is J∞ = – KD 1/2 1/2 (p − pm2 ) , ∆x m1 (18.5) where K is called the Sieverts constant. The diﬀusivity D is then determined from the ﬂux, provided that K is known from solubility measurements. The Sieverts constant is thermally activated via the heat of solution for hydrogen. A ﬁne example of permeation studies is the work of Hirscher and associates [37], in which H permeation through Pd, Ni, and Fe membranes has been investigated. In non-steady-state permeation the rapid establishment of a ﬁxed hydrogen concentration on the entry side of a membrane by contact with H2 gas induces a transient, time-dependent ﬂux, Jt , prior to the ﬁnal steady-state ﬂux, J∞ . It can be shown that ∆x2 Jt ∼ 2∆x exp − . (18.6) = √ J∞ 4Dt πDt 18.2 Hydrogen Diﬀusion in Metals – – – – 319 The diﬀusivity can be determined from the characteristics of the time-lag. In permeation studies, UHV gas-permeation systems are used and care must be taken to avoid problems related to surface layers. Resistometric methods make use of the resistivity change upon hydrogen incorporation in a metal. For example, the resistivity of Nb-H increases by about 0.7 µΩcm per percent hydrogen. Since the electric resistivity can be measured very accurately, this property can be used to monitor hydrogen redistribution in a sample. Electrochemical techniques are variations of the permeation methods. They use electrochemical techniques to measure and often, also, to produce the hydrogen ﬂux in a sample membrane in an electrolytic cell. Hydrogen is generated on the cathode side and the entry concentration is controlled by the applied voltage. On the exit side, the potential is maintained positive so that the arriving H atoms are oxidised. The equivalent electrical current generated by the oxidising process is a sensitive measure of the ﬂux through the membrane. Electrochemical permeation cells may be operated in several modes (step method, pulse method, oscillation method), which diﬀer by the boundary conditions imposed experimentally on the sample. Analyses for the associated time-lag relations can be found, e.g., in a paper by Züchner and Boes [21]. Electrochemical methods are useful over a relatively limited temperature range and may be subject to surface eﬀects. Absorption and desorption methods are based on the continuum description of in- or out-diﬀusion, e.g., for cylindrical or spherical samples (see Chap. 2 for solutions of the diﬀusion equation). These methods are applicable at relatively high temperatures; again, care must be taken to avoid problems related to surface layers. Mechanical relaxation methods include stress and strain relaxation, internal friction and modulus change measurements: – The Gorsky eﬀect enables studies of long-range diﬀusion driven by a dilation gradient. It occurs because hydrogen expands the lattice. A gradient in dilatation, produced, e.g., by bending the sample, may be used to set up a gradient in concentration. With the Gorsky technique, one measures the time required to establish the concentration gradient by hydrogen diﬀusion across the sample diameter. This is a macroscopic rather than a microscopic relaxation time. If the sample diameter is known, the absolute value of D can be determined (see Chap. 14). – Whereas the Snoek eﬀect has been widely used to study the diﬀusion of ‘heavy’ interstitials in bcc metals, its application to H-diﬀusion has not been successful despite several attempts having been made. Hydrogen-related internal friction peaks are often reported in the literature (see, e.g., Alefeld and Völkl [13] for references), but in no case has it been established that any of these peaks results from the 320 – – – 18 Diﬀusion of Interstitial Solutes in Metals Snoek eﬀect of hydrogen alone. Combinations with impurities, lattice defects or the formation of hydrogen pairs are suggested as causes. Magnetic relaxation studies are very sensitive, but they are limited to ferromagnetic materials [22]. For example, they have been applied by Hirscher and Kronmüller [38] in studies of H diﬀusion in several ferromagnetic alloys and amorphous metals. The extensive use of nuclear magnetic relaxation (NMR) for the study of diﬀusion in metal-hydrogen solid solutions or in metal hydrides is favoured by the properties of the proton. (i) The strength of the NMR signal is proportional to the gyromagnetic ratio γ of the nucleus. The proton has the largest γ of all stable nuclei. (ii) The proton spin of I = 1/2 produces only dipolar interactions with its surroundings; the lack of quadrupole coupling (present only for nuclei with I > 1/2) simpliﬁes the interpretation of NMR spectra. The NMR technique is a well-established tool for studying atomic motion in condensed matter. Data usually consist of measurements of longitudinal spin-lattice-relaxation time T1 , of the transverse spin-spin relaxation time T2 , or of the motional narrowing of the resonance line. A theoretical model is necessary to deduce the diﬀusion coeﬃcient therefrom. For details see Chap. 15 and reviews on nuclear magnetic relaxation techniques [24–26]. Quasielastic neutron scattering (QENS) is also well suited to the study of hydrogen diﬀusion. The neutron scattering cross-section of the proton is an order of magnitude larger than that of the deuteron and all other nuclei. The QENS method is based on the following physical phenomenon: a monoenergetic neutron beam is scattered incoherently by the protons in the metal. Because of the diﬀusion of the protons, the beam will be energetically broadened and the width of the line depends on the rate of diﬀusion. For small momentum transfer Q, i.e. for small scattering angles, the full width at half maximum in energy, ∆E, is given by ∆E = 2DQ2 , (18.7) where D is the diﬀusion coeﬃcient, the Planck constant divided by 2π, and Q the momentum transfer. From the linewidth at large scattering angles, atomistic details of the jump process (jump length, jump direction) can be obtained as discussed in Chap. 15. Further information can be found in a textbook by Hempelmann [27] and several reviews of the ﬁeld [28–31]. Both nuclear methods, NMR and QENS, are independent of surface related problems. 18.2.3 Examples of Hydrogen Diﬀusion In this section, typical examples for the temperature dependence of hydrogen diﬀusion and its isotope eﬀects are noted. Hydrogen forms an interstitial solid solution with most metallic elements. Some metals have a negative enthalpy of solution and a high solubility for hydrogen (Ti, Zr, Hf, Nb, Ta, 18.2 Hydrogen Diﬀusion in Metals 321 Pd, . . . ) and form hydrides at higher hydrogen concentrations. Other metals have a positive enthalpy of solution and a relatively low solubility (group-VI metals, group-VII metals, noble metals, Fe, Co, Ni, . . . ) [23]. We conﬁne ourselves to fcc and bcc cubic α-hydrides, i.e. to low hydrogen concentrations. For diﬀusion in hydrides with higher concentrations we refer to the literature mentioned at the beginning of Sect. 18.2. Metal-hydrogen systems are prototypes of fast solid-state diﬀusion. Diffusion of hydrogen can be observed still far below room temperature. The smallest activation enthalpies and the largest isotope eﬀects have been found for metal-hydrogen systems. Below room temperature, the diﬀusion coeﬃcients of hydrogen in several transition metals or alloys are the largest known for long-range diﬀusion in solids. The diﬀusivity of hydrogen in metals is even at room temperature very high. For example, H in Nb has a roomtemperature diﬀusivity of about 10−9 m2 s−1 , which corresponds to about 1012 jumps per second. It exceeds the diﬀusivity of heavy interstitial such as C, N, and O at this temperature by 10 to 15 orders of magnitude (see Sect. 18.1). Phenomenologically, this high diﬀusivity is a consequence of the very low activation enthalpies. Since hydrogen atoms have a small mass, quantum eﬀects can be expected for diﬀusion of hydrogen. The three isotopes of hydrogen (H, D, and T) have large mass ratios. Hence isotope eﬀects can be studied over a wide range, which is important to shed light on possible diﬀusion mechanisms. The palladium-hydrogen system along with nickel and iron has attracted perhaps the largest amount of attention. Most of the experimental methods were applied to Pd-H and the consistency of the data is remarkably good (for references see [19]). H-diﬀusion in Pd, Ni and Fe is displayed in Fig. 18.2. The Arrhenius line represents a best ﬁt to the available data suggested by [13] with the Arrhenius parameters listed in Table 18.2. A jump model seems to be appropriate. Quasielastic √ neutron scattering experiments have shown that the jump distance is a/ 2 (a = cubic lattice parameter). This distance corresponds to jumps between neighbouring octahedral sites and not to a/2 for jumps between tetrahedral sites [32]. Diﬀusion of hydrogen in nickel has been studied from about room temperature up to the melting temperature of Ni (1728 K) (for references see [19]). The data are remarkably consistent although most measurements have been performed with surface sensitive methods. Because of the low soluTable 18.2. Activation parameters of H diﬀusion in Pd, Ni, and Fe according to Alefeld and Völkl [13] Pd 0 2 −1 Ni (T < TC ) Ni (T > TC ) Fe (above 300 K) −7 D /m s 2.9 × 10 ∆H/eV (or kJ mol−1 ) 0.23 (22.1) 4.76 × 10−7 0.41 (39.4) 6.87 × 10−7 0.42 (40.4) 4.0 × 10−4 0.047 (4.5) 322 18 Diﬀusion of Interstitial Solutes in Metals Fig. 18.2. Diﬀusion of H in Pd, Ni and Fe according to Alefeld and Völkl [13] bility of H in Ni other methods such as Gorsky eﬀect, NMR, and QENS have limited applicability for the Ni-H system. The Arrhenius parameters below the magnetic transition (Curie temperature TC = 627 K) seem to be only slightly diﬀerent than above (see Fig. 18.2). Diﬀusion of hydrogen in iron has considerable importance due to the technical challenge of hydrogen embrittlement of iron and steels. The absolute values for H-diﬀusion in Fe are higher than those for Pd and Ni (see Fig 18.2). In spite of the technological interest and the large number of studies (for references see [19]), the scatter of the data is rather large especially below room temperature. Several reasons for this scatter have been discussed in the literature: surface eﬀects, trapping of hydrogen by impurities, dislocations, grain boundaries, or precipitates, and the formation of molecular hydrogen in micropores, either already existing in the material or produced by excess loading (for references see [18]). Hydrogen in niobium has been studied over a very wide temperature region (see Fig. 18.3). Because of the high diﬀusivities and its relatively small changes with temperature the Gorsky technique could be used for both H and D in nearly the whole temperature range. Tritium diﬀusion has been studied in a more limited temperature range. Isotope eﬀects of hydrogen diﬀusion in Nb are very evident from Fig. 18.3. Similar isotope eﬀect studies are available for V and Ta (see Table 18.3). 18.2 Hydrogen Diﬀusion in Metals 323 Fig. 18.3. Diﬀusion of H, D, and T in Nb according to [13] 18.2.4 Non-Classical Isotope Eﬀects Classical rate theory for the isotope eﬀect in diﬀusion predicts, if many-body eﬀects are neglected, for the ratio of the diﬀusivities [33, 34], D1 m2 = , (18.8) D2 m1 where m1 and m2 are the isotope masses. If manybody eﬀects are taken into account, Eq. (18.8) must be modiﬁed (see Chap. 9). Nevertheless, the isotope eﬀect is still completely attributed to the pre-exponential factors. In the classical limit, the activation enthalpies are independent of the isotope masses. For several metal-hydrogen systems non-classical isotope eﬀects have been reported. Figure 18.3 and Table 18.3 show that in group-V transition metals hydrogen (H) diﬀuses more rapidly than deuterium (D), and deuterium diffuses more rapidly than tritium (T). In addition, the activation enthalpies of hydrogen isotopes are diﬀerent and hence the ratio of the diﬀusivities varies with temperature. Interestingly, the characteristic features of the dependence of the diﬀusivity on the isotope mass are correlated with the structure of the host metal [13, 14]. In the bcc metals V, Nb and Ta, hydrogen diﬀuses faster than deuterium 324 18 Diﬀusion of Interstitial Solutes in Metals Table 18.3. Activation parameters for diﬀusion of H, D, and T in Nb, Ta and V according to Alefeld and Völkl [13] Isotope Parameters Nb Ta V H D0 /m2 s−1 5 × 10−8 (T > 273 K) 0.9 × 10−8 (T < 273 K) 0.106 (T > 273 K) 0.068 (T < 223 K) 5.4 × 10−8 0.129 4.5 × 10−8 0.125 4.4 × 10−8 2.9 × 10−8 0.140 0.043 4.9 × 10−8 0.163 3.7 × 10−8 0.08 ∆H/eV D T D0 /m2 s−1 ∆H/eV D0 /m2 s−1 ∆H/eV in the whole temperature regime investigated. For the activation enthalpies ∆HH < ∆HD (18.9) is observed (see Table 18.3). As a consequence, the ratio DH /DD for the group-V transition metals increases with decreasing temperature. For the fcc metals, the pre-exponential factors of H and D scale in accordance with Eq. (18.8) within the experimental errors. However, again the activation enthalpies are mass-dependent, but in contrast to bcc metals one observes ∆HH > ∆HD . (18.10) This fact leads to an inverse isotope eﬀect at lower temperatures. For example, in Pd below about 773 K deuterium diﬀuses faster than hydrogen. Because of the non-classical behaviour of hydrogen and the large temperature region over which diﬀusion coeﬃcients were measured, it is by no means evident that the diﬀusion coeﬃcient of hydrogen in metals should obey a linear Arrhenius relation over the entire temperature range. The break observed in the Arrhenius relation for H in Nb (see Fig. 18.3) was ﬁrst observed with the Gorsky eﬀect method and conﬁrmed independently by measurements of resistivity changes [35] and by QENS [36]. The deviation of hydrogen diﬀusion in Nb from an Arrhenius law at lower temperatures (Fig. 18.3) has also been observed in the tantalum-hydrogen system. It has been attributed to incoherent tunneling. References 1. A.D. Le Claire, Diﬀusion of C, N, and O in Metals Chap. 8 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol.Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990, p. 471 References 325 2. A.S. Nowick, B.S. Berry, Anelastic Relaxation in Crystalline Solids, Academic Press, New York, (1972) 3. R.D. Batist, Mechanical Spectroscopy, in: Materials Science and Technology, Vol. 2B: Characterisation of Materials, R.W. Cahn, P. Haasen, E.J. Cramer (Eds.), VCH, Weinheim, 1994, p. 159 4. H. Kronmüller, Nachwirkung in Ferromagnetika, Springer Tracts in Natural Philosophy, Springer-Verlag (1968) 5. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 6. Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, Berlin, 1992 7. A.J. Bosman, PhD Thesis, University of Amsterdam (1960) 8. D.C. Parris, R.B. McLellan, Acta Metall. 24, 523 (1976) 9. R.P. Smith, Acta Metall. 1, 576 (1953) 10. I.V. Belova, G.E. Murch, Philos. Mag. 36, 4515 (2006) 11. T. Graham, Phil. Trans. Roy. Soc. (London) 156, 399 (1866) 12. A. Sieverts, Z. Phys. Chem. 88, 451 (1914) 13. G. Alefeld, J. Völkl (Eds.), Hydrogen in Metals I – Application-oriented Properties, Topics in Applied Physics, Vol. 28, Springer-Verlag, 1978 14. G. Alefeld, J. Völkl (Eds.), Hydrogen in Metals II – Basic Properties, Topics in Applied Physics, Vol. 29, Springer-Verlag, 1979 15. H. Wipf (Ed.), Hydrogen in Metals III – Properties and Applications, Topics in Applied Physics Vol. 73, Springer-Verlag, 1997 16. H.K. Birnbaum, C.A. Wert, Ber. Bunsenges. Phys. Chem. 76, 806 (1972) 17. R. Hempelmann, J. Less Common Metals 101, 69 (1984) 18. J. Völkl, G. Alefeld, in Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.) Academic Press, 1975, p. 232 19. G.V. Kidson, The Diﬀusion of H, D, and T in Solid Metals, Chap. 9 in: Diffusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990, p. 504 20. H. Matzke, V.V. Rondinella, Diﬀusion in Carbides, Nitrides, Hydrides, and Borides, in: Diﬀusion in Semiconductors and Non-metallic Solids, D.L. Beke (Vol.Ed), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, Vol. 33, Subvolume B1, Springer-Verlag, 1999 21. H. Züchner, N. Boes, Ber. Bunsenges. Phys. Chem. 76, 783 (1972) 22. H. Kronmüller, Magnetic After-Eﬀects of Hydrogen Isotopes in Ferromagnetic Metals and Alloys, Ch. 11 in [13] 23. R.B. McLellan, W.A. Oates, Acta Metall. 21, 181 (1973) 24. R.M. Cotts, Ber. Bunsenges. Phys. Chem. 76, 760 (1972) 25. G. Majer, Die Methoden der Kernspinresonanz zum Studium der Diﬀusion von Wasserstoﬀ in Metallen und intermetallischen Verbindungen, Cuvillier Verlag, Göttingen, 2000 26. P. Heitjans, S. Indris, M. Wilkening, Solid-State Diﬀusion and NMR, in: Diﬀusion Fundamentals – Leipzig 2005, J. Kärger, F. Grinberg, P. Heitjans (Eds.), Leipziger Universitätsverlag 2005 27. R. Hempelmann, Quasielastic Neutron Scattering and Solid-State Diﬀusion, Oxford Science Publication, 2000 28. T. Springer, Z. Phys. Chem. NF 115, 317 (1979) 326 18 Diﬀusion of Interstitial Solutes in Metals 29. T. Springer, Diﬀusion Studies of Solids by Quasielastic Neutron Scattering, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Vieweg-Verlag, 1998, p. 59 30. T. Springer, R.E. Lechner, Diﬀusion Studies of Solids by Quasielastic Neutron Scattering, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005 31. H. Zabel, Quasielastic Neutron Scattering: a Powerful Tool for Investigating Diﬀusion in Solids, in: Nontraditional Methods in Diﬀusion, G.E. Murch, H.K. Birnbaum, J.R. Cost (Eds.), The Metallurgical Society of AIME, Warrendale, 1984, p. 1 32. K. Sköld, Quasielastic Neutron Scattering Studies of Metal Hydrides, Ch. 11 in [13] 33. C. Wert, C. Zener, Phys. Rev. 76, 1169 (1949) 34. C. H Vineyard, J. Phys. Chem. Sol. 3 121 (1957) 35. H. Wipf, G. Alefeld, Phys. Stat. Sol. (a) 23, 175 (1974) 36. D. Richter, B. Alefeld, A. Heidemann, N. Wakabayashi, J. Phys. F: Metal Phys. 7, 569 (1977) 37. K. Yamakawa, M. Ege, B. Ludescher, M. Hirscher, H. Kronmüller, J. of Alloys and Compounds 321, 17 (2001) 38. M. Hirscher, H. Kronmüller, J. of the Less-common Metals 172, 658–670 (1991) 19 Diﬀusion in Dilute Substitutional Alloys Diﬀusion in alloys is more complex than self-diﬀusion in pure metals. In this chapter, we consider dilute substitutional binary alloys of metals A and B with the mole fraction of B atoms much smaller than that of A atoms. Then A is denoted as the solvent (or matrix ) and B is denoted as the solute. Diffusion in a dilute alloy has two aspects: solute diﬀusion and solvent diﬀusion. We consider at ﬁrst solute diﬀusion at inﬁnite dilution. This is often called impurity diﬀusion. Impurity diﬀusion implies concentrations of the solute less than 1 %. In practice, the sensitivity for detection of radioactive solutes enables one to study diﬀusion of impurities at very high dilution of less than 1 ppm. In very dilute substitutional alloys solute and solvent diﬀusion can be analysed in terms of vacancy-atom exchange rates. 19.1 Diﬀusion of Impurities Impurity diﬀusion is a topic of diﬀusion research to which much scientiﬁc work has been devoted. We consider at ﬁrst ‘normal’ behaviour of substitutional impurities, which is illustrated for the solvent silver. Similar behaviour is observed for the other noble metals, for hexagonal Zn and Cd, and for Ni. There are exceptions from ‘normal’ impurity diﬀusion. A prominent example is the slow diﬀusion of transition elements in the trivalent solvent aluminium. Another example is the very fast diﬀusion of impurities in socalled ‘open’ metals. Lead is the most famous open metal, for which very fast impurity diﬀusion has been observed. The rapid diﬀusion of Au in Pb was discovered by the diﬀusion pioneer Roberts-Austen in 1896 (see Chap. 1). It is beyond the scope of this book to give a comprehensive overview of impurity diﬀusion. Instead, we refer the reader to the chapter of Le Claire and Neumann in the data collection edited by the present author [1] and to the review by Neumann and Tuijn [2]. 19.1.1 ‘Normal’ Impurity Diﬀusion Figure 19.1 shows an Arrhenius diagram for diﬀusion of many substitutional foreign atoms in a Ag matrix together with self-diﬀusion of Ag. A comparison 328 19 Diﬀusion in Dilute Substitutional Alloys Fig. 19.1. Diﬀusion of substitutional impurities in Ag and self-diﬀusion of Ag (dashed line). Diﬀusion parameters from [1, 2] of impurity diﬀusion and self-diﬀusion coeﬃcients, D2 and D, reveals the following features of ‘normal’ diﬀusion of substitutional impurities: – The diﬀusivities of impurities, D2 , lie in a relatively narrow band around self-diﬀusivities, D, of the solvent atoms. The following limits apply in the temperature range between the melting temperature Tm and about 2/3 Tm : (19.1) 1/100 ≤ D2 /D ≤ 100 . – The pre-exponential factors mostly lie in the interval 0.1 < – D0 (solute) < 10 . D0 (self ) (19.2) The activation enthalpies of impurity and self-diﬀusion, ∆H2 and ∆H, are not much diﬀerent: 0.75 < ∆H2 < 1.25 . ∆H (19.3) 19.1 Diﬀusion of Impurities 329 Substitutional impurities in other fcc metals (Cu, Au, Ni) and in the hcp metals (Zn, Cd) behave similarly as in Ag (for references see the chapter of Le Claire and Neumann in the data collection [1]). Like self-diﬀusion of the solvent, diﬀusion of substitutional impurities occurs via the vacancy mechanism. For impurity diﬀusion in a very dilute alloy it is justiﬁed to assume that solute atoms are isolated, i.e. interaction with other solute atoms (formation of solute pairs, triplets, etc.) is negligible. The theory of vacancy-mediated diﬀusion of substitutional impurities takes into account three aspects: 1. The formation of solute-vacancy pairs: we remind the reader of the Lomer equation introduced in Chap. 5, which shows that the probability of a vacancy occupying a nearest-neighbour site of a substitutional impurity is given by B F G S1V − S B HF − HB eq exp p = C1V exp − 1V = exp (19.4) kB T kB kB T where GB = H B − T S B is the Gibbs free energy of solute-vacancy intereq the atomic fraction of vacancies in the pure matrix in thermal action, C1V F F equilibrium. H1V and S1V denote the formation enthalpy and entropy of a monovacancy. For GB > 0 the interaction is attractive, for GB < 0 it is repulsive. 2. In contrast to the case of self-diﬀusion in the pure matrix, for impurity diﬀusion it is necessary to consider several atom-vacancy exchange rates. Five types of exchanges, between vacancy, impurity and host atoms have been introduced in Lidiards ‘ﬁve-frequency model’ (see Chap. 7). 3. The impurity correlation factor is then no longer a constant depending on the lattice geometry as in the case of self-diﬀusion. It depends on the various jump rates of the vacancy (see Chap. 7). From the atomistic description developed in Chap. 8, we get for the impurity diﬀusion coeﬃcient of vacancy-mediated diﬀusion in cubic Bravais lattices B G eq 2 2 , (19.5) D2 = f2 a ω2 p = f2 a ω2 C1V exp kB T where a is the lattice parameter, f2 the impurity correlation factor, and ω2 the vacancy-impurity exchange rate. To be speciﬁc, we consider in the following fcc solvents. As discussed in Chap. 7, within the framework of the ‘ﬁve-frequency model’ the correlation factor can be written as [3] f2 = ω1 + (7/2)F3 ω3 . ω2 + ω1 + (7/2)F3 ω3 (19.6) The various jumps rates in an fcc lattice are illustrated in Fig. 7.4. For convenience we remind the reader of their meaning: ω1 is the rotation rate of 330 19 Diﬀusion in Dilute Substitutional Alloys the solute-vacancy complex, ω3 and ω4 denote rates of its dissociation or association. The escape probability F3 is a function of the ratio ω/ω4 , where ω denotes the vacancy jump rate in the pure matrix. It is also useful to remember that in detailed thermal equilibrium according to B G ω4 = exp (19.7) ω3 kB T the dissociation and association rates are related to the Gibbs free energy of binding of the vacancy-impurity complex, GB = H B − T S B . Equation (19.5) can then be recast to give F F S1V − S B + S2M − H B + H2M H1V 2 0 D2 = f2 a ν exp exp − , (19.8) kB kB T where H B and S B denote the binding enthalpy and entropy of the vacancyimpurity complex and H2M and S2M the enthalpy and entropy of the vacancyimpurity exchange jump ω2 . Thus, the activation enthalpy of impurity diﬀusion is given by F − H B + H2M + C , (19.9) ∆H2 = H1V where C = −kB ∂ ln f2 . ∂(1/T ) (19.10) This term describes the temperature dependence of the impurity correlation factor1 . It is evident from Eqs. (19.5), (19.7), and Chap. 17 that the ratio of the diﬀusion coeﬃcients of impurity and self-diﬀusion can be written as f2 ω2 ω4 D2 = . D f ω ω3 (19.11) This expression shows that the diﬀusion coeﬃcient of a substitutional impurity diﬀers from the self-diﬀusion coeﬃcient of the pure solvent for three reasons, namely: (i) correlation eﬀects, because f2 = f , (ii) diﬀerences in the atom-vacancy exchange rates between impurity and solvent atoms, because ω2 = ω, and (iii) interaction between impurity and vacancy, because ω4 /ω3 = 1 or GB = 0. Since solute and solvent atoms are located on the same lattice and since the diﬀusion of both is mediated by vacancies, the rather small diﬀusivity dispersion (see Fig. 19.1) is not too surprising. It reﬂects the high eﬃciency of screening of point charges in some metals, which normally limits the vacancyimpurity interaction enthalpy H B to values between 0.1 and 0.3 eV. Such values are small relative to the vacancy formation enthalpies (see Chap. 5). Using 1 Sometimes in the literature C is deﬁned with the opposite sign. 19.1 Diﬀusion of Impurities 331 F M ∆H = H1V + H1V , we get for the diﬀerence of the activation enthalpies between impurity and self-diﬀusion M ∆Q ≡ ∆H2 − ∆H = −H B + (H2M − H1V )+C. (19.12) A useful theoretical approach is the so-called electrostatic model, which associates ∆Q with the valence diﬀerence between solute and solvent. Relatively positive impurities, generally those of higher nominal valence than the solvent, tend to attract vacancies and, hence, to diﬀuse more rapidly and with lower activation enthalpies than self-diﬀusion. In the electrostatic model of Lazarus [4] reﬁned by Le Claire [5], it is assumed that the excess charge ∆Ze (e = electron charge) is responsible for ∆Q. Vacancy and impurity are considered to behave as point charges −Ze and Z2 e, respectively. In the Thomas-Fermi approximation, the excess charge of the impurity gives rise to a perturbing potential V (r) = α ∆Ze exp(−qr) . r (19.13) This equation describes a screened Coulomb potential with a screening radius 1/q, which is independent of ∆Z and can be calculated from the Fermi energy of the host. α is a dimensionless screening parameter, which depends on ∆Z [5]. In the electrostatic model, the interaction enthalpy H B is equal to the electrostatic energy V (d) of the vacancy located at a nearest-neighbour distance, d, of the impurity. For the calculation of the diﬀerences in the migration enthalpies in the second and third term of Eq. (19.12), Le Claire describes the saddle-point conﬁguration by two ‘half-vacancies’ located on two neighbouring sites. Each half-vacancy carries a charge Ze/2 at a distance 11 16 d [5]. In a number of solvents, the quantity ∆Q varies indeed monotonically with the valence diﬀerence ∆Z = Z2 − Z (Z2 = valence of impurity, Z= valence of solvent). Impurities with Z2 > Z (Z2 < Z) diﬀuse faster (slower) than self-diﬀusion, the pertaining activation enthalpies fulﬁll ∆Q < 0 (∆Q > 0), and the impurity diﬀusion coeﬃcients increase with ∆Z. This behaviour is observed for the following solvents: noble metals and group-IIB hexagonal metals Zn and Cd (for references see [1]). Calculations of ∆Q based on the electrostatic model yield good agreement with experiments for impurity diffusion in these metals. For transition metal solutes in noble metals and for other solvents such as the alkali metals, the divalent magnesium, and the trivalent aluminium the values of ∆Q calculated on the basis of a screened Coulomb potential are at variance with the experimentel values [5, 6]. There are several reasons for the failure of the electrostatic model: (i) The choice of a screened Coulomb potential may not be appropriate for certain solute-solvent combinations. A self-consistent potential has an oscillatory form with so-called Friedel oscillations. The vacancy-solute 332 19 Diﬀusion in Dilute Substitutional Alloys interaction can then, for example, be attractive at the nearest neighbour positions but repulsive at the saddle-point position. (ii) A model based only on the diﬀerence in valence between solute and solvent atoms disregards the eﬀects of atomic size. (iii) Finally, the electrostatic model can only predict ∆Q. It says nothing about pre-exponential factors. Various attempts have been made in the literature to improve the theory of impurity diﬀusion. For details the reader may consult older textbooks [6, 8] and the review of Neumann and Tuijn [2]. 19.1.2 Impurity Diﬀusion in Al Aluminum like the noble metals has also an fcc structure. In contrast to the monovalent noble metals, Al is trivalent. The diﬀusion of impurities in Al is remarkably diﬀerent from that of impurities in noble metals. Figure 19.2 shows an Arrhenius diagram of impurity diﬀusion in Al together with Al self-diﬀusion. A striking feature of this ﬁgure is that most transition metals have extremely low diﬀusivities with respect to Al self-diﬀusion. In addition, they have high activation enthalpies, which are at variance with the simple form of the electrostatic model mentioned above. They also have very high pre-exponential factors, which violate the limits of Eq. (19.2). Non-transition elements have diﬀusivities similar or slightly higher than self-diﬀusion and show only small diﬀusivity dispersion. Their activation enthalpies are similar to those of Al self-diﬀusion, almost independent of their valence. The pressure dependence for diﬀusion of several impurities in aluminium has been studied by Rummel et al. [10] and Thürer et al. [11] (see also Chap. 8). The activation volumes of non-transition element diﬀusers (Zn, Ge) are close to one atomic volume (Ω) and not much diﬀerent from the activation volume of self-diﬀusion reported by Beyeler and Adda [12]. However, the transition elements (Co, Mn) are diﬀusers with high activation volumes between 2.7 and 1.67 Ω. These ﬁndings have been attributed to diﬀerences in vacancy-impurity interaction between transition and non-transition elements [10]. The large ∆H2 values of transition element solutes according to Eq. (19.9) indicate a strong repulsion between solute and vacancy (H B < 0) and/or a large activation enthalpy H2M for solute-vacancy exchange jumps. Ab initio calculations, based on the local density functional theory, of the solutevacancy interaction energy for 3d and 4sp and for 4d and 5sp solutes in aluminium have been performed by Hoshino et al. [13]. They have demonstrated that for 3d and 4d impurities this interaction is indeed strongly repulsive, whereas for 4sp and 5sp impurities it is weakly attractive. Unfortunately, according to the author’s knowledge ab initio calculations of H2M and of the activation volumes are not available. 19.2 Impurity Diﬀusion in ‘Open’ Metals – Dissociative Mechanism 333 Fig. 19.2. Diﬀusion of several impurities in Al and self-diﬀusion of Al (dashed line) according to [1, 9] 19.2 Impurity Diﬀusion in ‘Open’ Metals – Dissociative Mechanism The fast diﬀusion of gold in lead was already reported by Roberts-Austen [14], one of the pioneers of solid-state diﬀusion (see Chap. 1). After the measurements of self- and impurity diﬀusion in lead by von Hevesy and his coworkers [15, 16], the extreme rapidity of gold diﬀusion was appreciated. Since this pioneerig work the interest in the Au/Pb and analogous systems continues to the present day. Lead is still the most extensively studied metallic solvent where fast impurity diﬀusion plays an important role. Figure 19.3 shows an Arrhenius diagram of impurities in Pb together with self-diﬀusion (for references see the chapter of Le Claire and Neumann in [1] and the review of Neumann and Tuijn [2]). Some solutes (e.g., Tl, Sn) show ‘normal’ behaviour. However, noble metals, Ni-group elements, and Zn have diﬀusivities which are three or more orders of magnitude faster than self-diﬀusion. Fast diﬀusion of 3d transition metals is also observed in some other polyvalent metals (In, Sn, Sb, Ti, Zr, Hf), and for noble metal diﬀusion 334 19 Diﬀusion in Dilute Substitutional Alloys Fig. 19.3. Diﬀusion of impurities in Pb and self-diﬀusion of Pb (dashed line) according to [1, 2] in Na. Figure 19.4 shows diﬀusion of several impurities in Na according to Barr and associates [18–20]. Noble metal solutes are fast diﬀusers in the group-IVB metal Sn and in the group-IIIB metals In and Tl. Late transition elements in group-IVA metals (α-Ti, α-Zr, and α-Hf) are fast diﬀusers as well. Solvents that permit fast diﬀusion are sometimes denoted as ‘open’ metals [17]. ‘Open’ refers to the large ratio of atomic radii of solvent and solute. This solvent property appears to entail fast diﬀusion for solutes with relatively small radii. Fast solute diﬀusion in open metals is thought to be exceptional, because the diﬀusivities lie far above the range expected for the vacancy mechanism. On the other hand, the still relatively large atom size ratio (e.g., RAu /RP b ≈ 0.83) would seem to preclude large interstitial occupancies. Fast diﬀusion of solutes that are mainly dissolved on substitutional sites has been attributed to the dissociative mechanism (see, e.g., Warburton and Turnbull [21]). This mechanism operates for solutes which have a certain (small) interstitial component with a high mobility in the solvent metal (see Chap. 6). Such solutes are called hybrid solutes. As represented by equation 19.2 Impurity Diﬀusion in ‘Open’ Metals – Dissociative Mechanism 335 Fig. 19.4. Diﬀusion of impurities in Na and self-diﬀusion of Na according to Barr and associates [18–20] Bi + V Bs (19.14) B solutes are distributed over both interstitial (Bi ) and substitutional (Bs ) sites. Provided that local equilibrium in Eq. (19.14) is established, the concentrations fulﬁll the law of mass action C eq C eq Ci CV = K(T ) = i eqV Cs Cs (19.15) where Ci , Cs , and CV denote the molar fractions of interstitial solute, substitutional solute, and vacancies, respectively. K(T ) is a constant which depends on temperature. The superscript eq indicates thermal equilibrium. A metal with a normal content of dislocations has a suﬃcient abundance of vacancy sources or sinks to keep vacancies in equilibrium. The eﬀective diﬀusivity of a solute is then given by Def f = Di Cieq DV CVeq + , Cieq + Cseq Cieq + Cseq (19.16) where Di denotes the diﬀusivity of the solute in its interstitial state and DV the diﬀusivity of the vacancy-solute complex. Substitutional transport by vacancies is negligible if Cieq Di DV CVeq is fulﬁlled. Then, the eﬀective diﬀusivity of solutes is given by [21, 22] Def f ≈ Di Cieq Cieq + Cseq (19.17) 336 19 Diﬀusion in Dilute Substitutional Alloys For solutes with dominating interstitial solubility, i.e. for Cieq Cseq , the eﬀective diﬀusivity approaches the diﬀusivity of the solute in its interstitial state: (19.18) Def f ≈ Di . This corresponds to the direct interstitial mechanism, which is relevant for the interstitial diﬀusers C, N and O (see Sect. 18.1). For solutes with dominating substitutional solubility, i.e. for Cseq Cieq , the eﬀective diﬀusivity Def f ≈ contains the factor Cieq = exp Cseq Di Cieq Cseq −Gi kB T (19.19) . (19.20) Here Gi denotes the Gibbs free energy of forming an interstitial solute from a substitutional one. The rather wide diﬀusivity dispersion of fast solute diﬀusers can be largely attributed to this factor. The phenomenon of fast diﬀusion is also well-known for hybrid solutes in the semiconducting elements Si and Ge (see, e.g., [23, 24]) and is discussed in detail in Chap. 25. It has been attributed to interstitial-substitutional exchange mechanisms, which occur in two basic versions (see Chaps. 6 and 25). The dissociative mechanism was suggested in 1956 by Frank and Turnbull for Cu in Ge [25]. The kick-out mechanism, which involves selfinterstitials, was originally proposed by Gösele, Frank and Seeger for Au diﬀusion in Si [26]. In the meantime, further fast diﬀusing foreign elements in Si (e.g., Pt, Zn) were identiﬁed as kick-out diﬀusers [22, 28]. From a chemical viewpoint the elemental semiconductors Si and Ge are group-IV elements such as the ‘open’ metals Pb and Sn. Actually, the concepts growing out of studies of fast diﬀusion in semiconductors (see part IV of this book) have inﬂuenced the interpretation of fast diﬀusion in metals. 19.3 Solute Diﬀusion and Solvent Diﬀusion in Alloys Alloying one element with another can signiﬁcantly aﬀect diﬀusion. In a homogeneous binary A-B alloy a tracer self-diﬀusion coeﬃcient for A atoms, ∗ ∗ , and another one for B atoms, DB , can be measured. In this section, we DA discuss the variation of solute and solvent diﬀusion with the solute concentration. The major eﬀects of alloying on diﬀusion are to introduce vacancy-solute and solute-solute interactions and to change the vacancy jump rates. Let us consider, for example, the inﬂuence of solute atoms on solvent diﬀusion: in a very dilute alloy most of the solvent atoms are not near a solute atom; the mobility of such solvent atoms agrees with that of atoms in the pure solvent. Depending on the interaction energy, a solute attracts or repels vacancies and the jump rates of the solvent atoms in the vicinity of the 19.3 Solute Diﬀusion and Solvent Diﬀusion in Alloys 337 solute atom are altered. This inﬂuences the solvent diﬀusion coeﬃcient. As the solute concentration increases, the number of aﬀected solvent atoms increases. Depending on the energy landscape experienced by the vacancy in the vicinity of the solute, certain solutes accelerate solvent diﬀusion and others slow it down. In dilute alloys containing small atomic fractions XB of the solute B the self-diﬀusion coeﬃcient of the solvent can be written as ∗ ∗ (XB ) = DA (0) exp (bXB ) , DA (19.21) which for XB < 1 % can be approximated by ∗ ∗ DA (XB ) = DA (0)[1 + b1 XB + . . . ] . (19.22) The term b1 XB accounts for the change in the jump rates of those solvent atoms neighbouring solute atoms. Quadratic terms in XB correspond to the eﬀect of pairs of B atoms. b1 is sometimes denoted as the linear enhancement factor. An analogous expression holds for the solute diﬀusion coeﬃcient: ∗ ∗ DB (XB ) = DB (0)[1 + B1 XB + . . . ] . (19.23) ∗ DB (0) is the solute diﬀusion coeﬃcient for inﬁnite dilution, i.e. the impurity diﬀusion coeﬃcient discussed in the previous section. The term B1 expresses the inﬂuence of solute-solute pairs. The linear enhancement factor of solvent diﬀusion, b1 , has attracted particular interest. It is related to the various jump rates in the neighbourhood of the solute. Using the ﬁve-frequency model for fcc solvents, Lidiard [30] and Howard and Manning [31] have deduced the following expression ω 4 χ1 ω 1 χ2 + 14 b1 = −18 + 4 ω f ω3 f χ2 ω 3 GB χ1 ω 1 + 14 exp . (19.24) = −18 + 4 f ω f ω kb T Here f is the tracer correlation factor of self-diﬀusion in the pure solvent (only ω-jumps). The quantities χ1 and χ2 are partial correlation factors tabulated in [31]. Equation (19.24) is based on the assumption that the jump rates are independent of the solute concentration. It shows that an increase of solvent diﬀusivity can arise from an increase of the vacancy concentration due to vacancy-solute interaction and/or from an increase in the solvent jump frequencies near the solute (e.g., for ω1 > ω). Using Eqs. (19.5), (19.6), and (19.24), b1 can be expressed as a function ∗ ∗ of the ratio DB (0)/DA (0): b1 = −18 + 4 ∗ (0) f 4χ1 (ω1 /ω3 ) + 14χ2 DB . ∗ (0) 1 − f DA 2 f (4ω1 /ω + 14F3 ) (19.25) 338 19 Diﬀusion in Dilute Substitutional Alloys Fig. 19.5. Tracer diﬀusion of 113 Sn and 195 Au in dilute Au-Sn solid-solution alloys according to Herzig and Heumann [29] ∗ ∗ This expression shows that faster diﬀusing solutes (DB > DA ) have the tendency to increase the solvent diﬀusivity. This eﬀect is mainly due to an increase of the vacancy content. The last quotient in Eq. (19.25) has usually ∗ ∗ /DA around a value not much diﬀernet from unity. Thus, with values of DB 10 and f2 ≈ 0.5, b1 lies between 0 and 100. For slow diﬀusing solutes, b1 tends to be negative but never less than −18. We illustrate the inﬂuence of solute concentration on solvent and solute diﬀusion in a dilute fcc solid solution by an experimental example. The diffusion of the radiotracers 113 Sn and 195 Au in pure Au and in a dilute Au-Sn alloy is displayed for various temperatures and Sn concentrations in Fig. 19.5. In pure Au, the Sn solute is about one order of magnitude faster than Au self-diﬀusion. Au-diﬀusion in the alloy is enhanced by the presence of Sn additions [29]. The corresponding enhancement factors are listed in Fig. 19.5. As is the case in this ﬁgure, the experimental values of solvent and solute enhancement factors have often the same sign. We refrain from discussing further details and refer the reader to the textbooks of Philibert [6] and Heumann [8] and a more recent paper by Belova and Murch [32] and the references therein. . References 1. A.D. Le Claire, G. Neumann, Diﬀusion of Impurities in Solid Metallic Elements, Chap. 3 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), References 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 339 Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series Vol. III/26, Springer-Verlag, (1990) G. Neumann, C. Tuijn, Impurity Diﬀusion in Metals, Scitec Publications Ltd., Uetikon-Zürich, Switzerland, 2002 J.R. Manning, Diﬀusion Kinetics for Atoms in Crystals, van Nostrand Comp., Princeton, 1968 D. Lazarus, Phys. Rev. 93, 973 (1954) A.D. Le Claire, Philos. Mag. 7, 141 (1962) J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 R.M. Cotts, Ber. Bunsenges. Phys. Chem. 76, 760 (1972) Th. Heumann, Diﬀusion in Metallen, Springer-Verlag, Berlin, 1992 G. Rummel, Th. Zumkley, M. Eggersmann, K. Freitag, H. Mehrer, Z. Metallkd. 86, 121 (1995) G. Rummel, Th. Zumkley, M. Eggersmann, K. Freitag, H. Mehrer, Z. Metallkd. 86, 131 (1995) A. Thürer, G. Rummel, Th. Zumkley, K. Freitag, H. Mehrer, Phys. Stat. Sol. (a) 143, 535 (1995) M. Beyeler, Y. Adda, J. Phys. (Paris) 29, 345 (1968) T. Hoshino, R. Zeller, P.H. Dederichs, Phys. Rev. B 53, 8971 (1996) W.C. Roberts-Austen, Phil. Trans. Roy. Soc. 187, 383 (1896) J. Groh, G. von Hevesy, Ann. Physik 63, 85–92 (1920) J. Groh, G. von Hevesy, Ann. Physik 65, 216 (1921) G.M. Hood, Defect and Diﬀusion Forum 95–98, 755 (1993) L.W. Barr, J.N. Mundy, F.A. Smith, Philos. Mag. 13, 1299 (1966) L.W. Barr, J.N. Mundy, F.A. Smith, Philos. Mag. 20, 390 (1969) L.W. Barr, F.A. Smith, in: DIMETA-62, Diﬀusion in Metals and Alloys, F.J. Kedves, D.L. Beke (Eds.), Trans Tech Publications, Switzerland, 1983, p. 365 W.K. Warburton, D. Turnbull, in: Diﬀusion in Solids – Recent Developments, A.S. Nowick, J.J. Burton (Eds.), Academic Press, 1975, p. 171 W. Frank, U. Gösele, H. Mehrer, A. Seeger, Diﬀusion in Silicon and Germanium, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, 1984, p. 63 A. Seeger, K.P. Chik, Phys. Stat. Sol. 29, 455 (1968) N.A. Stolwijk, H. Bracht, in: Diﬀusion in Semiconductors and Non-Metallic Solids, D.L. Beke (Vol.-Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Condensed Matter, Vol. 33, Springer-Verlag, 1998, p. 2–1 F.C. Frank, D. Turnbull, Phys. Rev. 104, 617 (1956) U. Gösele, W. Frank, A. Seeger, Appl. Phys. A 23, 361 (1980) N.A. Stolwijk, G. Bösker, J. Pöpping, Defect and Diﬀusion Forum 194–199, 687 (2001) H. Bracht, N.A. Stolwijk, H. Mehrer, Phys. Rev. B. 52, 16542 (1995) Chr. Herzig, Th. Heumann, Z. für Naturforschung 27a, 1109 (1972) A.B. Lidiard, Philos. Mag. 5, 1171 (1960) R.E. Howard, J.R. Manning, Phys. Rev. 154, 5612 (1967) I.V. Belova, G.E. Murch, Philos. Mag. 33, 377 (2003) 20 Diﬀusion in Binary Intermetallics 20.1 General Remarks Intermetallics are compounds of metals or of metals and semimetals. The crystal structures of intermertallics are diﬀerent from those of their constituents. This deﬁnition includes intermetallic phases and ordered alloys. Intermetallics have a wide spectrum of properties ranging between metallic and non-metallic. Some intermetallics are interesting functional materials others have attracted attention as structural materials for high-temperature applications. For an introduction to the ﬁeld see, e.g., the books of Westbrook and Fleischer [1] and of Sauthoff [2]. Intermetallic-based materials have been used for a long time, based essentially on their chemical properties, on their high hardness and wear resistance. Examples are some dental alloys, amalgams, jewelry, and coatings. There are a large number of engineering alloys that ﬁnd applications because of some special physical or chemical properties – for example, magnetic behaviour, superconductivity, or chemical stability in corroding atmospheres. The last few decades have seen tremendous world-wide eﬀorts in intermetallics, which largely focused on aluminides with some smaller eﬀorts on silicides. The prime goals are high-temperature or power-generation applications, such as aeroengines, high-temperature edges on aircraft wings and rocket ﬁns, automobile engine valves, turbochargers and so on. Important properties in all these applications are the ability to withstand high temperature and aggressive oxidising or corrosive environments, as well as other properties such as low weight or inertia. This has triggered important materials developments and a ﬂood of conferences. It is impossible to make reference to more than a few of the books and review papers that cover this eﬀort. An atomistic understanding of diﬀusion in intermetallics in terms of defect structure and diﬀusion mechanisms is more complex than for metallic elements. An inspection of a collection of phase diagrams [3] shows the following: intermetallics crystallise in a variety of structures with ordered atom distributions. Examples are the B2, D03 , L12 , L10 , D019 , B20, C11b , and Laves-phase structures. Some intermetallics are ordered up to the melting temperature, others undergo order-disorder transitions because entropy favours a less ordered or even a random arrangement of atoms at high temperatures. We know intermetallic phases with wide phase ﬁelds and others which exist as 342 20 Diﬀusion in Binary Intermetallics line compounds. Some intermetallics occur for certain stoichiometric compositions, others are observed for oﬀ-stoichiometric compositions only. Some phases compensate oﬀ-stoichiometry by vacancies, others by antisite atoms. Some phases display small, others large diﬀerences between the diﬀusivities of the components. Some non-cubic intermetallics are highly anisotropic in their diﬀusion behaviour. Let us ﬁrst illustrate structures of some of the more common intermetallics (see Figs. 20.1 and 20.2): The B2 (or CsCl) structure is cubic with the approximate composition AB. The B2 structure can be derived from the bcc lattice, if the two primitive cubic sublattices are occupied by diﬀerent kinds of atoms. Examples are FeAl, CoAl, NiAl, CoGa, PdIn, CuZn, AuZn, AuCd, and in an intermediate temperature range NiMn. The D03 (or Fe3 Si) structure is cubic with the approximate composition A3 B. The D03 structure can be considered also as an ordered structure derived from the bcc lattice. In Fig. 20.1, A atoms occupy white and grey sites, B atoms occupy black sites. D03 order is observed, for example, in Fe3 Si Fig. 20.1. Ideally ordered structures of some cubic intermetallics: B2 (left), D03 (middle), L12 (right) Fig. 20.2. Ideally ordered structures of titanium aluminides: L10 (left), D019 (right) 20.1 General Remarks 343 over a wide temperature range, in Fe3 Al below about 825 K, and in Cu3 Sn, Cu3 Sb, and Ni3 Sb at high temperatures. The L12 (or Cu3 Au) structure is cubic with the approximate composition A3 B. The L12 structure is an ordered structure derived from the fcc lattice. In Fig. 20.1, A atoms occupy white sites, B atoms occupy black sites. Examples are the Ni-based compounds Ni3 Al, Ni3 Ga, and Ni3 Ge. The prototype Cu3 Au shows L12 order only at low temperatures; above 660 K it is disordered fcc. The L10 (or CuAu) structure is tetragonal with the approximate composition AB. The L10 structure can be considered as an ordered fcc structure with A and B atoms occupying sequential (001)-planes. The structure has a slight tetragonal distortion in the 001 -direction. An example of technologically interest for structural applications is β-TiAl. Other L10 systems such as NiPt, FePt, CoPt, FePd and NiMn are studied because they are candidtaes for high-density magnetic storage media due to their high magnetic anisotropy related to their tetragonal anisotropy. The D019 structure is hexagonal with the approximate composition A3 B. It can be considered as an ordered structure derived from the hcp lattice. In Fig. 20.2, the majority atoms occupy white sites, B atoms occupy black sites. Ti3 Al crystallises in this structure. The diﬀusion behaviour of intermetallics is of interest for the production of these materials and for their practical use, especially when high-temperature applications are intended. Whereas self- and solute diﬀusion in pure metals is thoroughly investigated and reasonably well understood, systematic diﬀusion studies for intermetallics are still relatively scarce, although considerable progress has been achieved [4–13]. Just as in metallic elements, self-diﬀusion is the most basic diﬀusion process in alloys and compounds as well. Studies of self-diﬀusion utilise such tiny amounts of tracer atoms (see Sect. 13.3) of the diﬀusing species. Then, in practice the chemical composition of the sample does not change due to diﬀusion. In a binary system, two tracer self-diﬀusion coeﬃcients – one for A atoms and another one for B atoms – can be determined. Such complete studies have been performed only for a limited number of binary intermetallics. Table 20.1 compiles binary intermetallics with B2, D03 , L12 , L10 , D019 , C15, and C11b structures for which self-diﬀusion data are available. In some cases self-diﬀusion of both components has indeed been studied. For the aluminides of Ni, Fe, and Ti impurity diﬀusion of some solutes has been studied, since for Al no suitable tracer is available. The intention was to mimic self-diﬀusion. Similarly, for Fe3 Si a radioisotope of Ge was used to simulate Si diﬀusion, since Si has only a very short-lived isotope with a 2.6 hours half-life. The validity of this approach has been conﬁrmed by diﬀusion studies with an enriched stable Si isotope and SIMS proﬁling. For the C11b structured MoSi2 diﬀusion of the short-lived 31 Si isotope and of the chemically related 71 Ge as well as diﬀusion of 99 Mo has been investigated. 344 20 Diﬀusion in Binary Intermetallics Table 20.1. Self-diﬀusion in several intermetallics. For the underlined elements data of tracer self-diﬀusion and of substitutional substitutes (in brackets) are available. The latter data provide ‘good estimates’ for self-diﬀusion of the Al and Si components. For references see, e.g., [7, 8, 11] and this chapter Structure Intermetallic B2 CuZn, AuCd, AuZn, CoGa, PdIn, FeCo, NiAl(Ga), FeAl(Zn,In), AgMg, NiGa, NiMn Ni3 Al, Ni3 Ge, Ni3 Ga, Co3 Ti, Pt3 Mn, Cu3 Au (disordered) Fe3 Si(Ge), Cu3 Sn, Cu3 Sb, Ni3 Sb, Fe3 Al TiAl(Ga, Ge), FePt Ti3 Al(Ga,In,Ge) Co2 Nb (cubic Laves phase) MoSi2 (Ge), both principal tetragonal directions L12 D03 L10 D019 C15 C11b 20.2 Inﬂuence of Order-Disorder Transitions Order-disorder alloys are characterised by an ordered arrangement of atoms at low temperatures, which becomes progressively disordered as the temperature is raised until the long-range order disappears at a critical temperature. Ordering implies the arrangement of atoms on distinct sublattices of an intermetallic. Disordering occurs by an exchange of atoms, i.e. by the creation of antisite atoms. The proportion of antisite atoms rises rapidly as temperature approaches the critical temperature, where the distinction between the sublattices disappears. Ordering transitions are accompanied by anomalies in many physical properties including diﬀusion. An order-disorder transition occurs, for example, between the β- and β -brass phases of the Cu-Zn system. Below the order-disorder transition (at about 741 K) CuZn shows B2 order (β -brass). At high temperatures the disordered A2 structure (β-brass) is formed. The pioneering but still valid work of Kuper et al. [17] on self-diﬀusion of 64 Cu and 65 Zn in CuZn is displayed in Fig. 20.3. The inﬂuence of the order-disorder transition on the diﬀusion behaviour of both components is visible as a change in slope of the Arrhenius plot. The activation enthalpies of both components obey the inequality (20.1) ∆HB2 > ∆HA2 . Figure 20.3 also shows that occurrence of order impedes the diﬀusion of both components in a similar way. The Fe-Co system undergoes an order-disorder transition from a disordered A2 high-temperature phase to an ordered B2 phase at lower temperatures. At the equiatomic composition the transformation temperature is 1003 K. Similar eﬀects of the B2-A2 transition as in the CuZn system were observed for diﬀusion of Fe and Co in FeCo by Fishman et al.[18, 19]. The 1 measurements of Fishman et al. and at diﬀusivities of about 10−19 m2 s . 20.2 Inﬂuence of Order-Disorder Transitions 345 Fig. 20.3. Self-diﬀusion of 64 Cu and 65 Zn in CuZn according to Kuper et al. [17] Diﬀusion studies have been extended by Iijima and coworkers [20, 21] down to 2 × 10−21 m2 s−1 . The ratio DF e /DCo exeeds unity by not more than 20 % above about 940 K corresponding to diﬀusivities around 10−20 m2 s−1 . This ratio becomes slightly smaller than unity in the B2 phase. The diﬀusion of Fe in Fe3 Al has been studied over a wide temperature range by Tökei et al. [24] and by Eggersmann and Mehrer [23]. Fe3 Al undergoes two ordering transitions at about 825 K from D03 order to B2 order and to the disordered A2 structure near 1000 K. At the critical temperatures the slope of the Arrhenius diagram changes slightly and the activation enthalpies obey the following sequence ∆HD03 > ∆HB2 > ∆HA2 . (20.2) The activation enthalpy is highest for the structure with the highest degree of order and lowest for the disordered structure. The eﬀect of ordering transitions is, however, less pronounced in Fe3 Al than in CuZn. 346 20 Diﬀusion in Binary Intermetallics 20.3 B2 Intermetallics Intermetallics with B2 structure form one of the largest group of intermetallics with a broad variation of chemical, physical, and mechanical properties. The classical B2 phase is CuZn (β-brass). It is a prototype of B2 phases consisting of noble metals and group-II metals. The B2 phase NiAl has attracted much interest for its potential in high-temperature applications. The B2 aluminides of Fe and Co are closely related to NiAl since Ni, Fe, and Co can substitute for each other in the B2 structure. The B2 structure is also adopted by compounds of group-VIII and group-IV transition metals. Much of the diﬀusion work on intermetallics concerns B2 phases (see Table 20.1). Figure 20.3 reveals a fairly general feature of self-diﬀusion in B2 intermetallics. We recognise that Zn in β-brass diﬀuses only slightly faster than Cu and that the ratio DZn /DCu never exceeds 2.3 [17]. For equiatomic FeCo, the ratio DF e /DCo is always close to unity [18–21]. This type of ‘cou- Fig. 20.4. Self-diﬀusion in B2 structure intermetallics from [7]. The diﬀusing species is underlined 20.3 B2 Intermetallics 347 pling’ between the diﬀusivities of the components seems to be typical for B2 phases. It can be observed in Fig. 20.4 for practically all B2 compounds, for which both constituents have been investigated. In some cases (e.g., NiGa, CoGa) the bounds for the diﬀusivity ratio are somewhat wider than in the cases of CuZn and FeCo. However, in any case the diﬀerence between the diﬀusivities is less than one order of magnitude. This ‘coupling’ between the diﬀusivities of the components indicates that diﬀusion of both atomic species is mediated by the same defect(s). 20.3.1 Diﬀusion Mechanisms in B2 Phases It is generally recognised that diﬀusion in B2 phases is mediated by vacancytype defects. An intriguing question is, how do these defects move in a structure with long-range order? The B2 structure consists of two primitive cubic sublattices (see Fig. 20.1). In the completely ordered state of a stoichiometric B2 compound, A atoms occupy one sublattice and B atoms the other. This implies that each A atom is surrounded by 8 B atoms on nearest-neighbour sites and vice versa. If A and B atoms are distributed at random, a bodycentered cubic (bcc) structure (A2 structure) is obtained. When atomic diffusion in a B2 compound would take place by random interchanges between vacancy-type defects and atoms of both sublattices, migrating defects would leave trails of antisite defects (AB and BA ) behind and ﬁnally cause complete disordering of the compound. Vacancy-type defects should, therefore, move in a highly correlated way to preserve the equilibrium degree of long-range order. In order to maintain order, disordered regions must either be avoided or compensated during the diﬀusion process. If the ordering energy is very high, sublattice diﬀusion of each component via second nearest-neighbour jumps is conceivable. Diﬀusion of the components in ionic crystals and in simple oxides occurs by sublattice diﬀusion (see Chap. 26 and [14]). However, sublattice diﬀusion cannot be the dominating mechanism in B2 intermetallics since separate diﬀusion on each sublattice diﬀusion hardly would entail similar diﬀusivities of the components. Ingenious order-retaining mechanisms, for which diﬀusion of both components is coupled, have been proposed for B2 intermetallics: – Six-jump-cycle (6JC) mechanism: This mechanism is an order-retaining vacancy mechanism, which was originally proposed by Elcock and McCombie [25, 26] and advocated later by Huntington [27] and others [28, 31]. A vacancy trajectory of 6 consecutive nearest-neighbour jumps displaces atoms in such a way that after the cycle is completed the order is re-established. Several possibilities for six-jump-vacancy-cycles are illustrated in Fig. 20.5. Because of the participation of both species in the 6JC with a ﬁxed ratio of the number of jumps the diﬀusivities of both components cannot be very diﬀerent. In a highly ordered state, the ratio of the diﬀusivities of 348 20 Diﬀusion in Binary Intermetallics Fig. 20.5. Schematic illustration of six-jump vacancy cycles in the B2 structure. The arrows show vacancy jumps; the numbers indicate the jump sequence both components, DA /DB , lies within the following fairly narrow limits: 1 DA < < q. (20.3) q DB – q was ﬁrst estimated to be 2 [29, 5] and by including correlation eﬀects was later slightly corrected to q = 2.034 [30]. The upper (lower) limit is attained when vacancies are preferentially formed on the B (A) sublattice As the chemical composition deviates from the stoichiometric one and as disorder increases at high temperatures, antisite atoms appear. As shown by Belova and Murch [32], interaction of the six-jump-cycles with antisite atoms remarkable widens the limits of Eq. (20.3). Thus, in a B2 alloy with some disorder values of DA /DB beyond the limits of Eq. (20.3) cannot be considered as an indication that the 6JC mechanism does not operate. Triple-defect mechanism: In a B2 compound triple-defect disorder can occur according to the reaction VA + VB 2VA + AB . (20.4) VA (VB ) denotes a vacancy on the A (B) sublattice and AB an A atom on the B sublattice (see also Chap. 5). Triple-defect disorder does not change the composition. Instead of forming equal numbers of vacancies 20.3 B2 Intermetallics 349 Fig. 20.6. Illustration of the triple-defect diﬀusion mechanism in the B2 structure. The arrows show vacancy jumps; the numbers indicate the jump sequence on both sublattices, two vacancies on one sublattice and an antisite atom on the other sublattice can appear. Triple-defect formation according to Eq. (20.4) is favoured in intermetallics with high formation enthalpies of VB vacancies. Vacancies and antisite defects can associate to form bound triple defects (see also Chap. 5). A triple-defect mechanism involving bound triple defects was proposed by Stolwijk et al. [33] for the B2 compound CoGa. The triple-defect mechanism in CoGa was attributed to two nearestneighbour jumps of Co atoms and to a next-nearest neighbour jumps of Ga atoms. Detailed calculations for NiAl predict that an Al atom performs two nearest-neighbour jumps instead of one second-nearest neighbour jump [34]. Figure 20.6 shows the triple-defect mechanism with this Fig. 20.7. Illustration of the antistructural-bridge (ASB) mechanism. The arrows show vacancy jumps; the numbers indicate the jump sequence 350 20 Diﬀusion in Binary Intermetallics modiﬁcation. The ratio of the diﬀusivities for this mechanism lies within the following limits [35]: 1/13.3 < DA /DB < 13.3 . – – (20.5) The triple-defect mechanism is closely related to the vacancy-pair mechanism (see below). The conﬁgurations which appear after jumps 1 and 3 of Fig. 20.6 are nearest-neighbour vacancy pairs. Antistructural-bridge (ASB) mechanism: This mechanism was proposed by Kao and Chang [38] and is illustrated in Fig. 20.7. As a result of the two jumps indicated, the vacancy and the antisite atom exchange their position. For a B2 phase with some substitutional disorder, antisite defects can act as ‘bridges’ to establish low energy sequences for vacancy jumps. It is important to note that the ASB mechanism has a percolation threshold. Long-range diﬀusion via the ASB mechanism requires a suﬃcient concentration of antistructure atoms to reach the percolation threshold. A relatively high threshold was estimated from purely geometrical arguments [38]. Monte Carlo simulations yielded lower values for the percolation threshold of about 6 % [36, 37]. Such antistructure atom concentrations can indeed occur in B2 intermetallics with a wide phase ﬁeld like NiAl (see below). Vacancy-pair mechanism: A bound pair of vacancies, i.e. a vacancy in one sublattice and a scond vacancy on a neighbour site of the other sublattice, can mediate diﬀusion of both components by successive correlated next-nearest-neighbour jumps. Whereas this mechanism has some rele- Fig. 20.8. Defect site fractions in B2 NiAl as a function of composition at 0.75 Tm from [39] 20.3 B2 Intermetallics 351 vance for ionic crystals such as alkali halides (see Chap.26), it is unlikely for B2 intermetallics. It seems that in those B2 compounds, which are composed of a group VIIIB metal (Co, Fe, Ni, Pd, etc.) and a group IIIA metal (Al, Ga, In, etc.), the triple-defect mechanism is important. By contrast, B2 phases composed of a noble metal (Cu, Ag, Au) and a divalent metal (Mg, Zn, Cd) and FeCo are considered as candidates for the six-jump-cycle mechanism. Clearly, the antistructural-bridge (or antisite bridge) mechanism becomes more important at larger deviations from stoichiometry, because of its percolation threshold. 20.3.2 Example B2 NiAl The phaseﬁeld of B2 NiAl is fairly wide. It extends from about 45 % Ni on the Al-rich side to about 65 % Ni on the Ni-rich side [3]. Theoretical calculations of defect concentrations performed for various intermetallics have been summarised by Herzig and Divinski [39]. The concentrations of defects Fig. 20.9. Ni tracer diﬀusion in B2 NiAl at various compositions X according to Frank et al. [48] and Divinski and Herzig [49] 352 20 Diﬀusion in Binary Intermetallics in NiAl are shown in Fig. 20.8. NiAl reveals a triple-defect type of disorder: structural Ni vacancies (VN i ) are the dominating defects on the Ni-lean side, whereas Ni antisite atoms (N iAl ) dominate on the Ni-rich side of the stoichiometric composition. Moreover, vacancies form mainly on the Ni sublattice whereas the concentration of vacancies on the Al sublattice (VAl ) is remarkably smaller even on the Al-lean side. Ni diﬀusion in B2 NiAl alloys has been measured at various compositions on both Al- and Ni-rich sides and over wide temperature intervals by Frank et al. [48] and reviewed in a paper on NiAl interdiﬀusion by Divinski and Herzig [49]1 . These data are displayed in Fig. 20.9 for various compositions. The diﬀusivity increases notably on the Ni-rich side of the stoichiometric composition. It is practically independent of composition on the Al-rich side in spite of the considerable amount of structural Ni vacancies (see Fig. 20.8). Theoretical studies of the atomic mechanism using embedded atom potentials showed that the triple-defect mechanism dominates self-diﬀusion Fig. 20.10. Self-diﬀusion of Fe and Al in Fe3 Al 1 Older measurements of Ni diﬀusion in NiAl [40] are very likely inﬂuenced by grain-boundary contributions [39] and are not considered here. 20.3 B2 Intermetallics 353 Fig. 20.11. Self-diﬀusion of Fe and Al and interdiﬀusion in Fe2 Al on the Al-rich side and for stoichiometric NiAl. The widely abundant isolated Ni vacancies do not contribute signiﬁcantly to Ni diﬀusion, because their motion via the six-jump-cycle mechanism is energetically unfavourable. With increasing Ni content, after reaching the percolation threshold, the antistructural-bridge mechanism on the Ni-rich side leads to an increase in the Ni diﬀusivity [48]. 20.3.3 Example B2 Fe-Al The phaseﬁeld of B2 order in the Fe-Al system is fairly extended [3]. B2 order exists between about 22 and 50 at.% Al. In contrast to NiAl, B2 order does hardly extend to compositions on the Al-rich side of stoichiometry. At higher temperatures an order-disorder transition to the disordered A2 structure occurs. The corresponding transition temperature increases with increasing Al content. Some tracer data for 26 Al in aluminides are available from the work of Larikov et al. [22]. Tracer measurements of Fe self-diﬀusion were carried out by Tökei et al.[24] and by Eggersmann and Mehrer [23]. Interdiﬀu- 354 20 Diﬀusion in Binary Intermetallics Fig. 20.12. Solute diﬀusion of Zn, In, Ni, Co, Mn, and Cr in Fe3 Al according to [23, 51]. Fe self-diﬀusion in Fe3 Al is also shown for comparison sion in the whole B2 phaseﬁeld of Fe-Al alloys has been studied by Salamon and Mehrer [50]. These authors used the Darken-Manning equation (see Chap. 10), the Kirkendall shift, calculated thermodynamic factors, and Fe tracer data of the Fe-Al system and deduced Al tracer diﬀusivities for alloys with the approximate compositions Fe3 Al, Fe2 Al, and FeAl. Some of the results for diﬀusion in iron-alumindes are shown in Figs. 20.10 and 20.11. Fe3 Al reveals A2 disordered, B2 ordered, and D03 ordered structures with decreasing temperature. As already indicated in Eq. (20.2), the increase in the degree of order results in an increase of the activation enthalpy, which can be seen in Fig. 20.10. Self-diﬀusion in Fe2 Al and FeAl has been investigated almost exclusively in the B2 phase region. For all three compositions the diﬀusivities of Fe and Al are not much diﬀerent indicating a coupled diﬀusion of both components. Solute diﬀusion in Fe-Al alloys has also been investigated. Typical results for ternary alloying elements in Fe3 Al are compiled in Fig. 20.12 and compared with Fe self-diﬀusion. Zn and In are incorporated on Al sites and diﬀuse slightly faster than self-diﬀusion of both components Fe and Al [23]. Ni and 20.4 L12 Intermetallics 355 Co substitute Fe atoms. They are slower diﬀusers and have higher activation enthalpies than self-diﬀusion. The diﬀusivities of Mn and Cr are both fairly similar to Fe self-diﬀusion [51]. 20.4 L12 Intermetallics In completely ordered L12 compounds, each A atom is surrounded by 8 A atoms and 4 B atoms on nearest-neighbour sites (see Fig. 20.1). In contrast to this situation, a B atom faces only A atoms on nearest-neighbour sites. This implies that the sublattice of the majority component A is interconnected by nearest-neighbour bonds, whereas this is not the case for the sublattice of the minority component B. Vacancy motion restricted to the majority sublattice can promote diﬀusion of A atoms as illustrated in Fig. 20.13. Diﬀusion of B atoms on its own sublattice requires jump lengths larger than the nearest-neighbour distance, which are energetically unfavourable. Another possibility is the formation of antisite defects and diﬀusion via vacancies of the majority sublattice. Perhaps the best known L12 intermetallic is Ni3 Al. It has been used as a strengthening phase in Ni-base superalloys for a long time. The Ni3 Al phaseﬁeld in the Ni-Al system exists on both sides of the stoichiometric compositions, but in a faily narrow composition interval. The concentrations of defects in Ni3 Al taken from the review [39] are shown in Fig. 20.14. Ni3 Al belongs to the antistructural-defect type of intermetallics, in which antisite atoms (NiAl and AlN i ) are preferentially formed to accommodate deviations from stoichiometry. Vacancies are mainly formed on the Ni sublattice. Their concentrations are similar to thermal vacancy concentrations in pure Ni at the same homologous temperature. Vacancy formation on the Al sublattice is energetically less favourable. Ni diﬀusion has been studied using tracer techniques by Bronfin et al. [41], Hoshino et al. [42], Shi et al. [43], and Frank et al. [44]. Fig. 20.13. Schematic illustration of the sublattice vacancy mechanism in the majority sublattice of an L12 structured intermetallic. Full circles: majority atoms; open circles: minority atoms 356 20 Diﬀusion in Binary Intermetallics Fig. 20.14. Defect site fractions in L12 structured Ni3 Al as a function of composition at 0.75 Tm from [39] Unfortunately, diﬀusion studies on Ni3 Al, as for other aluminides, suﬀer from the lack of a suitable radiotracer for Al. On the other hand, interdiﬀusion coeﬃcients across the phase ﬁeld of Ni3 Al were measured by Ikeda et al.[45] and Watanabe et al. [46]. Using the Darken-Manning equation and the Kirkendall shift, Fujiwara and Horita [47] deduced Al tracer diﬀusivities. It was found that the Ni and Al diﬀusivities are not much diﬀerent. Suitable substitutes for Al (e.g., Ge and Ga) have been studied (see Table 20.1 and [39]) and support this ﬁnding. Diﬀusion in the L12 compounds Ni3 Ge and Ni3 Ga has also been studied. Fortunately, in these cases suitable radiotracers for both constituents are available. As can be seen from Fig. 20.16, diﬀusion of the majority component Ni in Ni3 Ge is indeed signiﬁcantly faster than that of the minority component Ge. Experiments on Ni3 Ga revealed a trend similar to the case of Ni3 Ge, but the diﬀerence of the diﬀusivities is not so large [52]. For Ni3 Al only Ni selfdiﬀusion is indicated. According to the above reasoning the ratio of the two tracer diﬀusivities, DN i /DAl , in Ni3 Al is not much diﬀerent from unity. It is quite natural that diﬀusion of the majority component in L12 compounds occurs by a sublattice vacancy mechanism. The diﬀusion coeﬃcient is expressed as 2 DA = a2 f CVeq ω , (20.6) 3 where a is the lattice parameter, CVeq the concentration of vacancies in the majority sublattice, and ω the vacancy jump rate. The random walk properties and the tracer correlation factor for sublattice diﬀusion of the majority component in L12 compounds via the vacancy mechanism have been discussed by Koiwa et al. [53]. A value of f = 0.6889 has been reported for the tracer correlation factor. 20.5 D03 Intermetallics 357 Fig. 20.15. Self-diﬀusion in L12 structured Ni3 Al according to [39] The diﬀusion mechanism of the minority elements in L12 compounds is less obvious. As can be seen from Fig. 20.16 and from the discussion of diﬀusion in Ni3 Al, the tracer diﬀusivities of the minority elements in these compounds can vary from very diﬀerent to similar of those of the majority elements. The diﬀusivity of Ge in Ni3 Ge is rather low, whereas the diﬀusivity of Ga in Ni3 Ga and very likely the diﬀusivity of Al in Ni3 Al are not much diﬀerent from the respective majority components. Possible mechanisms are discussed in [8]. Minority elements most likely diﬀuse as antisite atoms in the majority sublattice. 20.5 D03 Intermetallics A prominent example of a D03 intermetallic is Fe3 Si. Its phase ﬁeld is located between the stoichiometric composition and Fe-rich compositions up to about 82 at.% Fe. Information about the diﬀusion of both constituents and of Ge diﬀusion is available. Fe3 Al also shows D03 order but only at fairly low 358 20 Diﬀusion in Binary Intermetallics Fig. 20.16. Self-diﬀusion in the L12 intermetallics Ni3 Ge, Ni3 Ga, and Ni3 Al. The temperature scale is normalised to the corresounding melting temperatures. For comparison self-diﬀusion in Ni is also shown. For references see [7] tempertaures. Fe3 Al is formed on cooling by ordering reactions in the solid state that transform the bcc ordered solid solution, which is stable above about 1000 K, into a B2 phase and then at about 800 K into the D03 structure. Diﬀusion studies in D03 ordered Fe3 Al are diﬃcult due to the fairly low diﬀusivities (see above). Some high-temperature intermetallics (Cu3 Sn, Ni3 Sn, . . . ) crystallise in the D03 structure. Only for Cu3 Sn diﬀusion of both constituents has been investigated (see Table 20.1). The majority sublattice (A sublattice) in D03 compounds, similar to the L12 structure, is interconnected by nearest-neighbour bonds, whereas this is not the case for the B sublattice (see Fig. 20.1). An A atom can diﬀuse within its own sublattice via nearest-neighbour jumps. If B atoms migrate within their own sublattice, their jump vector would be a third-nearest neighbour jump with respect to the bcc unit cell. An alternative for the diﬀusion of B atoms are nearest-neighbour jumps, which create B antisite defects. Then, B atoms can diﬀuse as ‘imperities’ in the majority sublattice. Both options require higher activation enthalpies for diﬀusion of B atoms. Figure 20.17 shows an Arrhenius plot of Fe- and Ge tracer diﬀusion for three compositions of Fe3 Si according to Gude and Mehrer [54]. The data cover rather wide temperature ranges mostly within the D03 phaseﬁeld. One experiment with the short-lived isotope 31 Si conﬁrmed that Ge and Si diﬀuse 20.5 D03 Intermetallics 359 Fig. 20.17. Fe self-diﬀusion and Ge solute diﬀusion in three compositions of the D03 phase Fe3 Si according to Gude and Mehrer [54]. The temperatures are normalised to the corresponding liquidus temperatures. A slight inﬂuence of the paramagnetic-ferromagnetic transition can be seen for Fe diﬀusion in Fe79 Si21 and Fe82 Si18 at very similar rates [54]. Diﬀusion studies of Si and Ge after ion implantation using SIMS proﬁling also showed that Ge is a ‘good’ substitute to mimic Si diﬀusion [55]. The most salient features of Fig. 20.17 are: (i) The asymmetry between the fast Fe diﬀusion and the relatively slow Ge or Si diﬀusion is large. (ii) The Fe diﬀusivity increases with Si content and Fe diﬀuses fastest in the nearly stoichiometric compound. Positron annihilation studies by Schaefer and coworkers [56] have shown that the increase in Fe diﬀusivity is accompanied by a comparable increase of the content in thermal vacancies. In addition, Mössbauer experiments on stoichiometric Fe3 Si by Sepiol and Vogl [57] have demonstrated that the atomic jump vector of Fe atoms is in agreement with nearestneighbour jumps in the Fe sublattice. These ﬁndings clearly support a sub- 360 20 Diﬀusion in Binary Intermetallics lattice vacancy mechanism for Fe diﬀusion. The diﬀusion mechanism of Ge and Si is not completely clear. Ge diﬀusion is less aﬀected by the increase of vacancy concentration with increasing Si content than Fe diﬀusion. For the high-temperature phase Cu3 Sn (see Table 20.1) diﬀusion data for both constituents are also available. As in the case of Fe3 Si the majority component is signiﬁcantly faster than the minority component. 20.6 Uniaxial Intermetallics For non-cubic materials a diﬀusion ansiotropy can be expected as dicussed in Chap. 2. Diﬀusion in uniaxial materials, such as intermetallics with a tetragonal, hexagonal or trigonal axis, is described by a diﬀusivity tensor with two principal components. In general, the diﬀusivity parallel to the axis, D , and the diﬀusivity perpendicular to the crystal axis, D⊥ , are diﬀerent. A comprehensive study of diﬀusion then requires measurements on single crystals in at least two independent directions. Experiments on polycrystalline samples conceal the anisotropy eﬀects and reveal average values of the diﬀusivities only. Nevertheless, they can provide useful information, if single crystals are not available. According to the author’s knowledge, diﬀusion studies on single cystalline intermetallics are very scarce. A few studies concern L10 intermetallics such as γ-TiAl and FePt. Another well-studied example concerns the tetragonal C11b structured material molybdenum disilicide. 20.6.1 L10 Intermetallics As already discussed at the beginning of this chapter, the L10 structure shown in Fig. 20.2 is tetragonal and has an approximate composition AB. Its atomic arrangement can be considered as an ordered fcc structure with A and B atoms occupying sequential (001)-planes. An example of technologically interest for structural applications is β-TiAl. Other L10 intermetallics such as NiPt, FePt, CoPt, FePd, and NiMn are candidates for high-density magnetic storage media due to their high magnetic anisotropy related to their tetragonal anisotropy. γ-TiAl: This intermetallic has attracted much attention as a structural material for high-temperature applications because of its mechanical properties and its low density. The tracer diﬀusivities of 44 Ti [58, 59] and of several substitutional impurities [60–62] have been studied in polycrystalline γ-TiAl. Tracer diﬀusion studies on single crystals of γ-TiAl have been reported by Nakajima and associates [63, 64]. The self-diﬀusivities of 44 Ti and diﬀusivities of the impurities Fe, Ni, and In have been studied. As In is isoelectonic to Al, its diﬀusivities are belived to be good estimates for the Al self-diﬀusivities of the material. Figure 20.18 shows the diﬀusivities of Ti and 20.6 Uniaxial Intermetallics 361 Fig. 20.18. Ti and In diﬀusion along the two principal directions of γ-TiAl according to Nakajima and associates [63, 64]. Diﬀusion of Ga is shown for polycrystalline γ-TiAl according to Herzig et al. [60] In. In both cases, the diﬀusion is faster perpendicular to the tetragonal axis than parallel to it. For Ti self-diﬀusion the anisotropy ratio D⊥ /D is almost one decade, whereas for In it is slightly smaller. As can be expected, diﬀusion along the layers of the L10 structure is faster than along the tetragonal axis. A detailed model has been suggested by Nose et al. [64]. Diﬀusion of Ga, which like In is isoelectronic to Al has been studied by Herzig et al. [60] in polycrystalline γ-TiAl. The Ga diﬀusivities are similar to those of In diﬀusion. NiMn: Equiatomic NiMn thin ﬁlms are of interest for use in magnetoresistive sensors. In these sensors, exchange coupling between an antiferromagnetic ﬁlm, such as NiMn, is required to ‘pin’ the magnetisation within the ferromagnetic layers. Diﬀusion information is of importance, because interdiffusion is a primary long-term failure mechanism of magnetoresistive sensors. The phase diagram of the Ni-Mn system [65] shows that equiatomic NiMn occurs in three diﬀerent crystal structures as the temperature varies. At temperatures below about 1000 K the L10 structure forms. At intermediate temperatures between about 1000 and 1180 K the alloy shows B2 order and above 1180 K NiMn is a disordered fcc alloy. Self-diﬀusion of Ni and Mn tracers has been investigated by Peteline et al. [66] for polycrystalline samples. The data are shown in the Arrhenius diagram of Fig. 20.19. The diﬀusivities of Mn are higher by factors of 3 to 5 than those of Ni in both the fcc and the B2 structures. There is more than 362 20 Diﬀusion in Binary Intermetallics Fig. 20.19. Self-diﬀusion of 54 Mn and according to Peteline et al. [66] 63 Ni in polycrystalline, equiatomic NiMn one decade increase of the diﬀusivities of both components upon the phase transition from the high-temperature fcc to the B2 structure in the intermediate temperature region. This increase is in agreement with the general observation that diﬀusion in bcc related structures is faster than in closepacked fcc structures (see, for example, self-diﬀusion in fcc and bcc Fe in Fig. 17.9). There is also a decrease of the Ni diﬀusivity upon the phase transition from the B2 phase to the low-temperature L10 phase. As mentioned in the introduction to this chapter, the L10 phase can be considered as a slightly distorted, ordered structure of an fcc lattice. Since the experiments were performed on polycrystalline samples nothing can be said about the diﬀusion anisotropy in the L10 NiMn phase. 20.6.2 Molybdenum Disilicide (C11b structure) Molybdenum disilicide (MoSi2 ) is a highly stoichiometric compound with a very high melting temperature. It has found widespread use as a functional material in heating elements of high-temperature furnaces for temperatures up to 2000 K, because of its advantageous electrical properties and its excellent oxidation resistance. It is considered as a material with high potential for high-temperature structural applications as well [2, 67]. Molybdenum disilicide is an intermetallic with non-cubic crystal structure. It is a material which exhibits an extraordinary large diﬀusion asymmetry between Si and 20.6 Uniaxial Intermetallics 363 Fig. 20.20. Unit cell of tetragonal MoSi2 with the lattice parameters a and c Mo similar to that of the components of ceramic materials. In addition, MoSi2 shows a considerable diﬀusion anisotropy. The tetragonal unit cell of the C11b structure is shown in Fig. 20.20. As mentioned above, a tetragonal crystal has two principal components of the diﬀusion tensor. Two diﬀusivities, D and D⊥ , parallel and perpendicular to the tetragonal axis need to be considered for each component and for the diﬀusion of solute elements. The structure of MoSi2 can be considered as a sequential stacking of one Mo layer followed by two Si layers. Each Mo atom resides in a ‘cage’ of 10 Si atoms whereas each Si atom has ﬁve Si and ﬁve Mo neighbours. With respect to the diﬀusivity ratio of the two components, this structure is a good candidate for the Cu3 Au rule dicussed below. For MoSi2 the rule suggests that Si self-diﬀusion and diﬀusion of solutes in the Si sublattice is much faster than Mo diﬀusion. Diﬀusion of 31 Si, 99 Mo, and 71 Ge tracers has been measured on MoSi2 monocrystals in both principal directions using radiotracer techniques by Salamon and coworkers [68, 69]. An Arrhenius diagram is displayed in Fig. 20.21. For both principal directions, Si diﬀusion is indeed many orders of magnitude faster than Mo diﬀusion: D (Si), D⊥ (Si) D (Mo), D⊥ (Mo) . (20.7) This complies with the observation that the activation enthalpies of Si diﬀusion are remarkably smaller than those of Mo diﬀusion. This large diﬀusion asymmetry of the components suggests that Si and Mo diﬀuse independently. Figure 20.21 also shows that Ge and Si diﬀusion are not much diﬀerent. Diﬀusion in MoSi2 reveals a fairly large anisotropy. For both components and for Ge the diﬀusivity perpendicular to the tetragonal axis is faster than parallel to it (Fig. 20.21): D⊥ (Si)/D (Si) 1 and D⊥ (Mo)/D (Mo) 1 . (20.8) 364 20 Diﬀusion in Binary Intermetallics Fig. 20.21. Mo, Si, and Ge diﬀusion along the two principal directions of MoSi2 according to Salamon and Mehrer [68] The anisotropy ratios are about 100 for Mo diﬀusion and around several ten for Si diﬀusion: Positron annihilation studies by Sprengel et al. [71] indicate that thermal vacancies are formed on the Si sublattice of MoSi2 . This observation and the large diﬀusion asymmetry suggest that Si diﬀusion occurs via thermal vacancies on the Si sublattice. The anisotropy of Si diﬀusion indicates that vacancies are considerably more mobile within the Si layers perpendicular than parallel to the tetragonal axis. Correlation eﬀects of vacancy-mediated self-diﬀusion in the Si sublattice have been treated in [70]. The slightly faster diﬀusion of Ge as compared to Si suggests an attractive interaction between Ge and vacancies of the Si sublattice. According to the author’s knowledge, no information is available about vacancies in the Mo sublattice except that their formation deﬁnitely requires more energy that the formation of Si vacancies. It is possible that Mo diﬀusion occurs via thermal vacancies in the minority sublattice. Another possibility is that Mo atoms invade the majority sublattice and diﬀuse as antisite atoms. The high energy to form Mo antisite atoms would then be a substantial contribution to the activation enthalpy of Mo diﬀusion. 20.7 Laves Phases A very numerous group of intermetallic phases are the Laves phases, which belong to the family of Frank-Kaspar phases with topologically close-packed 20.7 Laves Phases 365 Fig. 20.22. C15 type cubic Laves phase Co2 Nb. Full circles represent majority atoms and open circles minority atoms structures [2]. More than 900 binary and ternary Laves phases are known including more that 360 binary Laves phases. Binary Laves phases can be formed if the eﬀective atomic radii of the two components exhibit a ratio of approximately 3/2 ≈ 1.25, which allows a high packing density [72]. Laves phases have an approximate composition AB2 and crystallise in three intimately related structures: C15 (cubic, Mg2 Cu type), C14 (hexagonal, MgCu2 type), and C36 (hexagonal, MgNi2 -type). Information about diﬀusion in Laves phases is very scarce [4]. According to the author’s knowledge, the only study of self-diﬀusion for both constituents concerns the cubic C15-type phase with the approximate composition Co2 Nb. The C15 structure of the cubic Laves phase Co2 Nb is shown in Fig. 20.22. In the completely ordered state, the unit cell would contain 8 A atoms and 16 B atoms. The structure consists of two interpenetrating sublattices where the larger A atoms (open circles) form a diamond-type sublattice. The smaller B atoms (full circles) form a network of tetrahedra being joined to each other at their vertices. Co2 Nb mainly exists on the Co-rich side of the stoichiometric composition. Co atoms are considerably smaller than Nb atoms. This suggests that the deviation from stoichiometry on the Co-rich side is compensated by Co-antisite atoms. Figure 20.23 shows the self-diﬀusion data according to Denkinger and Mehrer [73]. The Co diﬀusivity has been measured for two compositions, namely Nb31 Co69 and Nb29 Co71 . Both compositions lie inside the phaseﬁeld of the C15 phase of the Co-Nb system [3]. The Nb diﬀusivity is reported for Nb31 Co69 only. Some conclusions from Fig. 20.23 are the following: (i) diﬀusion of the majority component Co is signiﬁcantly faster than that of the minority component Nb. This is in accordance with the Cu3 Au rule (see below). Similarities to diﬀusion in the L12 phases, which are also close-packed structures, suggest that self-diﬀusion in Co2 Nb also occurs via thermal vacancies. (ii) The rela- 366 20 Diﬀusion in Binary Intermetallics Fig. 20.23. Self-diﬀusion of Co and Nb in the cubic C15 Laves phase Co2 Nb according to Denkinger and Mehrer [73] tively slow self-diﬀusion of the large Nb atoms is probably restricted to the Nb sublattice. (iii) The increase of the Co diﬀusivity with increasing Co concentration can be attributed to the occurrence of additional diﬀusion paths via anti-structural bridges due to additional Co antisite atoms [73]. 20.8 The Cu3 Au Rule An empirical rule suggested by d’Heurle and coworkers [74, 75], called the Cu3 Au rule2 , provides often a good guess for self-diﬀusion in nonequiatomic intermetallics. It states that in compounds of type Am Bn , where the ratio m/n is 2 or greater, the majority element diﬀuses faster than the minority element: (20.9) DA > DB or DA DB . Here DA (DB ) denote the tracer diﬀusion coeﬃcients of the majority (minority) component. 2 This name is a bit misleading. According to the author’s knowledge, tracer diffusion experiments of both components in the ordered Cu3 Au phase are not available. Due to the fairly low ordering temperature of this alloy, the diﬀusivities are very low and thus diﬃcult to measure. References 367 For geometrical reasons discussed above, A3 B intermetallics with L12 or D03 structure are good candidates to test the validity ‘Cu3 Au’ rule. The L12 phases Ni3 Ge and Ni3 Ga clearly conﬁrm this rule (see Fig. 20.16). However, Ni3 Al is at the border line. The asymmetry of diﬀusion between majority and minority component in D03 phases is in full accordance with the Cu3 Au rule (see Fig. 20.17). Diﬀusion in molybdenum disilicide and in the cubic Laves phase Co2 Nb also conﬁrm the rule very well (see Figs. 20.21 and 20.23). The Cu3 Au rule is explained by a diﬀusion mechanism where atoms of the majority component can diﬀuse by energetically favourable jumps in their own sublattice. Atoms of the minority component diﬀuse either via energetically unfavourable jumps to more distant sites on their own sublattice or as antisite atoms on the wrong sublattice. Of course, the Cu3 Au rule should be applied to those intermetallics only in which diﬀusion occurs via vacancies. Phases such as carbides, nitrides, and metal hydrides, where one of the two elements is suﬃciently small to occupy interstitial sites, must be considered separately. References 1. J.H. Westbrook, R.L. Fleischer (Eds.), Intermetallic Compounds, Vol.1, Principles, Vol. 2 Practise, J. Wiley and Sons Ltd., 1995 2. G. Sauthoﬀ, Intermetallics, VCH Weinheim, 1995 3. T.B. Massalski (Ed.), Binary Alloy Phase Diagrams, Am. Soc. for Metals, Metals Park, Ohio, 1986 4. H. Bakker, Self-diﬀusion in Binary Alloys and Intermediate Phases, Chap. 4 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990. p. 213 5. H. Bakker, Tracer Diﬀusion in Concentrated Alloys, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Eds.), Academic Press, Orlando, 1984, p. 189 6. H. Wever, Defect and Diﬀusion Forum 83, 55 (1992) 7. H. Mehrer, Materials Transactions, JIM, 37, 1259 (1996) 8. M. Koiwa, H. Numakura, S. Ishioka, Defect and Diﬀusion Forum 143–147, 209 (1997) 9. H. Mehrer, F. Wenwer, Diﬀusion in Metals, in: Diﬀusion in Condensed Matter, J. Kärger, P. Heitjans, R. Haberlandt (Eds.), Verlag Vieweg, Braunschweig, 1998, p.1 10. H. Nakajima, W. Sprengel, K. Nonaka, Intermetallics 4, 517 (1996) 11. H. Mehrer, Chr. Herzig, in: Advances in Science and Technology 29, Mass and Charge Transport in Inorganic Materials: Fundamentals to Devices, P. Vicenzini, V. Buscaglia (Eds.), Techna Srl. 2000, p.187 12. Chr. Herzig, S.V. Divinski, St. Frank, T. Przeorski, Defect and Diﬀusion Forum 194–199, 317 (2001) 13. H. Mehrer, Diﬀusion: Introduction and Case Studies in Metals and Binary Alloys, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), Springer-Verlag, 2005, p.3 368 20 Diﬀusion in Binary Intermetallics 14. J. Philibert, Atom Movements – Diﬀusion and Mass Transport in Solids, Les Editions de Physique, Les Ulis, 1991 15. R.M. Cotts, Ber. Bunsenges. Phys. Chem. 76, 760 (1972) 16. Th. Heumann, Diﬀusion in Metallen, Springer Verlag, Berlin, 1992 17. A.B. Kuper, D. Lazarus, J.R. Manning, C.T. Tomizuka, Phys. Rev. 104, 1536 (1956) 18. S.G. Fishman, D. Gupta, D.S. Lieberman, Phys. Rev. B 2, 1451 (1970) 19. S.G. Fishman, R.N. Jeﬀrey, Phys. Rev. B 120, 4424 (1971) 20. Y. Iijima, Ch.-G. Lee, Acta Metall. Mater. 43, 1183 (1995) 21. H. Nitta, Y. Iijima, K. Tanaka, Y. Yamazaki, Ch.-G. Lee, T. Matsuzaki, T. Watanabe, Mater. Sci. Eng. A 382, 243, 250 (2004) 22. L.N. Larikov, V.V. Geichenko, V.M. Gal’chenko, Diﬀusion Processes in Ordered Alloys, translated from Russion, Amerind Publ. Co. Ltd, New Dehli, 1981 23. M. Eggersmann, H. Mehrer, Philos. Mag. A 80, 1219 (2000) 24. Zs. Tökei, J. Bernardini, P. Gas, D.L. Beke, Acta Mater. 45, 541 (1997) 25. E.W. Elcock, C.W. McCombie, Phys. Rev. 109, 605 (1958) 26. E.W. Elcock, Proc. Phys. Soc. 73, 250 (1959) 27. H.B. Huntington, N.C. Miller, V. Nerses, Acta Metall. 9, 749 (1961) 28. P. Wynblatt, Acta Metall. 47, 2437 (1967) 29. H.A. Domian, H.I. Aaronson, in: Diﬀusion in Body-Centered Cubic Metals, American Society for Metals, 1965, p. 209 30. M. Arita, M. Koiwa, S. Ishioka, Acta Metall. 37, 1363 (1989) 31. R. Drautz, M. Fähnle, Acta Mater. 47, 2437 (1999) 32. I.V. Belova, G.E. Murch, Philos. Mag. A 82, 269 (2002) 33. N.A. Stolwijk, M. van Gend, H. Bakker, Philos. Mag, A 42, 283 (1980) 34. S. Frank, S.V. Divinski, U. Södervall, Chr. Herzig, Acta Mater. 49, 1399 (2001) 35. H. Bakker, N.A. Stolwijk, M.A. Hoetjes-Eijkel, Philos. Mag. A 43, 251 (1981) 36. S.V. Divinski, L.N. Larikov, J. Phys.: Condensed Matter 35, 7377 (1997) 37. I.V. Belova, G.E. Murch, Intermetallics 6, 115 (1998) 38. C.R. Kao, Y.A. Chang, Intermetallics 1, 237 (1993) 39. Ch. Herzig, S. Divinski, Diﬀusion in Intermetallic Compounds, in: Diﬀusion Processes in Advanced Technological Materials, D. Gupta (Ed.), William Andrew, Inc., 2005 40. G.F. Hancock, B.R. McDonnel, Phys. Stat. Sol. A 4, 143 (1971) 41. M.B. Bronﬁn, G.S. Bulatov, I.A. Drugova, Fiz. Metal. Metalloved. 40, 363 (1975) 42. K. Hoshino, S.J. Rothman, R.S. Averback, Acta Metall. 36, 1271 (1988) 43. Y. Shi, G. Frohberg, H. Wever, Phys. Stat. Sol. A 191, 361 (1995) 44. S. Frank, U. Södervall, Chr. Herzig, Phys. Stat. Sol. B 191, 45 (1995) 45. T. Ikeda, A. Almazouzi, H. Numakura, M. Koiwa, W. Sprengel, H. Nakajima, Acta Mater. 46, 5369 (1998) 46. M. Watanabe, Z. Horita, M. Nemoto, Defect and Diﬀusion Forum 143–147, 345 (1997) 47. K. Fujiwara, Z. Horita, Acta Mater. 50, 1571 (2002) 48. S. Frank, S.V. Divinski, U. Södervall, Chr. Herzig, Acta Mater. 49, 1399 (2001) 49. S.V. Divinski, Chr. Herzig, Defect and Diﬀusion Forum 203–205, 177 (2002) 50. M. Salamon, H. Mehrer, Z. Metallkd. 96, 1 (2005) 51. S. Peteline, E.M. Tanguep Njiokep, S. Divinski, H. Mehrer, Defect and Diﬀusion Forum 216–217, 175 (2003) References 369 52. K. Nonaka, T. Arayashiki, H. Nakajima, A. Almazouzi, T. Ikeda, K. Tanaka, H. Numakura, M. Koiwa, Defect and Diﬀusion Forum 143–147, 209 (1997) 53. M. Koiwa, S. Ishioka, Philos. Mag. A 48, 1 (1983) 54. A. Gude, H. Mehrer, Philos. Mag. A 76, 1 (1997) 55. M. Wellen, B. Fielitz, G. Borchardt, S. Weber, S. Scherrer, H. Mehrer, H. Baumann, B. Sepiol, Defect and Diﬀusion Forum 194–199, 499 (2001) 56. E.A. Kümmerle, K. Badura, B. Sepiol, H. Mehrer, H.-E. Schaefer, Phys. Rev. B 52, R6947 (1995) 57. B. Sepiol, G. Vogl, Phys. Rev. Lett. 71, 731 (1995) 58. S. Kroll, N.A. Stolwijk, Chr. Herzig, H. Mehrer, Defect and Diﬀusion Forum 95–98, 865 (1992) 59. Chr. Herzig, T. Przeorski, Y. Mishin, Intermetallics 7, 389 (1999) 60. Chr. Herzig, M. Friesel, D. Derdau, S.V. Divinski, Intermetallics 7, 1141 (1999) 61. Y. Iijima, C.G. Lee, S.E. Kim, High Temp. Mater. Process. 18, 305 (1999) 62. Y. Mishin, Chr. Herzig, Acta Mater. 48, 589 (2000) 63. T. Ikeda, H. Kadowski, H. Nakajima, Acta Mater. 49 3475 (2001) 64. Y. Nose, N. Terashita, T. Ikeda, H. Nakajima, Acta Mater. 54, 2511 (2006) 65. L. Ding, P.F. Ladwig, X. Yan, Y.A. Chang, Appl. Phys. Letters 80, 1186 (2002) 66. S. Peteline, H. Mehrer, M.-L. Huang, Y.A. Chang, Defect and Diﬀusion Forum 237–240, 352 (2005) 67. M. Yamaguchi, H. Inui, K. Ito, Acta Mater 48, 307 (2000) 68. M. Salamon, A. Strohm, T. Voss, P. Laitinen, I. Rihimäki, S. Divinski, W. Frank, J. Räisänen, H. Mehrer, Philos. Mag. 84, 737 (2004) 69. M. Salamon, H. Mehrer, Z. Metallkd. 96, 833 (2005) 70. S. Divinski, M. Salamon, H. Mehrer, Philos. Mag. 84, 757 (2005) 71. W. Sprengel, X.Y. Zhang, H. Inui, H.-E. Schaefer, Verhandl. DPG 5, 339 (2003) 72. D.J. Thoma, J.H. Perepezko, J. Alloys and Compounds 224, 330 (1995) 73. M. Denkinger, H. Mehrer, Philos. Mag. A 80, 1245 (2000) 74. F.M. d’Heurle, P. Gas, J. Philibert, Solid State Phenomena 41, 93 (1995) 75. F.M. d’Heurle, P. Gas, C. Lavoie, J. Philibert, Z. Metallkd. 95, 852 (2004) 21 Diﬀusion in Quasicrystalline Alloys 21.1 General Remarks on Quasicrystals The quasicrystalline state is a third form of solid matter besides the crystalline and amorphous state. The atomic positions are ordered, but with ﬁve-, eight-, ten-, or twelvefold rotational symmetries, which violate canonical rules of classical crystallography. These symmetries forbid a periodic structure and, instead, enforce quasiperiodicity. Quasicrystalline alloys can also be considered as complex intermetallics. Most quasicrystals are indeed composed of metallic components. Usually, quasicrystals have crystalline intermetallics as neighbour phases. The discovery of the ﬁrst quasicrystal, Al86 Mn14 , was announced by Shechtman et al. in 1984 [1]. In the early days, only metastable quasicrystalline alloys, such as Al86 Mn14 and other Al-TM alloys (TM = transition metal), were produced. Since these times a large number of quasicrystalline systems are known and progress in the understanding of their physical properties has been achieved [2–5]. Some of them crystallise in quasiperiodic lattices upon slow cooling and exist as stable phases. Stable quasicrystals are mostly formed in ternary or higher component systems (see Table 21.1). The ﬁrst stable quasicrystals were discovered by Tsai and coworkers are all Aldominated. These were icosahedral Al-Cu-Fe [6], decagonal Al-Ni-Co [7], and icosahedral Al-Pd-Mn [8]. The ﬁrst Al-free icosahedral phase was found in 1993 in the Zn-Mg-Y system [9]. Meanwhile, several Zn-Mg-RE quasicrystals (RE = rare earth elements Y, Ho, Er, Gd, Tb, or Dy) are known. They are prototypes of non-Al-based quasicrystalline phases. After the growth of large single-quasicrystals was mastered, one could start to check structure and atomic dynamics with elastic and inelastic scattering methods. Transport measurements revealed fairly high electric resistivities in Al-based alloys. Mechanical experiments showed brittleness and hardness at low temperatures, but ductility with extreme plasticity at high temperatures. Other observations, for example low friction, high corrosion and oxidation resistance, low wetting of surfaces, and strength of composites with quasicrystals promised technological applications [11, 12]. Quasicrystals are a prominent example for systems whose properties are mainly determined by their structure. 372 21 Diﬀusion in Quasicrystalline Alloys Table 21.1. Examples of some stable quasicrystalline phases Icosahedral quasicrystals Decagonal quasicrystals Dodecagonal quasicrystals Al70 Pd21 Re9 Al70 Pd21 Mn9 Al62 Cu25 TM13 (TM = Fe, Ru, Os) Ni17 Ti41.5 Zr41.5 Ga20 Mg43 Zn37 Al37 Cu10.8 Li32.2 Al43 Mg43 Pd14 Zn64.2 Mg26.4 Ho9.4 Zn60.7 Mg30.6 Y8.7 Al64 Co16 Cu20 Al71.5 Co14 Ni14.5 Al69.8 Pd18.1 Mn12.3 Al71 Fe5 Ni24 Al40 Fe15 Ge20 Mn25 Ta1.6 Te Fig. 21.1. Icosahedral single-quasicrystal (Zn-Mg-Ho) with the habit of a dodecahedron. A dodecahedron has 12 pentagon-shaped faces and 20 vertices Nowadays, quasicrystals are no longer laboratory curiosities. Quasicrystalline phases such as icosahedral Al-Pd-Mn, icosahedral Zn-Mg-RE, and decagonal Al-Ni-Co can be grown in the form of centimeter-size singlequasicrystals with high structural quality by Bridgman-, Czochralski-, and ﬂux-growth techniques [15–17]. Figure 21.1 shows an icosahedral Zn-Mg-Y quasicrystal grown by the ﬂux-growth technique. Its habit is a dodecahedron – one of the ﬁve regular (Platonian) polyhedra1 . Quasicrystalline structures are fairly complex, because there is no periodicity. In addition, most quasicrystals are ternary, quaternary, or multicomponent alloys. Quasicrystals have rotational order and sharp diﬀraction peaks. Quasiperiodic space tiling procedures such as two-dimensional Penrose tiling and its three-dimensional analogues [18], projections or cuts from higher di- 1 The ﬁve Platonian polyhedra are: tetrahedron, cube, octahedron, icosahedron, dodecahedron. 21.2 Diﬀusion Properties of Quasicrystals 373 Fig. 21.2. The pseudo-Mackay cluster suggested for icosahedral Al-Pd-Mn [19]. It consists of a central cube (ﬁlled grey circles), an icosahedron (ﬁlled black circles), and an icosidodecahedron (open circles) mensional periodic lattices, and cluster covering models have been developed to describe quasi-crystallography (see [2] and Chap. 2 in [5]). In order to illustrate the structural complexity of quasicrystals we mention just one example: the ﬁrst structure determinations of icosahedral AlPd-Mn by diﬀraction techniques has been published by Boudard et al. in 1992 [19]. The authors found evidence for the presence of so-called pseudoMackay clusters (Fig. 21.2). In their structure model, the most simple cluster consists of Al atoms on the central cube and on the 30 vertices of the icosidodecahedron, whereas Pd and Mn atoms are distributed on the 12 vertices of the icosahedron. However, other decorations have also been suggested in the literature. A further property of the Al-Pd-Mn quasicrystal structure is its self-similarity based on an inﬂated cluster hierarchy [20]. There seems to be no completely accepted structure model for icosahedral Al-Pd-Mn [10]. 21.2 Diﬀusion Properties of Quasicrystals Diﬀusion in solids – irrespective of whether they are crystalline, quasicrystalline, or amorphous – is an important topic of materials science. Thorough diﬀusion studies on single quasicrystals have been performed on the icosahedral phases Al-Pd-Mn and Zn-Mg-RE and on the decagonal phase Al-Ni-Co. Tracer techniques have mainly been applied and the diﬀusers were either labeled by their radioactivity or, when SIMS proﬁling was employed, by their atomic mass. As already stated, both icosahedral Al-Pd-Mn and decagonal Al-Ni-Co are Al dominated. Tracer diﬀusion of Al has not been studied. This 374 21 Diﬀusion in Quasicrystalline Alloys is because natural Al is monoisotopic, which forbids SIMS studies, and a suitable radioisotope for tracer studies is missing2 . Instead, diﬀusion of several solutes was investigated, especially in icosahedral Al-Pd-Mn. Single crystals should be used for basic studies to avoid complications due to diﬀusion along grain boundaries (see Chap. 32). The diﬀusion coeﬃcient in a quasicrystal, like in a crystal, is a symmetric second rank tensor. Icosahedral quasicrystals are highly symmetric, diﬀusion is isotropic, and the diﬀusion coeﬃcient is a scalar quantity. Decagonal quasicrystals are uniaxial and the diﬀusion coeﬃcient has two principal components, like in uniaxial crystals. One component corresponds to diﬀusion parallel to the decagonal axis and the other one to diﬀusion perpendicular to the axis. A thorough diﬀusion study on decagonal quasicrystals requires diﬀusivity measurements on monocrystalline samples with two diﬀerent orientations. Diﬀusion in quasicrystalline alloys has been reviewed by Nakajima and Zumkley [13] and by Mehrer et al. [14]. In this chapter, we summarise the state-of-the-art in this area, compare diﬀusion in quasicrystals with diﬀusion in related crystalline metals, and discuss possible diﬀusion mechanisms. 21.2.1 Icosahedral Quasicrystals Icosahedral Al-Pd-Mn: The information on the phase diagram for the ternary Al-Pd-Mn system is rather complete and has been reviewed by Lück [21]. Al-Pd-Mn was the ﬁrst system for which stable icosahedral as well as decagonal quasicrystals were detected [22]. The formation of the icosahedral phase occurs in a ternary peritectic reaction from the melt. Conventional procedures permit the growth of single crystals [15]. The formation of the decagonal phase is sluggish, and the determination of the phase diagram in the decagonal region is diﬃcult. Icosahedral Al-Pd-Mn contains about 70 at. % Al (see Table 21.1). The contents of transition elements Pd and Mn are about 21 and 9 at. %, respectively. Icosahedral Al-Pd-Mn is not a stoichiometric compound. It possesses a relatively narrow phase ﬁeld, which widens with increasing temperature, but its width never exceeds a few percent [21]. Al-Pd-Mn is the quasicrystalline material for which the largest body of diﬀusion data is available. These data are displayed in the Arrhenius diagram of Fig. 21.3. Self-diﬀusion of the Mn and Pd components as well as solute diﬀusion of the transition elements Co, Cr, Fe, Ni, and Au and of the nontransition elements Zn, Ga, In, and Ge has been investigated. For detailed references, the reader may consult the already mentioned reviews [13, 14]. Inspection of Fig. 21.3 shows that the diﬀusivities can be grouped into two major categories: 2 The radiosisotope 26 Al has a half-life of 7 × 105 years. Its speciﬁc activity is very low, its production requires an accelerator and is very expensive. 21.2 Diﬀusion Properties of Quasicrystals 375 Fig. 21.3. Tracer diﬀusion in single-crystals of icosahedral Al-Pd-Mn according to Mehrer et al. [14]. Self-diﬀusion in Al is indicated as a long-dashed line – – Non-transition elements are relatively fast diﬀusers. Their diﬀusivities are comparable, within one order of magnitude, to the self-diﬀusivity of metallic aluminium (long-dashed line). Ga and Zn were studied to mimic Al self-diﬀusion in the quasicrystal. Ga is isoelectronic to Al. Zn diﬀusion is believed to be close to Al self-diﬀusion, since in metallic Al it is only about a factor of 2 faster than Al [23]. Transition elements are slow, in some cases extremely slow diﬀusers. For example, diﬀusion of Fe at 700 K is about 7 orders of magnitude slower than Ga and Zn diﬀusion. The diﬀusion enthalpies of Fe, Co, and Cr are high, almost twice as large as for Ga and Zn. The pre-exponential factors of the transition elements are two to three orders of magnitude larger than those of Zn and Ga [14]. Most of the diﬀusivities in Fig. 21.3 follow linear Arrhenius behaviour in the whole temperature range investigated. For Pd and Au diﬀusion, studied after implantation of the radioisotopes, a kink was reported in the Arrhenius diagram around 773 K by Frank and coworkers [25, 26]. The Arrhenius parameters in the high-temperature regime are similar to those of the other transition elements, whereas in the low-temperature regime very low values of the activation parameters have been reported. 376 21 Diﬀusion in Quasicrystalline Alloys The pressure dependence of diﬀusion of the non-transition element Zn and of the transition element Mn has been studied [27]. The following activation volumes were deduced: ∆V (Zn) = 0.74 Ω at 776 K , (21.1) ∆V (M n) = 0.67 Ω at 1023 K . (21.2) Ω denotes the mean atomic volume of icosahedral Al-Pd-Mn, which in the case of Al-based Al-Pd-Mn is not much diﬀerent from the atomic volume of Al. It is remarkable that there is no signiﬁcant diﬀerence between the activation volumes of the transition and the non-transition element indicating that the diﬀusion mechanism of both elements is basically the same. The magnitudes and signs of these activation volumes are similar to those observed for metals, which are attributed to vacancy-mediated diﬀusion (see Chap. 8). Diﬀusion in crystalline materials is mediated by point defects (Chaps. 6, 17, 19, 20, 26). In metallic elements and alloys, vacancy-type defects are responsible for the diﬀusion of matrix atoms and of substitutional solutes. In quasicrystals, as in crystalline alloys, vacancies are present in thermal equilibrium as demonstrated in positron annihilation studies by Schaefer and coworkers [28, 29]. Phasons are additional point defects which are speciﬁc to quasicrystalline materials [30]. It has been suggested theoretically by Kalugin and Katz [31] that, in addition to vacancies, phason ﬂips might contribute to some extend to self- and solute diﬀusion in quasicrystals. Remembering that Al is the major component in icosahedral Al-Pd-Mn, one is prompted to compare its diﬀusion data to those of aluminium. Figure 21.4 shows an Arrhenius diagram of Al self-diﬀusion together with the diﬀusivities of those transition and non-transition elements which were also studied in icosahedral Al-Pd-Mn. A comparison of Fig. 21.3 and 21.4 supports the following conclusions: 1. Diﬀusion of Zn and Ga in icosahedral Al-Pd-Mn and in Al obey very similar Arrhenius laws. This suggests that Zn and Ga diﬀusion in icosahedral Al-Pd-Mn is vacancy-mediated as well and restricted to the Alsubnetwork of the quasicrystalline structure (Fig. 21.2). 2. The diﬀusivities of Zn and Ga are close to self-diﬀusion of Al. The activation enthalpies and pre-exponential factors of Ga (113 kJ mol−1 , 1.2 × 10−5 m2 s−1 ) and Zn (121 kJ mol−1 , 2.7 × 10−5 m2 s−1 ) in icosahedral AlPd-Mn [14] and those of Al self-diﬀusion in metallic Al (123.5 kJ mol−1 , 1.37 × 10−5 m2 s−1 [24]) are very similar. This suggests that Zn and Ga diﬀusion provide indeed good estimates for Al self-diﬀusion in icosahedral Al-Pd-Mn. Al self-diﬀusion could not be investigated due to the lack of a suitable Al tracer (see above). 3. Diﬀusion of solutes in icosahedral Al-Pd-Mn and in Al are both characterised by a ‘wide spectrum’ of diﬀusivities, ranging from very slow diﬀusing transition elements to relatively fast diﬀusing non-transition elements. Self-diﬀusion and diﬀusion of substitutional solutes in Al are both 21.2 Diﬀusion Properties of Quasicrystals 377 Fig. 21.4. Self-diﬀusion and diﬀusion of solutes in Al according to [14] mediated by vacancies. The striking similarities between the spectra of solute diﬀusion in both materials, apart from minor diﬀerences in detail, are a strong argument in favour of a vacancy-type mechanism in icosahedral Al-Pd-Mn as well. As discussed in Chap. 19, the slow diﬀusion of transition elements in Al can be attributed to a repulsive interaction between vacancy and solute. In the low-diﬀusivity regime, the diﬀusivities of Pd and Au in icosahedral Al-Pd-Mn are distinctly higher than expected from an extrapolation of the Arrhenius-laws corresponding to the high-diﬀusivity regime. The low preexponential factors found for Pd and Au diﬀusion in this regime are orders of magnitude too small to be reconcilable with diﬀusion mechanisms operating in crystalline solids. A tentative explanation attributes this low-diﬀusivity regime to phason-ﬂip assisted diﬀusion [14, 25, 26]. This explanation is intimately related to the quasicrystalline structure. Hence, it cannot work for substitutional solutes, like the normal diﬀusers Zn or Ga, residing almost exclusively in the Al subnetwork. However, it does work for intermediate diﬀusers such as Au and Pd by promoting their interchange between the subnetworks. 378 21 Diﬀusion in Quasicrystalline Alloys Icosahedral Zn-Mg-RE: Zn-Mg-RE alloys (RE = rare earth element) are the prototype of non-Al-based quasicrystalline alloys. In these phases, Zn is the base element with a content of about 60 at. % (Table 21.1). These quasicrystals are considered to belong to the Frank-Kaspar type phases, which are characterised by an electron to atom ratio of about 2.1. Their structureal units are Bergman clusters [32], which are formed by dense stacking of tetrahedra, relating them to the Frank-Kaspar phases [33]. Three quasicrystalline phases have been found: a face-centered icosahedral (fci) phase, a simple cubic icosahedral (si) phase, and a phase with decagonal structure. Crystalline structures which are related to the quasicrystalline phases are found as well (for references see, e.g., [16]). Tracer diﬀusion experiments of 65 Zn have been performed on icosahedral Zn64.2 Mg26.4 Ho9.4 and Zn60.7 Mg30.6 Y8.7 quasicrystals [34] grown by the top-seeded solution-growth technique [16]. Diﬀusion data are displayed in Fig. 21.5 together with tracer diﬀusion of 65 Zn in a related crystalline ZnMg-Y phase with hexagonal structure. It is not surprising that Zn diﬀusion Fig. 21.5. Self-diﬀusion of 65 Zn in icosahedral Zn64.2 Mg26.4 Ho9.4 and Zn60.7 Mg30.6 Y8.7 quasicrystals and in a related hexagonal phase (h-ZnMgY) according to Galler et al. [34]. Dashed lines: self-diﬀusion in Zn parallel and perpendicular to its hexagonal axis; dotted line: Zn diﬀusion in icosahedral Al-Pd-Mn 21.2 Diﬀusion Properties of Quasicrystals 379 in the closely related Zn-Mg-Ho and Zn-Mg-Y quasicrystals proceeds at almost identical rates. Its diﬀusion is, however, slower than self-diﬀusion in metallic Zn. This diﬀerence can be attributed only partly to the diﬀerent melting temperatures of Zn (693 K) and Zn-Mg-Ho (863 K). In a temperature scale normalised to the respective melting temperatures, Zn self-diﬀusion in hexagonal Zn is still about one order of magnitude faster. Zn diﬀusion in icosahedral Al-Pd-Mn (dotted line) proceeds about one order of magnitude faster than Zn diﬀusion in the Zn-based quasicrystals. A comparison between Zn diﬀusion in the Zn-based quasicrystals and the ternary crystalline compound with similar composition reveals similar diﬀusivities of Zn diﬀusion in particular for diﬀusion perpendicular to the hexagonal axis. These facts and the magnitude of the pre-exponential factors for Zn diﬀusion in both quasicrystals (Zn-Mg-Ho: 3.9 × 10−3 m2 s−1 ; Zn-Mg-Y: 3.3 × 10−3 m2 s−1 ) are hints that diﬀusion in these materials is vacancy-mediated as well. 21.2.2 Decagonal Quasicrystals Decagonal phases belong to the category of two-dimensional quasicrystals. They exhibit quasiperiodic order in layers perpendicular to the decagonal axis, whereas they are periodic parallel to the decagonal axis [35]. The ternary systems Al-CoAl-NiAl and Al-CoAl-CuAl are characterised by the formation of decagonal phases; no icosahedral phases are observed [21]. The ﬁeld of the decagonal phase is elongated with respect to a widely varying Ni to Co ratio. In contrast, only a slight variation of the Al content is possible without leaving the phase ﬁeld with quasicrystalline order. Diﬀusion of several tracers has been studied on oriented single crystals parallel and perpendicular to the decagonal axis and also in polycrystals. Diﬀusion data for decagonal Al-Ni-Co are summarised in Fig. 21.6. Selfdiﬀusion of both minority components (solid lines) has been studied on single crystals of Al72.6 Ni10.5 Co16.9 using 57 Co and 63 Ni as radiotracers by Khoukaz et al. [37, 38]. Diﬀusion of 63 Ni has been studied by the same authors studied on polycrystals of the composition Al70.2 Ni15.1 Co14.7 . Data obtained by Nakajima and coworkers for diﬀusion of 60 Co in decagonal Al72.2 Ni11.8 Co16 are shown as dashed lines [13, 36]. Employing SIMS proﬁling, diﬀusion of Ga has been studied to mimic Al diﬀusion by Galler et al. [34]. Co diﬀusion data are available for two slightly diﬀerent alloys. Co diﬀusion depends only weakly on composition. Diﬀusion of Co and Ni in both principal directions obey Arrrhenius laws. It is remarkable that no signiﬁcant deviation from Arrhenius behaviour has been detected down to the lowest temperatures. In a temperature scale normalised with the melting temperatures, the diﬀusivities of Co and Ni in decagonal Al-Ni-Co and the (vacancy-mediated) self-diﬀusivities of metallic Co and Ni [39] are fairly close to each other. Diffusion of Ga is several orders of magnitude faster than diﬀusion of the transition elements Co and Ni. As in icosahedral Al-Pd-Mn, the non-transition 380 21 Diﬀusion in Quasicrystalline Alloys Fig. 21.6. Self-diﬀusion of 65 Ni, 60 Co, and 57 Co in decagonal Al-Ni-Co quasicrystals from [14, 34, 36]. Monte Carlo simulations of Al diﬀusion are also shown [40] element diﬀuses signiﬁcantly faster than the transition elements. Diﬀusivities deduced from molecular dynamic simulations for Al self-diﬀusion in Al-Ni-Co by Gähler and Hocker [40] also shown in Fig. 21.6. The magnitude of the Al diﬀusivities and the sign of the diﬀusion anisotropy are similar to those of Ga diﬀusion, supporting the view that Ga is indeed suitable to mimic Al self-diﬀusion. The combination of crystalline and quasicrystalline order makes decagonal Al-Ni-Co particularly interesting from the viewpoint of diﬀusion mechanisms. Quasicrystalline order exists only in layers perpendicular to the decagonal axis, whereas periodic (crystalline) order prevails parallel to the decagonal axis. If a diﬀusion mechanism would dominate, which is speciﬁc to quasiperiodic order, one should expect that diﬀusion within the layers perpendicular to the decagonal axis is faster than parallel to it. Phasons are speciﬁc to quasiperiodic order and phason-mediated diﬀusion should cause a diﬀusion anisotropy with slower diﬀusion in the direction of the decagonal axis. Figure 21.6 shows that for Co and Ni diﬀusion the anisotropy is very small. For 60 Co diﬀusion in Al72.2 Ni11.8 Co16 the anisotropy is even opposite to the expectation for phason-dominated diﬀusion in the whole temperature References 381 range [13]. This is even more so for Ga diﬀusion, where diﬀusion parallel to decagonal axis is clearly faster than perpendicular to the axis. The magnitude of the diﬀusion anisotropy Co and Ni in decagonal Al-NiCo is similar to the anisotropies reported for uniaxial metals (see Chap. 17). For self-diﬀusion in the hexagonal metals Be, Mg, Zn, and Cd and for tetragonal In and Sn, the diﬀusivities parallel and perpendicular to the axis, diﬀer by not more than a factor of 2 (see Chap. 17 and [39]). Whereas in Zn and Cd, diﬀusion parallel to the hexagonal axis is slightly faster, the opposite is true in Be and Mg. The similarities between the small diﬀusion anisotropies of uniaxial metals and the decagonal quasicrystals provides additional evidence for vacancy-mediated diﬀusion in decagonal Al-Ni-Co. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. D. Shechtman, I.A. Blech, J.W. Cahn, Phys. Rev. Lett. 53, 1951 (1984) C. Janot, Quasicrystals – a Primer, Clarendon Press, Oxford, 1994 Z. Stadnik (Ed.), Physical Properties of Quasicrystals, Springer-Verlag, 1999 J.-B. Suck, M. Schreiber, P. Häussler (Eds.), Quasicrystals – an Introduction to Structure, Physical Properties, and Applications, Springer-Series in Materials Science, Vol. 55, 2002 H.-R. Trebin (Ed.), Quasicrystals – Structure and Physical Properties, WileyVCH, 2003 A.P. Tsai, A. Inoue, T. Masumoto, Jap. J. Appl. Phys. 36, L1505 (1987) A.P. Tsai, A. Inoue, T. Masumoto, Acta Met. 37, 1443 (1989) A.P. Tsai, A. Inoue, Y. Yokoyama, T. Masumoto, Mater. Trans. Japan Inst. Met. 31, 98 (1990) Z.P. Luo, S. Zhang, Y. Tang, D. Zhao, Scripta Metal. et Mat. 28, 1513 (1993) H.-U. Nissen, C. Beeli, Electron Microscopy and Surface Investigations of Quasicrystals, Chap. 6 in [4] J.-M. Dubois, Bulk and Surface Properties of Quasicrystalline Materials and their Potential Applications, Chap. 28 in [4] J.-M. Dubois, Useful Quasicrystals, World Scientiﬁc Publ. Comp., Singapore, 2005 H. Nakajima, Th. Zumkley, Defect and Diﬀusion Forum 194–199, 789 (2001) H. Mehrer, R. Galler, W. Frank, R. Blüher, A. Strohm, Diﬀusion in Quasicrystals, Chap. 4.1 in [5] M. Feuerbacher, C. Thomas, K. Urban, Single Quasicrystal Growth, Chap. 1.1 in [5] R. Sterzel, E. Uhrig, E. Dahlmann, A. Langsdorf, W. Assmus, Preparation of Zn-Mg-RE Quasicrystals and Related Compounds (RE = Y, Ho, Er, Dy), Chap. 1.3 in [5] P. Gille, R.-U. Barz, L.M. Zhang, Growth of Decagonal Al-Ni-Co and Al-Co-Cu Quasicrystals by the Czochralski Method, Chap. 1.5 in [5] D. Levine, P.J. Steinhardt, Phys. Rev. Lett. 53, 2477 (1984) M. Boudard, M. de Boissieu, H. Vincent, G. Heger, C. Beeli, H.-U. Nissen, R. Ibberson, M. Audier, J.-M. Dubois, C. Janot, J. Phys: Cond. Matter 4, 10149 (1992) 382 21 Diﬀusion in Quasicrystalline Alloys 20. C. Janot, Phys. Rev. B 73, 181 (1996) 21. R. Lück, Production of Quasicrystalline Alloys and Phase Diagrams, p. 222 in [4], 2002 22. C. Beeli, H.-U. Nissen, J. Robadey, Philos. Mag. Lett. 63, 87 (1991) 23. A.D. Le Claire, G. Neumann, Diﬀusion of Impurities in Metallic Elements, Chap. 3 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), Landolt Börnstein, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 24. R. Messer, S. Dais, D. Wolf, in: Proc. 18th Ampere Congress, P.S. Allen, E.R. Andrew, C.A. Bates (Eds.), Nottingham, England, 1974 25. R. Blüher, P. Scharwächter, W. Frank, H. Kronmüller, Phys. Rev. Lett. 80, 1014 (1998) 26. W. Frank, R. Blüher, I. Schmich, in: Mass and Charge Transport in Inorganic Materials – Fundamentals to Devices, P. Vincencini, V. Buscaglia (Eds.), Techna, Faenza, 2000, p. 205 27. H. Mehrer, R. Galler, Mat. Res. Soc. Symp. Proc. 553, 67 (1999) 28. F. Baier, H.-E. Schaefer, Phys. Rev. B 66, 064208 (2002) 29. W. Sprengel, F. Baier, K. Sato, X.Y. Zhang, K. Reimann, R. Würschum, R. Sterzel, W. Assmus, F. Frey, H.-E. Schaefer, Vacancies, Atomic Processes, and Structural Transformations in Quasicrystals, Chap. 4.5 in [5] 30. H.-R. Trebin, Phasons, Dislocations, and Cracks, Chap. 12 in [4] 31. P.A. Kalugin, A. Katz, Europhys. Lett 21, 921 (1993) 32. G. Bergman, J.L.T. Waugh, L. Pauling, Acta Cryst. 10, 254 (1957) 33. F.C. Frank, J.S. Kaspar, Acta Cryst. 11, 184 (1958); 12, 483 (1959) 34. R. Galler, E. Uhrig, W. Assmus, S. Flege, H. Mehrer, Defect and Diﬀusion Forum 237–240, 358 (2005) 35. W. Steurer, T. Haibach, p. 51 in [3] 36. Th. Zumkley, J.Q. Guo, A.-P. Tsai, H. Nakajima, Mat. Sci. A 294–296, 702 (2000) 37. C. Khoukaz, R. Galler, H. Mehrer, P.C. Canﬁeld, I.R. Fisher, M. Feuerbacher, Mater. Sci. Eng. A 294–296, 697 (2000) 38. C. Khoukaz, R. Galler, M. Feuerbacher, H. Mehrer, Defect and Diﬀusion Forum 194–199, 867 (2001) 39. H. Mehrer, N. Stolica, N.A. Stolwijk, Self-Diﬀusion of Solid Metallic Elements, Chap. 2 in: Diﬀusion in Solid Metals and Alloys, H. Mehrer (Vol. Ed.), Landolt Börnstein, New Series, Group III: Crystal and Solid State Physics, Vol. 26, Springer-Verlag, 1990 40. F. Gähler, S. Hocker, J. Non-Cryst. Solids 334–335, 308 (2004) Part IV Diﬀusion in Semiconductors 22 General Remarks on Semiconductors The present chapter and the two subsequent ones deal with diﬀusion in the elemental semiconductors Si and Ge. Semiconducting materials play a major rôle in high-tech equipment used in industry and in daily life. Silicon (Si) is the most important semiconductor for the fabrication of microelectronic devices such as memory and processor chips for computers and solar cells for energy production in photovoltaic devices. Germanium (Ge) constitutes the base material for γ-radiation detectors. Gallium arsenide (GaAs) and other compounds of group III and group V elements of the periodic table are mainly used in opto-electronic and high-frequency devices such as solid-state lasers in compact-disc players and receivers in cellular phones. SiC is a semiconductor with large band gap and has potential for applications in devices that must operate at high temperatures, high frequencies, and under irradiation. We remind the reader that both Si and Ge crystallise in the diamond structure. Many III-V compounds like GaAs occur in the zinc blende structure, which is closely related to the diamond structure. In both structures, the Bravais lattice is face-centered cubic and the structure can be created by the translation of two atoms at the positions (0,0,0) and a4 (1,1,1), where a is the cubic lattice parameter. In the diamond structure, both positions are occupied by the same type of atoms; in the zinc blende structure, the basis is formed by two diﬀerent types of atoms (Fig. 22.1). In both cases the Fig. 22.1. Diamond structure of Si and Ge (right) and zinc blende structure (left) 386 22 General Remarks on Semiconductors Table 22.1. Crystal structure, lattice parameters, and band gaps of Si, Ge, and of some III-V compound semiconductors according to Shaw [1] Crystal Structure Lattice parameter in nm Band gap at 300 K in eV, type of band gap Silicon (Si) Germanium (Ge) Gallium nitride (GaN) Diamond Diamond Wurtzite 1.120, indirect 0.663, indirect Gallium phosphide (GaP) Gallium arsenide (GaAs) Gallium antimonide (GaSb) Indium phosphide (InP) Indium arsenide (InAs) Indium antimonide (InSb) Zinc blende Zinc blende Zinc blende Zinc blende Zinc blende Zinc blende 0.543095 0.564613 a: 0.3111, c: 0.4978 0.54512 0.56532 0.60959 0.58687 0.60584 0.64794 3.7, direct 2.261, indirect 1.435, direct 0.72, direct 1.351, direct 0.35, direct 0.280, direct coordination number is 4, each atom is surrounded by a tetrahedron of four neighbouring atoms, and the bonding is covalent. The crystal structure, the lattice constant, the ambient temperature band gap energy, and the type of band gap are listed for the elemental group IV semiconductors and for some III-V compound semiconductors in Table 22.1. We note that both Si and Ge are semiconductors with indirect band gaps, whereas most compound semiconductors have direct band gaps. We also note that the packing density of atoms in semiconductor structures is considerably lower than in close-packed metals. Silicon-carbide (SiC) crystallises in various polytypes and has a very high melting temperature of 2545 ◦ C. Depending on the polytype the band gap lies between 2.39 and 3.26 eV. 22.1 ‘Semiconductor Age’ and Diﬀusion Periods of mankind are named after materials: stone age, bronze age, and iron age. In the 1970s the number of publications about semiconductors outnumbered for the ﬁrst time those about steels and some people started to denote the present period as the ‘semiconductor age’. This development was initiated in 1945, when a research group at the Bell Telephone Laboratories in the United States was established to focus on a better understanding of semiconductors. Vacuum tube technology had fully matured at that time but it had become also clear that the short life and the high power consumption of tubes would limit further progress in telephony and other electronic endeavours. The transistor eﬀect was discovered in 1947 by William B. Shockley, John Bardeen and Walter H. Brattain, three members of the Bell Labs group, who received the Nobel prize in physics in 1956 ‘. . . for their studies 22.1 ‘Semiconductor Age’ and Diﬀusion 387 of semiconductors and the invention of the transistor eﬀect.’ This invention triggered one of the most remarkable odysseys in the history of mankind, from the point-contact transistor via grown-junction transistors, alloy transistors, mesa transistors to planar transistor and numerous other microelectronic devices. This journey continues until the present day. Semiconductors produced a revolution in mankind at least as profound as the introduction of steam engines and steel. Nowadays, semiconductor electronics pervades our life and has an impact on everything that we do at work or at home. There was some basis for an understanding of the physics of semiconductor materials already in the 1940s. The concept of band gaps existed. Two types of conduction, already named n-type and p-type, had been identiﬁed and attributed to the presence of certain impurities (nowadays called dopants) in very small concentrations. What were called p-n junctions had been found within ingots formed by melting and refreezing the purest silicon then commercially available. In pure semiconductor crystals all valence electrons are used to form bonds of a completely occupied valence band, which is separated by the band gap from the conduction band. The latter is empty at low temperatures. Thermal excitation across the band gap can create electrons in the conduction band and ‘missing electrons in the valence band’, which are called holes. Electrons and holes give rise to the intrinsic carrier density and the associated conductivity of a semiconductor. The carrier density increases according to a Boltzmann factor containing the gap energy. Although the ﬁrst transistor – and about ten years later the ﬁrst integrated circuits – were made not from Si but from its sister element Ge, it was soon understood that Si would be a better transistor material than Ge for most applications. This mainly resulted from the higher band gap of Si (see Table 22.1). In Ge at room temperature, the thermal generation of minority carriers led to substantial reverse currents in p-n junctions. The reverse current in Si was orders of magnitude smaller and made the material a superior rectiﬁer. However, at the beginning of the odyssey there was much uncertainty, much still unknown. The highest purity of semiconductors available was orders of magnitude above the purity that was eventually needed. Semiconductor materials were polycrystals and frequently used in powder form. The chemist Jan Czochralski (1885–1953), who was born in West Prussia, Germany, (now part of Poland), developed the Czochralski (CZ) process. This process has been used since the 1950s to grow semiconductor single crystals. The most serious problem with Si was that critical chemical and metallurgical processes all took place at higher temperatures than with Ge. These problems were solved and oriented single crystals of silicon, germanium and of III-V compounds could be grown. Nowadays, high-purity and high-perfection CZ silicon single crystals 30 cm in diameter and 2 m long, weighing 150 kg are commercial standard and are used in the production of silicon wafers. The production of larger crystals is on the way. 388 22 General Remarks on Semiconductors Foreign atoms incorporated in the crystal lattice are vital for the electronic properties of semiconductors. The group III elements boron (B), aluminium (Al), gallium (Ga), indium (In) in Si and Ge and Zn in GaAs act as acceptors since they can pick an electron from the valence band by creating a hole. The donor elements phosphorus (P), arsenic (As), antimony (Sb), bismuth (Bi) in Si and Ge can provide electrons to the conduction band. The conductivity (resistivity) of a semiconductor can be changed by the process of doping by several orders of magnitude, about eight orders in the case of silicon (Fig. 22.2). The in-diﬀusion of doping elements into the semiconductor surface is an important process during device fabrication, whereas background doping is performed by adding the doping element to the semiconductor melt during the crystal growth process. A further important observation was made at Bell Laboratories in 1955. A thin layer of silicon dioxide grown by thermal oxidation on the surface of silicon prior to diﬀusion could mask the diﬀusion of certain donor and acceptor elements into Si. It was also discovered that diﬀusion would occur unimpeded through windows etched into the oxide layer. Somewhat later it was shown that certain photoresists deposited at the oxide surface prevent etching of the oxide. Hence, optical exposure of the resist by projection or through contact masks could be used to create precise window patterns in Fig. 22.2. Resistivity of various materials and silicon of various doping levels 22.2 Speciﬁc Features of Semiconductor Diﬀusion 389 the oxide and in turn provide precise control of the areas in which diﬀusion would occur. This combined process of photolithography and oxide masking (photoresist process) has since been developed to a precision that can be controlled to sub-micrometer scales. This development complements the precision of the depth control of junctions diﬀused into the Si surface, providing the means to control the fabrication of devices in three dimensions to the precision of a fraction of a micron. These advances also ended the rôle of Ge as a major player. No material was found that would provide diﬀusion masking for Ge. Transistor densities on integrated circuits manufactured on Si wafers have increased exponentially over decades, by a succession of lithography techniques, which are used in chip making to project patterns on wafers. Gordon Moore, a co-founder of the Intel Company, says ‘. . . the number of elements on a microchip and the switching speed double every eighteen month’ – a rule that has worked for over 40 years. The greatest impact of the III-V compound semiconductors has not been in the areas dominated by Si. Its applications depend one unique properties of these compounds. One class of applications is based on the transfer of highmobility electrons from the conduction-band minimum to the low-mobility indirect minimum such as that found in GaAs and other direct band gap semiconductors. One rapidly evolving technology based on electroluminescence is optoelectronics, where Si and Ge still cannot compete with direct band gap III-V compounds. Electroluminescence is the emission of light associated with the application of a small voltage. In 1962, the observation of high quantum eﬃciencies in the infrared for GaAs and in the visible for GaP, and the achievement of laser action in GaAs resulted in considerable research and development activity on III-V compounds. It has been demonstrated later that high-brightness light emitting diodes (LED’s) based on III-V GaN compound devices can be used for interior and exterior applications in automobiles and in traﬃc lights. Silicon-carbide is a material with high potential for some niche applications due to its high melting temperature, its large band gap and its high thermal conductivity. These applications include high-temperatures up to 1000 ◦ C, high voltages, and applications under conditions of particle irradiation. Recent improvements of the quality and size of SiC wafers are promising for SiC microelectronic devices. We end this section by drawing the reader’s attention to literature about the signiﬁcance of semiconductors [2–5]. 22.2 Speciﬁc Features of Semiconductor Diﬀusion The advent of microelectronic and optoelectronic devices has strongly stimulated the interest in diﬀusion processes in semiconductors, because solid-state diﬀusion is used as a fundamental process in their manufacture. Elements 390 22 General Remarks on Semiconductors from diﬀerent parts of the periodic table have been studied with respect to their diﬀusion behaviour for various reasons: – – – – – – Shallow dopants such as B, P in Si, As, Ga in Ge and Zn in GaAs determine the conductivity type of the material. The light elements O and C are major contaminants and diﬃcult to eliminate during chemical processing and crystal growth. In Czochralski-grown Si single crystals, oxygen plays a crucial rôle for impurity gettering. Some impurities introduce deep levels in the forbidden gap of the semiconductors. Such impurities like Au in Si are useful for eﬀective electron-hole recombination in fast switching devices. Another example is Cr, which is used for electronic compensation of hard to avoid donors and acceptors in GaAs. Fast diﬀusing metallic impurities are feared for their detrimental eﬀects on device performance. Well-known examples are Fe and Ni in Si and Cu in Ge. Without taking severe precautions, these metals are unintentionally introduced during high-temperature processes. Other metallic elements are deliberately deposited on semiconductor surfaces to produce ohmic or rectifying contacts. Last but not least, several elements are of interest from a fundamental point of view: – Diﬀusion of self-atoms is the most basic diﬀusion process. Therefore, its understanding is important. – The diﬀusion of hybrid solutes such as Au, Pt, Zn, Ir in Si and Cd, Zn in GaAs can provide information on native point defects. Hybrid solutes dissolve on substitutional and interstitial sites of the host crystal. Their diﬀusivity in the interstitial state is much higher than in the substitutional state. To be able to predict and control diﬀusion steps is important for the design and development of semiconductor devices. If diﬀusion exhibited only simple behaviour following from Fick’s laws for constant diﬀusivity, the prediction of the diﬀusion behaviour would then be a straightforward task, limited only by the accuracy of the diﬀusion data. That diﬀusion in semiconductors can be considerably more complicated became apparent in the early 1960s and continues to the present day. The scientiﬁc and technological problems that have emerged are associated with the fact that in semiconductors particular factors inﬂuence diﬀusion. Such factors are: 1. The covalent bonding entails relatively high formation enthalpies of intrinsic point defects such as vacancies and self-interstitials. As a consequence, the concentrations of point defects in thermal equilibrium are orders of magnitude lower than in metals (see Chap. 5). 2. The open structure of the diamond and zinc blende lattice favours interstitial incorporation of self- and foreign atoms. For this reason, interstitial 22.2 Speciﬁc Features of Semiconductor Diﬀusion 3. 4. 5. 6. 7. 8. 9. 391 diﬀusion and interstitial-substitutional exchange diﬀusion of hybrid solutes via the dissociative or kick-out mechanisms, (see Chaps. 6 and 25) are more prominent in semiconductors than in metals. Beside vacancies, self-interstitials may act as diﬀusion vehicles. It is generally accepted that shallow dopants in silicon and host atoms exchange with both types of intrinsic point defects. This so-called dual mechanism gives rise to a variety of complex diﬀusion phenomena. The covalent bonding between the host atoms limits the solubility of most foreign atoms to ppm ranges. This also implies that small amounts of solute substance can act as inexhaustible diﬀusion sources. Commercially available semiconductors are extremely pure. Impurity levels are commonly below about 0.1 ppm. Therefore, stringent precautions must be taken in order to reduce impurity contamination during sample preparation and diﬀusion treatments. Some semiconductor materials can be grown as single crystals with very high perfection. Dislocations densities vary from values as low as 103 to 104 cm2 (GaAs) to virtually zero (Si). Germanium crystals with dislocation densities in the range 103 to 105 cm−2 are quite common. Grain boundaries and dislocations, which usually help attain the equilibrium concentration of point defects, are often absent. Then, only free surfaces can act as sinks or sources for the annihilation or creation of point defects. Electronic eﬀects play an important rôle in semiconductors: a) The electric-ﬁeld eﬀect accounts for the diﬀusion drift, which is due to the electric ﬁeld built-up by inhomogeneous distributions of dopants. b) The Fermi-level eﬀect describes changes in the equilibrium concentration of intrinsic point defects or in the solute solubilities, caused by shifts of the Fermi level. These changes are due to the fact that point defects and solute atoms can occur in various charge states (neutral and ionised). Shifts of the Fermi level originate either by background doping or can be induced by the diﬀusing species itself. c) Self-doping during the diﬀusion of a solute, which acts as dopant, can lead to non-Fickian diﬀusion proﬁles. Due to the larger band gap the Fermi-level eﬀect is more important in GaAs than in Si and Ge. For the elemental semiconductors it is detectable in diﬀusion mainly at high doping concentrations. d) Ion-pairing eﬀects arise from the Coulomb interaction between charged solute atoms and intrinsic point defects. Surface reactions proceeding under certain ambient conditions may strongly inﬂuence solute diﬀusion. Oxidation-enhanced or -retarded diﬀusion is a well-known example. The crucial rôle of self-interstitials injected into silicon by the oxidising SiO2 /Si interface is a widely accepted example. Point defects such as vacancies and self-interstitial, if created or annihilated for example in dissociative or kick-out reactions with hybrid solutes, 392 22 General Remarks on Semiconductors can occur in under- or oversaturation (see Chap. 25). This is because grain boundaries and dislocations, which usually help attain the equilibrium concentration of point defects, are often absent in perfect semiconductor crystals. A comprehensive collection of diﬀusion data in Si and Ge, Si-Ge, and SiC alloys has been assembled by Stolwijk and Bracht [6]. Diﬀusion data for silicides are summarised by Gas and d’Heurle [7] and those for compound semiconductors by Dutt and Sharma [8]. Solubility data for solutes in Si have been collected by Bracht and Stolwijk and for solutes in Ge by Stolwijk and Bracht and can be found in [10]. Chemical diﬀusion data in inhomogeneous semiconductor compounds are summarised by Bruff and Murch [9]. The subjects of diﬀusion and point defects in semiconductors have been treated in a textbook [1] and many reviews [11–20]. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. D. Shaw (Ed.), Atomic Diﬀusion in Semiconductors, Plenum Press, 1973 I.M. Ross, The Foundation of Semiconductor Age, Physics Today, 34–47 (1997) H. Queisser, The Conquest of the Microchip, Havard Univerity Press, 1998 M. Eckert, H. Schubert, Crystals, Electrons, Transistors, AIP, 1997 M. Riordan, L. Hoddeson, Crystal Fire, W.W. Norton and Co., 1997 N.A. Stolwijk, H. Bracht, Diﬀusion in Silicon, Germanium and their Alloys, in: Diﬀusion in Semiconductors and Non-Metallic Solids, D.L. Beke (Vol. Ed.), Landolt-Börnstein, New Series, Group III, Vol. 33, Subvolume A, SpringerVerlag, Berlin, 1998 P. Gas, F.M. d’Heurle, Diﬀusion in Silicides, in: Diﬀusion in Semiconductors and Non-Metallic Solids, D.L. Beke (Vol. Ed.), Landolt-Börnstein, New Series, Group III, Vol. 33, Subvolume A, Springer-Verlag, Berlin, 1998 M.B. Dutt, B.L. Sharma, Diﬀusion in Compound Semiconductors, in: Diﬀusion in Semiconductors and Non-Metallic Solids, D.L. Beke (Vol. Ed.), LandoltBörnstein, New Series, Group III, Vol. 33, Subvolume A, Springer-Verlag, Berlin, 1998 C.M. Bruﬀ, G.E. Murch, Chemical Diﬀusion in Semiconductors, in: Diﬀusion in Semiconductors and Non-Metallic Solids, D.L. Beke (Vol. Ed.), LandoltBörnstein, New Series, Group III, Vol. 33, Subvolume A, Springer-Verlag, Berlin, 1998 M. Schulz (Vol. Ed.), Impurities and Defects in Group IV Elements and IIIV Compounds, Landolt-Börnstein, New Series, Group III, Vol. 22b, SpringerVerlag, Berlin, 1989 A. Seeger, K.P. Chik, Diﬀusion Mechanisms and Point Defects in Silicon and Germanium, Phys. Stat. Sol. 29, 455–542 (1968) D. Shaw, Self- and Impurity Diﬀusion in Ge and Si, Phys. Stat. Sol. (b) 72, 11–39 (1975) A.F. Willoughby, Atomic Diﬀusion in Semiconductors, Rep. Progr. Phys. 41, 1665–1705 (1978) References 393 14. W. Frank, U. Gösele, H. Mehrer, A. Seeger, Diﬀusion in Silicon and Germanium, in: Diﬀusion in Crystalline Solids, G.E. Murch, A.S. Nowick (Vol. Eds.), Academic Press Inc., 1984 15. P.M. Fahey, P.B. Griﬃn, J.D. Plummer, Point Defects and Dopant Diﬀusion in Silicon, Rev. Mod. Phys. 61, 289–384 (1989) 16. N.A. Stolwijk, Atomic Transport in Semiconductors: Diﬀusion Mechanisms and Chemical Trends, Defect and Diﬀusion Forum 95–98, 895–916 (1993) 17. S.M. Hu, Mater. Sci. Eng. R13, 105 (1994) 18. N.A. Stolwijk, G. Bösker, J. Pöpping, Hybrid Impurity and Self-Diﬀusion in GaAs and Related Compounds: Recent Progress, Defect and Diﬀusion Forum 194–199, 687–702 (2000) 19. H. Bracht, Diﬀusion and Intrinsic Point-Defect Properties in Silicon, MRS Bulletin, 22–27. June 2000 20. T.Y. Tan, U. Gösele, Diﬀusion in Semiconductors, in: Diﬀusion in Condensed Matter – Methods, Materials, Models, P. Heitjans, J. Kärger (Eds.), SpringerVerlag, 2005, p. 165 23 Self-diﬀusion in Elemental Semiconductors Compared with metals, self-diﬀusion in semiconductors is a very slow process. For the elemental semiconductors this is illustrated in Fig. 23.1, in which the self-diﬀusivities of Si and Ge are compared with those of typical metals. At the melting temperature Tm , self-diﬀusion in Si and Ge is at least four orders of magnitude slower than in metals. This diﬀerence increases at lower temperatures due to the relatively large activation enthalpies of the semiconducting materials. Generally speaking, the origin of these diﬀerences and of others to be discussed in the present chapter and in the two subsequent ones lies in the diﬀerence between metallic and covalent bonding. The basic question is the same as in the case of metals: What are the mechanisms of self-diﬀusion? Does it occur by a vacancy or an interstitialcy mechanism (see Chap. 6)? The usual way to answer this question is to determine the mobility and the equilibrium concentration of point defects sep- Fig. 23.1. Self-diﬀusion of Si and Ge and of some metals (Cu, Au, Na) in a homologous temperature scale 396 23 Self-diﬀusion in Elemental Semiconductors arately as functions of temperature and to check whether they are able to account for the measured values of self-diﬀusion. In the case of metals, direct techniques such as diﬀerential dilatometry, positron annihilation, or quenching from high temperatures (see Chap. 5) have thrown considerable light on point defects and diﬀusion. Up to now, it has not been possible to deduce reliable information on the concentration of equilibrium point defects in semiconductors by any of the direct techniques. Very likely, these ‘conventional’ techniques fail for semiconductors, because the equilibrium concentrations of intrinsic point defects are extremely small, presumably less or much less than one ppm near the melting temperature. This implies that point defect concentrations are below the present detection limits of the above mentioned techniques. This is in accordance with the low self-diﬀusivities, which can be attributed largely to low equilibrium concentrations of intrinsic defects. For Si and Ge, the above questions had to be answered by employing less direct approaches. In this context, the study and thorough analysis of foreign atom diﬀusion turned out to be a useful tool. For example, this tool permitted to separate the contributions of vacancies and self-interstitials to the self-diﬀusion coeﬃcient of silicon (see below). 23.1 Intrinsic Point Defects and Diﬀusion Unlike in metals, in semiconductors not only vacancies (V ) but also selfinterstitials (I) are relevant for atomic transport. The thermal concentration of self-interstitials, CIeq , and their diﬀusivity, DI , are described by F SI HIF eq CI = exp exp − and kB kB T M SI HM exp − I , (23.1) DI = gI a2 νI0 exp kB kB T where HIF and HIM are the formation and migration enthalpies, SIF and SIM denote the respective entropies of self-interstitial formation and migration, a is the lattice parameter, gI = 1/4 is the geometry factor for interstitialcy diﬀusion, and νI0 an attempt frequency of the order of the Debye frequency. The thermal concentration of vacancies, CVeq , and their diﬀusivity, DV , are described by F SV HVF eq CV = exp exp − and kB kB T M HM SV exp − V , (23.2) DV = gV a2 νV0 exp kB kB T 23.1 Intrinsic Point Defects and Diﬀusion 397 where HVF and HVM are the formation and migration enthalpies, SVF and SVM denote the respective entropies. gV = 1/8 is the geometry factor for vacancy diﬀusion in the diamond structure and νV0 the vacancy attempt frequency. Vacancies and self-interstitials in semiconductors may carry electronic charge due to the energy levels of the defects in the band gap (see Chap. 5). At room temperature, the relative abundancies among the diﬀerently charged point defects can be readily changed by n- or p-doping of the base material. By contrast, at the elevated temperatures usually encountered in diﬀusion experiments, doping levels as high as 1025 m−3 are necessary to render Ge or Si electronically extrinsic (see, e.g., the textbook of Sze [1]). In GaAs lower dopant concentrations of 1024 m−3 are already enough for extrinsic behaviour at 1200 K. This is a consequence of the higher band gap energy of GaAs and of the associated lower intrinsic carrier concentrations compared to Ge and Si. In what follows, we concentrate on elemental semiconductors. Then, it is often suﬃcient to consider intrinsic conditions. Despite their weak sensitivity in elemental semiconductors to doping, CIeq and CVeq as well as CIeq DI and DVeq DV contain contributions of several charge states [2, 3]: CIeq = CIeq0 + CIeq+ + CIeq2+ + . . . (23.3) CVeq = CVeq+ + CVeq0 + CVeq− . . . , (23.4) and CIeq DI = CIeq0 DI 0 + CIeq+ DI + + CIeq2+ DI 2+ + . . . (23.5) CVeq DV (23.6) = CVeq+ DV + + CVeq0 DV 0 + CVeq− DV − + ... . I 0 , I + , I 2+ , V + , V 0 , V − , . . . denote charge states of self-interstitials and vacancies. Unfortunately, it is still not unambigously known which conﬁgurations dominate at various temperatures in Si [3]. On the other hand, there is more information on vacancy charge states in Ge [5] (see below). However, for Ge and Si self-diﬀusion in intrinsic material it often suﬃces to utilise the overall transport product of self-interstitials, CIeq DI , relative to that of vacancies, CVeq DV . The transport products are intimately connected with the tracer diﬀusivities of host atoms [4–6]. Taking into account contributions of the vacancy and of the interstitialcy mechanism to self-diﬀusion, the tracer diﬀusivity is given by (23.7) D∗ = fI CIeq DI + fV CVeq DV + Dex . ≈0 fI = 0.7273 is the correlation factor for the interstitialcy mechanism and fV = 0.5 for the vacancy mechanism in the diamond lattice (see Table 7.2). Dex stands for a possible contribution from a direct exchange of 398 23 Self-diﬀusion in Elemental Semiconductors crystal atoms. However, ﬁrst-principles calculations of self-diﬀusion coeﬃcients have shown that Dex plays no rôle [26] and no experimental evidence has been found for direct exchange. In the following we omit this term in Eq. (23.7). The self-interstitial can be the major diﬀusion vehicle under certain conditions, e.g., in Si at high temperatures or in GaAs under heavy p-doping. This does not necessarily mean that the self-interstitial concentration in thermal equilibrium, CIeq , is higher than the equilibrium concentration of vacancies, CVeq . What counts from the standpoint of diﬀusion is the magnitude of the transport product CIeq DI relative to DVeq DV . A low defect concentration may be overcompensated by a high defect mobility. This is the case for Si, where CIeq CVeq but nevertheless CIeq DI > DVeq DV holds at high temperatures. By contrast, vacancies are the major diﬀusion vehicles in Ge (see below). 23.2 Germanium Self-diﬀusion studies in germanium have been performed by radioactive tracers (71 Ge or 68 Ge). Letaw et al. [7] and Valenta and Ramasashtry [8] used radiotracer techniques in combination with either mechanical or chemical sectioning techniques. In the latter case, the eﬀect of heavy doping was also studied. Widmer and Gunter-Mohr [9] employed neutron activated natural Ge, in which 71 Ge is the most abundant radioisotope, and either the Steigmann or the Gruzin technique (see Chap. 13) in combination with grinder sectioning. Campbell [10] studied the simultaneous diﬀusion of the radioisotopes 71 Ge and 77 Ge at 900 and 925 ◦ C and deduced the isotope eﬀect therefrom. Vogel et al. [11] and Werner et al. [12] used 71 Ge and employed a sputtering technique for serial sectioning (see Chap. 13). In [12] the inﬂuence of n- and p-doping and the eﬀect of hydrostatic pressure on self-diﬀusion was also investigated. Fuchs et al. [13] used stable 70 Ge/74 Ge isotope heterostructures grown by molecular-beam epitaxy and SIMS proﬁling after interdiﬀusion. The overall agreement between self-diﬀusion data of various authors is good (Fig 23.2). The temperature dependences are well described by Arrhenius laws and the activation parameters obtained from the measurements of diﬀerent groups (D0 : 7.8×10−4 to 44 ×10−4 m2 s−1 ; ∆H: 2.97 eV to 3.14 eV) are not much diﬀerent. The pre-exponential factors of Ge are larger than the D0 values for typical metals (see Chap. 17). The corresponding self-diﬀusion entropy is about 10 kB for Ge, whereas for close-packed metals values between 1 and 3 kB are common. It is commonly agreed (see, e.g., [4–6]) that self-diﬀusion in Ge occurs by a vacancy mechanism. This interpretation is among other observations (see also Chaps. 24 and 25) supported by the following ones: – Measurements of the dependence of the diﬀusion coeﬃcient on the isotope mass (isotope eﬀect) have been performed by Campbell using the isotope 23.2 Germanium 399 Fig. 23.2. Self-diﬀusion coeﬃcients of Ge measured by tracer methods [7–9, 11, 12] pair 71 Ge/77 Ge [10]. The following values of the isotope eﬀect parameter E (see Chaps. 24 and 25) have been reported: E = f ∆K = 0.25 to – 0.3 (23.8) The correlation factor f for a vacancy mechanism in the diamond structure is 0.5. Hence, the interpretation in terms of a vacancy mechanism requires values of the kinetic energy factor ∆K = 0.5 to 0.6. Such values are smaller than the values of ∆K ≈ 0.9, which are typical for monovacancies in close-packed metals. ∆K decreases with the number of atoms with which the diﬀusing atom shares its kinetic energy in the saddle point. It has been concluded that in close-packed metals the vacancy is rather localised with only small relaxation of neighbouring atoms whereas in germanium it is more relaxed [5]. This is in accordance with the relatively large diﬀusion entropy mentioned above. The doping dependence of Ge self-diﬀusion has been attributed to the vacancy mechanism with contributions of neutral and charged vacancies. 400 23 Self-diﬀusion in Elemental Semiconductors Diﬀusion-mediating defects in semiconductors occur in various charge states (see above and Chap. 5). The equilibrium concentration of charged defects depends on the position of the Fermi level. A vacancy in germanium has an acceptor level in the lower half of the band gap [4]. If self-diﬀusion proceeds via neutral vacancies (V 0 ) and singly charged vacancies (V − ), the total tracer self-diﬀusion coeﬃcient D∗ is given by D∗ = DV∗ 0 + DV∗ − , (23.9) where DV∗ 0 denotes the contribution of neutral vacancies and DV∗ − that of charged vacancies. These contributions are given by DV∗ 0 = fV gV a2 ωV 0 CVeq0 DV∗ − = fV gV a 2 and ωV − CVeq− , (23.10) where fV is the correlation factor, gV a geometrical factor, and a the lattice parameter. For the vacancy mechanism in the diamond lattice, we have fV = 0.5 and gV = 1/8. CVeq0 and CVeq− denote the concentrations of neutral and charged vacancies in thermal equilibrium, ωV 0 and ωV − the exchange jump rates between tracer atom and neutral and charged vacancies, respectively. For non-degenerate semiconductors it is readily shown (see Chap. 5) that CVeq− (n) n = , eq CV − (ni ) ni (23.11) where n and ni are the free electron densities in the doped and intrinsic material, respectively. Combining Eqs. (23.9), (23.10), and (23.11) yields for the ratios of self-diﬀusion under extrinsic and intrinsic conditions D∗ 0 (ni ) n DV∗ − (ni ) D∗ (n) = V∗ + . ∗ D (ni ) D (ni ) ni D∗ (ni ) (23.12) This equation predicts a linear dependence of the tracer diﬀusivity on the ratio n/ni . It is based on the assumption that the vacancy occurs in a neutral and a single-acceptor state. The occurrence of additional charge states would lead to additional terms in Eq. (23.12) with factors (n/ni )r for an acceptor level and to (ni /n)r for a donor level, where r is the multiplicity of the ionised state. Figure 23.3 shows the ratio of Ge self-diﬀusion in doped germanium to that in intrinsic germanium, D∗ (n)/D∗ (ni ), versus the ratio of the free electron densities, n/ni , according to [12]. The diﬀusivity increases with n-doping and decreases with p-doping. In addition, Fig. 23.3 shows that vacancies with a single-acceptor state are responsible for Ge self-diﬀusion and that additional levels are not essential for the description of the doping dependence of self-diﬀusion. 23.2 Germanium 401 Fig. 23.3. Doping dependence of Ge self-diﬀusion according to Werner et al. [12] – Further information about the nature and properties of point defects involved in the diﬀusion process has been deduced from the eﬀect of pressure on diﬀusion (see Chap. 8). Measurements of Ge self-diﬀusion under pressure are reported in [12]. The activation volumes are comparatively small and vary from 0.24 to 0.41 atomic volumes (Ω) as the temperature increases from 876 to 1086 K (Fig. 23.4). Values of the activation volume for self-diﬀusion of gold are shown for comparison [14]. These larger values are typical for vacancy-mediated diﬀusion in close-packed metals. The lower values for Ge support the concept that self-diﬀusion in Ge occurs via vacancies, which are more relaxed or ‘spread-out’ than in close-packed materials. The positive sign very likely excludes self-interstitials as the defects responsible for Ge self-diﬀusion. For an interstitialcy mechanism the activation volume should be negative (see Chap. 8). The experimental activation volume increases with temperature. This increase can be attributed to the fact that neutral and negatively charged vacancies with diﬀernet activation volumes contribute to self-diﬀusion. The activation volume of the neutral vacancy contribution (∆VV 0 = 0.56 Ω) is larger than that of the negatively charged vacancy (∆VV − = 0.28 Ω) [12]. The experimental activation volume is an average value weighted with t